#------------------------------------------------------------------------------
#$Date: 2018-11-16 15:31:04 +0200 (Fri, 16 Nov 2018) $
#$Revision: 212008 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/35/2103512.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2103512
loop_
_publ_author_name
'Pavlovska, A.'
'Werner, S.'
'Maximov, B.'
'Mill, B.'
_publ_section_title
;
 Pressure-induced phase transitions of piezoelectric single crystals
 from the langasite family: La₃Nb~0.5~Ga~5.5~O₁₄ and
 La₃Ta~0.5~Ga~5.5~O₁₄
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              939
_journal_page_last               947
_journal_paper_doi               10.1107/S0108768102010273
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Ga11 La6 O28 Ta'
_chemical_formula_weight         2229.33
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'A 2y'
_symmetry_space_group_name_H-M   'A 1 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   5.013
_cell_length_b                   7.944
_cell_length_c                   13.759
_cell_measurement_temperature    293(2)
_cell_volume                     547.9
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_pressure         14.4E+6
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.505
_diffrn_measured_fraction_theta_max 0.505
_diffrn_radiation_source         synchrotron
_diffrn_radiation_wavelength     0.56000
_diffrn_reflns_av_R_equivalents  0.0436
_diffrn_reflns_av_sigmaI/netI    0.0506
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            963
_diffrn_reflns_theta_full        22.97
_diffrn_reflns_theta_max         22.97
_diffrn_reflns_theta_min         3.96
_exptl_absorpt_coefficient_mu    15.715
_exptl_crystal_density_diffrn    6.756
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             980
_refine_diff_density_max         1.896
_refine_diff_density_min         -1.727
_refine_diff_density_rms         0.409
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.08(11)
_refine_ls_extinction_coef       0.0043(13)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.144
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     75
_refine_ls_number_reflns         700
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.143
_refine_ls_R_factor_all          0.0460
_refine_ls_R_factor_gt           0.0460
_refine_ls_shift/su_max          0.417
_refine_ls_shift/su_mean         0.076
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1318
_refine_ls_wR_factor_ref         0.1318
_reflns_number_gt                700
_reflns_number_total             700
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            sn0021-14.4d3a2.cif
_cod_data_source_block           14.4d3a2
_cod_depositor_comments
;
The _diffrn_ambient_pressure was taken from the original data block
header, after comparison with the paper text and supplementary
material.

When more than one structure was present in the sn0021.cif file for a
given pressure, the structure with the minimal _refine_ls_R_factor_all
value was taken as the best one, and all others marked with the
'_cod_suboptimal_structure yes' tag.

Changing (with the help of Perl) all _diffrn_radiation_source values in
the files that were reportedly colected on the HASYLAB D3 beamline
(Hamburg) from 'fine-focus sealed tube' to synchrotron.

The command was:

perl -i -ne \
    "s/'fine-focus sealed tube'/synchrotron/; \
    print unless /_diffrn_radiation_type|_diffrn_radiation_monochromator/" \
    *d3*.cif \
    11.57split.cif \
    21.85split.cif \
    22.85split.cif

Saulius Gra\<zulis
;
_cod_database_code               2103512
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x, y+1/2, z+1/2'
'-x, y+1/2, -z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
La1 La -0.0021(9) 0.2160(4) 0.7807(4) 0.0233(10) Uani 1 1 d .
La2 La 0.0000 0.5638(6) 0.0000 0.0220(13) Uani 1 2 d S
Ga1 Ga 0.0000 0.0001(10) 0.0000 0.0289(9) Uani 0.50 2 d SP
Ta Ta 0.0000 0.0001(10) 0.0000 0.0289(9) Uani 0.50 2 d SP
Ga2 Ga 0.5178(7) 0.4963(14) 0.1654(7) 0.0212(10) Uani 1 1 d .
Ga3 Ga 0.5000 0.2286(15) 0.0000 0.019(3) Uani 1 2 d S
Ga4 Ga 0.495(2) 0.3846(10) 0.6194(7) 0.0204(15) Uani 1 1 d .
O1 O 0.166(4) 0.494(8) 0.170(5) 0.019(3) Uiso 1 1 d .
O2 O 0.297(11) 0.967(9) 0.222(5) 0.056(18) Uiso 1 1 d .
O3 O 0.704(7) 0.355(3) 0.079(3) 0.013(6) Uiso 1 1 d .
O4 O -0.348(11) 0.715(6) 0.190(5) 0.060(12) Uiso 1 1 d .
O5 O 0.276(7) 0.104(5) 0.083(3) 0.026(8) Uiso 1 1 d .
O6 O 0.796(6) 0.012(4) 0.120(2) 0.012(6) Uiso 1 1 d .
O7 O 0.226(7) 0.806(5) 0.032(3) 0.019(9) Uiso 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.9400 1.6200 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.9400 4.4000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2490 1.0600 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0028 0.0036 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O4 La1 O5 89.5(19) 3_545 2_556
O4 La1 O6 133.7(16) 3_545 2_656
O5 La1 O6 63.7(11) 2_556 2_656
O4 La1 O1 84.0(17) 3_545 2_556
O5 La1 O1 85.8(14) 2_556 2_556
O6 La1 O1 127.1(16) 2_656 2_556
O4 La1 O2 107(2) 3_545 3_545
O5 La1 O2 144.8(15) 2_556 3_545
O6 La1 O2 116.8(17) 2_656 3_545
O1 La1 O2 65.9(16) 2_556 3_545
O4 La1 O1 85.0(17) 3_545 3_545
O5 La1 O1 113.5(16) 2_556 3_545
O6 La1 O1 73.8(17) 2_656 3_545
O1 La1 O1 157.6(14) 2_556 3_545
O2 La1 O1 99.0(19) 3_545 3_545
O4 La1 O3 151.1(16) 3_545 2_656
O5 La1 O3 84.8(11) 2_556 2_656
O6 La1 O3 67.7(9) 2_656 2_656
O1 La1 O3 67.4(14) 2_556 2_656
O2 La1 O3 65.8(13) 3_545 2_656
O1 La1 O3 123.2(12) 3_545 2_656
O4 La1 O2 60.0(18) 3_545 2_546
O5 La1 O2 52.9(17) 2_556 2_546
O6 La1 O2 73.9(17) 2_656 2_546
O1 La1 O2 121.6(17) 2_556 2_546
O2 La1 O2 161.2(5) 3_545 2_546
O1 La1 O2 68.0(18) 3_545 2_546
O3 La1 O2 132.5(14) 2_656 2_546
O4 La1 Ga2 31.0(14) 3_545 3_445
O5 La1 Ga2 77.1(9) 2_556 3_445
O6 La1 Ga2 103.3(8) 2_656 3_445
O1 La1 Ga2 111.0(9) 2_556 3_445
O2 La1 Ga2 131.1(16) 3_545 3_445
O1 La1 Ga2 65.5(7) 3_545 3_445
O3 La1 Ga2 161.9(7) 2_656 3_445
O2 La1 Ga2 31.8(15) 2_546 3_445
O4 La1 Ga2 135.6(15) 3_545 2_656
O5 La1 Ga2 117.7(9) 2_556 2_656
O6 La1 Ga2 90.6(8) 2_656 2_656
O1 La1 Ga2 65.5(7) 2_556 2_656
O2 La1 Ga2 32.3(15) 3_545 2_656
O1 La1 Ga2 111.0(8) 3_545 2_656
O3 La1 Ga2 33.9(6) 2_656 2_656
O2 La1 Ga2 164.2(15) 2_546 2_656
Ga2 La1 Ga2 163.4(2) 3_445 2_656
O4 La1 Ta 120.5(16) 3_545 1_556
O5 La1 Ta 33.8(8) 2_556 1_556
O6 La1 Ta 32.3(7) 2_656 1_556
O1 La1 Ta 101.8(15) 2_556 1_556
O2 La1 Ta 129.9(15) 3_545 1_556
O1 La1 Ta 100.6(16) 3_545 1_556
O3 La1 Ta 64.8(6) 2_656 1_556
O2 La1 Ta 67.7(15) 2_546 1_556
Ga2 La1 Ta 98.9(2) 3_445 1_556
Ga2 La1 Ta 97.6(2) 2_656 1_556
O4 La1 Ga1 120.5(16) 3_545 1_556
O5 La1 Ga1 33.8(8) 2_556 1_556
O6 La1 Ga1 32.3(7) 2_656 1_556
O1 La1 Ga1 101.8(15) 2_556 1_556
O2 La1 Ga1 129.9(15) 3_545 1_556
O1 La1 Ga1 100.6(16) 3_545 1_556
O3 La1 Ga1 64.8(6) 2_656 1_556
O2 La1 Ga1 67.7(15) 2_546 1_556
Ga2 La1 Ga1 98.9(2) 3_445 1_556
Ga2 La1 Ga1 97.6(2) 2_656 1_556
Ta La1 Ga1 0.0(2) 1_556 1_556
O7 La2 O7 64.6(19) . 2
O7 La2 O1 121.7(17) . 2
O7 La2 O1 81.0(15) 2 2
O7 La2 O1 81.0(15) . .
O7 La2 O1 121.7(17) 2 .
O1 La2 O1 155(3) 2 .
O7 La2 O3 141.3(13) . 1_455
O7 La2 O3 110.6(12) 2 1_455
O1 La2 O3 93.4(14) 2 1_455
O1 La2 O3 69.4(13) . 1_455
O7 La2 O3 110.6(12) . 2_655
O7 La2 O3 141.3(13) 2 2_655
O1 La2 O3 69.4(13) 2 2_655
O1 La2 O3 93.4(14) . 2_655
O3 La2 O3 95.8(13) 1_455 2_655
O7 La2 O4 65.8(15) . 2
O7 La2 O4 78.9(13) 2 2
O1 La2 O4 62.2(13) 2 2
O1 La2 O4 128.5(11) . 2
O3 La2 O4 152.8(12) 1_455 2
O3 La2 O4 65.7(11) 2_655 2
O7 La2 O4 78.9(13) . .
O7 La2 O4 65.8(15) 2 .
O1 La2 O4 128.5(11) 2 .
O1 La2 O4 62.2(13) . .
O3 La2 O4 65.7(11) 1_455 .
O3 La2 O4 152.8(12) 2_655 .
O4 La2 O4 138.3(18) 2 .
O7 La2 Ga2 111.3(10) . 1_455
O7 La2 Ga2 84.7(10) 2 1_455
O1 La2 Ga2 110.6(7) 2 1_455
O1 La2 Ga2 65.1(6) . 1_455
O3 La2 Ga2 33.5(7) 1_455 1_455
O3 La2 Ga2 128.3(7) 2_655 1_455
O4 La2 Ga2 162.8(10) 2 1_455
O4 La2 Ga2 32.7(9) . 1_455
O7 La2 Ga2 84.7(10) . 2_655
O7 La2 Ga2 111.3(10) 2 2_655
O1 La2 Ga2 65.1(6) 2 2_655
O1 La2 Ga2 110.6(7) . 2_655
O3 La2 Ga2 128.3(7) 1_455 2_655
O3 La2 Ga2 33.5(7) 2_655 2_655
O4 La2 Ga2 32.7(9) 2 2_655
O4 La2 Ga2 162.8(10) . 2_655
Ga2 La2 Ga2 161.6(4) 1_455 2_655
O7 La2 Ta 32.3(10) . 1_565
O7 La2 Ta 32.3(10) 2 1_565
O1 La2 Ta 102.6(14) 2 1_565
O1 La2 Ta 102.6(14) . 1_565
O3 La2 Ta 132.1(6) 1_455 1_565
O3 La2 Ta 132.1(6) 2_655 1_565
O4 La2 Ta 69.1(9) 2 1_565
O4 La2 Ta 69.1(9) . 1_565
Ga2 La2 Ta 99.2(2) 1_455 1_565
Ga2 La2 Ta 99.2(2) 2_655 1_565
O7 La2 Ga1 32.3(10) . 1_565
O7 La2 Ga1 32.3(10) 2 1_565
O1 La2 Ga1 102.6(14) 2 1_565
O1 La2 Ga1 102.6(14) . 1_565
O3 La2 Ga1 132.1(6) 1_455 1_565
O3 La2 Ga1 132.1(6) 2_655 1_565
O4 La2 Ga1 69.1(9) 2 1_565
O4 La2 Ga1 69.1(9) . 1_565
Ga2 La2 Ga1 99.2(2) 1_455 1_565
Ga2 La2 Ga1 99.2(2) 2_655 1_565
Ta La2 Ga1 0.000(1) 1_565 1_565
O6 Ga1 O6 174.3(17) 1_455 2_655
O6 Ga1 O7 85.7(15) 1_455 2_545
O6 Ga1 O7 98.8(14) 2_655 2_545
O6 Ga1 O7 98.8(14) 1_455 1_545
O6 Ga1 O7 85.7(15) 2_655 1_545
O7 Ga1 O7 77(2) 2_545 1_545
O6 Ga1 O5 81.8(13) 1_455 .
O6 Ga1 O5 95.8(12) 2_655 .
O7 Ga1 O5 149.7(14) 2_545 .
O7 Ga1 O5 78.2(19) 1_545 .
O6 Ga1 O5 95.8(12) 1_455 2
O6 Ga1 O5 81.8(13) 2_655 2
O7 Ga1 O5 78.2(19) 2_545 2
O7 Ga1 O5 149.7(14) 1_545 2
O5 Ga1 O5 130(2) . 2
O6 Ga1 O2 122.4(14) 1_455 2_545
O6 Ga1 O2 58.1(14) 2_655 2_545
O7 Ga1 O2 59.2(17) 2_545 2_545
O7 Ga1 O2 113.2(18) 1_545 2_545
O5 Ga1 O2 148.8(15) . 2_545
O5 Ga1 O2 37.7(16) 2 2_545
O6 Ga1 O2 58.1(14) 1_455 1_545
O6 Ga1 O2 122.4(14) 2_655 1_545
O7 Ga1 O2 113.2(18) 2_545 1_545
O7 Ga1 O2 59.2(17) 1_545 1_545
O5 Ga1 O2 37.7(16) . 1_545
O5 Ga1 O2 148.8(15) 2 1_545
O2 Ga1 O2 171(2) 2_545 1_545
O6 Ga1 La2 92.9(9) 1_455 1_545
O6 Ga1 La2 92.9(9) 2_655 1_545
O7 Ga1 La2 38.3(12) 2_545 1_545
O7 Ga1 La2 38.3(12) 1_545 1_545
O5 Ga1 La2 114.8(11) . 1_545
O5 Ga1 La2 114.8(11) 2 1_545
O2 Ga1 La2 85.6(12) 2_545 1_545
O2 Ga1 La2 85.6(12) 1_545 1_545
O6 Ga1 La1 40.4(9) 1_455 2_556
O6 Ga1 La1 135.4(9) 2_655 2_556
O7 Ga1 La1 125.7(12) 2_545 2_556
O7 Ga1 La1 101.0(13) 1_545 2_556
O5 Ga1 La1 44.7(11) . 2_556
O5 Ga1 La1 107.3(11) 2 2_556
O2 Ga1 La1 144.9(11) 2_545 2_556
O2 Ga1 La1 42.0(11) 1_545 2_556
La2 Ga1 La1 119.61(13) 1_545 2_556
O6 Ga1 La1 135.4(9) 1_455 1_554
O6 Ga1 La1 40.4(9) 2_655 1_554
O7 Ga1 La1 101.0(13) 2_545 1_554
O7 Ga1 La1 125.7(12) 1_545 1_554
O5 Ga1 La1 107.3(11) . 1_554
O5 Ga1 La1 44.7(11) 2 1_554
O2 Ga1 La1 42.0(11) 2_545 1_554
O2 Ga1 La1 144.9(11) 1_545 1_554
La2 Ga1 La1 119.61(13) 1_545 1_554
La1 Ga1 La1 120.8(3) 2_556 1_554
O6 Ga1 O3 56.8(10) 1_455 1_455
O6 Ga1 O3 117.6(10) 2_655 1_455
O7 Ga1 O3 118.3(13) 2_545 1_455
O7 Ga1 O3 147.2(15) 1_545 1_455
O5 Ga1 O3 76.8(14) . 1_455
O5 Ga1 O3 61.7(13) 2 1_455
O2 Ga1 O3 99.2(13) 2_545 1_455
O2 Ga1 O3 88.1(10) 1_545 1_455
La2 Ga1 O3 146.9(5) 1_545 1_455
La1 Ga1 O3 46.2(7) 2_556 1_455
La1 Ga1 O3 82.2(6) 1_554 1_455
O6 Ta O6 174.3(17) 1_455 2_655
O6 Ta O7 85.7(15) 1_455 2_545
O6 Ta O7 98.8(14) 2_655 2_545
O6 Ta O7 98.8(14) 1_455 1_545
O6 Ta O7 85.7(15) 2_655 1_545
O7 Ta O7 77(2) 2_545 1_545
O6 Ta O5 81.8(13) 1_455 .
O6 Ta O5 95.8(12) 2_655 .
O7 Ta O5 149.7(14) 2_545 .
O7 Ta O5 78.2(19) 1_545 .
O6 Ta O5 95.8(12) 1_455 2
O6 Ta O5 81.8(13) 2_655 2
O7 Ta O5 78.2(19) 2_545 2
O7 Ta O5 149.7(14) 1_545 2
O5 Ta O5 130(2) . 2
O6 Ta Ga3 113.4(10) 1_455 .
O6 Ta Ga3 62.9(10) 2_655 .
O7 Ta Ga3 158.2(12) 2_545 .
O7 Ta Ga3 89.6(11) 1_545 .
O5 Ta Ga3 35.5(11) . .
O5 Ta Ga3 108.8(11) 2 .
O6 Ta Ga3 62.9(9) 1_455 1_455
O6 Ta Ga3 113.4(10) 2_655 1_455
O7 Ta Ga3 89.6(11) 2_545 1_455
O7 Ta Ga3 158.2(12) 1_545 1_455
O5 Ta Ga3 108.8(11) . 1_455
O5 Ta Ga3 35.5(11) 2 1_455
Ga3 Ta Ga3 108.2(5) . 1_455
O6 Ta Ga4 31.8(9) 1_455 3_444
O6 Ta Ga4 151.5(10) 2_655 3_444
O7 Ta Ga4 54.9(12) 2_545 3_444
O7 Ta Ga4 96.8(12) 1_545 3_444
O5 Ta Ga4 112.6(11) . 3_444
O5 Ta Ga4 81.9(11) 2 3_444
Ga3 Ta Ga4 145.2(2) . 3_444
Ga3 Ta Ga4 61.36(19) 1_455 3_444
O6 Ta Ga4 151.5(10) 1_455 4_645
O6 Ta Ga4 31.8(9) 2_655 4_645
O7 Ta Ga4 96.8(12) 2_545 4_645
O7 Ta Ga4 54.9(12) 1_545 4_645
O5 Ta Ga4 81.9(11) . 4_645
O5 Ta Ga4 112.6(11) 2 4_645
Ga3 Ta Ga4 61.36(19) . 4_645
Ga3 Ta Ga4 145.2(2) 1_455 4_645
Ga4 Ta Ga4 146.2(5) 3_444 4_645
O6 Ta Ga4 92.5(10) 1_455 4_545
O6 Ta Ga4 89.2(10) 2_655 4_545
O7 Ta Ga4 35.9(12) 2_545 4_545
O7 Ta Ga4 110.3(13) 1_545 4_545
O5 Ta Ga4 170.6(11) . 4_545
O5 Ta Ga4 42.3(12) 2 4_545
Ga3 Ta Ga4 144.9(2) . 4_545
Ga3 Ta Ga4 61.80(14) 1_455 4_545
Ga4 Ta Ga4 63.2(3) 3_444 4_545
Ga4 Ta Ga4 106.2(3) 4_645 4_545
O6 Ta Ga4 89.2(10) 1_455 3_544
O6 Ta Ga4 92.5(10) 2_655 3_544
O7 Ta Ga4 110.3(13) 2_545 3_544
O7 Ta Ga4 35.9(12) 1_545 3_544
O5 Ta Ga4 42.3(12) . 3_544
O5 Ta Ga4 170.6(11) 2 3_544
Ga3 Ta Ga4 61.80(13) . 3_544
Ga3 Ta Ga4 144.9(2) 1_455 3_544
Ga4 Ta Ga4 106.2(3) 3_444 3_544
Ga4 Ta Ga4 63.2(3) 4_645 3_544
Ga4 Ta Ga4 145.7(4) 4_545 3_544
O3 Ga2 O1 121(2) . .
O3 Ga2 O2 102(2) . 4_645
O1 Ga2 O2 119(3) . 4_645
O3 Ga2 O4 119.0(19) . 1_655
O1 Ga2 O4 111(2) . 1_655
O2 Ga2 O4 77(2) 4_645 1_655
O3 Ga2 O1 60.9(15) . 1_655
O1 Ga2 O1 177(3) . 1_655
O2 Ga2 O1 58(2) 4_645 1_655
O4 Ga2 O1 69(2) 1_655 1_655
O3 Ga2 La1 104.6(11) . 3_654
O1 Ga2 La1 135(2) . 3_654
O2 Ga2 La1 46(2) 4_645 3_654
O4 Ga2 La1 35.6(16) 1_655 3_654
O1 Ga2 La1 44.0(11) 1_655 3_654
O3 Ga2 La2 46.5(9) . 1_655
O1 Ga2 La2 138(2) . 1_655
O2 Ga2 La2 103.2(18) 4_645 1_655
O4 Ga2 La2 73.7(18) 1_655 1_655
O1 Ga2 La2 45.1(12) 1_655 1_655
La1 Ga2 La2 73.90(16) 3_654 1_655
O3 Ga2 La1 52.4(11) . 2_656
O1 Ga2 La1 135(2) . 2_656
O2 Ga2 La1 50(2) 4_645 2_656
O4 Ga2 La1 108.1(16) 1_655 2_656
O1 Ga2 La1 43.5(11) 1_655 2_656
La1 Ga2 La1 74.02(13) 3_654 2_656
La2 Ga2 La1 74.75(17) 1_655 2_656
O3 Ga2 La1 96.9(10) . 2_556
O1 Ga2 La1 41(2) . 2_556
O2 Ga2 La1 97(2) 4_645 2_556
O4 Ga2 La1 144.1(18) 1_655 2_556
O1 Ga2 La1 137.2(12) 1_655 2_556
La1 Ga2 La1 139.4(3) 3_654 2_556
La2 Ga2 La1 141.0(4) 1_655 2_556
La1 Ga2 La1 93.7(3) 2_656 2_556
O3 Ga2 La1 161.5(12) . 3_554
O1 Ga2 La1 41(2) . 3_554
O2 Ga2 La1 93(2) 4_645 3_554
O4 Ga2 La1 74.1(17) 1_655 3_554
O1 Ga2 La1 137.4(11) 1_655 3_554
La1 Ga2 La1 93.4(3) 3_654 3_554
La2 Ga2 La1 139.4(4) 1_655 3_554
La1 Ga2 La1 139.6(3) 2_656 3_554
La1 Ga2 La1 70.85(7) 2_556 3_554
O3 Ga2 La2 92.7(12) . .
O1 Ga2 La2 44(2) . .
O2 Ga2 La2 162.3(18) 4_645 .
O4 Ga2 La2 103.9(17) 1_655 .
O1 Ga2 La2 139.0(12) 1_655 .
La1 Ga2 La2 139.3(4) 3_654 .
La2 Ga2 La2 93.9(2) 1_655 .
La1 Ga2 La2 141.1(4) 2_656 .
La1 Ga2 La2 71.71(18) 2_556 .
La1 Ga2 La2 70.54(16) 3_554 .
O3 Ga2 O2 145.3(16) . .
O1 Ga2 O2 74(2) . .
O2 Ga2 O2 95(2) 4_645 .
O4 Ga2 O2 37.0(17) 1_655 .
O1 Ga2 O2 106.2(14) 1_655 .
La1 Ga2 O2 67.6(9) 3_654 .
La2 Ga2 O2 100.5(10) 1_655 .
La1 Ga2 O2 141.0(10) 2_656 .
La1 Ga2 O2 110.6(8) 2_556 .
La1 Ga2 O2 40.4(9) 3_554 .
La2 Ga2 O2 77.1(10) . .
O5 Ga3 O5 116(2) . 2_655
O5 Ga3 O3 105.6(15) . .
O5 Ga3 O3 108.5(16) 2_655 .
O5 Ga3 O3 108.5(16) . 2_655
O5 Ga3 O3 105.6(15) 2_655 2_655
O3 Ga3 O3 112(2) . 2_655
O5 Ga3 Ta 37.5(11) . .
O5 Ga3 Ta 100.1(13) 2_655 .
O3 Ga3 Ta 142.1(10) . .
O3 Ga3 Ta 82.3(10) 2_655 .
O5 Ga3 Ta 100.1(13) . 1_655
O5 Ga3 Ta 37.5(11) 2_655 1_655
O3 Ga3 Ta 82.3(10) . 1_655
O3 Ga3 Ta 142.1(10) 2_655 1_655
Ta Ga3 Ta 108.2(5) . 1_655
O5 Ga3 O1 68.6(15) . .
O5 Ga3 O1 171.2(13) 2_655 .
O3 Ga3 O1 62.7(12) . .
O3 Ga3 O1 78.3(14) 2_655 .
Ta Ga3 O1 88.1(6) . .
Ta Ga3 O1 136.7(9) 1_655 .
O5 Ga3 O1 171.2(13) . 2_655
O5 Ga3 O1 68.6(15) 2_655 2_655
O3 Ga3 O1 78.3(14) . 2_655
O3 Ga3 O1 62.7(11) 2_655 2_655
Ta Ga3 O1 136.7(9) . 2_655
Ta Ga3 O1 88.1(6) 1_655 2_655
O1 Ga3 O1 107(2) . 2_655
O5 Ga3 O2 22.2(15) . 1_545
O5 Ga3 O2 110.9(14) 2_655 1_545
O3 Ga3 O2 88.4(13) . 1_545
O3 Ga3 O2 129.2(11) 2_655 1_545
Ta Ga3 O2 57.8(9) . 1_545
Ta Ga3 O2 84.1(10) 1_655 1_545
O1 Ga3 O2 70.9(15) . 1_545
O1 Ga3 O2 165.4(12) 2_655 1_545
O5 Ga3 O2 110.9(14) . 2_645
O5 Ga3 O2 22.2(15) 2_655 2_645
O3 Ga3 O2 129.2(11) . 2_645
O3 Ga3 O2 88.4(13) 2_655 2_645
Ta Ga3 O2 84.1(10) . 2_645
Ta Ga3 O2 57.8(9) 1_655 2_645
O1 Ga3 O2 165.4(12) . 2_645
O1 Ga3 O2 71.0(15) 2_655 2_645
O2 Ga3 O2 114.5(19) 1_545 2_645
O5 Ga3 O3 53.8(12) . 1_455
O5 Ga3 O3 147.0(13) 2_655 1_455
O3 Ga3 O3 104.4(11) . 1_455
O3 Ga3 O3 59.2(13) 2_655 1_455
Ta Ga3 O3 51.6(4) . 1_455
Ta Ga3 O3 153.9(6) 1_655 1_455
O1 Ga3 O3 41.7(8) . 1_455
O1 Ga3 O3 117.9(8) 2_655 1_455
O2 Ga3 O3 71.0(9) 1_545 1_455
O2 Ga3 O3 125.4(10) 2_645 1_455
O5 Ga3 O3 147.0(13) . 2_755
O5 Ga3 O3 53.8(12) 2_655 2_755
O3 Ga3 O3 59.2(13) . 2_755
O3 Ga3 O3 104.4(11) 2_655 2_755
Ta Ga3 O3 153.9(6) . 2_755
Ta Ga3 O3 51.6(4) 1_655 2_755
O1 Ga3 O3 117.9(8) . 2_755
O1 Ga3 O3 41.7(8) 2_655 2_755
O2 Ga3 O3 125.4(10) 1_545 2_755
O2 Ga3 O3 71.0(9) 2_645 2_755
O3 Ga3 O3 152.7(8) 1_455 2_755
O2 Ga4 O7 103(2) 3_545 3_545
O2 Ga4 O4 95(3) 3_545 3_645
O7 Ga4 O4 113(2) 3_545 3_645
O2 Ga4 O6 104(2) 3_545 3
O7 Ga4 O6 140.3(14) 3_545 3
O4 Ga4 O6 93(2) 3_645 3
O2 Ga4 Ta 137(2) 3_545 3_655
O7 Ga4 Ta 109.4(13) 3_545 3_655
O4 Ga4 Ta 98.4(19) 3_645 3_655
O6 Ga4 Ta 34.3(9) 3 3_655
O2 Ga4 Ta 83(2) 3_545 3
O7 Ga4 Ta 37.1(12) 3_545 3
O4 Ga4 Ta 146.7(18) 3_645 3
O6 Ga4 Ta 119.9(11) 3 3
Ta Ga4 Ta 106.2(3) 3_655 3
O2 Ga4 O1 62(2) 3_545 2_656
O7 Ga4 O1 162.3(14) 3_545 2_656
O4 Ga4 O1 62(2) 3_645 2_656
O6 Ga4 O1 56.7(12) 3 2_656
Ta Ga4 O1 88.3(7) 3_655 2_656
Ta Ga4 O1 139.1(8) 3 2_656
O2 Ga4 O1 85(2) 3_545 3_545
O7 Ga4 O1 60.9(14) 3_545 3_545
O4 Ga4 O1 57.3(18) 3_645 3_545
O6 Ga4 O1 149.9(13) 3 3_545
Ta Ga4 O1 136.3(8) 3_655 3_545
Ta Ga4 O1 89.4(8) 3 3_545
O1 Ga4 O1 106.3(11) 2_656 3_545
O2 Ga4 La1 92(2) 3_545 1_655
O7 Ga4 La1 139.2(12) 3_545 1_655
O4 Ga4 La1 26.6(18) 3_645 1_655
O6 Ga4 La1 68.0(10) 3 1_655
Ta Ga4 La1 82.4(3) 3_655 1_655
Ta Ga4 La1 171.3(3) 3 1_655
O1 Ga4 La1 40.5(9) 2_656 1_655
O1 Ga4 La1 83.2(8) 3_545 1_655
O2 Ga4 La1 45(2) 3_545 .
O7 Ga4 La1 77.2(13) 3_545 .
O4 Ga4 La1 72.3(18) 3_645 .
O6 Ga4 La1 141.3(10) 3 .
Ta Ga4 La1 170.4(4) 3_655 .
Ta Ga4 La1 83.3(3) 3 .
O1 Ga4 La1 85.2(7) 2_656 .
O1 Ga4 La1 40.4(8) 3_545 .
La1 Ga4 La1 88.06(19) 1_655 .
O2 Ga4 O3 85(2) 3_545 3
O7 Ga4 O3 114.2(14) 3_545 3
O4 Ga4 O3 131.3(19) 3_645 3
O6 Ga4 O3 41.2(11) 3 3
Ta Ga4 O3 55.5(5) 3_655 3
Ta Ga4 O3 81.8(6) 3 3
O1 Ga4 O3 75.5(11) 2_656 3
O1 Ga4 O3 167.5(8) 3_545 3
La1 Ga4 O3 104.7(6) 1_655 3
La1 Ga4 O3 128.9(5) . 3
O2 Ga4 O3 32(2) 3_545 2_656
O7 Ga4 O3 115.4(14) 3_545 2_656
O4 Ga4 O3 63.0(19) 3_645 2_656
O6 Ga4 O3 102.8(10) 3 2_656
Ta Ga4 O3 135.2(6) 3_655 2_656
Ta Ga4 O3 110.0(6) 3 2_656
O1 Ga4 O3 46.9(8) 2_656 2_656
O1 Ga4 O3 70.0(11) 3_545 2_656
La1 Ga4 O3 63.0(5) 1_655 2_656
La1 Ga4 O3 38.6(5) . 2_656
O3 Ga4 O3 104.7(6) 3 2_656
Ga2 O1 La1 111(3) . 2_556
Ga2 O1 La2 107(3) . .
La1 O1 La2 110(2) 2_556 .
Ga2 O1 La1 111(3) . 3_554
La1 O1 La1 110.7(19) 2_556 3_554
La2 O1 La1 108(2) . 3_554
Ga2 O1 O3 143(3) . 1_455
La1 O1 O3 60.1(12) 2_556 1_455
La2 O1 O3 54.3(12) . 1_455
La1 O1 O3 105.6(9) 3_554 1_455
Ga2 O1 O4 145(3) . .
La1 O1 O4 101.7(12) 2_556 .
La2 O1 O4 72.0(15) . .
La1 O1 O4 42.8(13) 3_554 .
O3 O1 O4 65.7(13) 1_455 .
Ga2 O1 O2 149(4) . 4_545
La1 O1 O2 60.0(18) 2_556 4_545
La2 O1 O2 103.7(18) . 4_545
La1 O1 O2 55.8(18) 3_554 4_545
O3 O1 O2 61.6(16) 1_455 4_545
O4 O1 O2 45.8(16) . 4_545
Ga2 O1 O7 83(2) . .
La1 O1 O7 156(2) 2_556 .
La2 O1 O7 45.9(14) . .
La1 O1 O7 81.0(18) 3_554 .
O3 O1 O7 97(2) 1_455 .
O4 O1 O7 72.0(17) . .
O2 O1 O7 118(2) 4_545 .
Ga2 O1 O3 30.8(12) . .
La1 O1 O3 94.6(17) 2_556 .
La2 O1 O3 89.6(17) . .
La1 O1 O3 141.3(18) 3_554 .
O3 O1 O3 112(2) 1_455 .
O4 O1 O3 159(3) . .
O2 O1 O3 154(3) 4_545 .
O7 O1 O3 87.5(15) . .
Ga2 O1 O5 80(2) . .
La1 O1 O5 47.5(11) 2_556 .
La2 O1 O5 85.8(18) . .
La1 O1 O5 158(2) 3_554 .
O3 O1 O5 67.6(14) 1_455 .
O4 O1 O5 133.0(17) . .
O2 O1 O5 105(2) 4_545 .
O7 O1 O5 120(2) . .
O3 O1 O5 53.1(12) . .
Ga2 O1 O6 88(2) . 4_655
La1 O1 O6 77.8(17) 2_556 4_655
La2 O1 O6 157.9(19) . 4_655
La1 O1 O6 51.1(14) 3_554 4_655
O3 O1 O6 120.5(17) 1_455 4_655
O4 O1 O6 86.3(18) . 4_655
O2 O1 O6 61(2) 4_545 4_655
O7 O1 O6 124(2) . 4_655
O3 O1 O6 110.8(17) . 4_655
O5 O1 O6 113(2) . 4_655
Ga2 O1 O2 31.1(16) . 4_645
La1 O1 O2 95(2) 2_556 4_645
La2 O1 O2 138(2) . 4_645
La1 O1 O2 93(2) 3_554 4_645
O3 O1 O2 153(3) 1_455 4_645
O4 O1 O2 136(3) . 4_645
O2 O1 O2 118(3) 4_545 4_645
O7 O1 O2 105.2(19) . 4_645
O3 O1 O2 54.8(14) . 4_645
O5 O1 O2 88(2) . 4_645
O6 O1 O2 57.7(18) 4_655 4_645
Ga2 O1 Ga2 177(3) . 1_455
La1 O1 Ga2 71.0(8) 2_556 1_455
La2 O1 Ga2 69.8(9) . 1_455
La1 O1 Ga2 70.6(7) 3_554 1_455
O3 O1 Ga2 35.2(6) 1_455 1_455
O4 O1 Ga2 34.4(10) . 1_455
O2 O1 Ga2 34.0(14) 4_545 1_455
O7 O1 Ga2 94.7(16) . 1_455
O3 O1 Ga2 148(2) . 1_455
O5 O1 Ga2 99.3(13) . 1_455
O6 O1 Ga2 94.7(13) 4_655 1_455
O2 O1 Ga2 152(3) 4_645 1_455
Ga2 O1 O4 35.9(14) . 1_655
La1 O1 O4 140(2) 2_556 1_655
La2 O1 O4 103(2) . 1_655
La1 O1 O4 79(2) 3_554 1_655
O3 O1 O4 157(3) 1_455 1_655
O4 O1 O4 109(3) . 1_655
O2 O1 O4 132(3) 4_545 1_655
O7 O1 O4 61.3(16) . 1_655
O3 O1 O4 63.4(12) . 1_655
O5 O1 O4 115.9(16) . 1_655
O6 O1 O4 80(2) 4_655 1_655
O2 O1 O4 44.7(14) 4_645 1_655
Ga2 O1 O4 144(2) 1_455 1_655
Ga2 O1 O4 74(2) . 4_545
La1 O1 O4 43.6(13) 2_556 4_545
La2 O1 O4 146(3) . 4_545
La1 O1 O4 103(2) 3_554 4_545
O3 O1 O4 104(2) 1_455 4_545
O4 O1 O4 126.2(17) . 4_545
O2 O1 O4 82(2) 4_545 4_545
O7 O1 O4 157.0(16) . 4_545
O3 O1 O4 75.1(15) . 4_545
O5 O1 O4 60.7(16) . 4_545
O6 O1 O4 52.5(16) 4_655 4_545
O2 O1 O4 52.3(17) 4_645 4_545
Ga2 O1 O4 108.1(18) 1_455 4_545
O4 O1 O4 96.9(15) 1_655 4_545
Ga2 O1 Ga3 61.0(15) . .
La1 O1 Ga3 78.8(15) 2_556 .
La2 O1 Ga3 71.4(14) . .
La1 O1 Ga3 169.7(17) 3_554 .
O3 O1 Ga3 82.2(16) 1_455 .
O4 O1 Ga3 141(2) . .
O2 O1 Ga3 135(2) 4_545 .
O7 O1 Ga3 91.6(16) . .
O3 O1 Ga3 30.2(8) . .
O5 O1 Ga3 31.3(9) . .
O6 O1 Ga3 130.6(17) 4_655 .
O2 O1 Ga3 82.3(15) 4_645 .
Ga2 O1 Ga3 117.5(16) 1_455 .
O4 O1 Ga3 91.5(13) 1_655 .
O4 O1 Ga3 81.0(16) 4_545 .
Ga2 O1 Ga4 62.7(18) . 2_656
La1 O1 Ga4 72.8(16) 2_556 2_656
La2 O1 Ga4 169.4(11) . 2_656
La1 O1 Ga4 80.1(17) 3_554 2_656
O3 O1 Ga4 132(2) 1_455 2_656
O4 O1 Ga4 118(2) . 2_656
O2 O1 Ga4 87(2) 4_545 2_656
O7 O1 Ga4 131.0(16) . 2_656
O3 O1 Ga4 80.0(12) . 2_656
O5 O1 Ga4 89.2(16) . 2_656
O6 O1 Ga4 31.6(9) 4_655 2_656
O2 O1 Ga4 32.1(13) 4_645 2_656
Ga2 O1 Ga4 120.3(16) 1_455 2_656
O4 O1 Ga4 70.9(14) 1_655 2_656
O4 O1 Ga4 31.9(12) 4_545 2_656
Ga3 O1 Ga4 99.7(11) . 2_656
Ga2 O1 Ga4 61.7(17) . 3_554
La1 O1 Ga4 171.0(18) 2_556 3_554
La2 O1 Ga4 77.6(16) . 3_554
La1 O1 Ga4 70.2(14) 3_554 3_554
O3 O1 Ga4 129(2) 1_455 3_554
O4 O1 Ga4 85.0(18) . 3_554
O2 O1 Ga4 124(2) 4_545 3_554
O7 O1 Ga4 32.2(9) . 3_554
O3 O1 Ga4 80.5(10) . 3_554
O5 O1 Ga4 130.8(14) . 3_554
O6 O1 Ga4 96.9(17) 4_655 3_554
O2 O1 Ga4 75.6(15) 4_645 3_554
Ga2 O1 Ga4 116.9(16) 1_455 3_554
O4 O1 Ga4 30.9(11) 1_655 3_554
O4 O1 Ga4 127.5(17) 4_545 3_554
Ga3 O1 Ga4 99.8(11) . 3_554
Ga4 O1 Ga4 98.8(12) 2_656 3_554
Ga2 O1 O2 80(2) . .
La1 O1 O2 151(2) 2_556 .
La2 O1 O2 90.9(19) . .
La1 O1 O2 41.9(13) 3_554 .
O3 O1 O2 126(2) 1_455 .
O4 O1 O2 65.2(16) . .
O2 O1 O2 97(2) 4_545 .
O7 O1 O2 48.0(15) . .
O3 O1 O2 105.5(15) . .
O5 O1 O2 158.4(13) . .
O6 O1 O2 75.8(18) 4_655 .
O2 O1 O2 80.2(17) 4_645 .
Ga2 O1 O2 99.6(15) 1_455 .
O4 O1 O2 44.2(15) 1_655 .
O4 O1 O2 122(2) 4_545 .
Ga3 O1 O2 128.0(14) . .
Ga4 O1 O2 90.2(17) 2_656 .
Ga4 O1 O2 28.3(10) 3_554 .
Ga2 O1 O3 78.1(19) . 2_655
La1 O1 O3 92.7(18) 2_556 2_655
La2 O1 O3 42.6(10) . 2_655
La1 O1 O3 149(2) 3_554 2_655
O3 O1 O3 67.5(16) 1_455 2_655
O4 O1 O3 114(2) . 2_655
O2 O1 O3 129(2) 4_545 2_655
O7 O1 O3 69.9(15) . 2_655
O3 O1 O3 51.2(14) . 2_655
O5 O1 O3 50.1(12) . 2_655
O6 O1 O3 159.4(18) 4_655 2_655
O2 O1 O3 106.0(17) 4_645 2_655
Ga2 O1 O3 99.4(15) 1_455 2_655
O4 O1 O3 96.9(16) 1_655 2_655
O4 O1 O3 108.4(19) 4_545 2_655
Ga3 O1 O3 28.8(7) . 2_655
Ga4 O1 O3 128.2(13) 2_656 2_655
Ga4 O1 O3 90.0(13) 3_554 2_655
O2 O1 O3 116.0(19) . 2_655
Ga2 O1 O6 116(2) . 1_455
La1 O1 O6 25.9(8) 2_556 1_455
La2 O1 O6 84.6(14) . 1_455
La1 O1 O6 125.6(12) 3_554 1_455
O3 O1 O6 40.2(10) 1_455 1_455
O4 O1 O6 99.1(13) . 1_455
O2 O1 O6 69.9(19) 4_545 1_455
O7 O1 O6 130(2) . 1_455
O3 O1 O6 89.6(15) . 1_455
O5 O1 O6 36.5(7) . 1_455
O6 O1 O6 103.3(17) 4_655 1_455
O2 O1 O6 113(2) 4_645 1_455
Ga2 O1 O6 64.6(9) 1_455 1_455
O4 O1 O6 151.5(17) 1_655 1_455
O4 O1 O6 65.6(15) 4_545 1_455
Ga3 O1 O6 64.6(10) . 1_455
Ga4 O1 O6 96.9(15) 2_656 1_455
Ga4 O1 O6 159.6(19) 3_554 1_455
O2 O1 O6 164.2(11) . 1_455
O3 O1 O6 70.0(12) 2_655 1_455
Ga2 O1 O5 124(3) . 4
La1 O1 O5 77.4(14) 2_556 4
La2 O1 O5 122.2(11) . 4
La1 O1 O5 33.3(9) 3_554 4
O3 O1 O5 90.5(11) 1_455 4
O4 O1 O5 50.9(14) . 4
O2 O1 O5 29.3(17) 4_545 4
O7 O1 O5 112.4(17) . 4
O3 O1 O5 148(2) . 4
O5 O1 O5 124.8(18) . 4
O6 O1 O5 37.5(9) 4_655 4
O2 O1 O5 95(2) 4_645 4
Ga2 O1 O5 58.7(8) 1_455 4
O4 O1 O5 103(2) 1_655 4
O4 O1 O5 78.2(18) 4_545 4
Ga3 O1 O5 155.7(19) . 4
Ga4 O1 O5 68.1(12) 2_656 4
Ga4 O1 O5 102.8(15) 3_554 4
O2 O1 O5 74.6(14) . 4
O3 O1 O5 157.8(12) 2_655 4
O6 O1 O5 95.0(11) 1_455 4
Ga2 O1 O7 116(3) . 2
La1 O1 O7 123.9(14) 2_556 2
La2 O1 O7 27.4(10) . 2
La1 O1 O7 80.2(14) 3_554 2
O3 O1 O7 63.9(14) 1_455 2
O4 O1 O7 49.1(14) . 2
O2 O1 O7 90.4(18) 4_545 2
O7 O1 O7 35.0(12) . 2
O3 O1 O7 110.1(19) . 2
O5 O1 O7 112.6(19) . 2
O6 O1 O7 131.2(17) 4_655 2
O2 O1 O7 140(2) 4_645 2
Ga2 O1 O7 61.2(10) 1_455 2
O4 O1 O7 95.6(18) 1_655 2
O4 O1 O7 167.4(18) 4_545 2
Ga3 O1 O7 97.9(16) . 2
Ga4 O1 O7 158.0(18) 2_656 2
Ga4 O1 O7 65.1(11) 3_554 2
O2 O1 O7 68.4(14) . 2
O3 O1 O7 69.2(14) 2_655 2
O6 O1 O7 102.6(13) 1_455 2
O5 O1 O7 99.7(10) 4 2
Ga2 O1 O3 83(2) . 4_655
La1 O1 O3 113.8(19) 2_556 4_655
La2 O1 O3 127.6(19) . 4_655
La1 O1 O3 29.6(9) 3_554 4_655
O3 O1 O3 134.0(12) 1_455 4_655
O4 O1 O3 72.3(16) . 4_655
O2 O1 O3 76(2) 4_545 4_655
O7 O1 O3 87.0(15) . 4_655
O3 O1 O3 113.5(12) . 4_655
O5 O1 O3 145.9(18) . 4_655
O6 O1 O3 36.8(10) 4_655 4_655
O2 O1 O3 63.3(17) 4_645 4_655
Ga2 O1 O3 98.8(12) 1_455 4_655
O4 O1 O3 56.3(17) 1_655 4_655
O4 O1 O3 86.2(18) 4_545 4_655
Ga3 O1 O3 143.7(8) . 4_655
Ga4 O1 O3 56.7(9) 2_656 4_655
Ga4 O1 O3 62.3(10) 3_554 4_655
O2 O1 O3 39.0(11) . 4_655
O3 O1 O3 151.6(15) 2_655 4_655
O6 O1 O3 138.0(15) 1_455 4_655
O5 O1 O3 47.1(9) 4 4_655
O7 O1 O3 101.4(13) 2 4_655
Ga2 O1 Ga3 136(3) . 1_455
La1 O1 Ga3 58.9(10) 2_556 1_455
La2 O1 Ga3 52.7(8) . 1_455
La1 O1 Ga3 113.1(6) 3_554 1_455
O3 O1 Ga3 7.5(7) 1_455 1_455
O4 O1 Ga3 72.8(12) . 1_455
O2 O1 Ga3 68.1(17) 4_545 1_455
O7 O1 Ga3 97.3(16) . 1_455
O3 O1 Ga3 104.9(16) . 1_455
O5 O1 Ga3 61.0(10) . 1_455
O6 O1 Ga3 125.2(13) 4_655 1_455
O2 O1 Ga3 148(2) 4_645 1_455
Ga2 O1 Ga3 42.7(6) 1_455 1_455
O4 O1 Ga3 155(2) 1_655 1_455
O4 O1 Ga3 101.7(17) 4_545 1_455
Ga3 O1 Ga3 74.7(11) . 1_455
Ga4 O1 Ga3 131.7(16) 2_656 1_455
Ga4 O1 Ga3 129.5(17) 3_554 1_455
O2 O1 Ga3 131.5(16) . 1_455
O3 O1 Ga3 60.9(10) 2_655 1_455
O6 O1 Ga3 36.6(6) 1_455 1_455
O5 O1 Ga3 97.2(7) 4 1_455
O7 O1 Ga3 66.1(9) 2 1_455
O3 O1 Ga3 141.5(8) 4_655 1_455
Ga2 O1 O2 82(2) . 1_545
La1 O1 O2 29.3(10) 2_556 1_545
La2 O1 O2 115(2) . 1_545
La1 O1 O2 130(2) 3_554 1_545
O3 O1 O2 79.6(16) 1_455 1_545
O4 O1 O2 131.0(18) . 1_545
O2 O1 O2 88(2) 4_545 1_545
O7 O1 O2 149.0(19) . 1_545
O3 O1 O2 66.2(13) . 1_545
O5 O1 O2 30.5(13) . 1_545
O6 O1 O2 82.5(16) 4_655 1_545
O2 O1 O2 73.6(19) 4_645 1_545
Ga2 O1 O2 99.2(15) 1_455 1_545
O4 O1 O2 115.3(16) 1_655 1_545
O4 O1 O2 31.5(14) 4_545 1_545
Ga3 O1 O2 57.4(13) . 1_545
Ga4 O1 O2 62.6(12) 2_656 1_545
Ga4 O1 O2 143.7(10) 3_554 1_545
O2 O1 O2 152(2) . 1_545
O3 O1 O2 80.5(14) 2_655 1_545
O6 O1 O2 39.4(11) 1_455 1_545
O5 O1 O2 98.5(16) 4 1_545
O7 O1 O2 139.1(18) 2 1_545
O3 O1 O2 117.6(17) 4_655 1_545
Ga3 O1 O2 75.5(13) 1_455 1_545
Ga2 O1 Ga4 139(3) . 2_556
La1 O1 Ga4 53.0(8) 2_556 2_556
La2 O1 Ga4 113.2(6) . 2_556
La1 O1 Ga4 59.2(9) 3_554 2_556
O3 O1 Ga4 67.0(9) 1_455 2_556
O4 O1 Ga4 56.1(12) . 2_556
O2 O1 Ga4 10.8(15) 4_545 2_556
O7 O1 Ga4 128.0(13) . 2_556
O3 O1 Ga4 144(2) . 2_556
O5 O1 Ga4 99.9(13) . 2_556
O6 O1 Ga4 54.1(9) 4_655 2_556
O2 O1 Ga4 109(2) 4_645 2_556
Ga2 O1 Ga4 43.5(6) 1_455 2_556
O4 O1 Ga4 130(2) 1_655 2_556
O4 O1 Ga4 70.9(15) 4_545 2_556
Ga3 O1 Ga4 130.9(15) . 2_556
Ga4 O1 Ga4 76.8(11) 2_656 2_556
Ga4 O1 Ga4 129.3(15) 3_554 2_556
O2 O1 Ga4 101.1(14) . 2_556
O3 O1 Ga4 132.7(13) 2_655 2_556
O6 O1 Ga4 67.2(8) 1_455 2_556
O5 O1 Ga4 28.1(6) 4 2_556
O7 O1 Ga4 101.3(7) 2 2_556
O3 O1 Ga4 74.6(9) 4_655 2_556
Ga3 O1 Ga4 72.7(5) 1_455 2_556
O2 O1 Ga4 79.3(12) 1_545 2_556
Ga2 O1 Ga4 136(3) . 3_454
La1 O1 Ga4 113.7(6) 2_556 3_454
La2 O1 Ga4 58.6(9) . 3_454
La1 O1 Ga4 50.9(9) 3_554 3_454
O3 O1 Ga4 66.7(9) 1_455 3_454
O4 O1 Ga4 16.2(12) . 3_454
O2 O1 Ga4 61.4(16) 4_545 3_454
O7 O1 Ga4 56.6(10) . 3_454
O3 O1 Ga4 143(2) . 3_454
O5 O1 Ga4 133.0(14) . 3_454
O6 O1 Ga4 99.4(13) 4_655 3_454
O2 O1 Ga4 139(2) 4_645 3_454
Ga2 O1 Ga4 42.9(6) 1_455 3_454
O4 O1 Ga4 102.2(18) 1_655 3_454
O4 O1 Ga4 142.4(17) 4_545 3_454
Ga3 O1 Ga4 129.8(17) . 3_454
Ga4 O1 Ga4 130.4(15) 2_656 3_454
Ga4 O1 Ga4 74.1(10) 3_554 3_454
O2 O1 Ga4 60.1(12) . 3_454
O3 O1 Ga4 101.2(14) 2_655 3_454
O6 O1 Ga4 105.0(7) 1_455 3_454
O5 O1 Ga4 66.1(7) 4 3_454
O7 O1 Ga4 33.6(6) 2 3_454
O3 O1 Ga4 78.2(10) 4_655 3_454
Ga3 O1 Ga4 72.7(6) 1_455 3_454
O2 O1 Ga4 142.1(11) 1_545 3_454
Ga4 O1 Ga4 71.9(4) 2_556 3_454
Ga2 O1 Ta 100(2) . .
La1 O1 Ta 47.1(10) 2_556 .
La2 O1 Ta 70.3(13) . .
La1 O1 Ta 148.1(9) 3_554 .
O3 O1 Ta 46.1(10) 1_455 .
O4 O1 Ta 111.8(15) . .
O2 O1 Ta 93(2) 4_545 .
O7 O1 Ta 112.5(18) . .
O3 O1 Ta 70.1(12) . .
O5 O1 Ta 21.9(7) . .
O6 O1 Ta 123.7(18) 4_655 .
O2 O1 Ta 109.9(19) 4_645 .
Ga2 O1 Ta 79.4(10) 1_455 .
O4 O1 Ta 133.1(17) 1_655 .
O4 O1 Ta 76.0(16) 4_545 .
Ga3 O1 Ta 41.8(7) . .
Ga4 O1 Ta 107.2(14) 2_656 .
Ga4 O1 Ta 135.9(16) 3_554 .
O2 O1 Ta 160(2) . .
O3 O1 Ta 46.0(8) 2_655 .
O6 O1 Ta 24.7(5) 1_455 .
O5 O1 Ta 119.6(12) 4 .
O7 O1 Ta 94.7(13) 2 .
O3 O1 Ta 160.5(16) 4_655 .
Ga3 O1 Ta 39.2(5) 1_455 .
O2 O1 Ta 44.6(11) 1_545 .
Ga4 O1 Ta 91.6(9) 2_556 .
Ga4 O1 Ta 111.2(9) 3_454 .
Ga2 O1 Ga1 100(2) . .
La1 O1 Ga1 47.1(10) 2_556 .
La2 O1 Ga1 70.3(13) . .
La1 O1 Ga1 148.1(9) 3_554 .
O3 O1 Ga1 46.1(10) 1_455 .
O4 O1 Ga1 111.8(15) . .
O2 O1 Ga1 93(2) 4_545 .
O7 O1 Ga1 112.5(18) . .
O3 O1 Ga1 70.1(12) . .
O5 O1 Ga1 21.9(7) . .
O6 O1 Ga1 123.7(18) 4_655 .
O2 O1 Ga1 109.9(19) 4_645 .
Ga2 O1 Ga1 79.4(10) 1_455 .
O4 O1 Ga1 133.1(17) 1_655 .
O4 O1 Ga1 76.0(16) 4_545 .
Ga3 O1 Ga1 41.8(7) . .
Ga4 O1 Ga1 107.2(14) 2_656 .
Ga4 O1 Ga1 135.9(16) 3_554 .
O2 O1 Ga1 160(2) . .
O3 O1 Ga1 46.0(8) 2_655 .
O6 O1 Ga1 24.7(5) 1_455 .
O5 O1 Ga1 119.6(12) 4 .
O7 O1 Ga1 94.7(13) 2 .
O3 O1 Ga1 160.5(16) 4_655 .
Ga3 O1 Ga1 39.2(5) 1_455 .
O2 O1 Ga1 44.6(11) 1_545 .
Ga4 O1 Ga1 91.6(9) 2_556 .
Ga4 O1 Ga1 111.2(9) 3_454 .
Ta O1 Ga1 0.00(11) . .
Ga2 O1 O4 78(2) . 2
La1 O1 O4 128(2) 2_556 2
La2 O1 O4 29.6(9) . 2
La1 O1 O4 113(2) 3_554 2
O3 O1 O4 82.0(17) 1_455 2
O4 O1 O4 92.4(19) . 2
O2 O1 O4 132(2) 4_545 2
O7 O1 O4 33.1(11) . 2
O3 O1 O4 66.6(14) . 2
O5 O1 O4 86.8(16) . 2
O6 O1 O4 154.0(18) 4_655 2
O2 O1 O4 108.8(17) 4_645 2
Ga2 O1 O4 98.8(16) 1_455 2
O4 O1 O4 76.0(18) 1_655 2
O4 O1 O4 140(2) 4_545 2
Ga3 O1 O4 60.4(11) . 2
Ga4 O1 O4 140.8(8) 2_656 2
Ga4 O1 O4 57.1(10) 3_554 2
O2 O1 O4 80.0(14) . 2
O3 O1 O4 36.9(9) 2_655 2
O6 O1 O4 102.6(14) 1_455 2
O5 O1 O4 141.6(14) 4 2
O7 O1 O4 43.5(10) 2 2
O3 O1 O4 118.5(13) 4_655 2
Ga3 O1 O4 78.7(12) 1_455 2
O2 O1 O4 116.8(16) 1_545 2
Ga4 O1 O4 142.2(12) 2_556 2
Ga4 O1 O4 76.4(11) 3_454 2
Ta O1 O4 80.9(12) . 2
Ga1 O1 O4 80.9(12) . 2
Ga2 O1 O5 53.2(18) . 4_655
La1 O1 O5 99.9(19) 2_556 4_655
La2 O1 O5 149.2(18) . 4_655
La1 O1 O5 66.8(13) 3_554 4_655
O3 O1 O5 156(2) 1_455 4_655
O4 O1 O5 109.6(19) . 4_655
O2 O1 O5 97(2) 4_545 4_655
O7 O1 O5 104.2(14) . 4_655
O3 O1 O5 80.6(12) . 4_655
O5 O1 O5 110.3(15) . 4_655
O6 O1 O5 36.3(8) 4_655 4_655
O2 O1 O5 26.3(16) 4_645 4_655
Ga2 O1 O5 129.4(16) 1_455 4_655
O4 O1 O5 46.6(15) 1_655 4_655
O4 O1 O5 58.7(16) 4_545 4_655
Ga3 O1 O5 108.6(8) . 4_655
Ga4 O1 O5 27.2(7) 2_656 4_655
Ga4 O1 O5 72.0(10) 3_554 4_655
O2 O1 O5 64.3(14) . 4_655
O3 O1 O5 131.1(9) 2_655 4_655
O6 O1 O5 124.1(16) 1_455 4_655
O5 O1 O5 70.7(11) 4 4_655
O7 O1 O5 132.6(15) 2 4_655
O3 O1 O5 37.8(7) 4_655 4_655
Ga3 O1 O5 158.1(16) 1_455 4_655
O2 O1 O5 88.1(14) 1_545 4_655
Ga4 O1 O5 90.4(12) 2_556 4_655
Ga4 O1 O5 115.8(13) 3_454 4_655
Ta O1 O5 131.1(13) . 4_655
Ga1 O1 O5 131.1(13) . 4_655
O4 O1 O5 122.3(11) 2 4_655
Ga2 O1 O7 116(3) . 4_545
La1 O1 O7 48.9(11) 2_556 4_545
La2 O1 O7 136.1(8) . 4_545
La1 O1 O7 63.5(14) 3_554 4_545
O3 O1 O7 85.4(13) 1_455 4_545
O4 O1 O7 76.0(14) . 4_545
O2 O1 O7 33.9(17) 4_545 4_545
O7 O1 O7 143.5(16) . 4_545
O3 O1 O7 125.3(18) . 4_545
O5 O1 O7 94.8(14) . 4_545
O6 O1 O7 35.7(9) 4_655 4_545
O2 O1 O7 86(2) 4_645 4_545
Ga2 O1 O7 66.8(9) 1_455 4_545
O4 O1 O7 116(2) 1_655 4_545
O4 O1 O7 50.2(14) 4_545 4_545
Ga3 O1 O7 124.7(15) . 4_545
Ga4 O1 O7 53.6(10) 2_656 4_545
Ga4 O1 O7 128.7(16) 3_554 4_545
O2 O1 O7 102.2(16) . 4_545
O3 O1 O7 141.3(15) 2_655 4_545
O6 O1 O7 71.5(8) 1_455 4_545
O5 O1 O7 31.2(8) 4 4_545
O7 O1 O7 123.8(10) 2 4_545
O3 O1 O7 66.6(10) 4_655 4_545
Ga3 O1 O7 89.6(8) 1_455 4_545
O2 O1 O7 67.3(11) 1_545 4_545
Ga4 O1 O7 23.5(6) 2_556 4_545
Ga4 O1 O7 92.2(8) 3_454 4_545
Ta O1 O7 95.3(10) . 4_545
Ga1 O1 O7 95.3(10) . 4_545
O4 O1 O7 165.6(11) 2 4_545
O5 O1 O7 70.5(11) 4_655 4_545
Ga2 O1 Ga1 102(2) . 3
La1 O1 Ga1 71.0(14) 2_556 3
La2 O1 Ga1 147.4(10) . 3
La1 O1 Ga1 47.6(11) 3_554 3
O3 O1 Ga1 106.7(13) 1_455 3
O4 O1 Ga1 75.9(15) . 3
O2 O1 Ga1 47.2(18) 4_545 3
O7 O1 Ga1 127.2(18) . 3
O3 O1 Ga1 123.0(17) . 3
O5 O1 Ga1 112.8(17) . 3
O6 O1 Ga1 14.3(7) 4_655 3
O2 O1 Ga1 71.5(18) 4_645 3
Ga2 O1 Ga1 80.6(10) 1_455 3
O4 O1 Ga1 92.7(19) 1_655 3
O4 O1 Ga1 56.2(15) 4_545 3
Ga3 O1 Ga1 137.3(16) . 3
Ga4 O1 Ga1 43.0(7) 2_656 3
Ga4 O1 Ga1 105.3(14) 3_554 3
O2 O1 Ga1 80.6(15) . 3
O3 O1 Ga1 162.9(17) 2_655 3
O6 O1 Ga1 95.0(12) 1_455 3
O5 O1 Ga1 25.2(6) 4 3
O7 O1 Ga1 123.9(11) 2 3
O3 O1 Ga1 43.1(6) 4_655 3
Ga3 O1 Ga1 111.9(8) 1_455 3
O2 O1 Ga1 82.6(13) 1_545 3
Ga4 O1 Ga1 39.9(5) 2_556 3
Ga4 O1 Ga1 90.5(8) 3_454 3
Ta O1 Ga1 118.1(13) . 3
Ga1 O1 Ga1 118.1(13) . 3
O4 O1 Ga1 160.2(15) 2 3
O5 O1 Ga1 50.5(8) 4_655 3
O7 O1 Ga1 24.0(6) 4_545 3
Ga2 O1 Ta 102(2) . 3
La1 O1 Ta 71.0(14) 2_556 3
La2 O1 Ta 147.4(10) . 3
La1 O1 Ta 47.6(11) 3_554 3
O3 O1 Ta 106.7(13) 1_455 3
O4 O1 Ta 75.9(15) . 3
O2 O1 Ta 47.2(18) 4_545 3
O7 O1 Ta 127.2(18) . 3
O3 O1 Ta 123.0(17) . 3
O5 O1 Ta 112.8(17) . 3
O6 O1 Ta 14.3(7) 4_655 3
O2 O1 Ta 71.5(18) 4_645 3
Ga2 O1 Ta 80.6(10) 1_455 3
O4 O1 Ta 92.7(19) 1_655 3
O4 O1 Ta 56.2(15) 4_545 3
Ga3 O1 Ta 137.3(16) . 3
Ga4 O1 Ta 43.0(7) 2_656 3
Ga4 O1 Ta 105.3(14) 3_554 3
O2 O1 Ta 80.6(15) . 3
O3 O1 Ta 162.9(17) 2_655 3
O6 O1 Ta 95.0(12) 1_455 3
O5 O1 Ta 25.2(6) 4 3
O7 O1 Ta 123.9(11) 2 3
O3 O1 Ta 43.1(6) 4_655 3
Ga3 O1 Ta 111.9(8) 1_455 3
O2 O1 Ta 82.6(13) 1_545 3
Ga4 O1 Ta 39.9(5) 2_556 3
Ga4 O1 Ta 90.5(8) 3_454 3
Ta O1 Ta 118.1(13) . 3
Ga1 O1 Ta 118.1(13) . 3
O4 O1 Ta 160.2(15) 2 3
O5 O1 Ta 50.5(8) 4_655 3
O7 O1 Ta 24.0(6) 4_545 3
Ga1 O1 Ta 0.0(2) 3 3
Ga2 O1 Ga1 99(2) . 1_565
La1 O1 Ga1 147.7(13) 2_556 1_565
La2 O1 Ga1 45.8(11) . 1_565
La1 O1 Ga1 68.9(14) 3_554 1_565
O3 O1 Ga1 88.3(15) 1_455 1_565
O4 O1 Ga1 54.8(14) . 1_565
O2 O1 Ga1 100.6(19) 4_545 1_565
O7 O1 Ga1 17.3(7) . 1_565
O3 O1 Ga1 104.6(15) . 1_565
O5 O1 Ga1 129.5(19) . 1_565
O6 O1 Ga1 117.5(17) 4_655 1_565
O2 O1 Ga1 116.8(19) 4_645 1_565
Ga2 O1 Ga1 79.1(11) 1_455 1_565
O4 O1 Ga1 72.2(15) 1_655 1_565
O4 O1 Ga1 167(2) 4_545 1_565
Ga3 O1 Ga1 105.3(15) . 1_565
Ga4 O1 Ga1 135.5(15) 2_656 1_565
Ga4 O1 Ga1 41.3(7) 3_554 1_565
O2 O1 Ga1 45.4(12) . 1_565
O3 O1 Ga1 80.1(12) 2_655 1_565
O6 O1 Ga1 127.0(13) 1_455 1_565
O5 O1 Ga1 97.6(11) 4 1_565
O7 O1 Ga1 24.6(6) 2 1_565
O3 O1 Ga1 82.3(10) 4_655 1_565
Ga3 O1 Ga1 90.7(10) 1_455 1_565
O2 O1 Ga1 159.9(18) 1_545 1_565
Ga4 O1 Ga1 110.8(8) 2_556 1_565
Ga4 O1 Ga1 39.4(5) 3_454 1_565
Ta O1 Ga1 116.1(13) . 1_565
Ga1 O1 Ga1 116.1(13) . 1_565
O4 O1 Ga1 44.9(8) 2 1_565
O5 O1 Ga1 108.6(12) 4_655 1_565
O7 O1 Ga1 128.1(10) 4_545 1_565
Ga1 O1 Ga1 116.5(12) 3 1_565
Ta O1 Ga1 116.5(12) 3 1_565
Ga2 O1 Ta 99(2) . 1_565
La1 O1 Ta 147.7(13) 2_556 1_565
La2 O1 Ta 45.8(11) . 1_565
La1 O1 Ta 68.9(14) 3_554 1_565
O3 O1 Ta 88.3(15) 1_455 1_565
O4 O1 Ta 54.8(14) . 1_565
O2 O1 Ta 100.6(19) 4_545 1_565
O7 O1 Ta 17.3(7) . 1_565
O3 O1 Ta 104.6(15) . 1_565
O5 O1 Ta 129.5(19) . 1_565
O6 O1 Ta 117.5(17) 4_655 1_565
O2 O1 Ta 116.8(19) 4_645 1_565
Ga2 O1 Ta 79.1(11) 1_455 1_565
O4 O1 Ta 72.2(15) 1_655 1_565
O4 O1 Ta 167(2) 4_545 1_565
Ga3 O1 Ta 105.3(15) . 1_565
Ga4 O1 Ta 135.5(15) 2_656 1_565
Ga4 O1 Ta 41.3(7) 3_554 1_565
O2 O1 Ta 45.4(12) . 1_565
O3 O1 Ta 80.1(12) 2_655 1_565
O6 O1 Ta 127.0(13) 1_455 1_565
O5 O1 Ta 97.6(11) 4 1_565
O7 O1 Ta 24.6(6) 2 1_565
O3 O1 Ta 82.3(10) 4_655 1_565
Ga3 O1 Ta 90.7(10) 1_455 1_565
O2 O1 Ta 159.9(18) 1_545 1_565
Ga4 O1 Ta 110.8(8) 2_556 1_565
Ga4 O1 Ta 39.4(5) 3_454 1_565
Ta O1 Ta 116.1(13) . 1_565
Ga1 O1 Ta 116.1(13) . 1_565
O4 O1 Ta 44.9(8) 2 1_565
O5 O1 Ta 108.6(12) 4_655 1_565
O7 O1 Ta 128.1(10) 4_545 1_565
Ga1 O1 Ta 116.5(12) 3 1_565
Ta O1 Ta 116.5(12) 3 1_565
Ga1 O1 Ta 0.00(10) 1_565 1_565
Ga2 O1 O6 113(2) . 1_465
La1 O1 O6 135.8(8) 2_556 1_465
La2 O1 O6 62.2(13) . 1_465
La1 O1 O6 46.7(11) 3_554 1_465
O3 O1 O6 87.4(13) 1_455 1_465
O4 O1 O6 34.4(12) . 1_465
O2 O1 O6 79.0(18) 4_545 1_465
O7 O1 O6 40.2(9) . 1_465
O3 O1 O6 127.0(17) . 1_465
O5 O1 O6 147(2) . 1_465
O6 O1 O6 97.5(16) 4_655 1_465
O2 O1 O6 119(2) 4_645 1_465
Ga2 O1 O6 65.6(10) 1_455 1_465
O4 O1 O6 79.5(17) 1_655 1_465
O4 O1 O6 150(2) 4_545 1_465
Ga3 O1 O6 128.8(18) . 1_465
Ga4 O1 O6 123.3(16) 2_656 1_465
Ga4 O1 O6 51.5(9) 3_554 1_465
O2 O1 O6 39.1(12) . 1_465
O3 O1 O6 101.9(16) 2_655 1_465
O6 O1 O6 127.1(11) 1_455 1_465
O5 O1 O6 73.6(10) 4 1_465
O7 O1 O6 35.0(7) 2 1_465
O3 O1 O6 66.7(10) 4_655 1_465
Ga3 O1 O6 92.5(10) 1_455 1_465
O2 O1 O6 164.8(10) 1_545 1_465
Ga4 O1 O6 88.4(8) 2_556 1_465
Ga4 O1 O6 22.8(5) 3_454 1_465
Ta O1 O6 127.9(13) . 1_465
Ga1 O1 O6 127.9(13) . 1_465
O4 O1 O6 68.5(12) 2 1_465
O5 O1 O6 101.0(13) 4_655 1_465
O7 O1 O6 104.1(11) 4_545 1_465
Ga1 O1 O6 93.7(10) 3 1_465
Ta O1 O6 93.7(10) 3 1_465
Ga1 O1 O6 24.1(5) 1_565 1_465
Ta O1 O6 24.1(5) 1_565 1_465
Ga2 O1 La1 30.0(15) . 2_656
La1 O1 La1 80.6(12) 2_556 2_656
La2 O1 La1 121.3(13) . 2_656
La1 O1 La1 122.5(17) 3_554 2_656
O3 O1 La1 126.4(18) 1_455 2_656
O4 O1 La1 165(2) . 2_656
O2 O1 La1 128(2) 4_545 2_656
O7 O1 La1 111.5(10) . 2_656
O3 O1 La1 31.9(9) . 2_656
O5 O1 La1 58.9(9) . 2_656
O6 O1 La1 79.8(12) 4_655 2_656
O2 O1 La1 30.1(15) 4_645 2_656
Ga2 O1 La1 151.6(18) 1_455 2_656
O4 O1 La1 63.1(10) 1_655 2_656
O4 O1 La1 47.0(11) 4_545 2_656
Ga3 O1 La1 53.8(5) . 2_656
Ga4 O1 La1 48.5(5) 2_656 2_656
Ga4 O1 La1 91.4(5) 3_554 2_656
O2 O1 La1 105.8(12) . 2_656
O3 O1 La1 80.6(9) 2_655 2_656
O6 O1 La1 89.4(11) 1_455 2_656
O5 O1 La1 116.5(15) 4 2_656
O7 O1 La1 140.9(13) 2 2_656
O3 O1 La1 93.3(9) 4_655 2_656
Ga3 O1 La1 119.8(13) 1_455 2_656
O2 O1 La1 52.6(9) 1_545 2_656
Ga4 O1 La1 117.6(14) 2_556 2_656
Ga4 O1 La1 165.3(12) 3_454 2_656
Ta O1 La1 80.7(8) . 2_656
Ga1 O1 La1 80.7(8) . 2_656
O4 O1 La1 97.7(9) 2 2_656
O5 O1 La1 55.7(7) 4_655 2_656
O7 O1 La1 95.3(12) 4_545 2_656
Ga1 O1 La1 91.2(11) 3 2_656
Ta O1 La1 91.2(11) 3 2_656
Ga1 O1 La1 128.2(8) 1_565 2_656
Ta O1 La1 128.2(8) 1_565 2_656
O6 O1 La1 142.5(11) 1_465 2_656
Ga2 O1 La2 27.9(15) . 1_655
La1 O1 La2 121.9(14) 2_556 1_655
La2 O1 La2 79.3(11) . 1_655
La1 O1 La2 120.8(15) 3_554 1_655
O3 O1 La2 122.4(19) 1_455 1_655
O4 O1 La2 134(2) . 1_655
O2 O1 La2 176(2) 4_545 1_655
O7 O1 La2 62.2(10) . 1_655
O3 O1 La2 27.4(7) . 1_655
O5 O1 La2 78.0(10) . 1_655
O6 O1 La2 114.9(11) 4_655 1_655
O2 O1 La2 59.0(12) 4_645 1_655
Ga2 O1 La2 149.1(19) 1_455 1_655
O4 O1 La2 43.8(12) 1_655 1_655
O4 O1 La2 97.4(12) 4_545 1_655
Ga3 O1 La2 49.0(4) . 1_655
Ga4 O1 La2 90.5(5) 2_656 1_655
Ga4 O1 La2 53.7(5) 3_554 1_655
O2 O1 La2 80.4(11) . 1_655
O3 O1 La2 55.0(7) 2_655 1_655
O6 O1 La2 113.5(12) 1_455 1_655
O5 O1 La2 146.6(14) 4 1_655
O7 O1 La2 91.1(12) 2 1_655
O3 O1 La2 99.9(9) 4_655 1_655
Ga3 O1 La2 116.0(13) 1_455 1_655
O2 O1 La2 93.5(11) 1_545 1_655
Ga4 O1 La2 167.2(14) 2_556 1_655
Ga4 O1 La2 118.8(14) 3_454 1_655
Ta O1 La2 90.5(9) . 1_655
Ga1 O1 La2 90.5(9) . 1_655
O4 O1 La2 50.5(8) 2 1_655
O5 O1 La2 78.8(7) 4_655 1_655
O7 O1 La2 143.8(12) 4_545 1_655
Ga1 O1 La2 129.1(10) 3 1_655
Ta O1 La2 129.1(10) 3 1_655
Ga1 O1 La2 79.4(9) 1_565 1_655
Ta O1 La2 79.4(9) 1_565 1_655
O6 O1 La2 100.2(12) 1_465 1_655
La1 O1 La2 50.4(2) 2_656 1_655
Ga2 O1 O6 51.1(17) . .
La1 O1 O6 64.0(11) 2_556 .
La2 O1 O6 104.3(16) . .
La1 O1 O6 147(2) 3_554 .
O3 O1 O6 98.9(16) 1_455 .
O4 O1 O6 163.6(18) . .
O2 O1 O6 123(2) 4_545 .
O7 O1 O6 117.4(13) . .
O3 O1 O6 31.0(9) . .
O5 O1 O6 31.3(7) . .
O6 O1 O6 97.6(14) 4_655 .
O2 O1 O6 57.5(16) 4_645 .
Ga2 O1 O6 129.2(16) 1_455 .
O4 O1 O6 87.0(12) 1_655 .
O4 O1 O6 49.3(13) 4_545 .
Ga3 O1 O6 33.1(6) . .
Ga4 O1 O6 67.3(9) 2_656 .
Ga4 O1 O6 110.2(6) 3_554 .
O2 O1 O6 131.2(11) . .
O3 O1 O6 61.8(9) 2_655 .
O6 O1 O6 64.6(8) 1_455 .
O5 O1 O6 127.4(16) 4 .
O7 O1 O6 130.9(16) 2 .
O3 O1 O6 119.7(12) 4_655 .
Ga3 O1 O6 92.2(11) 1_455 .
O2 O1 O6 35.2(10) 1_545 .
Ga4 O1 O6 113.9(13) 2_556 .
Ga4 O1 O6 161.8(15) 3_454 .
Ta O1 O6 53.0(7) . .
Ga1 O1 O6 53.0(7) . .
O4 O1 O6 90.9(10) 2 .
O5 O1 O6 81.9(9) 4_655 .
O7 O1 O6 97.9(12) 4_545 .
Ga1 O1 O6 104.8(13) 3 .
Ta O1 O6 104.8(13) 3 .
Ga1 O1 O6 134.0(12) 1_565 .
Ta O1 O6 134.0(12) 1_565 .
O6 O1 O6 157.6(14) 1_465 .
La1 O1 O6 27.7(5) 2_656 .
La2 O1 O6 58.3(5) 1_655 .
Ga2 O1 La1 30.1(14) . 3_654
La1 O1 La1 122.3(17) 2_556 3_654
La2 O1 La1 120.0(15) . 3_654
La1 O1 La1 80.7(12) 3_554 3_654
O3 O1 La1 172.3(19) 1_455 3_654
O4 O1 La1 118.9(19) . 3_654
O2 O1 La1 126(2) 4_545 3_654
O7 O1 La1 79.5(11) . 3_654
O3 O1 La1 60.8(8) . 3_654
O5 O1 La1 108.1(9) . 3_654
O6 O1 La1 66.8(11) 4_655 3_654
O2 O1 La1 27.0(13) 4_645 3_654
Ga2 O1 La1 151.2(17) 1_455 3_654
O4 O1 La1 18.2(11) 1_655 3_654
O4 O1 La1 78.8(14) 4_545 3_654
Ga3 O1 La1 91.0(4) . 3_654
Ga4 O1 La1 53.0(6) 2_656 3_654
Ga4 O1 La1 48.7(5) 3_554 3_654
O2 O1 La1 55.7(11) . 3_654
O3 O1 La1 104.8(8) 2_655 3_654
O6 O1 La1 138.9(13) 1_455 3_654
O5 O1 La1 97.2(13) 4 3_654
O7 O1 La1 113.7(13) 2 3_654
O3 O1 La1 53.0(7) 4_655 3_654
Ga3 O1 La1 165.4(12) 1_455 3_654
O2 O1 La1 99.9(11) 1_545 3_654
Ga4 O1 La1 120.6(14) 2_556 3_654
Ga4 O1 La1 115.8(12) 3_454 3_654
Ta O1 La1 129.0(8) . 3_654
Ga1 O1 La1 129.0(8) . 3_654
O4 O1 La1 91.5(9) 2 3_654
O5 O1 La1 31.0(6) 4_655 3_654
O7 O1 La1 101.5(13) 4_545 3_654
Ga1 O1 La1 80.7(9) 3 3_654
Ta O1 La1 80.7(9) 3 3_654
Ga1 O1 La1 89.9(9) 1_565 3_654
Ta O1 La1 89.9(9) 1_565 3_654
O6 O1 La1 94.0(11) 1_465 3_654
La1 O1 La1 50.2(3) 2_656 3_654
La2 O1 La1 49.9(3) 1_655 3_654
O6 O1 La1 77.0(6) . 3_654
Ga2 O1 O1 108(3) . 2
La1 O1 O1 98.6(13) 2_556 2
La2 O1 O1 12.6(14) . 2
La1 O1 O1 117.8(13) 3_554 2
O3 O1 O1 46.8(12) 1_455 2
O4 O1 O1 79.0(15) . 2
O2 O1 O1 103.0(18) 4_545 2
O7 O1 O1 57.5(14) . 2
O3 O1 O1 85.1(17) . 2
O5 O1 O1 73.8(14) . 2
O6 O1 O1 163.8(10) 4_655 2
O2 O1 O1 138(2) 4_645 2
Ga2 O1 O1 69.4(9) 1_455 2
O4 O1 O1 111.1(19) 1_655 2
O4 O1 O1 133.6(16) 4_545 2
Ga3 O1 O1 62.7(12) . 2
Ga4 O1 O1 162.0(11) 2_656 2
Ga4 O1 O1 88.5(12) 3_554 2
O2 O1 O1 103.4(14) . 2
O3 O1 O1 34.8(10) 2_655 2
O6 O1 O1 72.9(9) 1_455 2
O5 O1 O1 126.4(8) 4 2
O7 O1 O1 38.9(9) 2 2
O3 O1 O1 140.0(8) 4_655 2
Ga3 O1 O1 43.6(6) 1_455 2
O2 O1 O1 102.1(12) 1_545 2
Ga4 O1 O1 111.2(6) 2_556 2
Ga4 O1 O1 67.4(6) 3_454 2
Ta O1 O1 57.7(8) . 2
Ga1 O1 O1 57.7(8) . 2
O4 O1 O1 35.2(9) 2 2
O5 O1 O1 157.4(12) 4_655 2
O7 O1 O1 132.0(7) 4_545 2
Ga1 O1 O1 150.0(6) 3 2
Ta O1 O1 150.0(6) 3 2
Ga1 O1 O1 58.3(7) 1_565 2
Ta O1 O1 58.3(7) 1_565 2
O6 O1 O1 73.9(8) 1_465 2
La1 O1 O1 115.4(11) 2_656 2
La2 O1 O1 80.5(11) 1_655 2
O6 O1 O1 94.8(11) . 2
La1 O1 O1 126.5(12) 3_654 2
Ga2 O1 Ga2 72.2(19) . 4_645
La1 O1 Ga2 40.7(9) 2_556 4_645
La2 O1 Ga2 135.9(19) . 4_645
La1 O1 Ga2 114(2) 3_554 4_645
O3 O1 Ga2 98.9(16) 1_455 4_645
O4 O1 Ga2 133.3(17) . 4_645
O2 O1 Ga2 88(2) 4_545 4_645
O7 O1 Ga2 154.2(9) . 4_645
O3 O1 Ga2 67.7(12) . 4_645
O5 O1 Ga2 50.2(11) . 4_645
O6 O1 Ga2 63.3(12) 4_655 4_645
O2 O1 Ga2 55.2(16) 4_645 4_645
Ga2 O1 Ga2 109.9(14) 1_455 4_645
O4 O1 Ga2 99.6(14) 1_655 4_645
O4 O1 Ga2 10.8(11) 4_545 4_645
Ga3 O1 Ga2 70.6(10) . 4_645
Ga4 O1 Ga2 40.6(7) 2_656 4_645
Ga4 O1 Ga2 130.5(9) 3_554 4_645
O2 O1 Ga2 130.5(17) . 4_645
O3 O1 Ga2 97.6(12) 2_655 4_645
O6 O1 Ga2 59.2(9) 1_455 4_645
O5 O1 Ga2 87.8(13) 4 4_645
O7 O1 Ga2 161.1(15) 2 4_645
O3 O1 Ga2 96.4(12) 4_655 4_645
Ga3 O1 Ga2 95.8(11) 1_455 4_645
O2 O1 Ga2 22.0(9) 1_545 4_645
Ga4 O1 Ga2 77.2(10) 2_556 4_645
Ga4 O1 Ga2 149.1(10) 3_454 4_645
Ta O1 Ga2 66.6(8) . 4_645
Ga1 O1 Ga2 66.6(8) . 4_645
O4 O1 Ga2 130.5(12) 2 4_645
O5 O1 Ga2 66.3(9) 4_655 4_645
O7 O1 Ga2 58.4(8) 4_545 4_645
Ga1 O1 Ga2 66.7(9) 3 4_645
Ta O1 Ga2 66.7(9) 3 4_645
Ga1 O1 Ga2 171.0(5) 1_565 4_645
Ta O1 Ga2 171.0(5) 1_565 4_645
O6 O1 Ga2 160.4(15) 1_465 4_645
La1 O1 Ga2 42.9(5) 2_656 4_645
La2 O1 Ga2 92.1(6) 1_655 4_645
O6 O1 Ga2 39.8(6) . 4_645
La1 O1 Ga2 82.2(7) 3_654 4_645
O1 O1 Ga2 123.6(8) 2 4_645
Ga2 O1 Ga2 69.2(19) . 2_655
La1 O1 Ga2 112.0(18) 2_556 2_655
La2 O1 Ga2 40.2(7) . 2_655
La1 O1 Ga2 134(2) 3_554 2_655
O3 O1 Ga2 81.5(16) 1_455 2_655
O4 O1 Ga2 110.6(19) . 2_655
O2 O1 Ga2 141(2) 4_545 2_655
O7 O1 Ga2 52.7(12) . 2_655
O3 O1 Ga2 49.6(11) . 2_655
O5 O1 Ga2 67.3(12) . 2_655
O6 O1 Ga2 157.1(10) 4_655 2_655
O2 O1 Ga2 100.0(14) 4_645 2_655
Ga2 O1 Ga2 108.0(15) 1_455 2_655
O4 O1 Ga2 79.9(15) 1_655 2_655
O4 O1 Ga2 119.9(16) 4_545 2_655
Ga3 O1 Ga2 39.7(7) . 2_655
Ga4 O1 Ga2 129.2(6) 2_656 2_655
Ga4 O1 Ga2 70.4(10) 3_554 2_655
O2 O1 Ga2 96.8(15) . 2_655
O3 O1 Ga2 19.6(5) 2_655 2_655
O6 O1 Ga2 89.6(12) 1_455 2_655
O5 O1 Ga2 161.4(14) 4 2_655
O7 O1 Ga2 61.8(11) 2 2_655
O3 O1 Ga2 132.3(12) 4_655 2_655
Ga3 O1 Ga2 76.0(9) 1_455 2_655
O2 O1 Ga2 96.5(14) 1_545 2_655
Ga4 O1 Ga2 148.4(11) 2_556 2_655
Ga4 O1 Ga2 95.3(12) 3_454 2_655
Ta O1 Ga2 65.5(8) . 2_655
Ga1 O1 Ga2 65.5(8) . 2_655
O4 O1 Ga2 20.8(6) 2 2_655
O5 O1 Ga2 120.9(7) 4_655 2_655
O7 O1 Ga2 160.9(14) 4_545 2_655
Ga1 O1 Ga2 171.4(7) 3 2_655
Ta O1 Ga2 171.4(7) 3 2_655
Ga1 O1 Ga2 65.6(9) 1_565 2_655
Ta O1 Ga2 65.6(9) 1_565 2_655
O6 O1 Ga2 89.3(12) 1_465 2_655
La1 O1 Ga2 81.5(6) 2_656 2_655
La2 O1 Ga2 42.2(4) 1_655 2_655
O6 O1 Ga2 70.6(7) . 2_655
La1 O1 Ga2 91.0(6) 3_654 2_655
O1 O1 Ga2 38.6(7) 2 2_655
Ga2 O1 Ga2 109.9(10) 4_645 2_655
Ga2 O1 Ga2 71.4(18) . 4_655
La1 O1 Ga2 136(2) 2_556 4_655
La2 O1 Ga2 111.0(18) . 4_655
La1 O1 Ga2 40.5(8) 3_554 4_655
O3 O1 Ga2 142.0(15) 1_455 4_655
O4 O1 Ga2 76.5(16) . 4_655
O2 O1 Ga2 95(2) 4_545 4_655
O7 O1 Ga2 66.5(13) . 4_655
O3 O1 Ga2 101.2(10) . 4_655
O5 O1 Ga2 150.3(10) . 4_655
O6 O1 Ga2 58.1(12) 4_655 4_655
O2 O1 Ga2 63.0(17) 4_645 4_655
Ga2 O1 Ga2 109.3(13) 1_455 4_655
O4 O1 Ga2 38.3(14) 1_655 4_655
O4 O1 Ga2 101.7(18) 4_545 4_655
Ga3 O1 Ga2 129.7(7) . 4_655
Ga4 O1 Ga2 69.9(10) 2_656 4_655
Ga4 O1 Ga2 39.5(6) 3_554 4_655
O2 O1 Ga2 20.4(11) . 4_655
O3 O1 Ga2 129.0(13) 2_655 4_655
O6 O1 Ga2 160.8(16) 1_455 4_655
O5 O1 Ga2 67.5(10) 4 4_655
O7 O1 Ga2 88.7(11) 2 4_655
O3 O1 Ga2 22.8(5) 4_655 4_655
Ga3 O1 Ga2 148.6(11) 1_455 4_655
O2 O1 Ga2 132.2(15) 1_545 4_655
Ga4 O1 Ga2 95.6(11) 2_556 4_655
Ga4 O1 Ga2 75.9(9) 3_454 4_655
Ta O1 Ga2 171.2(5) . 4_655
Ga1 O1 Ga2 171.2(5) . 4_655
O4 O1 Ga2 96.2(11) 2 4_655
O5 O1 Ga2 44.2(7) 4_655 4_655
O7 O1 Ga2 89.4(12) 4_545 4_655
Ga1 O1 Ga2 65.8(8) 3 4_655
Ta O1 Ga2 65.8(8) 3 4_655
Ga1 O1 Ga2 65.8(8) 1_565 4_655
Ta O1 Ga2 65.8(8) 1_565 4_655
O6 O1 Ga2 57.5(8) 1_465 4_655
La1 O1 Ga2 91.5(7) 2_656 4_655
La2 O1 Ga2 81.3(6) 1_655 4_655
O6 O1 Ga2 119.0(8) . 4_655
La1 O1 Ga2 42.5(4) 3_654 4_655
O1 O1 Ga2 123.4(8) 2 4_655
Ga2 O1 Ga2 110.2(11) 4_645 4_655
Ga2 O1 Ga2 109.5(10) 2_655 4_655
Ga2 O1 O1 111(2) . 4_545
La1 O1 O1 11.2(5) 2_556 4_545
La2 O1 O1 119.1(18) . 4_545
La1 O1 O1 101(2) 3_554 4_545
O3 O1 O1 66.6(12) 1_455 4_545
O4 O1 O1 97.7(15) . 4_545
O2 O1 O1 53(2) 4_545 4_545
O7 O1 O1 163.4(19) . 4_545
O3 O1 O1 100.7(12) . 4_545
O5 O1 O1 57.6(7) . 4_545
O6 O1 O1 66.9(19) 4_655 4_545
O2 O1 O1 91(2) 4_645 4_545
Ga2 O1 O1 70.6(11) 1_455 4_545
O4 O1 O1 135(2) 1_655 4_545
O4 O1 O1 39.1(12) 4_545 4_545
Ga3 O1 O1 88.6(9) . 4_545
Ga4 O1 O1 65.2(16) 2_656 4_545
Ga4 O1 O1 163(2) 3_554 4_545
O2 O1 O1 140(2) . 4_545
O3 O1 O1 103.9(14) 2_655 4_545
O6 O1 O1 36.5(7) 1_455 4_545
O5 O1 O1 67.3(16) 4 4_545
O7 O1 O1 128.6(12) 2 4_545
O3 O1 O1 103(2) 4_655 4_545
Ga3 O1 O1 66.7(9) 1_455 4_545
O2 O1 O1 34.6(8) 1_545 4_545
Ga4 O1 O1 44.9(10) 2_556 4_545
Ga4 O1 O1 111.6(8) 3_454 4_545
Ta O1 O1 58.3(7) . 4_545
Ga1 O1 O1 58.3(7) . 4_545
O4 O1 O1 138.9(19) 2 4_545
O5 O1 O1 91.5(19) 4_655 4_545
O7 O1 O1 37.9(12) 4_545 4_545
Ga1 O1 O1 59.8(15) 3 4_545
Ta O1 O1 59.8(15) 3 4_545
Ga1 O1 O1 149.7(8) 1_565 4_545
Ta O1 O1 149.7(8) 1_565 4_545
O6 O1 O1 131.9(9) 1_465 4_545
La1 O1 O1 81.8(9) 2_656 4_545
La2 O1 O1 127.9(8) 1_655 4_545
O6 O1 O1 69.7(5) . 4_545
La1 O1 O1 117.1(17) 3_654 4_545
O1 O1 O1 108.4(13) 2 4_545
Ga2 O1 O1 39.3(6) 4_645 4_545
Ga2 O1 O1 123.1(15) 2_655 4_545
Ga2 O1 O1 125(2) 4_655 4_545
Ga2 O1 O1 111(2) . 4
La1 O1 O1 119.7(19) 2_556 4
La2 O1 O1 97.4(16) . 4
La1 O1 O1 11.1(9) 3_554 4
O3 O1 O1 103.8(12) 1_455 4
O4 O1 O1 38.4(14) . 4
O2 O1 O1 62(2) 4_545 4
O7 O1 O1 70.2(11) . 4
O3 O1 O1 139.4(13) . 4
O5 O1 O1 166.8(13) . 4
O6 O1 O1 61.7(18) 4_655 4
O2 O1 O1 98(2) 4_645 4
Ga2 O1 O1 70.1(10) 1_455 4
O4 O1 O1 76.0(16) 1_655 4
O4 O1 O1 114(3) 4_545 4
Ga3 O1 O1 161.2(18) . 4
Ga4 O1 O1 89.5(19) 2_656 4
Ga4 O1 O1 62.4(5) 3_554 4
O2 O1 O1 34.8(8) . 4
O3 O1 O1 138(2) 2_655 4
O6 O1 O1 130.8(9) 1_455 4
O5 O1 O1 43.1(12) 4 4
O7 O1 O1 70.0(11) 2 4
O3 O1 O1 35.2(10) 4_655 4
Ga3 O1 O1 111.1(9) 1_455 4
O2 O1 O1 141(2) 1_545 4
Ga4 O1 O1 67.0(11) 2_556 4
Ga4 O1 O1 43.0(7) 3_454 4
Ta O1 O1 149.5(8) . 4
Ga1 O1 O1 149.5(8) . 4
O4 O1 O1 102.3(14) 2 4
O5 O1 O1 73.0(14) 4_655 4
O7 O1 O1 73.9(15) 4_545 4
Ga1 O1 O1 58.7(14) 3 4
Ta O1 O1 58.7(14) 3 4
Ga1 O1 O1 57.8(8) 1_565 4
Ta O1 O1 57.8(8) 1_565 4
O6 O1 O1 35.8(7) 1_465 4
La1 O1 O1 127.9(16) 2_656 4
La2 O1 O1 115.2(8) 1_655 4
O6 O1 O1 154.9(19) . 4
La1 O1 O1 81.5(10) 3_654 4
O1 O1 O1 108.4(12) 2 4
Ga2 O1 O1 125(2) 4_645 4
Ga2 O1 O1 122.8(16) 2_655 4
Ga2 O1 O1 39.2(5) 4_655 4
O1 O1 O1 110.2(19) 4_545 4
Ga2 O1 O5 114(2) . 2
La1 O1 O5 60.1(12) 2_556 2
La2 O1 O5 51.0(11) . 2
La1 O1 O5 134.1(9) 3_554 2
O3 O1 O5 28.8(10) 1_455 2
O4 O1 O5 92.5(16) . 2
O2 O1 O5 87(2) 4_545 2
O7 O1 O5 96.3(17) . 2
O3 O1 O5 83.7(14) . 2
O5 O1 O5 43.7(10) . 2
O6 O1 O5 136.8(17) 4_655 2
O2 O1 O5 131.2(19) 4_645 2
Ga2 O1 O5 64.0(10) 1_455 2
O4 O1 O5 139(2) 1_655 2
O4 O1 O5 96.6(17) 4_545 2
Ga3 O1 O5 53.5(8) . 2
Ga4 O1 O5 128.4(15) 2_656 2
Ga4 O1 O5 126.1(17) 3_554 2
O2 O1 O5 141.3(19) . 2
O3 O1 O5 42.6(9) 2_655 2
O6 O1 O5 34.3(7) 1_455 2
O5 O1 O5 116.7(11) 4 2
O7 O1 O5 73.1(11) 2 2
O3 O1 O5 162.7(8) 4_655 2
Ga3 O1 O5 21.3(5) 1_455 2
O2 O1 O5 66.0(12) 1_545 2
Ga4 O1 O5 90.1(8) 2_556 2
Ga4 O1 O5 89.4(9) 3_454 2
Ta O1 O5 22.4(4) . 2
Ga1 O1 O5 22.4(4) . 2
O4 O1 O5 69.3(11) 2 2
O5 O1 O5 153.5(15) 4_655 2
O7 O1 O5 102.3(10) 4_545 2
Ga1 O1 O5 126.2(11) 3 2
Ta O1 O5 126.2(11) 3 2
Ga1 O1 O5 95.9(12) 1_565 2
Ta O1 O5 95.9(12) 1_565 2
O6 O1 O5 105.5(12) 1_465 2
La1 O1 O5 101.2(10) 2_656 2
La2 O1 O5 96.6(10) 1_655 2
O6 O1 O5 73.7(9) . 2
La1 O1 O5 144.3(9) 3_654 2
O1 O1 O5 38.9(8) 2 2
Ga2 O1 O5 88.0(10) 4_645 2
Ga2 O1 O5 60.3(8) 2_655 2
Ga2 O1 O5 161.7(15) 4_655 2
O1 O1 O5 70.5(11) 4_545 2
O1 O1 O5 130.8(13) 4 2
Ga2 O1 O7 49.0(18) . 2_655
La1 O1 O7 146.8(17) 2_556 2_655
La2 O1 O7 64.2(12) . 2_655
La1 O1 O7 101.9(16) 3_554 2_655
O3 O1 O7 117(2) 1_455 2_655
O4 O1 O7 106.6(18) . 2_655
O2 O1 O7 152(2) 4_545 2_655
O7 O1 O7 35.2(11) . 2_655
O3 O1 O7 54.1(10) . 2_655
O5 O1 O7 99.6(13) . 2_655
O6 O1 O7 120.6(15) 4_655 2_655
O2 O1 O7 76.2(14) 4_645 2_655
Ga2 O1 O7 128.4(18) 1_455 2_655
O4 O1 O7 40.8(14) 1_655 2_655
O4 O1 O7 123.0(13) 4_545 2_655
Ga3 O1 O7 68.3(10) . 2_655
Ga4 O1 O7 107.6(8) 2_656 2_655
Ga4 O1 O7 31.8(6) 3_554 2_655
O2 O1 O7 60.1(11) . 2_655
O3 O1 O7 60.2(11) 2_655 2_655
O6 O1 O7 129.7(16) 1_455 2_655
O5 O1 O7 134.6(15) 4 2_655
O7 O1 O7 67.2(11) 2 2_655
O3 O1 O7 91.4(10) 4_655 2_655
Ga3 O1 O7 113.9(15) 1_455 2_655
O2 O1 O7 120.2(12) 1_545 2_655
Ga4 O1 O7 160.1(14) 2_556 2_655
Ga4 O1 O7 91.7(12) 3_454 2_655
Ta O1 O7 105.0(12) . 2_655
Ga1 O1 O7 105.0(12) . 2_655
O4 O1 O7 35.5(9) 2 2_655
O5 O1 O7 86.7(10) 4_655 2_655
O7 O1 O7 156.2(16) 4_545 2_655
Ga1 O1 O7 132.6(12) 3 2_655
Ta O1 O7 132.6(12) 3 2_655
Ga1 O1 O7 52.3(8) 1_565 2_655
Ta O1 O7 52.3(8) 1_565 2_655
O6 O1 O7 72.9(10) 1_465 2_655
La1 O1 O7 76.5(6) 2_656 2_655
La2 O1 O7 27.4(5) 1_655 2_655
O6 O1 O7 85.1(7) . 2_655
La1 O1 O7 56.1(6) 3_654 2_655
O1 O1 O7 70.7(12) 2 2_655
Ga2 O1 O7 119.0(7) 4_645 2_655
Ga2 O1 O7 41.1(7) 2_655 2_655
Ga2 O1 O7 68.9(8) 4_655 2_655
O1 O1 O7 154.7(10) 4_545 2_655
O1 O1 O7 93.4(8) 4 2_655
O5 O1 O7 101.2(13) 2 2_655
Ga2 O1 O1 178(2) . 1_455
La1 O1 O1 70.4(7) 2_556 1_455
La2 O1 O1 70.8(5) . 1_455
La1 O1 O1 70.1(7) 3_554 1_455
O3 O1 O1 35.8(11) 1_455 1_455
O4 O1 O1 34.5(14) . 1_455
O2 O1 O1 33.0(19) 4_545 1_455
O7 O1 O1 95.5(8) . 1_455
O3 O1 O1 148.2(12) . 1_455
O5 O1 O1 99.4(6) . 1_455
O6 O1 O1 93.7(7) 4_655 1_455
O2 O1 O1 150.8(16) 4_645 1_455
Ga2 O1 O1 1.0(12) 1_455 1_455
O4 O1 O1 143.9(14) 1_655 1_455
O4 O1 O1 107.2(11) 4_545 1_455
Ga3 O1 O1 118.0(6) . 1_455
Ga4 O1 O1 119.3(5) 2_656 1_455
Ga4 O1 O1 117.4(6) 3_554 1_455
O2 O1 O1 99.7(9) . 1_455
O3 O1 O1 100.3(7) 2_655 1_455
O6 O1 O1 64.5(6) 1_455 1_455
O5 O1 O1 57.8(8) 4 1_455
O7 O1 O1 62.1(6) 2 1_455
O3 O1 O1 98.2(5) 4_655 1_455
Ga3 O1 O1 43.3(5) 1_455 1_455
O2 O1 O1 98.8(8) 1_545 1_455
Ga4 O1 O1 42.5(7) 2_556 1_455
Ga4 O1 O1 43.4(6) 3_454 1_455
Ta O1 O1 79.7(2) . 1_455
Ga1 O1 O1 79.7(2) . 1_455
O4 O1 O1 99.9(7) 2 1_455
O5 O1 O1 128.5(6) 4_655 1_455
O7 O1 O1 65.8(6) 4_545 1_455
Ga1 O1 O1 79.6(3) 3 1_455
Ta O1 O1 79.6(3) 3 1_455
Ga1 O1 O1 79.8(2) 1_565 1_455
Ta O1 O1 79.8(2) 1_565 1_455
O6 O1 O1 66.0(5) 1_465 1_455
La1 O1 O1 151.1(7) 2_656 1_455
La2 O1 O1 150.2(7) 1_655 1_455
O6 O1 O1 129.1(6) . 1_455
La1 O1 O1 150.8(6) 3_654 1_455
O1 O1 O1 70.4(5) 2 1_455
Ga2 O1 O1 109.2(3) 4_645 1_455
Ga2 O1 O1 109.0(4) 2_655 1_455
Ga2 O1 O1 109.1(3) 4_655 1_455
O1 O1 O1 69.9(6) 4_545 1_455
O1 O1 O1 69.9(6) 4 1_455
O5 O1 O1 64.6(5) 2 1_455
O7 O1 O1 129.3(7) 2_655 1_455
Ga2 O1 O1 2(2) . 1_655
La1 O1 O1 109.6(7) 2_556 1_655
La2 O1 O1 109.2(5) . 1_655
La1 O1 O1 109.9(7) 3_554 1_655
O3 O1 O1 144.2(11) 1_455 1_655
O4 O1 O1 145.5(14) . 1_655
O2 O1 O1 147.1(19) 4_545 1_655
O7 O1 O1 84.5(8) . 1_655
O3 O1 O1 31.8(12) . 1_655
O5 O1 O1 80.6(6) . 1_655
O6 O1 O1 86.3(7) 4_655 1_655
O2 O1 O1 29.2(16) 4_645 1_655
Ga2 O1 O1 179.0(12) 1_455 1_655
O4 O1 O1 36.1(14) 1_655 1_655
O4 O1 O1 72.8(11) 4_545 1_655
Ga3 O1 O1 62.0(6) . 1_655
Ga4 O1 O1 60.7(5) 2_656 1_655
Ga4 O1 O1 62.6(6) 3_554 1_655
O2 O1 O1 80.3(9) . 1_655
O3 O1 O1 79.7(7) 2_655 1_655
O6 O1 O1 115.5(6) 1_455 1_655
O5 O1 O1 122.2(8) 4 1_655
O7 O1 O1 117.9(6) 2 1_655
O3 O1 O1 81.8(5) 4_655 1_655
Ga3 O1 O1 136.7(5) 1_455 1_655
O2 O1 O1 81.2(8) 1_545 1_655
Ga4 O1 O1 137.5(7) 2_556 1_655
Ga4 O1 O1 136.6(6) 3_454 1_655
Ta O1 O1 100.3(2) . 1_655
Ga1 O1 O1 100.3(2) . 1_655
O4 O1 O1 80.1(7) 2 1_655
O5 O1 O1 51.5(6) 4_655 1_655
O7 O1 O1 114.2(6) 4_545 1_655
Ga1 O1 O1 100.4(3) 3 1_655
Ta O1 O1 100.4(3) 3 1_655
Ga1 O1 O1 100.2(2) 1_565 1_655
Ta O1 O1 100.2(2) 1_565 1_655
O6 O1 O1 114.0(5) 1_465 1_655
La1 O1 O1 28.9(7) 2_656 1_655
La2 O1 O1 29.8(7) 1_655 1_655
O6 O1 O1 50.9(6) . 1_655
La1 O1 O1 29.2(6) 3_654 1_655
O1 O1 O1 109.6(5) 2 1_655
Ga2 O1 O1 70.8(3) 4_645 1_655
Ga2 O1 O1 71.0(4) 2_655 1_655
Ga2 O1 O1 70.9(3) 4_655 1_655
O1 O1 O1 110.1(6) 4_545 1_655
O1 O1 O1 110.1(6) 4 1_655
O5 O1 O1 115.4(5) 2 1_655
O7 O1 O1 50.7(7) 2_655 1_655
O1 O1 O1 179.999(11) 1_455 1_655
Ga2 O1 Ga4 71.6(18) . 3_544
La1 O1 Ga4 45.5(9) 2_556 3_544
La2 O1 Ga4 100.7(16) . 3_544
La1 O1 Ga4 149(2) 3_554 3_544
O3 O1 Ga4 80.6(14) 1_455 3_544
O4 O1 Ga4 143.2(16) . 3_544
O2 O1 Ga4 106(2) 4_545 3_544
O7 O1 Ga4 129.1(16) . 3_544
O3 O1 Ga4 49.3(9) . 3_544
O5 O1 Ga4 15.6(8) . 3_544
O6 O1 Ga4 99.1(15) 4_655 3_544
O2 O1 Ga4 73.8(17) 4_645 3_544
Ga2 O1 Ga4 108.8(13) 1_455 3_544
O4 O1 Ga4 107.4(13) 1_655 3_544
O4 O1 Ga4 46.6(13) 4_545 3_544
Ga3 O1 Ga4 37.5(6) . 3_544
Ga4 O1 Ga4 73.8(10) 2_656 3_544
Ga4 O1 Ga4 129.8(7) 3_554 3_544
O2 O1 Ga4 151.5(11) . 3_544
O3 O1 Ga4 62.2(9) 2_655 3_544
O6 O1 Ga4 44.2(7) 1_455 3_544
O5 O1 Ga4 118.5(15) 4 3_544
O7 O1 Ga4 127.9(15) 2 3_544
O3 O1 Ga4 130.4(13) 4_655 3_544
Ga3 O1 Ga4 74.5(9) 1_455 3_544
O2 O1 Ga4 20.0(9) 1_545 3_544
Ga4 O1 Ga4 98.1(11) 2_556 3_544
Ga4 O1 Ga4 147.2(11) 3_454 3_544
Ta O1 Ga4 36.6(5) . 3_544
Ga1 O1 Ga4 36.6(5) . 3_544
O4 O1 Ga4 97.4(11) 2 3_544
O5 O1 Ga4 94.8(10) 4_655 3_544
O7 O1 Ga4 87.3(10) 4_545 3_544
Ga1 O1 Ga4 101.4(12) 3 3_544
Ta O1 Ga4 101.4(12) 3 3_544
Ga1 O1 Ga4 142.1(14) 1_565 3_544
Ta O1 Ga4 142.1(14) 1_565 3_544
O6 O1 Ga4 162.8(16) 1_465 3_544
La1 O1 Ga4 46.1(5) 2_656 3_544
La2 O1 Ga4 76.4(6) 1_655 3_544
O6 O1 Ga4 20.5(4) . 3_544
La1 O1 Ga4 96.3(6) 3_654 3_544
O1 O1 Ga4 88.9(8) 2 3_544
Ga2 O1 Ga4 35.9(4) 4_645 3_544
Ga2 O1 Ga4 76.9(8) 2_655 3_544
Ga2 O1 Ga4 136.8(9) 4_655 3_544
O1 O1 Ga4 53.2(4) 4_545 3_544
O1 O1 Ga4 160(2) 4 3_544
O5 O1 Ga4 58.9(7) 2 3_544
O7 O1 Ga4 101.8(8) 2_655 3_544
O1 O1 Ga4 108.6(3) 1_455 3_544
O1 O1 Ga4 71.4(3) 1_655 3_544
Ga2 O1 Ga4 69.6(19) . 4_655
La1 O1 Ga4 147(2) 2_556 4_655
La2 O1 Ga4 44.8(9) . 4_655
La1 O1 Ga4 99.0(17) 3_554 4_655
O3 O1 Ga4 99.1(18) 1_455 4_655
O4 O1 Ga4 90.3(17) . 4_655
O2 O1 Ga4 136(2) 4_545 4_655
O7 O1 Ga4 19.4(8) . 4_655
O3 O1 Ga4 68.8(11) . 4_655
O5 O1 Ga4 102.6(14) . 4_655
O6 O1 Ga4 134.1(16) 4_655 4_655
O2 O1 Ga4 97.0(15) 4_645 4_655
Ga2 O1 Ga4 107.7(15) 1_455 4_655
O4 O1 Ga4 58.2(14) 1_655 4_655
O4 O1 Ga4 142.5(12) 4_545 4_655
Ga3 O1 Ga4 72.9(10) . 4_655
Ga4 O1 Ga4 127.9(8) 2_656 4_655
Ga4 O1 Ga4 37.2(7) 3_554 4_655
O2 O1 Ga4 61.4(12) . 4_655
O3 O1 Ga4 54.6(9) 2_655 4_655
O6 O1 Ga4 122.5(14) 1_455 4_655
O5 O1 Ga4 131.3(14) 4 4_655
O7 O1 Ga4 46.7(8) 2 4_655
O3 O1 Ga4 99.0(11) 4_655 4_655
Ga3 O1 Ga4 96.9(11) 1_455 4_655
O2 O1 Ga4 130.1(13) 1_545 4_655
Ga4 O1 Ga4 146.3(11) 2_556 4_655
Ga4 O1 Ga4 74.3(9) 3_454 4_655
Ta O1 Ga4 100.1(11) . 4_655
Ga1 O1 Ga4 100.1(11) . 4_655
O4 O1 Ga4 19.9(6) 2 4_655
O5 O1 Ga4 104.8(9) 4_655 4_655
O7 O1 Ga4 162.4(13) 4_545 4_655
Ga1 O1 Ga4 141.9(13) 3 4_655
Ta O1 Ga4 141.9(13) 3 4_655
Ga1 O1 Ga4 36.0(5) 1_565 4_655
Ta O1 Ga4 36.0(5) 1_565 4_655
O6 O1 Ga4 59.5(9) 1_465 4_655
La1 O1 Ga4 95.5(5) 2_656 4_655
La2 O1 Ga4 45.1(5) 1_655 4_655
O6 O1 Ga4 98.2(8) . 4_655
La1 O1 Ga4 75.3(6) 3_654 4_655
O1 O1 Ga4 53.4(8) 2 4_655
Ga2 O1 Ga4 136.4(6) 4_645 4_655
Ga2 O1 Ga4 35.7(5) 2_655 4_655
Ga2 O1 Ga4 76.5(8) 4_655 4_655
O1 O1 Ga4 158.3(18) 4_545 4_655
O1 O1 Ga4 88.5(10) 4 4_655
O5 O1 Ga4 89.1(11) 2 4_655
O7 O1 Ga4 21.0(6) 2_655 4_655
O1 O1 Ga4 108.6(4) 1_455 4_655
O1 O1 Ga4 71.4(4) 1_655 4_655
Ga4 O1 Ga4 110.2(9) 3_544 4_655
Ga2 O1 Ga3 72.7(19) . 3
La1 O1 Ga3 100.8(18) 2_556 3
La2 O1 Ga3 146(2) . 3
La1 O1 Ga3 46.7(11) 3_554 3
O3 O1 Ga3 141.6(15) 1_455 3
O4 O1 Ga3 89.2(18) . 3
O2 O1 Ga3 80(2) 4_545 3
O7 O1 Ga3 102.4(15) . 3
O3 O1 Ga3 101.3(12) . 3
O5 O1 Ga3 126.1(16) . 3
O6 O1 Ga3 24.3(8) 4_655 3
O2 O1 Ga3 47.2(16) 4_645 3
Ga2 O1 Ga3 109.6(13) 1_455 3
O4 O1 Ga3 56.5(16) 1_655 3
O4 O1 Ga3 67.3(16) 4_545 3
Ga3 O1 Ga3 129.4(9) . 3
Ga4 O1 Ga3 36.9(6) 2_656 3
Ga4 O1 Ga3 73.1(10) 3_554 3
O2 O1 Ga3 55.6(13) . 3
O3 O1 Ga3 150.6(7) 2_655 3
O6 O1 Ga3 126.6(15) 1_455 3
O5 O1 Ga3 51.5(9) 4 3
O7 O1 Ga3 121.1(13) 2 3
O3 O1 Ga3 19.9(5) 4_655 3
Ga3 O1 Ga3 147.7(10) 1_455 3
O2 O1 Ga3 98.8(14) 1_545 3
Ga4 O1 Ga3 75.0(9) 2_556 3
Ga4 O1 Ga3 97.2(10) 3_454 3
Ta O1 Ga3 143.3(14) . 3
Ga1 O1 Ga3 143.3(14) . 3
O4 O1 Ga3 129.8(12) 2 3
O5 O1 Ga3 20.8(5) 4_655 3
O7 O1 Ga3 59.6(9) 4_545 3
Ga1 O1 Ga3 36.2(5) 3 3
Ta O1 Ga3 36.2(5) 3 3
Ga1 O1 Ga3 100.6(11) 1_565 3
Ta O1 Ga3 100.6(11) 1_565 3
O6 O1 Ga3 86.5(11) 1_465 3
La1 O1 Ga3 76.0(7) 2_656 3
La2 O1 Ga3 95.9(6) 1_655 3
O6 O1 Ga3 101.0(10) . 3
La1 O1 Ga3 46.0(5) 3_654 3
O1 O1 Ga3 159.0(7) 2 3
Ga2 O1 Ga3 77.1(9) 4_645 3
Ga2 O1 Ga3 136.2(7) 2_655 3
Ga2 O1 Ga3 35.9(5) 4_655 3
O1 O1 Ga3 90.3(19) 4_545 3
O1 O1 Ga3 54.3(12) 4 3
O5 O1 Ga3 160.8(14) 2 3
O7 O1 Ga3 96.7(9) 2_655 3
O1 O1 Ga3 108.8(2) 1_455 3
O1 O1 Ga3 71.2(2) 1_655 3
Ga4 O1 Ga3 110.5(11) 3_544 3
Ga4 O1 Ga3 110.0(9) 4_655 3
Ga2 O1 O2 139(3) . 1_455
La1 O1 O2 107.3(9) 2_556 1_455
La2 O1 O2 74.2(11) . 1_455
La1 O1 O2 37.6(10) 3_554 1_455
O3 O1 O2 72.4(11) 1_455 1_455
O4 O1 O2 6.8(13) . 1_455
O2 O1 O2 49.6(14) 4_545 1_455
O7 O1 O2 68.6(13) . 1_455
O3 O1 O2 156(2) . 1_455
O5 O1 O2 139.8(11) . 1_455
O6 O1 O2 83.8(13) 4_655 1_455
O2 O1 O2 130(2) 4_645 1_455
Ga2 O1 O2 41.2(9) 1_455 1_455
O4 O1 O2 102.6(19) 1_655 1_455
O4 O1 O2 127.7(18) 4_545 1_455
Ga3 O1 O2 144.9(16) . 1_455
Ga4 O1 O2 115.2(14) 2_656 1_455
Ga4 O1 O2 79.0(12) 3_554 1_455
O2 O1 O2 58.4(11) . 1_455
O3 O1 O2 116.6(15) 2_655 1_455
O6 O1 O2 105.8(8) 1_455 1_455
O5 O1 O2 50.3(10) 4 1_455
O7 O1 O2 49.4(9) 2 1_455
O3 O1 O2 66.7(10) 4_655 1_455
Ga3 O1 O2 79.3(7) 1_455 1_455
O2 O1 O2 136.5(15) 1_545 1_455
Ga4 O1 O2 59.4(8) 2_556 1_455
Ga4 O1 O2 15.9(8) 3_454 1_455
Ta O1 O2 118.4(9) . 1_455
Ga1 O1 O2 118.4(9) . 1_455
O4 O1 O2 91.8(12) 2 1_455
O5 O1 O2 104.3(12) 4_655 1_455
O7 O1 O2 77.7(10) 4_545 1_455
Ga1 O1 O2 74.7(9) 3 1_455
Ta O1 O2 74.7(9) 3 1_455
Ga1 O1 O2 51.5(8) 1_565 1_455
Ta O1 O2 51.5(8) 1_565 1_455
O6 O1 O2 29.5(8) 1_465 1_455
La1 O1 O2 159.9(14) 2_656 1_455
La2 O1 O2 129.6(14) 1_655 1_455
O6 O1 O2 170.4(12) . 1_455
La1 O1 O2 112.1(13) 3_654 1_455
O1 O1 O2 82.2(8) 2 1_455
Ga2 O1 O2 136.0(12) 4_645 1_455
Ga2 O1 O2 111.1(13) 2_655 1_455
Ga2 O1 O2 69.8(10) 4_655 1_455
O1 O1 O2 102.5(11) 4_545 1_455
O1 O1 O2 32.1(9) 4 1_455
O5 O1 O2 98.7(9) 2 1_455
O7 O1 O2 102.4(12) 2_655 1_455
O1 O1 O2 41.3(8) 1_455 1_455
O1 O1 O2 138.7(8) 1_655 1_455
Ga4 O1 O2 149.9(10) 3_544 1_455
Ga4 O1 O2 87.4(11) 4_655 1_455
Ga3 O1 O2 84.3(10) 3 1_455
Ga2 O1 O1 52.5(13) . 2_655
La1 O1 O1 114.9(13) 2_556 2_655
La2 O1 O1 56.2(12) . 2_655
La1 O1 O1 134.4(12) 3_554 2_655
O3 O1 O1 97(2) 1_455 2_655
O4 O1 O1 124(2) . 2_655
O2 O1 O1 158(3) 4_545 2_655
O7 O1 O1 56.8(12) . 2_655
O3 O1 O1 35.4(10) . 2_655
O5 O1 O1 67.4(11) . 2_655
O6 O1 O1 140.5(13) 4_655 2_655
O2 O1 O1 83.3(13) 4_645 2_655
Ga2 O1 O1 125(2) 1_455 2_655
O4 O1 O1 66.7(13) 1_655 2_655
O4 O1 O1 109.7(12) 4_545 2_655
Ga3 O1 O1 36.3(10) . 2_655
Ga4 O1 O1 113.2(7) 2_656 2_655
Ga4 O1 O1 64.8(7) 3_554 2_655
O2 O1 O1 93.0(10) . 2_655
O3 O1 O1 30.2(10) 2_655 2_655
O6 O1 O1 97.0(12) 1_455 2_655
O5 O1 O1 167.6(10) 4 2_655
O7 O1 O1 74.8(13) 2 2_655
O3 O1 O1 122.4(7) 4_655 2_655
Ga3 O1 O1 90.6(14) 1_455 2_655
O2 O1 O1 92.7(9) 1_545 2_655
Ga4 O1 O1 162.8(13) 2_556 2_655
Ga4 O1 O1 107.6(13) 3_454 2_655
Ta O1 O1 72.3(9) . 2_655
Ga1 O1 O1 72.3(9) . 2_655
O4 O1 O1 31.3(9) 2 2_655
O5 O1 O1 104.7(8) 4_655 2_655
O7 O1 O1 159.3(8) 4_545 2_655
Ga1 O1 O1 154.7(12) 3 2_655
Ta O1 O1 154.7(12) 3 2_655
Ga1 O1 O1 72.6(9) 1_565 2_655
Ta O1 O1 72.6(9) 1_565 2_655
O6 O1 O1 96.6(11) 1_465 2_655
La1 O1 O1 66.8(3) 2_656 2_655
La2 O1 O1 26.0(3) 1_655 2_655
O6 O1 O1 61.4(5) . 2_655
La1 O1 O1 75.6(4) 3_654 2_655
O1 O1 O1 55.3(12) 2 2_655
Ga2 O1 O1 101.0(3) 4_645 2_655
Ga2 O1 O1 16.7(6) 2_655 2_655
Ga2 O1 O1 100.9(3) 4_655 2_655
O1 O1 O1 124.9(10) 4_545 2_655
O1 O1 O1 124.9(10) 4 2_655
O5 O1 O1 72.7(12) 2 2_655
O7 O1 O1 33.0(7) 2_655 2_655
O1 O1 O1 125.7(9) 1_455 2_655
O1 O1 O1 54.3(9) 1_655 2_655
Ga4 O1 O1 72.8(5) 3_544 2_655
Ga4 O1 O1 37.5(7) 4_655 2_655
Ga3 O1 O1 121.6(7) 3 2_655
O2 O1 O1 122.6(13) 1_455 2_655
Ga2 O1 O3 139(3) . 2
La1 O1 O3 74.5(11) 2_556 2
La2 O1 O3 40.0(6) . 2
La1 O1 O3 104.5(9) 3_554 2
O3 O1 O3 14.8(11) 1_455 2
O4 O1 O3 61.9(14) . 2
O2 O1 O3 70.3(18) 4_545 2
O7 O1 O3 82.2(13) . 2
O3 O1 O3 110.5(17) . 2
O5 O1 O3 74.4(11) . 2
O6 O1 O3 131.5(10) 4_655 2
O2 O1 O3 162(2) 4_645 2
Ga2 O1 O3 38.6(8) 1_455 2
O4 O1 O3 143(2) 1_655 2
O4 O1 O3 117.8(17) 4_545 2
Ga3 O1 O3 81.4(11) . 2
Ga4 O1 O3 146.4(14) 2_656 2
Ga4 O1 O3 114.1(14) 3_554 2
O2 O1 O3 115.7(16) . 2
O3 O1 O3 60.8(9) 2_655 2
O6 O1 O3 53.0(7) 1_455 2
O5 O1 O3 97.2(7) 4 2
O7 O1 O3 49.9(8) 2 2
O3 O1 O3 134.1(10) 4_655 2
Ga3 O1 O3 16.3(4) 1_455 2
O2 O1 O3 91.6(13) 1_545 2
Ga4 O1 O3 77.5(5) 2_556 2
Ga4 O1 O3 58.7(6) 3_454 2
Ta O1 O3 52.5(6) . 2
Ga1 O1 O3 52.5(6) . 2
O4 O1 O3 68.6(10) 2 2
O5 O1 O3 167.7(11) 4_655 2
O7 O1 O3 98.0(7) 4_545 2
Ga1 O1 O3 117.2(6) 3 2
Ta O1 O3 117.2(6) 3 2
Ga1 O1 O3 74.5(8) 1_565 2
Ta O1 O3 74.5(8) 1_565 2
O6 O1 O3 76.9(9) 1_465 2
La1 O1 O3 132.2(12) 2_656 2
La2 O1 O3 113.5(12) 1_655 2
O6 O1 O3 104.7(11) . 2
La1 O1 O3 160.0(14) 3_654 2
O1 O1 O3 34.0(4) 2 2
Ga2 O1 O3 112.1(11) 4_645 2
Ga2 O1 O3 71.3(8) 2_655 2
Ga2 O1 O3 134.1(11) 4_655 2
O1 O1 O3 81.4(10) 4_545 2
O1 O1 O3 99.9(11) 4 2
O5 O1 O3 31.0(6) 2 2
O7 O1 O3 104.0(13) 2_655 2
O1 O1 O3 39.5(6) 1_455 2
O1 O1 O3 140.5(6) 1_655 2
Ga4 O1 O3 89.0(9) 3_544 2
Ga4 O1 O3 84.8(9) 4_655 2
Ga3 O1 O3 148.1(8) 3 2
O2 O1 O3 67.8(8) 1_455 2
O1 O1 O3 87.6(13) 2_655 2
Ga2 O1 Ga2 128(3) . 4_545
La1 O1 Ga2 20.6(4) 2_556 4_545
La2 O1 Ga2 108.6(11) . 4_545
La1 O1 Ga2 92.4(12) 3_554 4_545
O3 O1 Ga2 54.4(11) 1_455 4_545
O4 O1 Ga2 81.8(12) . 4_545
O2 O1 Ga2 39.5(17) 4_545 4_545
O7 O1 Ga2 147.9(11) . 4_545
O3 O1 Ga2 115.2(16) . 4_545
O5 O1 Ga2 66.5(10) . 4_545
O6 O1 Ga2 71.1(11) 4_655 4_545
O2 O1 Ga2 107(2) 4_645 4_545
Ga2 O1 Ga2 53.8(8) 1_455 4_545
O4 O1 Ga2 148(2) 1_655 4_545
O4 O1 Ga2 55.2(13) 4_545 4_545
Ga3 O1 Ga2 97.6(12) . 4_545
Ga4 O1 Ga2 77.7(11) 2_656 4_545
Ga4 O1 Ga2 162.6(14) 3_554 4_545
O2 O1 Ga2 134.3(14) . 4_545
O3 O1 Ga2 105.6(12) 2_655 4_545
O6 O1 Ga2 35.8(6) 1_455 4_545
O5 O1 Ga2 59.9(8) 4 4_545
O7 O1 Ga2 112.9(7) 2 4_545
O3 O1 Ga2 102.7(11) 4_655 4_545
Ga3 O1 Ga2 56.4(5) 1_455 4_545
O2 O1 Ga2 49.4(9) 1_545 4_545
Ga4 O1 Ga2 33.4(4) 2_556 4_545
Ga4 O1 Ga2 95.0(4) 3_454 4_545
Ta O1 Ga2 60.4(6) . 4_545
Ga1 O1 Ga2 60.4(6) . 4_545
O4 O1 Ga2 134.5(13) 2 4_545
O5 O1 Ga2 101.9(13) 4_655 4_545
O7 O1 Ga2 36.5(5) 4_545 4_545
Ga1 O1 Ga2 60.5(6) 3 4_545
Ta O1 Ga2 60.5(6) 3 4_545
Ga1 O1 Ga2 132.9(5) 1_565 4_545
Ta O1 Ga2 132.9(5) 1_565 4_545
O6 O1 Ga2 116.2(6) 1_465 4_545
La1 O1 Ga2 98.6(11) 2_656 4_545
La2 O1 Ga2 142.5(12) 1_655 4_545
O6 O1 Ga2 84.5(10) . 4_545
La1 O1 Ga2 130.7(13) 3_654 4_545
O1 O1 Ga2 100.0(5) 2 4_545
Ga2 O1 Ga2 56.1(6) 4_645 4_545
Ga2 O1 Ga2 125.0(12) 2_655 4_545
Ga2 O1 Ga2 125.4(12) 4_655 4_545
O1 O1 Ga2 16.8(4) 4_545 4_545
O1 O1 Ga2 100.4(11) 4 4_545
O5 O1 Ga2 66.0(7) 2 4_545
O7 O1 Ga2 165.4(14) 2_655 4_545
O1 O1 Ga2 53.1(5) 1_455 4_545
O1 O1 Ga2 126.9(5) 1_655 4_545
Ga4 O1 Ga2 66.1(7) 3_544 4_545
Ga4 O1 Ga2 153.3(11) 4_655 4_545
Ga3 O1 Ga2 95.4(10) 3 4_545
O2 O1 Ga2 87.0(8) 1_455 4_545
O1 O1 Ga2 132.3(8) 2_655 4_545
O3 O1 Ga2 69.0(5) 2 4_545
Ga2 O1 O1 55(2) . 4_645
La1 O1 O1 57.0(7) 2_556 4_645
La2 O1 O1 135.1(19) . 4_645
La1 O1 O1 117(3) 3_554 4_645
O3 O1 O1 112.3(13) 1_455 4_645
O4 O1 O1 148(2) . 4_645
O2 O1 O1 103(2) 4_545 4_645
O7 O1 O1 137.4(11) . 4_645
O3 O1 O1 53.5(10) . 4_645
O5 O1 O1 52.8(7) . 4_645
O6 O1 O1 66.8(17) 4_655 4_645
O2 O1 O1 40.9(19) 4_645 4_645
Ga2 O1 O1 127.1(14) 1_455 4_645
O4 O1 O1 83.8(15) 1_655 4_645
O4 O1 O1 21.8(11) 4_545 4_645
Ga3 O1 O1 64.0(6) . 4_645
Ga4 O1 O1 37.5(11) 2_656 4_645
Ga4 O1 O1 114.3(9) 3_554 4_645
O2 O1 O1 120.5(17) . 4_645
O3 O1 O1 92.7(11) 2_655 4_645
O6 O1 O1 72.1(6) 1_455 4_645
O5 O1 O1 98.1(18) 4 4_645
O7 O1 O1 161.8(19) 2 4_645
O3 O1 O1 93.4(16) 4_655 4_645
Ga3 O1 O1 107.9(8) 1_455 4_645
O2 O1 O1 32.7(8) 1_545 4_645
Ga4 O1 O1 92.7(14) 2_556 4_645
Ga4 O1 O1 163.9(18) 3_454 4_645
Ta O1 O1 73.1(5) . 4_645
Ga1 O1 O1 73.1(5) . 4_645
O4 O1 O1 119.6(13) 2 4_645
O5 O1 O1 58.0(13) 4_655 4_645
O7 O1 O1 71.8(13) 4_545 4_645
Ga1 O1 O1 74.2(15) 3 4_645
Ta O1 O1 74.2(15) 3 4_645
Ga1 O1 O1 153.8(6) 1_565 4_645
Ta O1 O1 153.8(6) 1_565 4_645
O6 O1 O1 159.0(16) 1_465 4_645
La1 O1 O1 25.9(5) 2_656 4_645
La2 O1 O1 75.9(7) 1_655 4_645
O6 O1 O1 30.9(5) . 4_645
La1 O1 O1 67.4(10) 3_654 4_645
O1 O1 O1 124.6(14) 2 4_645
Ga2 O1 O1 17.2(3) 4_645 4_645
Ga2 O1 O1 100.4(11) 2_655 4_645
Ga2 O1 O1 101.6(14) 4_655 4_645
O1 O1 O1 56.5(7) 4_545 4_645
O1 O1 O1 127(3) 4 4_645
O5 O1 O1 95.5(8) 2 4_645
O7 O1 O1 102.3(8) 2_655 4_645
O1 O1 O1 126.4(4) 1_455 4_645
O1 O1 O1 53.6(4) 1_655 4_645
Ga4 O1 O1 37.2(4) 3_544 4_645
Ga4 O1 O1 120.9(8) 4_655 4_645
Ga3 O1 O1 73.6(14) 3 4_645
O2 O1 O1 148.5(18) 1_455 4_645
O1 O1 O1 88.4(6) 2_655 4_645
O3 O1 O1 123.8(9) 2 4_645
Ga2 O1 O1 73.3(7) 4_545 4_645
Ga2 O1 O1 54.1(19) . 4_655
La1 O1 O1 136(2) 2_556 4_655
La2 O1 O1 113.7(16) . 4_655
La1 O1 O1 57.3(9) 3_554 4_655
O3 O1 O1 157.7(14) 1_455 4_655
O4 O1 O1 93.4(15) . 4_655
O2 O1 O1 110(2) 4_545 4_655
O7 O1 O1 67.9(10) . 4_655
O3 O1 O1 84.0(11) . 4_655
O5 O1 O1 133.6(8) . 4_655
O6 O1 O1 62.4(16) 4_655 4_655
O2 O1 O1 48.8(18) 4_645 4_655
Ga2 O1 O1 126.6(12) 1_455 4_655
O4 O1 O1 22.3(13) 1_655 4_655
O4 O1 O1 95(2) 4_545 4_655
Ga3 O1 O1 113.3(9) . 4_655
Ga4 O1 O1 63.8(14) 2_656 4_655
Ga4 O1 O1 36.2(2) 3_554 4_655
O2 O1 O1 31.3(10) . 4_655
O3 O1 O1 118.3(14) 2_655 4_655
O6 O1 O1 160.5(17) 1_455 4_655
O5 O1 O1 81.2(14) 4 4_655
O7 O1 O1 97.0(9) 2 4_655
O3 O1 O1 34.1(8) 4_655 4_655
Ga3 O1 O1 162.6(12) 1_455 4_655
O2 O1 O1 121.9(15) 1_545 4_655
Ga4 O1 O1 108.7(16) 2_556 4_655
Ga4 O1 O1 91.0(6) 3_454 4_655
Ta O1 O1 153.9(6) . 4_655
Ga1 O1 O1 153.9(6) . 4_655
O4 O1 O1 91.8(11) 2 4_655
O5 O1 O1 36.6(11) 4_655 4_655
O7 O1 O1 97.3(17) 4_545 4_655
Ga1 O1 O1 73.4(14) 3 4_655
Ta O1 O1 73.4(14) 3 4_655
Ga1 O1 O1 72.5(6) 1_565 4_655
Ta O1 O1 72.5(6) 1_565 4_655
O6 O1 O1 70.4(5) 1_465 4_655
La1 O1 O1 75.5(8) 2_656 4_655
La2 O1 O1 66.1(7) 1_655 4_655
O6 O1 O1 102.5(8) . 4_655
La1 O1 O1 25.6(7) 3_654 4_655
O1 O1 O1 124.6(14) 2 4_655
Ga2 O1 O1 101.4(13) 4_645 4_655
Ga2 O1 O1 100.1(11) 2_655 4_655
Ga2 O1 O1 17.3(3) 4_655 4_655
O1 O1 O1 127(3) 4_545 4_655
O1 O1 O1 56.5(7) 4 4_655
O5 O1 O1 160.4(18) 2 4_655
O7 O1 O1 59.2(8) 2_655 4_655
O1 O1 O1 126.4(4) 1_455 4_655
O1 O1 O1 53.6(4) 1_655 4_655
Ga4 O1 O1 121.5(7) 3_544 4_655
Ga4 O1 O1 72.2(8) 4_655 4_655
Ga3 O1 O1 38.1(10) 3 4_655
O2 O1 O1 86.6(8) 1_455 4_655
O1 O1 O1 88.4(6) 2_655 4_655
O3 O1 O1 146.4(11) 2 4_655
Ga2 O1 O1 133.5(18) 4_545 4_655
O1 O1 O1 89.4(13) 4_645 4_655
Ga2 O1 Ga2 125(2) . 2
La1 O1 Ga2 91.5(13) 2_556 2
La2 O1 Ga2 20.9(5) . 2
La1 O1 Ga2 106.9(13) 3_554 2
O3 O1 Ga2 33.5(11) 1_455 2
O4 O1 Ga2 65.1(14) . 2
O2 O1 Ga2 86.1(17) 4_545 2
O7 O1 Ga2 64.6(13) . 2
O3 O1 Ga2 101.1(16) . 2
O5 O1 Ga2 79.3(12) . 2
O6 O1 Ga2 146.9(9) 4_655 2
O2 O1 Ga2 155.3(19) 4_645 2
Ga2 O1 Ga2 52.4(9) 1_455 2
O4 O1 Ga2 123.8(19) 1_655 2
O4 O1 Ga2 133.0(18) 4_545 2
Ga3 O1 Ga2 75.9(11) . 2
Ga4 O1 Ga2 164.3(15) 2_656 2
Ga4 O1 Ga2 96.8(13) 3_554 2
O2 O1 Ga2 104.3(16) . 2
O3 O1 Ga2 49.9(9) 2_655 2
O6 O1 Ga2 67.6(8) 1_455 2
O5 O1 Ga2 109.9(7) 4 2
O7 O1 Ga2 35.9(7) 2 2
O3 O1 Ga2 134.1(11) 4_655 2
Ga3 O1 Ga2 32.7(4) 1_455 2
O2 O1 Ga2 103.2(14) 1_545 2
Ga4 O1 Ga2 94.5(5) 2_556 2
Ga4 O1 Ga2 56.3(6) 3_454 2
Ta O1 Ga2 59.5(7) . 2
Ga1 O1 Ga2 59.5(7) . 2
O4 O1 Ga2 49.9(9) 2 2
O5 O1 Ga2 168.3(15) 4_655 2
O7 O1 Ga2 116.3(6) 4_545 2
Ga1 O1 Ga2 133.0(4) 3 2
Ta O1 Ga2 133.0(4) 3 2
Ga1 O1 Ga2 59.7(7) 1_565 2
Ta O1 Ga2 59.7(7) 1_565 2
O6 O1 Ga2 68.6(9) 1_465 2
La1 O1 Ga2 129.7(11) 2_656 2
La2 O1 Ga2 97.4(11) 1_655 2
O6 O1 Ga2 105.6(11) . 2
La1 O1 Ga2 141.0(13) 3_654 2
O1 O1 Ga2 17.0(2) 2 2
Ga2 O1 Ga2 125.1(12) 4_645 2
Ga2 O1 Ga2 55.6(7) 2_655 2
Ga2 O1 Ga2 124.6(12) 4_655 2
O1 O1 Ga2 99.4(12) 4_545 2
O1 O1 Ga2 99.2(13) 4 2
O5 O1 Ga2 37.3(6) 2 2
O7 O1 Ga2 85.1(12) 2_655 2
O1 O1 Ga2 53.4(4) 1_455 2
O1 O1 Ga2 126.6(4) 1_655 2
Ga4 O1 Ga2 94.9(10) 3_544 2
Ga4 O1 Ga2 65.8(8) 4_655 2
Ga3 O1 Ga2 153.4(10) 3 2
O2 O1 Ga2 69.5(8) 1_455 2
O1 O1 Ga2 72.3(12) 2_655 2
O3 O1 Ga2 19.0(3) 2 2
Ga2 O1 Ga2 87.9(6) 4_545 2
O1 O1 Ga2 132.1(12) 4_645 2
O1 O1 Ga2 131.8(13) 4_655 2
Ga2 O1 Ga2 127(2) . 4
La1 O1 Ga2 108.4(10) 2_556 4
La2 O1 Ga2 90.9(12) . 4
La1 O1 Ga2 19.6(6) 3_554 4
O3 O1 Ga2 87.6(9) 1_455 4
O4 O1 Ga2 23.3(13) . 4
O2 O1 Ga2 48.5(17) 4_545 4
O7 O1 Ga2 75.3(12) . 4
O3 O1 Ga2 155.3(15) . 4
O5 O1 Ga2 151.5(9) . 4
O6 O1 Ga2 67.0(11) 4_655 4
O2 O1 Ga2 112(2) 4_645 4
Ga2 O1 Ga2 53.5(7) 1_455 4
O4 O1 Ga2 92.4(18) 1_655 4
O4 O1 Ga2 115.5(18) 4_545 4
Ga3 O1 Ga2 162.4(16) . 4
Ga4 O1 Ga2 97.8(12) 2_656 4
Ga4 O1 Ga2 75.5(10) 3_554 4
O2 O1 Ga2 49.7(10) . 4
O3 O1 Ga2 133.6(14) 2_655 4
O6 O1 Ga2 115.1(6) 1_455 4
O5 O1 Ga2 37.8(6) 4 4
O7 O1 Ga2 64.6(8) 2 4
O3 O1 Ga2 49.0(7) 4_655 4
Ga3 O1 Ga2 94.9(4) 1_455 4
O2 O1 Ga2 134.6(13) 1_545 4
Ga4 O1 Ga2 55.7(5) 2_556 4
Ga4 O1 Ga2 32.6(4) 3_454 4
Ta O1 Ga2 132.9(5) . 4
Ga1 O1 Ga2 132.9(5) . 4
O4 O1 Ga2 104.0(12) 2 4
O5 O1 Ga2 86.4(10) 4_655 4
O7 O1 Ga2 68.4(7) 4_545 4
Ga1 O1 Ga2 59.7(6) 3 4
Ta O1 Ga2 59.7(6) 3 4
Ga1 O1 Ga2 59.8(6) 1_565 4
Ta O1 Ga2 59.8(6) 1_565 4
O6 O1 Ga2 35.8(5) 1_465 4
La1 O1 Ga2 142.1(12) 2_656 4
La2 O1 Ga2 129.1(12) 1_655 4
O6 O1 Ga2 164.4(15) . 4
La1 O1 Ga2 98.0(10) 3_654 4
O1 O1 Ga2 99.9(5) 2 4
Ga2 O1 Ga2 125.5(12) 4_645 4
Ga2 O1 Ga2 124.6(12) 2_655 4
Ga2 O1 Ga2 55.8(6) 4_655 4
O1 O1 Ga2 100.6(12) 4_545 4
O1 O1 Ga2 16.7(5) 4 4
O5 O1 Ga2 115.4(7) 2 4
O7 O1 Ga2 104.4(11) 2_655 4
O1 O1 Ga2 53.2(4) 1_455 4
O1 O1 Ga2 126.8(4) 1_655 4
Ga4 O1 Ga2 153.8(11) 3_544 4
Ga4 O1 Ga2 94.7(10) 4_655 4
Ga3 O1 Ga2 66.2(7) 3 4
O2 O1 Ga2 18.1(7) 1_455 4
O1 O1 Ga2 132.1(9) 2_655 4
O3 O1 Ga2 85.1(5) 2 4
Ga2 O1 Ga2 88.0(5) 4_545 4
O1 O1 Ga2 133.6(18) 4_645 4
O1 O1 Ga2 73.1(6) 4_655 4
Ga2 O1 Ga2 87.6(6) 2 4
Ga2 O1 La1 97(2) . 1_554
La1 O1 La1 82.3(15) 2_556 1_554
La2 O1 La1 36.3(9) . 1_554
La1 O1 La1 141.6(17) 3_554 1_554
O3 O1 La1 48.4(12) 1_455 1_554
O4 O1 La1 100.1(17) . 1_554
O2 O1 La1 110(2) 4_545 1_554
O7 O1 La1 76.1(14) . 1_554
O3 O1 La1 68.3(13) . 1_554
O5 O1 La1 49.5(11) . 1_554
O6 O1 La1 160.0(18) 4_655 1_554
O2 O1 La1 122.8(17) 4_645 1_554
Ga2 O1 La1 80.9(11) 1_455 1_554
O4 O1 La1 115.0(18) 1_655 1_554
O4 O1 La1 110.1(18) 4_545 1_554
Ga3 O1 La1 41.0(7) . 1_554
Ga4 O1 La1 137.7(13) 2_656 1_554
Ga4 O1 La1 102.6(13) 3_554 1_554
O2 O1 La1 124.1(17) . 1_554
O3 O1 La1 19.1(6) 2_655 1_554
O6 O1 La1 57.1(8) 1_455 1_554
O5 O1 La1 138.8(9) 4 1_554
O7 O1 La1 63.4(10) 2 1_554
O3 O1 La1 163.0(14) 4_655 1_554
Ga3 O1 La1 41.9(5) 1_455 1_554
O2 O1 La1 78.9(13) 1_545 1_554
Ga4 O1 La1 114.3(8) 2_556 1_554
Ga4 O1 La1 90.7(9) 3_454 1_554
Ta O1 La1 36.4(5) . 1_554
Ga1 O1 La1 36.4(5) . 1_554
O4 O1 La1 45.5(8) 2 1_554
O5 O1 La1 148.9(7) 4_655 1_554
O7 O1 La1 127.3(10) 4_545 1_554
Ga1 O1 La1 151.3(10) 3 1_554
Ta O1 La1 151.3(10) 3 1_554
Ga1 O1 La1 81.0(10) 1_565 1_554
Ta O1 La1 81.0(10) 1_565 1_554
O6 O1 La1 98.4(12) 1_465 1_554
La1 O1 La1 94.7(8) 2_656 1_554
La2 O1 La1 74.1(8) 1_655 1_554
O6 O1 La1 71.2(8) . 1_554
La1 O1 La1 123.9(8) 3_654 1_554
O1 O1 La1 24.5(6) 2 1_554
Ga2 O1 La1 99.7(10) 4_645 1_554
Ga2 O1 La1 35.2(4) 2_655 1_554
Ga2 O1 La1 141.7(13) 4_655 1_554
O1 O1 La1 93.4(12) 4_545 1_554
O1 O1 La1 132.7(17) 4 1_554
O5 O1 La1 25.2(5) 2 1_554
O7 O1 La1 76.0(10) 2_655 1_554
O1 O1 La1 81.71(18) 1_455 1_554
O1 O1 La1 98.29(18) 1_655 1_554
Ga4 O1 La1 64.5(7) 3_544 1_554
Ga4 O1 La1 65.3(7) 4_655 1_554
Ga3 O1 La1 169.5(4) 3 1_554
O2 O1 La1 104.5(10) 1_455 1_554
O1 O1 La1 48.8(9) 2_655 1_554
O3 O1 La1 42.4(5) 2 1_554
Ga2 O1 La1 90.9(8) 4_545 1_554
O1 O1 La1 100.3(10) 4_645 1_554
O1 O1 La1 135.2(14) 4_655 1_554
Ga2 O1 La1 35.0(4) 2 1_554
Ga2 O1 La1 122.6(8) 4 1_554
Ga2 O1 La2 100(2) . 3_545
La1 O1 La2 36.5(11) 2_556 3_545
La2 O1 La2 144.0(13) . 3_545
La1 O1 La2 83.4(15) 3_554 3_545
O3 O1 La2 89.9(14) 1_455 3_545
O4 O1 La2 98.2(15) . 3_545
O2 O1 La2 53.6(18) 4_545 3_545
O7 O1 La2 164.2(18) . 3_545
O3 O1 La2 103.1(15) . 3_545
O5 O1 La2 75.9(13) . 3_545
O6 O1 La2 41.5(10) 4_655 3_545
O2 O1 La2 72.7(18) 4_645 3_545
Ga2 O1 La2 82.6(11) 1_455 3_545
O4 O1 La2 112.9(18) 1_655 3_545
O4 O1 La2 28.2(12) 4_545 3_545
Ga3 O1 La2 103.5(13) . 3_545
Ga4 O1 La2 42.3(7) 2_656 3_545
Ga4 O1 La2 137.3(15) 3_554 3_545
O2 O1 La2 116.9(17) . 3_545
O3 O1 La2 125.8(14) 2_655 3_545
O6 O1 La2 62.3(9) 1_455 3_545
O5 O1 La2 53.1(9) 4 3_545
O7 O1 La2 143.5(7) 2 3_545
O3 O1 La2 78.0(9) 4_655 3_545
Ga3 O1 La2 91.3(8) 1_455 3_545
O2 O1 La2 46.3(10) 1_545 3_545
Ga4 O1 La2 42.8(6) 2_556 3_545
Ga4 O1 La2 114.3(7) 3_454 3_545
Ta O1 La2 82.4(9) . 3_545
Ga1 O1 La2 82.4(9) . 3_545
O4 O1 La2 162.7(14) 2 3_545
O5 O1 La2 66.8(10) 4_655 3_545
O7 O1 La2 22.7(5) 4_545 3_545
Ga1 O1 La2 37.1(5) 3 3_545
Ta O1 La2 37.1(5) 3 3_545
Ga1 O1 La2 150.6(10) 1_565 3_545
Ta O1 La2 150.6(10) 1_565 3_545
O6 O1 La2 126.6(10) 1_465 3_545
La1 O1 La2 74.9(9) 2_656 3_545
La2 O1 La2 125.2(9) 1_655 3_545
O6 O1 La2 75.2(9) . 3_545
La1 O1 La2 95.3(10) 3_654 3_545
O1 O1 La2 134.1(5) 2 3_545
Ga2 O1 La2 35.8(5) 4_645 3_545
Ga2 O1 La2 142.8(12) 2_655 3_545
Ga2 O1 La2 99.6(11) 4_655 3_545
O1 O1 La2 26.0(11) 4_545 3_545
O1 O1 La2 94.4(16) 4 3_545
O5 O1 La2 96.5(10) 2 3_545
O7 O1 La2 148.7(9) 2_655 3_545
O1 O1 La2 81.7(2) 1_455 3_545
O1 O1 La2 98.3(2) 1_655 3_545
Ga4 O1 La2 66.0(8) 3_544 3_545
Ga4 O1 La2 169.7(6) 4_655 3_545
Ga3 O1 La2 64.4(7) 3 3_545
O2 O1 La2 100.3(10) 1_455 3_545
O1 O1 La2 136.6(5) 2_655 3_545
O3 O1 La2 104.5(7) 2 3_545
Ga2 O1 La2 35.5(4) 4_545 3_545
O1 O1 La2 50.0(9) 4_645 3_545
O1 O1 La2 101.2(16) 4_655 3_545
Ga2 O1 La2 123.3(7) 2 3_545
Ga2 O1 La2 90.8(7) 4 3_545
La1 O1 La2 118.5(10) 1_554 3_545
Ga2 O1 La1 98(2) . 2_566
La1 O1 La1 143.6(13) 2_556 2_566
La2 O1 La1 81.2(14) . 2_566
La1 O1 La1 35.1(10) 3_554 2_566
O3 O1 La1 108.6(13) 1_455 2_566
O4 O1 La1 47.4(13) . 2_566
O2 O1 La1 83.9(19) 4_545 2_566
O7 O1 La1 46.2(11) . 2_566
O3 O1 La1 120.6(13) . 2_566
O5 O1 La1 165.8(19) . 2_566
O6 O1 La1 81.0(13) 4_655 2_566
O2 O1 La1 97.7(19) 4_645 2_566
Ga2 O1 La1 81.7(10) 1_455 2_566
O4 O1 La1 62.1(15) 1_655 2_566
O4 O1 La1 133(2) 4_545 2_566
Ga3 O1 La1 136.5(14) . 2_566
Ga4 O1 La1 102.6(13) 2_656 2_566
Ga4 O1 La1 40.2(6) 3_554 2_566
O2 O1 La1 18.3(10) . 2_566
O3 O1 La1 115.7(14) 2_655 2_566
O6 O1 La1 146.3(7) 1_455 2_566
O5 O1 La1 67.8(9) 4 2_566
O7 O1 La1 55.4(8) 2 2_566
O3 O1 La1 46.4(7) 4_655 2_566
Ga3 O1 La1 114.2(9) 1_455 2_566
O2 O1 La1 163.5(17) 1_545 2_566
Ga4 O1 La1 90.6(8) 2_556 2_566
Ga4 O1 La1 41.9(5) 3_454 2_566
Ta O1 La1 149.9(12) . 2_566
Ga1 O1 La1 149.9(12) . 2_566
O4 O1 La1 79.0(10) 2 2_566
O5 O1 La1 78.9(9) 4_655 2_566
O7 O1 La1 98.5(10) 4_545 2_566
Ga1 O1 La1 81.3(8) 3 2_566
Ta O1 La1 81.3(8) 3 2_566
Ga1 O1 La1 36.5(4) 1_565 2_566
Ta O1 La1 36.5(4) 1_565 2_566
O6 O1 La1 22.2(5) 1_465 2_566
La1 O1 La1 124.1(8) 2_656 2_566
La2 O1 La1 93.8(9) 1_655 2_566
O6 O1 La1 148.9(7) . 2_566
La1 O1 La1 73.9(8) 3_654 2_566
O1 O1 La1 93.6(6) 2 2_566
Ga2 O1 La1 142.8(13) 4_645 2_566
Ga2 O1 La1 98.8(11) 2_655 2_566
Ga2 O1 La1 35.3(4) 4_655 2_566
O1 O1 La1 134.8(14) 4_545 2_566
O1 O1 La1 24.7(5) 4 2_566
O5 O1 La1 127.6(11) 2 2_566
O7 O1 La1 69.5(8) 2_655 2_566
O1 O1 La1 81.9(2) 1_455 2_566
O1 O1 La1 98.1(2) 1_655 2_566
Ga4 O1 La1 169.4(5) 3_544 2_566
Ga4 O1 La1 63.9(7) 4_655 2_566
Ga3 O1 La1 65.8(7) 3 2_566
O2 O1 La1 40.7(8) 1_455 2_566
O1 O1 La1 100.2(5) 2_655 2_566
O3 O1 La1 98.9(8) 2 2_566
Ga2 O1 La1 123.4(7) 4_545 2_566
O1 O1 La1 136.8(13) 4_645 2_566
O1 O1 La1 49.16(11) 4_655 2_566
Ga2 O1 La1 90.4(8) 2 2_566
Ga2 O1 La1 35.4(4) 4 2_566
La1 O1 La1 117.3(11) 1_554 2_566
La2 O1 La1 118.1(10) 3_545 2_566
Ga2 O1 O3 85(2) . 4_645
La1 O1 O3 30.6(10) 2_556 4_645
La2 O1 O3 136.7(18) . 4_645
La1 O1 O3 105.9(18) 3_554 4_645
O3 O1 O3 90.7(16) 1_455 4_645
O4 O1 O3 119.7(16) . 4_645
O2 O1 O3 74.0(19) 4_545 4_645
O7 O1 O3 168.0(10) . 4_645
O3 O1 O3 81.0(14) . 4_645
O5 O1 O3 54.9(12) . 4_645
O6 O1 O3 58.4(12) 4_655 4_645
O2 O1 O3 65.2(17) 4_645 4_645
Ga2 O1 O3 96.8(12) 1_455 4_645
O4 O1 O3 109.9(16) 1_655 4_645
O4 O1 O3 13.0(11) 4_545 4_645
Ga3 O1 O3 80.2(11) . 4_645
Ga4 O1 O3 43.5(8) 2_656 4_645
Ga4 O1 O3 140.5(11) 3_554 4_645
O2 O1 O3 132.3(17) . 4_645
O3 O1 O3 104.8(13) 2_655 4_645
O6 O1 O3 53.4(9) 1_455 4_645
O5 O1 O3 76.6(11) 4 4_645
O7 O1 O3 154.5(10) 2 4_645
O3 O1 O3 94.4(11) 4_655 4_645
Ga3 O1 O3 89.1(10) 1_455 4_645
O2 O1 O3 24.4(10) 1_545 4_645
Ga4 O1 O3 63.7(8) 2_556 4_645
Ga4 O1 O3 135.3(8) 3_454 4_645
Ta O1 O3 66.8(8) . 4_645
Ga1 O1 O3 66.8(8) . 4_645
O4 O1 O3 140.6(12) 2 4_645
O5 O1 O3 70.7(10) 4_655 4_645
O7 O1 O3 46.1(7) 4_545 4_645
Ga1 O1 O3 58.4(8) 3 4_645
Ta O1 O3 58.4(8) 3 4_645
Ga1 O1 O3 174.2(10) 1_565 4_645
Ta O1 O3 174.2(10) 1_565 4_645
O6 O1 O3 150.2(12) 1_465 4_645
La1 O1 O3 56.5(7) 2_656 4_645
La2 O1 O3 105.9(8) 1_655 4_645
O6 O1 O3 51.8(7) . 4_645
La1 O1 O3 91.8(9) 3_654 4_645
O1 O1 O3 124.3(6) 2 4_645
Ga2 O1 O3 13.8(4) 4_645 4_645
Ga2 O1 O3 119.9(11) 2_655 4_645
Ga2 O1 O3 112.2(12) 4_655 4_645
O1 O1 O3 26.6(7) 4_545 4_645
O1 O1 O3 117.0(18) 4 4_645
O5 O1 O3 85.9(10) 2 4_645
O7 O1 O3 132.8(8) 2_655 4_645
O1 O1 O3 96.0(4) 1_455 4_645
O1 O1 O3 84.0(4) 1_655 4_645
Ga4 O1 O3 43.1(6) 3_544 4_645
Ga4 O1 O3 149.7(8) 4_655 4_645
Ga3 O1 O3 76.7(9) 3 4_645
O2 O1 O3 122.8(10) 1_455 4_645
O1 O1 O3 113.2(4) 2_655 4_645
O3 O1 O3 105.0(9) 2 4_645
Ga2 O1 O3 43.2(6) 4_545 4_645
O1 O1 O3 30.7(5) 4_645 4_645
O1 O1 O3 107.2(14) 4_655 4_645
Ga2 O1 O3 121.0(10) 2 4_645
Ga2 O1 O3 114.4(10) 4 4_645
La1 O1 O3 102.5(10) 1_554 4_645
La2 O1 O3 23.6(4) 3_545 4_645
La1 O1 O3 139.2(12) 2_566 4_645
Ga2 O1 O2 137(3) . 1_445
La1 O1 O2 26.9(8) 2_556 1_445
La2 O1 O2 91.4(13) . 1_445
La1 O1 O2 99.9(10) 3_554 1_445
O3 O1 O2 37.3(12) 1_455 1_445
O4 O1 O2 77.5(14) . 1_445
O2 O1 O2 44.1(17) 4_545 1_445
O7 O1 O2 133.2(15) . 1_445
O3 O1 O2 114.5(16) . 1_445
O5 O1 O2 61.7(10) . 1_445
O6 O1 O2 87.8(13) 4_655 1_445
O2 O1 O2 121(2) 4_645 1_445
Ga2 O1 O2 44.7(10) 1_455 1_445
O4 O1 O2 165(2) 1_655 1_445
O4 O1 O2 69.0(16) 4_545 1_445
Ga3 O1 O2 90.4(13) . 1_445
Ga4 O1 O2 94.5(13) 2_656 1_445
Ga4 O1 O2 161.6(13) 3_554 1_445
O2 O1 O2 139.9(15) . 1_445
O3 O1 O2 91.7(12) 2_655 1_445
O6 O1 O2 25.8(7) 1_455 1_445
O5 O1 O2 70.4(10) 4 1_445
O7 O1 O2 98.5(11) 2 1_445
O3 O1 O2 116.5(11) 4_655 1_445
Ga3 O1 O2 39.0(8) 1_455 1_445
O2 O1 O2 54.5(9) 1_545 1_445
Ga4 O1 O2 42.4(6) 2_556 1_445
Ga4 O1 O2 87.6(8) 3_454 1_445
Ta O1 O2 49.4(8) . 1_445
Ga1 O1 O2 49.4(8) . 1_445
O4 O1 O2 117.3(14) 2 1_445
O5 O1 O2 119.3(15) 4_655 1_445
O7 O1 O2 52.4(8) 4_545 1_445
Ga1 O1 O2 76.2(9) 3 1_445
Ta O1 O2 76.2(9) 3 1_445
Ga1 O1 O2 121.2(10) 1_565 1_445
Ta O1 O2 121.2(10) 1_565 1_445
O6 O1 O2 110.3(8) 1_465 1_445
La1 O1 O2 107.0(13) 2_656 1_445
La2 O1 O2 139.3(13) 1_655 1_445
O6 O1 O2 86.7(11) . 1_445
La1 O1 O2 147.2(15) 3_654 1_445
O1 O1 O2 82.6(8) 2 1_445
Ga2 O1 O2 67.4(10) 4_645 1_445
Ga2 O1 O2 110.3(12) 2_655 1_445
Ga2 O1 O2 138.0(11) 4_655 1_445
O1 O1 O2 30.1(9) 4_545 1_445
O1 O1 O2 105.3(10) 4 1_445
O5 O1 O2 50.1(8) 2 1_445
O7 O1 O2 151.3(15) 2_655 1_445
O1 O1 O2 44.3(8) 1_455 1_445
O1 O1 O2 135.7(8) 1_655 1_445
Ga4 O1 O2 66.4(9) 3_544 1_445
Ga4 O1 O2 135.9(13) 4_655 1_445
Ga3 O1 O2 111.9(11) 3 1_445
O2 O1 O2 83.9(8) 1_455 1_445
O1 O1 O2 120.9(12) 2_655 1_445
O3 O1 O2 52.0(7) 2 1_445
Ga2 O1 O2 17.4(7) 4_545 1_445
O1 O1 O2 83.9(8) 4_645 1_445
O1 O1 O2 149.5(18) 4_655 1_445
Ga2 O1 O2 70.7(9) 2 1_445
Ga2 O1 O2 90.2(7) 4 1_445
La1 O1 O2 75.3(9) 1_554 1_445
La2 O1 O2 52.6(8) 3_545 1_445
La1 O1 O2 124.1(8) 2_566 1_445
O3 O1 O2 56.2(10) 4_645 1_445
Ga2 O1 O3 135(2) . 4
La1 O1 O3 91.4(10) 2_556 4
La2 O1 O3 100.4(10) . 4
La1 O1 O3 25.5(5) 3_554 4
O3 O1 O3 81.6(8) 1_455 4
O4 O1 O3 28.4(13) . 4
O2 O1 O3 32.1(17) 4_545 4
O7 O1 O3 92.3(12) . 4
O3 O1 O3 165.9(16) . 4
O5 O1 O3 137.0(11) . 4
O6 O1 O3 58.1(10) 4_655 4
O2 O1 O3 112(2) 4_645 4
Ga2 O1 O3 46.5(8) 1_455 4
O4 O1 O3 104.2(19) 1_655 4
O4 O1 O3 100.9(16) 4_545 4
Ga3 O1 O3 163.7(11) . 4
Ga4 O1 O3 89.6(11) 2_656 4
Ga4 O1 O3 91.8(11) 3_554 4
O2 O1 O3 64.7(11) . 4
O3 O1 O3 141.3(13) 2_655 4
O6 O1 O3 101.2(7) 1_455 4
O5 O1 O3 23.0(6) 4 4
O7 O1 O3 76.7(8) 2 4
O3 O1 O3 52.4(6) 4_655 4
Ga3 O1 O3 89.1(4) 1_455 4
O2 O1 O3 117.3(13) 1_545 4
Ga4 O1 O3 38.5(4) 2_556 4
Ga4 O1 O3 43.1(5) 3_454 4
Ta O1 O3 122.7(6) . 4
Ga1 O1 O3 122.7(6) . 4
O4 O1 O3 118.8(11) 2 4
O5 O1 O3 85.7(10) 4_655 4
O7 O1 O3 51.9(7) 4_545 4
Ga1 O1 O3 47.6(5) 3 4
Ta O1 O3 47.6(5) 3 4
Ga1 O1 O3 76.2(7) 1_565 4
Ta O1 O3 76.2(7) 1_565 4
O6 O1 O3 52.2(6) 1_465 4
La1 O1 O3 137.9(13) 2_656 4
La2 O1 O3 145.0(12) 1_655 4
O6 O1 O3 149.8(13) . 4
La1 O1 O3 105.2(11) 3_654 4
O1 O1 O3 106.7(5) 2 4
Ga2 O1 O3 110.1(10) 4_645 4
Ga2 O1 O3 138.4(11) 2_655 4
Ga2 O1 O3 66.0(7) 4_655 4
O1 O1 O3 83.3(11) 4_545 4
O1 O1 O3 29.8(7) 4 4
O5 O1 O3 110.4(6) 2 4
O7 O1 O3 121.7(11) 2_655 4
O1 O1 O3 45.9(5) 1_455 4
O1 O1 O3 134.1(5) 1_655 4
Ga4 O1 O3 136.5(10) 3_544 4
Ga4 O1 O3 111.7(10) 4_655 4
Ga3 O1 O3 64.9(7) 3 4
O2 O1 O3 27.3(7) 1_455 4
O1 O1 O3 148.8(9) 2_655 4
O3 O1 O3 83.5(5) 2 4
Ga2 O1 O3 71.3(5) 4_545 4
O1 O1 O3 121.2(16) 4_645 4
O1 O1 O3 82.8(9) 4_655 4
Ga2 O1 O3 91.5(5) 2 4
Ga2 O1 O3 17.4(3) 4 4
La1 O1 O3 125.3(7) 1_554 4
La2 O1 O3 74.6(6) 3_545 4
La1 O1 O3 52.2(5) 2_566 4
O3 O1 O3 98.0(9) 4_645 4
O2 O1 O3 75.5(7) 1_445 4
Ga2 O1 O2 82(2) . 3_544
La1 O1 O2 106.3(18) 2_556 3_544
La2 O1 O2 29.4(9) . 3_544
La1 O1 O2 132(2) 3_554 3_544
O3 O1 O2 68.8(15) 1_455 3_544
O4 O1 O2 101.3(19) . 3_544
O2 O1 O2 128.4(19) 4_545 3_544
O7 O1 O2 54.3(14) . 3_544
O3 O1 O2 60.4(13) . 3_544
O5 O1 O2 66.3(14) . 3_544
O6 O1 O2 170.2(11) 4_655 3_544
O2 O1 O2 112.7(16) 4_645 3_544
Ga2 O1 O2 95.1(14) 1_455 3_544
O4 O1 O2 91.6(18) 1_655 3_544
O4 O1 O2 124.5(19) 4_545 3_544
Ga3 O1 O2 43.9(10) . 3_544
Ga4 O1 O2 140.4(10) 2_656 3_544
Ga4 O1 O2 77.8(13) 3_554 3_544
O2 O1 O2 101.6(18) . 3_544
O3 O1 O2 16.4(8) 2_655 3_544
O6 O1 O2 81.8(12) 1_455 3_544
O5 O1 O2 151.5(12) 4 3_544
O7 O1 O2 54.2(11) 2 3_544
O3 O1 O2 139.9(14) 4_655 3_544
Ga3 O1 O2 63.6(9) 1_455 3_544
O2 O1 O2 96.8(15) 1_545 3_544
Ga4 O1 O2 135.6(11) 2_556 3_544
Ga4 O1 O2 87.2(12) 3_454 3_544
Ta O1 O2 59.4(9) . 3_544
Ga1 O1 O2 59.4(9) . 3_544
O4 O1 O2 21.6(8) 2 3_544
O5 O1 O2 134.0(10) 4_655 3_544
O7 O1 O2 152.2(12) 4_545 3_544
Ga1 O1 O2 175.5(8) 3 3_544
Ta O1 O2 175.5(8) 3 3_544
Ga1 O1 O2 63.7(10) 1_565 3_544
Ta O1 O2 63.7(10) 1_565 3_544
O6 O1 O2 85.7(13) 1_465 3_544
La1 O1 O2 91.9(9) 2_656 3_544
La2 O1 O2 55.3(8) 1_655 3_544
O6 O1 O2 76.8(10) . 3_544
La1 O1 O2 103.8(9) 3_654 3_544
O1 O1 O2 25.8(8) 2 3_544
Ga2 O1 O2 113.8(12) 4_645 3_544
Ga2 O1 O2 13.1(6) 2_655 3_544
Ga2 O1 O2 117.3(13) 4_655 3_544
O1 O1 O2 117.6(16) 4_545 3_544
O1 O1 O2 121.3(17) 4 3_544
O5 O1 O2 49.9(9) 2 3_544
O7 O1 O2 51.5(10) 2_655 3_544
O1 O1 O2 96.1(6) 1_455 3_544
O1 O1 O2 83.9(6) 1_655 3_544
Ga4 O1 O2 78.5(10) 3_544 3_544
Ga4 O1 O2 40.9(8) 4_655 3_544
Ga3 O1 O2 148.1(10) 3 3_544
O2 O1 O2 103.1(14) 1_455 3_544
O1 O1 O2 29.6(9) 2_655 3_544
O3 O1 O2 58.3(9) 2 3_544
Ga2 O1 O2 115.8(11) 4_545 3_544
O1 O1 O2 107.6(13) 4_645 3_544
O1 O1 O2 110.5(14) 4_655 3_544
Ga2 O1 O2 42.8(7) 2 3_544
Ga2 O1 O2 118.8(12) 4 3_544
La1 O1 O2 25.0(6) 1_554 3_544
La2 O1 O2 141.3(13) 3_545 3_544
La1 O1 O2 99.5(12) 2_566 3_544
O3 O1 O2 121.1(12) 4_645 3_544
O2 O1 O2 99.8(12) 1_445 3_544
O3 O1 O2 129.7(10) 4 3_544
Ga2 O1 La1 159(3) . 2_456
La1 O1 La1 48.8(4) 2_556 2_456
La2 O1 La1 82.6(6) . 2_456
La1 O1 La1 82.3(5) 3_554 2_456
O3 O1 La1 32.5(9) 1_455 2_456
O4 O1 La1 54.7(11) . 2_456
O2 O1 La1 30.0(17) 4_545 2_456
O7 O1 La1 115.7(11) . 2_456
O3 O1 La1 135.2(16) . 2_456
O5 O1 La1 82.3(9) . 2_456
O6 O1 La1 88.2(10) 4_655 2_456
O2 O1 La1 137(2) 4_645 2_456
Ga2 O1 La1 22.2(6) 1_455 2_456
O4 O1 La1 161(2) 1_655 2_456
O4 O1 La1 87.3(14) 4_545 2_456
Ga3 O1 La1 107.4(11) . 2_456
Ga4 O1 La1 106.0(11) 2_656 2_456
Ga4 O1 La1 139.0(11) 3_554 2_456
O2 O1 La1 118.5(11) . 2_456
O3 O1 La1 99.3(10) 2_655 2_456
O6 O1 La1 45.9(5) 1_455 2_456
O5 O1 La1 59.3(6) 4 2_456
O7 O1 La1 81.0(6) 2 2_456
O3 O1 La1 105.8(8) 4_655 2_456
Ga3 O1 La1 38.4(2) 1_455 2_456
O2 O1 La1 77.3(10) 1_545 2_456
Ga4 O1 La1 34.4(3) 2_556 2_456
Ga4 O1 La1 64.9(3) 3_454 2_456
Ta O1 La1 65.8(5) . 2_456
Ga1 O1 La1 65.8(5) . 2_456
O4 O1 La1 112.1(11) 2 2_456
O5 O1 La1 124.3(12) 4_655 2_456
O7 O1 La1 54.2(5) 4_545 2_456
Ga1 O1 La1 74.3(5) 3 2_456
Ta O1 La1 74.3(5) 3 2_456
Ga1 O1 La1 100.9(6) 1_565 2_456
Ta O1 La1 100.9(6) 1_565 2_456
O6 O1 La1 87.5(5) 1_465 2_456
La1 O1 La1 129.5(12) 2_656 2_456
La2 O1 La1 154.1(13) 1_655 2_456
O6 O1 La1 109.4(10) . 2_456
La1 O1 La1 155.0(13) 3_654 2_456
O1 O1 La1 77.9(5) 2 2_456
Ga2 O1 La1 88.0(8) 4_645 2_456
Ga2 O1 La1 114.0(9) 2_655 2_456
Ga2 O1 La1 122.8(8) 4_655 2_456
O1 O1 La1 48.8(6) 4_545 2_456
O1 O1 La1 85.4(7) 4 2_456
O5 O1 La1 57.5(6) 2 2_456
O7 O1 La1 146.5(13) 2_655 2_456
O1 O1 La1 21.6(5) 1_455 2_456
O1 O1 La1 158.4(5) 1_655 2_456
Ga4 O1 La1 88.9(8) 3_544 2_456
Ga4 O1 La1 125.7(9) 4_655 2_456
Ga3 O1 La1 109.3(8) 3 2_456
O2 O1 La1 61.1(7) 1_455 2_456
O1 O1 La1 129.1(14) 2_655 2_456
O3 O1 La1 43.9(4) 2 2_456
Ga2 O1 La1 32.22(19) 4_545 2_456
O1 O1 La1 105.1(7) 4_645 2_456
O1 O1 La1 139.1(12) 4_655 2_456
Ga2 O1 La1 62.2(3) 2 2_456
Ga2 O1 La1 69.2(3) 4 2_456
La1 O1 La1 80.4(6) 1_554 2_456
La2 O1 La1 64.5(5) 3_545 2_456
La1 O1 La1 101.7(5) 2_566 2_456
O3 O1 La1 75.4(7) 4_645 2_456
O2 O1 La1 22.9(6) 1_445 2_456
O3 O1 La1 56.9(4) 4 2_456
O2 O1 La1 101.2(9) 3_544 2_456
Ga2 O1 La2 156(3) . 1_455
La1 O1 La2 82.6(7) 2_556 1_455
La2 O1 La2 48.5(4) . 1_455
La1 O1 La2 81.4(7) 3_554 1_455
O3 O1 La2 28.6(8) 1_455 1_455
O4 O1 La2 39.0(12) . 1_455
O2 O1 La2 55.2(16) 4_545 1_455
O7 O1 La2 78.3(11) . 1_455
O3 O1 La2 132.2(18) . 1_455
O5 O1 La2 95.7(10) . 1_455
O6 O1 La2 115.1(9) 4_655 1_455
O2 O1 La2 173(2) 4_645 1_455
Ga2 O1 La2 21.3(7) 1_455 1_455
O4 O1 La2 137.0(19) 1_655 1_455
O4 O1 La2 124.6(15) 4_545 1_455
Ga3 O1 La2 104.2(11) . 1_455
Ga4 O1 La2 141.5(10) 2_656 1_455
Ga4 O1 La2 106.2(12) 3_554 1_455
O2 O1 La2 98.1(13) . 1_455
O3 O1 La2 81.1(10) 2_655 1_455
O6 O1 La2 67.7(6) 1_455 1_455
O5 O1 La2 78.0(6) 4 1_455
O7 O1 La2 43.3(6) 2 1_455
O3 O1 La2 111.0(8) 4_655 1_455
Ga3 O1 La2 34.8(3) 1_455 1_455
O2 O1 La2 106.8(12) 1_545 1_455
Ga4 O1 La2 64.7(3) 2_556 1_455
Ga4 O1 La2 38.2(3) 3_454 1_455
Ta O1 La2 73.9(6) . 1_455
Ga1 O1 La2 73.9(6) . 1_455
O4 O1 La2 77.7(10) 2 1_455
O5 O1 La2 147.0(10) 4_655 1_455
O7 O1 La2 87.9(5) 4_545 1_455
Ga1 O1 La2 101.3(4) 3 1_455
Ta O1 La2 101.3(4) 3 1_455
Ga1 O1 La2 65.2(6) 1_565 1_455
Ta O1 La2 65.2(6) 1_565 1_455
O6 O1 La2 59.4(6) 1_465 1_455
La1 O1 La2 154.6(12) 2_656 1_455
La2 O1 La2 127.9(13) 1_655 1_455
O6 O1 La2 126.9(11) . 1_455
La1 O1 La2 153.3(13) 3_654 1_455
O1 O1 La2 48.8(4) 2 1_455
Ga2 O1 La2 123.3(9) 4_645 1_455
Ga2 O1 La2 87.2(9) 2_655 1_455
Ga2 O1 La2 113.8(9) 4_655 1_455
O1 O1 La2 85.5(8) 4_545 1_455
O1 O1 La2 77.2(9) 4 1_455
O5 O1 La2 53.6(6) 2 1_455
O7 O1 La2 109.2(12) 2_655 1_455
O1 O1 La2 22.3(5) 1_455 1_455
O1 O1 La2 157.7(5) 1_655 1_455
Ga4 O1 La2 109.2(9) 3_544 1_455
Ga4 O1 La2 88.2(9) 4_655 1_455
Ga3 O1 La2 126.2(8) 3 1_455
O2 O1 La2 45.1(6) 1_455 1_455
O1 O1 La2 103.9(14) 2_655 1_455
O3 O1 La2 23.0(3) 2 1_455
Ga2 O1 La2 69.6(3) 4_545 1_455
O1 O1 La2 139.0(6) 4_645 1_455
O1 O1 La2 129.2(6) 4_655 1_455
Ga2 O1 La2 31.9(2) 2 1_455
Ga2 O1 La2 62.1(3) 4 1_455
La1 O1 La2 64.0(5) 1_554 1_455
La2 O1 La2 102.1(5) 3_545 1_455
La1 O1 La2 80.0(6) 2_566 1_455
O3 O1 La2 112.1(7) 4_645 1_455
O2 O1 La2 56.1(8) 1_445 1_455
O3 O1 La2 61.3(4) 4 1_455
O2 O1 La2 74.6(9) 3_544 1_455
La1 O1 La2 37.91(16) 2_456 1_455
Ga2 O1 La1 159(3) . 3_454
La1 O1 La1 82.7(5) 2_556 3_454
La2 O1 La1 81.8(6) . 3_454
La1 O1 La1 48.4(3) 3_554 3_454
O3 O1 La1 57.4(7) 1_455 3_454
O4 O1 La1 19.3(11) . 3_454
O2 O1 La1 27.3(15) 4_545 3_454
O7 O1 La1 90.9(11) . 3_454
O3 O1 La1 169.4(18) . 3_454
O5 O1 La1 119.7(9) . 3_454
O6 O1 La1 78.7(9) 4_655 3_454
O2 O1 La1 135(2) 4_645 3_454
Ga2 O1 La1 22.2(6) 1_455 3_454
O4 O1 La1 124.4(19) 1_655 3_454
O4 O1 La1 108.9(15) 4_545 3_454
Ga3 O1 La1 139.5(11) . 3_454
Ga4 O1 La1 108.7(11) 2_656 3_454
Ga4 O1 La1 103.5(10) 3_554 3_454
O2 O1 La1 80.9(11) . 3_454
O3 O1 La1 118.5(11) 2_655 3_454
O6 O1 La1 83.5(5) 1_455 3_454
O5 O1 La1 41.2(5) 4 3_454
O7 O1 La1 63.9(6) 2 3_454
O3 O1 La1 76.8(7) 4_655 3_454
Ga3 O1 La1 64.9(2) 1_455 3_454
O2 O1 La1 111.9(11) 1_545 3_454
Ga4 O1 La1 38.0(3) 2_556 3_454
Ga4 O1 La1 34.3(2) 3_454 3_454
Ta O1 La1 101.0(5) . 3_454
Ga1 O1 La1 101.0(5) . 3_454
O4 O1 La1 107.0(11) 2 3_454
O5 O1 La1 109.9(11) 4_655 3_454
O7 O1 La1 59.9(6) 4_545 3_454
Ga1 O1 La1 65.9(4) 3 3_454
Ta O1 La1 65.9(4) 3 3_454
Ga1 O1 La1 73.6(5) 1_565 3_454
Ta O1 La1 73.6(5) 1_565 3_454
O6 O1 La1 53.7(5) 1_465 3_454
La1 O1 La1 155.2(13) 2_656 3_454
La2 O1 La1 153.0(13) 1_655 3_454
O6 O1 La1 146.3(11) . 3_454
La1 O1 La1 129.1(11) 3_654 3_454
O1 O1 La1 85.2(5) 2 3_454
Ga2 O1 La1 114.8(9) 4_645 3_454
Ga2 O1 La1 122.0(10) 2_655 3_454
Ga2 O1 La1 87.7(7) 4_655 3_454
O1 O1 La1 78.4(7) 4_545 3_454
O1 O1 La1 48.7(6) 4 3_454
O5 O1 La1 86.1(6) 2 3_454
O7 O1 La1 125.8(12) 2_655 3_454
O1 O1 La1 21.7(5) 1_455 3_454
O1 O1 La1 158.3(5) 1_655 3_454
Ga4 O1 La1 126.2(8) 3_544 3_454
Ga4 O1 La1 108.4(9) 4_655 3_454
Ga3 O1 La1 89.2(7) 3 3_454
O2 O1 La1 24.6(7) 1_455 3_454
O1 O1 La1 137.6(14) 2_655 3_454
O3 O1 La1 59.0(4) 2 3_454
Ga2 O1 La1 62.5(3) 4_545 3_454
O1 O1 La1 130.7(13) 4_645 3_454
O1 O1 La1 105.0(8) 4_655 3_454
Ga2 O1 La1 68.9(4) 2 3_454
Ga2 O1 La1 32.15(17) 4 3_454
La1 O1 La1 101.2(6) 1_554 3_454
La2 O1 La1 80.8(5) 3_545 3_454
La1 O1 La1 64.3(5) 2_566 3_454
O3 O1 La1 101.0(7) 4_645 3_454
O2 O1 La1 59.9(6) 1_445 3_454
O3 O1 La1 24.6(4) 4 3_454
O2 O1 La1 110.4(10) 3_544 3_454
La1 O1 La1 37.66(11) 2_456 3_454
La2 O1 La1 37.40(16) 1_455 3_454
Ga2 O1 O2 108(2) . 2
La1 O1 O2 126.1(15) 2_556 2
La2 O1 O2 20.3(11) . 2
La1 O1 O2 88.9(16) 3_554 2
O3 O1 O2 66.5(14) 1_455 2
O4 O1 O2 59.6(16) . 2
O2 O1 O2 100.3(19) 4_545 2
O7 O1 O2 30.5(11) . 2
O3 O1 O2 99.6(16) . 2
O5 O1 O2 106.0(16) . 2
O6 O1 O2 140.0(16) 4_655 2
O2 O1 O2 135(2) 4_645 2
Ga2 O1 O2 69.6(11) 1_455 2
O4 O1 O2 91.6(18) 1_655 2
O4 O1 O2 166(2) 4_545 2
Ga3 O1 O2 88.3(13) . 2
Ga4 O1 O2 160.8(15) 2_656 2
Ga4 O1 O2 62.4(11) 3_554 2
O2 O1 O2 71.2(18) . 2
O3 O1 O2 60.0(10) 2_655 2
O6 O1 O2 102.3(12) 1_455 2
O5 O1 O2 110.1(10) 4 2
O7 O1 O2 10.5(9) 2 2
O3 O1 O2 107.3(13) 4_655 2
Ga3 O1 O2 67.2(9) 1_455 2
O2 O1 O2 134.9(15) 1_545 2
Ga4 O1 O2 111.0(8) 2_556 2
Ga4 O1 O2 44.0(8) 3_454 2
Ta O1 O2 90.4(11) . 2
Ga1 O1 O2 90.4(11) . 2
O4 O1 O2 33.0(8) 2 2
O5 O1 O2 133.6(13) 4_655 2
O7 O1 O2 134.0(7) 4_545 2
Ga1 O1 O2 134.1(10) 3 2
Ta O1 O2 134.1(10) 3 2
Ga1 O1 O2 25.8(7) 1_565 2
Ta O1 O2 25.8(7) 1_565 2
O6 O1 O2 42.5(9) 1_465 2
La1 O1 O2 130.6(11) 2_656 2
La2 O1 O2 81.5(10) 1_655 2
O6 O1 O2 121.1(13) . 2
La1 O1 O2 109.8(11) 3_654 2
O1 O1 O2 32.8(8) 2 2
Ga2 O1 O2 156.2(14) 4_645 2
Ga2 O1 O2 51.3(8) 2_655 2
Ga2 O1 O2 91.6(11) 4_655 2
O1 O1 O2 133.0(14) 4_545 2
O1 O1 O2 78.3(13) 4 2
O5 O1 O2 70.2(11) 2 2
O7 O1 O2 59.1(10) 2_655 2
O1 O1 O2 70.5(5) 1_455 2
O1 O1 O2 109.5(5) 1_655 2
Ga4 O1 O2 120.6(12) 3_544 2
Ga4 O1 O2 38.2(7) 4_655 2
Ga3 O1 O2 126.3(12) 3 2
O2 O1 O2 59.8(12) 1_455 2
O1 O1 O2 64.3(11) 2_655 2
O3 O1 O2 51.8(7) 2 2
Ga2 O1 O2 118.8(7) 4_545 2
O1 O1 O2 151.7(16) 4_645 2
O1 O1 O2 97.0(11) 4_655 2
Ga2 O1 O2 34.8(7) 2 2
Ga2 O1 O2 74.4(8) 4 2
La1 O1 O2 56.5(9) 1_554 2
La2 O1 O2 152.1(6) 3_545 2
La1 O1 O2 60.9(9) 2_566 2
O3 O1 O2 155.7(12) 4_645 2
O2 O1 O2 103.0(7) 1_445 2
O3 O1 O2 87.1(8) 4 2
O2 O1 O2 44.4(8) 3_544 2
La1 O1 O2 88.0(7) 2_456 2
La2 O1 O2 50.1(6) 1_455 2
La1 O1 O2 74.2(7) 3_454 2
Ga2 O1 O2 33.9(17) . 1_655
La1 O1 O2 137.9(15) 2_556 1_655
La2 O1 O2 104.5(14) . 1_655
La1 O1 O2 80.0(12) 3_554 1_655
O3 O1 O2 159(2) 1_455 1_655
O4 O1 O2 111.4(18) . 1_655
O2 O1 O2 133(2) 4_545 1_655
O7 O1 O2 63.2(12) . 1_655
O3 O1 O2 61.9(11) . 1_655
O5 O1 O2 114.1(9) . 1_655
O6 O1 O2 79.3(12) 4_655 1_655
O2 O1 O2 42.6(13) 4_645 1_655
Ga2 O1 O2 145.9(16) 1_455 1_655
O4 O1 O2 2.3(12) 1_655 1_655
O4 O1 O2 94.8(14) 4_545 1_655
Ga3 O1 O2 90.3(6) . 1_655
Ga4 O1 O2 69.2(9) 2_656 1_655
Ga4 O1 O2 33.1(7) 3_554 1_655
O2 O1 O2 46.2(7) . 1_655
O3 O1 O2 96.8(9) 2_655 1_655
O6 O1 O2 149.5(11) 1_455 1_655
O5 O1 O2 103.8(12) 4 1_655
O7 O1 O2 97.7(11) 2 1_655
O3 O1 O2 56.9(8) 4_655 1_655
Ga3 O1 O2 155.5(13) 1_455 1_655
O2 O1 O2 113.0(13) 1_545 1_655
Ga4 O1 O2 130.5(13) 2_556 1_655
Ga4 O1 O2 104.5(12) 3_454 1_655
Ta O1 O2 131.8(8) . 1_655
Ga1 O1 O2 131.8(8) . 1_655
O4 O1 O2 77.0(10) 2 1_655
O5 O1 O2 45.4(8) 4_655 1_655
O7 O1 O2 114.9(13) 4_545 1_655
Ga1 O1 O2 92.3(10) 3 1_655
Ta O1 O2 92.3(10) 3 1_655
Ga1 O1 O2 74.4(9) 1_565 1_655
Ta O1 O2 74.4(9) 1_565 1_655
O6 O1 O2 81.8(11) 1_465 1_655
La1 O1 O2 60.9(7) 2_656 1_655
La2 O1 O2 43.1(6) 1_655 1_655
O6 O1 O2 84.9(7) . 1_655
La1 O1 O2 16.3(7) 3_654 1_655
O1 O1 O2 112.2(11) 2 1_655
Ga2 O1 O2 97.4(9) 4_645 1_655
Ga2 O1 O2 80.1(7) 2_655 1_655
Ga2 O1 O2 39.5(6) 4_655 1_655
O1 O1 O2 133.4(17) 4_545 1_655
O1 O1 O2 77.6(8) 4 1_655
O5 O1 O2 139.3(11) 2 1_655
O7 O1 O2 41.6(8) 2_655 1_655
O1 O1 O2 146.0(7) 1_455 1_655
O1 O1 O2 34.0(7) 1_655 1_655
Ga4 O1 O2 105.4(7) 3_544 1_655
Ga4 O1 O2 59.6(7) 4_655 1_655
Ga3 O1 O2 56.1(7) 3 1_655
O2 O1 O2 104.7(13) 1_455 1_655
O1 O1 O2 66.6(7) 2_655 1_655
O3 O1 O2 144.2(13) 2 1_655
Ga2 O1 O2 146.8(12) 4_545 1_655
O1 O1 O2 81.6(9) 4_645 1_655
O1 O1 O2 23.2(8) 4_655 1_655
Ga2 O1 O2 125.3(11) 2 1_655
Ga2 O1 O2 94.1(10) 4 1_655
La1 O1 O2 115.1(9) 1_554 1_655
La2 O1 O2 111.3(10) 3_545 1_655
La1 O1 O2 64.2(8) 2_566 1_655
O3 O1 O2 107.8(9) 4_645 1_655
O2 O1 O2 163.5(17) 1_445 1_655
O3 O1 O2 105.5(11) 4 1_655
O2 O1 O2 92.1(10) 3_544 1_655
La1 O1 O2 162.2(11) 2_456 1_655
La2 O1 O2 139.3(12) 1_455 1_655
La1 O1 O2 126.2(11) 3_454 1_655
O2 O1 O2 93.5(13) 2 1_655
Ga2 O1 O3 30.8(17) . 2_755
La1 O1 O3 106.0(12) 2_556 2_755
La2 O1 O3 81.1(10) . 2_755
La1 O1 O3 135.9(12) 3_554 2_755
O3 O1 O3 113.5(16) 1_455 2_755
O4 O1 O3 146.5(19) . 2_755
O2 O1 O3 166(2) 4_545 2_755
O7 O1 O3 75.0(10) . 2_755
O3 O1 O3 12.5(9) . 2_755
O5 O1 O3 61.9(8) . 2_755
O6 O1 O3 117.5(10) 4_655 2_755
O2 O1 O3 59.8(15) 4_645 2_755
Ga2 O1 O3 146.7(16) 1_455 2_755
O4 O1 O3 57.4(13) 1_655 2_755
O4 O1 O3 87.1(12) 4_545 2_755
Ga3 O1 O3 34.1(4) . 2_755
Ga4 O1 O3 88.4(5) 2_656 2_755
Ga4 O1 O3 69.9(6) 3_554 2_755
O2 O1 O3 96.4(10) . 2_755
O3 O1 O3 47.3(5) 2_655 2_755
O6 O1 O3 97.8(10) 1_455 2_755
O5 O1 O3 154.4(12) 4 2_755
O7 O1 O3 99.0(12) 2 2_755
O3 O1 O3 111.8(8) 4_655 2_755
Ga3 O1 O3 106.2(10) 1_455 2_755
O2 O1 O3 78.2(9) 1_545 2_755
Ga4 O1 O3 157.0(13) 2_556 2_755
Ga4 O1 O3 130.4(12) 3_454 2_755
Ta O1 O3 75.9(7) . 2_755
Ga1 O1 O3 75.9(7) . 2_755
O4 O1 O3 55.7(7) 2 2_755
O5 O1 O3 83.8(6) 4_655 2_755
O7 O1 O3 137.0(11) 4_545 2_755
Ga1 O1 O3 130.9(8) 3 2_755
Ta O1 O3 130.9(8) 3 2_755
Ga1 O1 O3 92.2(8) 1_565 2_755
Ta O1 O3 92.2(8) 1_565 2_755
O6 O1 O3 114.6(11) 1_465 2_755
La1 O1 O3 42.0(4) 2_656 2_755
La2 O1 O3 16.2(3) 1_655 2_755
O6 O1 O3 43.3(5) . 2_755
La1 O1 O3 59.1(4) 3_654 2_755
O1 O1 O3 78.7(10) 2 2_755
Ga2 O1 O3 80.0(5) 4_645 2_755
Ga2 O1 O3 40.9(4) 2_655 2_755
Ga2 O1 O3 95.6(5) 4_655 2_755
O1 O1 O3 112.8(7) 4_545 2_755
O1 O1 O3 131.2(7) 4 2_755
O5 O1 O3 85.4(8) 2 2_755
O7 O1 O3 41.9(6) 2_655 2_755
O1 O1 O3 147.6(6) 1_455 2_755
O1 O1 O3 32.4(6) 1_655 2_755
Ga4 O1 O3 60.5(5) 3_544 2_755
Ga4 O1 O3 56.4(4) 4_655 2_755
Ga3 O1 O3 103.5(5) 3 2_755
O2 O1 O3 143.6(13) 1_455 2_755
O1 O1 O3 25.0(5) 2_655 2_755
O3 O1 O3 108.1(10) 2 2_755
Ga2 O1 O3 126.5(10) 4_545 2_755
O1 O1 O3 65.3(7) 4_645 2_755
O1 O1 O3 79.4(7) 4_655 2_755
Ga2 O1 O3 95.5(9) 2 2_755
Ga2 O1 O3 145.3(10) 4 2_755
La1 O1 O3 66.0(6) 1_554 2_755
La2 O1 O3 115.3(8) 3_545 2_755
La1 O1 O3 110.0(8) 2_566 2_755
O3 O1 O3 93.5(7) 4_645 2_755
O2 O1 O3 123.5(12) 1_445 2_755
O3 O1 O3 161.0(11) 4 2_755
O2 O1 O3 53.0(8) 3_544 2_755
La1 O1 O3 141.5(10) 2_456 2_755
La2 O1 O3 127.4(10) 1_455 2_755
La1 O1 O3 162.6(12) 3_454 2_755
O2 O1 O3 88.6(8) 2 2_755
O2 O1 O3 56.3(6) 1_655 2_755
Ga2 O1 O2 66(2) . 2_655
La1 O1 O2 144.6(19) 2_556 2_655
La2 O1 O2 46.5(11) . 2_655
La1 O1 O2 102.8(17) 3_554 2_655
O3 O1 O2 100.4(18) 1_455 2_655
O4 O1 O2 94.9(18) . 2_655
O2 O1 O2 140(2) 4_545 2_655
O7 O1 O2 23.9(9) . 2_655
O3 O1 O2 64.1(12) . 2_655
O5 O1 O2 99.0(15) . 2_655
O6 O1 O2 134.9(15) 4_655 2_655
O2 O1 O2 94.1(16) 4_645 2_655
Ga2 O1 O2 111.3(15) 1_455 2_655
O4 O1 O2 57.1(16) 1_655 2_655
O4 O1 O2 138.2(14) 4_545 2_655
Ga3 O1 O2 68.8(11) . 2_655
Ga4 O1 O2 125.6(8) 2_656 2_655
Ga4 O1 O2 38.8(9) 3_554 2_655
O2 O1 O2 64.2(16) . 2_655
O3 O1 O2 51.9(9) 2_655 2_655
O6 O1 O2 120.9(14) 1_455 2_655
O5 O1 O2 135.5(14) 4 2_655
O7 O1 O2 50.6(10) 2 2_655
O3 O1 O2 101.0(12) 4_655 2_655
Ga3 O1 O2 97.7(12) 1_455 2_655
O2 O1 O2 125.8(11) 1_545 2_655
Ga4 O1 O2 150.8(11) 2_556 2_655
Ga4 O1 O2 78.9(10) 3_454 2_655
Ta O1 O2 97.7(12) . 2_655
Ga1 O1 O2 97.7(12) . 2_655
O4 O1 O2 19.3(8) 2 2_655
O5 O1 O2 103.7(10) 4_655 2_655
O7 O1 O2 166.2(13) 4_545 2_655
Ga1 O1 O2 144.1(13) 3 2_655
Ta O1 O2 144.1(13) 3 2_655
Ga1 O1 O2 40.6(7) 1_565 2_655
Ta O1 O2 40.6(7) 1_565 2_655
O6 O1 O2 64.1(10) 1_465 2_655
La1 O1 O2 91.2(7) 2_656 2_655
La2 O1 O2 40.8(7) 1_655 2_655
O6 O1 O2 93.5(9) . 2_655
La1 O1 O2 73.6(8) 3_654 2_655
O1 O1 O2 54.0(9) 2 2_655
Ga2 O1 O2 131.8(8) 4_645 2_655
Ga2 O1 O2 32.6(8) 2_655 2_655
Ga2 O1 O2 78.3(9) 4_655 2_655
O1 O1 O2 155.7(17) 4_545 2_655
O1 O1 O2 92.5(12) 4 2_655
O5 O1 O2 88.3(12) 2 2_655
O7 O1 O2 18.0(8) 2_655 2_655
O1 O1 O2 112.3(6) 1_455 2_655
O1 O1 O2 67.7(6) 1_655 2_655
Ga4 O1 O2 105.9(10) 3_544 2_655
Ga4 O1 O2 4.6(5) 4_655 2_655
Ga3 O1 O2 110.7(10) 3 2_655
O2 O1 O2 92.1(14) 1_455 2_655
O1 O1 O2 33.1(8) 2_655 2_655
O3 O1 O2 86.4(10) 2 2_655
Ga2 O1 O2 153.7(12) 4_545 2_655
O1 O1 O2 116.4(9) 4_645 2_655
O1 O1 O2 72.6(11) 4_655 2_655
Ga2 O1 O2 67.4(9) 2 2_655
Ga2 O1 O2 99.2(10) 4 2_655
La1 O1 O2 63.9(9) 1_554 2_655
La2 O1 O2 165.9(7) 3_545 2_655
La1 O1 O2 67.8(9) 2_566 2_655
O3 O1 O2 145.1(9) 4_645 2_655
O2 O1 O2 136.5(10) 1_445 2_655
O3 O1 O2 116.2(11) 4 2_655
O2 O1 O2 39.1(7) 3_544 2_655
La1 O1 O2 128.4(10) 2_456 2_655
La2 O1 O2 91.4(10) 1_455 2_655
La1 O1 O2 112.9(10) 3_454 2_655
O2 O1 O2 41.7(6) 2 2_655
O2 O1 O2 58.4(11) 1_655 2_655
O3 O1 O2 51.7(6) 2_755 2_655
Ga2 O1 O3 112(2) . 3_455
La1 O1 O3 92.0(14) 2_556 3_455
La2 O1 O3 124.3(13) . 3_455
La1 O1 O3 20.7(11) 3_554 3_455
O3 O1 O3 104.6(11) 1_455 3_455
O4 O1 O3 53.3(15) . 3_455
O2 O1 O3 45.0(19) 4_545 3_455
O7 O1 O3 101.7(14) . 3_455
O3 O1 O3 140.4(17) . 3_455
O5 O1 O3 138.2(16) . 3_455
O6 O1 O3 33.6(9) 4_655 3_455
O2 O1 O3 85.7(19) 4_645 3_455
Ga2 O1 O3 70.6(9) 1_455 3_455
O4 O1 O3 87.3(18) 1_655 3_455
O4 O1 O3 83.4(17) 4_545 3_455
Ga3 O1 O3 164.1(16) . 3_455
Ga4 O1 O3 64.9(9) 2_656 3_455
Ga4 O1 O3 87.2(11) 3_554 3_455
O2 O1 O3 59.3(11) . 3_455
O3 O1 O3 166.9(12) 2_655 3_455
O6 O1 O3 111.3(10) 1_455 3_455
O5 O1 O3 16.5(6) 4 3_455
O7 O1 O3 98.0(10) 2 3_455
O3 O1 O3 31.0(7) 4_655 3_455
Ga3 O1 O3 111.8(5) 1_455 3_455
O2 O1 O3 109.0(14) 1_545 3_455
Ga4 O1 O3 44.6(6) 2_556 3_455
Ga4 O1 O3 65.8(7) 3_454 3_455
Ta O1 O3 136.0(9) . 3_455
Ga1 O1 O3 136.0(9) . 3_455
O4 O1 O3 134.1(12) 2 3_455
O5 O1 O3 59.8(8) 4_655 3_455
O7 O1 O3 43.5(7) 4_545 3_455
Ga1 O1 O3 27.2(4) 3 3_455
Ta O1 O3 27.2(4) 3 3_455
Ga1 O1 O3 89.5(9) 1_565 3_455
Ta O1 O3 89.5(9) 1_565 3_455
O6 O1 O3 66.5(8) 1_465 3_455
La1 O1 O3 112.2(11) 2_656 3_455
La2 O1 O3 130.9(10) 1_655 3_455
O6 O1 O3 131.0(13) . 3_455
La1 O1 O3 82.9(9) 3_654 3_455
O1 O1 O3 132.3(6) 2 3_455
Ga2 O1 O3 93.9(10) 4_645 3_455
Ga2 O1 O3 154.4(13) 2_655 3_455
Ga2 O1 O3 51.0(6) 4_655 3_455
O1 O1 O3 81.3(15) 4_545 3_455
O1 O1 O3 31.8(11) 4 3_455
O5 O1 O3 132.2(7) 2 3_455
O7 O1 O3 118.8(11) 2_655 3_455
O1 O1 O3 69.9(4) 1_455 3_455
O1 O1 O3 110.1(4) 1_655 3_455
Ga4 O1 O3 128.4(12) 3_544 3_455
Ga4 O1 O3 119.2(10) 4_655 3_455
Ga3 O1 O3 39.2(5) 3 3_455
O2 O1 O3 50.3(8) 1_455 3_455
O1 O1 O3 151.7(6) 2_655 3_455
O3 O1 O3 108.9(5) 2 3_455
Ga2 O1 O3 75.8(6) 4_545 3_455
O1 O1 O3 100.1(16) 4_645 3_455
O1 O1 O3 65.0(10) 4_655 3_455
Ga2 O1 O3 117.7(6) 2 3_455
Ga2 O1 O3 33.5(5) 4 3_455
La1 O1 O3 151.2(6) 1_554 3_455
La2 O1 O3 62.7(6) 3_545 3_455
La1 O1 O3 55.6(6) 2_566 3_455
O3 O1 O3 85.3(8) 4_645 3_455
O2 O1 O3 86.9(8) 1_445 3_455
O3 O1 O3 26.2(7) 4 3_455
O2 O1 O3 152.0(13) 3_544 3_455
La1 O1 O3 74.9(5) 2_456 3_455
La2 O1 O3 87.3(5) 1_455 3_455
La1 O1 O3 50.1(5) 3_454 3_455
O2 O1 O3 107.6(10) 2 3_455
O2 O1 O3 87.9(9) 1_655 3_455
O3 O1 O3 141.9(8) 2_755 3_455
O2 O1 O3 122.7(11) 2_655 3_455
Ga2 O1 O3 68.3(19) . 3
La1 O1 O3 106.2(18) 2_556 3
La2 O1 O3 142.3(18) . 3
La1 O1 O3 48.1(10) 3_554 3
O3 O1 O3 147.0(16) 1_455 3
O4 O1 O3 90.9(18) . 3
O2 O1 O3 85(2) 4_545 3
O7 O1 O3 97.4(14) . 3
O3 O1 O3 97.7(13) . 3
O5 O1 O3 127.7(15) . 3
O6 O1 O3 30.3(9) 4_655 3
O2 O1 O3 44.8(16) 4_645 3
Ga2 O1 O3 113.9(13) 1_455 3
O4 O1 O3 50.4(16) 1_655 3
O4 O1 O3 70.8(16) 4_545 3
Ga3 O1 O3 126.8(8) . 3
Ga4 O1 O3 39.4(7) 2_656 3
Ga4 O1 O3 67.4(9) 3_554 3
O2 O1 O3 51.5(12) . 3
O3 O1 O3 145.5(6) 2_655 3
O6 O1 O3 132.0(14) 1_455 3
O5 O1 O3 56.6(9) 4 3
O7 O1 O3 118.6(12) 2 3
O3 O1 O3 19.2(6) 4_655 3
Ga3 O1 O3 153.4(9) 1_455 3
O2 O1 O3 102.0(14) 1_545 3
Ga4 O1 O3 80.8(10) 2_556 3
Ga4 O1 O3 97.4(10) 3_454 3
Ta O1 O3 146.6(13) . 3
Ga1 O1 O3 146.6(13) . 3
O4 O1 O3 123.9(11) 2 3
O5 O1 O3 18.8(6) 4_655 3
O7 O1 O3 65.7(9) 4_545 3
Ga1 O1 O3 42.3(6) 3 3
Ta O1 O3 42.3(6) 3 3
Ga1 O1 O3 96.9(9) 1_565 3
Ta O1 O3 96.9(9) 1_565 3
O6 O1 O3 84.6(10) 1_465 3
La1 O1 O3 74.4(7) 2_656 3
La2 O1 O3 90.5(6) 1_655 3
O6 O1 O3 100.5(9) . 3
La1 O1 O3 40.6(6) 3_654 3
O1 O1 O3 154.7(6) 2 3
Ga2 O1 O3 80.1(8) 4_645 3
Ga2 O1 O3 130.3(7) 2_655 3
Ga2 O1 O3 31.3(5) 4_655 3
O1 O1 O3 95.9(18) 4_545 3
O1 O1 O3 54.4(12) 4 3
O5 O1 O3 166.3(13) 2 3
O7 O1 O3 90.5(9) 2_655 3
O1 O1 O3 113.1(3) 1_455 3
O1 O1 O3 66.9(3) 1_655 3
Ga4 O1 O3 112.0(9) 3_544 3
Ga4 O1 O3 104.1(8) 4_655 3
Ga3 O1 O3 6.1(3) 3 3
O2 O1 O3 85.5(10) 1_455 3
O1 O1 O3 115.9(7) 2_655 3
O3 O1 O3 151.7(8) 2 3
Ga2 O1 O3 101.5(10) 4_545 3
O1 O1 O3 74.9(13) 4_645 3
O1 O1 O3 32.1(10) 4_655 3
Ga2 O1 O3 153.0(10) 2 3
Ga2 O1 O3 67.7(7) 4 3
La1 O1 O3 164.6(5) 1_554 3
La2 O1 O3 69.9(7) 3_545 3
La1 O1 O3 63.2(6) 2_566 3
O3 O1 O3 80.9(7) 4_645 3
O2 O1 O3 118.1(11) 1_445 3
O3 O1 O3 68.3(8) 4 3
O2 O1 O3 141.9(10) 3_544 3
La1 O1 O3 115.0(9) 2_456 3
La2 O1 O3 129.0(8) 1_455 3
La1 O1 O3 92.8(8) 3_454 3
O2 O1 O3 122.7(12) 2 3
O2 O1 O3 50.1(7) 1_655 3
O3 O1 O3 98.9(5) 2_755 3
O2 O1 O3 104.6(9) 2_655 3
O3 O1 O3 43.3(5) 3_455 3
Ga2 O1 O3 39.6(17) . 4_755
La1 O1 O3 119.0(16) 2_556 4_755
La2 O1 O3 127.7(14) . 4_755
La1 O1 O3 71.9(10) 3_554 4_755
O3 O1 O3 177.1(15) 1_455 4_755
O4 O1 O3 112.3(18) . 4_755
O2 O1 O3 115(2) 4_545 4_755
O7 O1 O3 84.3(12) . 4_755
O3 O1 O3 70.2(10) . 4_755
O5 O1 O3 114.0(10) . 4_755
O6 O1 O3 56.8(10) 4_655 4_755
O2 O1 O3 27.4(15) 4_645 4_755
Ga2 O1 O3 142.2(15) 1_455 4_755
O4 O1 O3 24.7(14) 1_655 4_755
O4 O1 O3 75.7(14) 4_545 4_755
Ga3 O1 O3 100.4(5) . 4_755
Ga4 O1 O3 46.9(6) 2_656 4_755
Ga4 O1 O3 52.3(7) 3_554 4_755
O2 O1 O3 52.8(11) . 4_755
O3 O1 O3 115.4(8) 2_655 4_755
O6 O1 O3 139.9(12) 1_455 4_755
O5 O1 O3 86.6(11) 4 4_755
O7 O1 O3 116.7(11) 2 4_755
O3 O1 O3 43.3(5) 4_655 4_755
Ga3 O1 O3 174.9(10) 1_455 4_755
O2 O1 O3 100.7(11) 1_545 4_755
Ga4 O1 O3 110.2(11) 2_556 4_755
Ga4 O1 O3 112.1(10) 3_454 4_755
Ta O1 O3 135.7(7) . 4_755
Ga1 O1 O3 135.7(7) . 4_755
O4 O1 O3 100.4(8) 2 4_755
O5 O1 O3 21.9(6) 4_655 4_755
O7 O1 O3 92.0(11) 4_545 4_755
Ga1 O1 O3 70.5(7) 3 4_755
Ta O1 O3 70.5(7) 3 4_755
Ga1 O1 O3 92.2(8) 1_565 4_755
Ta O1 O3 92.2(8) 1_565 4_755
O6 O1 O3 91.9(9) 1_465 4_755
La1 O1 O3 55.2(5) 2_656 4_755
La2 O1 O3 60.5(5) 1_655 4_755
O6 O1 O3 82.8(6) . 4_755
La1 O1 O3 10.6(4) 3_654 4_755
O1 O1 O3 135.6(9) 2 4_755
Ga2 O1 O3 80.9(6) 4_645 4_755
Ga2 O1 O3 101.4(5) 2_655 4_755
Ga2 O1 O3 36.4(4) 4_655 4_755
O1 O1 O3 112.0(16) 4_545 4_755
O1 O1 O3 74.1(10) 4 4_755
O5 O1 O3 153.8(8) 2 4_755
O7 O1 O3 64.9(7) 2_655 4_755
O1 O1 O3 141.6(4) 1_455 4_755
O1 O1 O3 38.4(4) 1_655 4_755
Ga4 O1 O3 100.7(6) 3_544 4_755
Ga4 O1 O3 82.9(6) 4_655 4_755
Ga3 O1 O3 35.5(3) 3 4_755
O2 O1 O3 105.8(11) 1_455 4_755
O1 O1 O3 86.1(6) 2_655 4_755
O3 O1 O3 166.4(12) 2 4_755
Ga2 O1 O3 123.7(10) 4_545 4_755
O1 O1 O3 68.1(9) 4_645 4_755
O1 O1 O3 21.4(7) 4_655 4_755
Ga2 O1 O3 148.3(10) 2 4_755
Ga2 O1 O3 90.2(8) 4 4_755
La1 O1 O3 134.5(6) 1_554 4_755
La2 O1 O3 88.3(7) 3_545 4_755
La1 O1 O3 70.4(6) 2_566 4_755
O3 O1 O3 88.6(8) 4_645 4_755
O2 O1 O3 140.9(13) 1_445 4_755
O3 O1 O3 95.7(9) 4 4_755
O2 O1 O3 114.0(7) 3_544 4_755
La1 O1 O3 144.6(10) 2_456 4_755
La2 O1 O3 150.1(10) 1_455 4_755
La1 O1 O3 120.1(9) 3_454 4_755
O2 O1 O3 114.7(10) 2 4_755
O2 O1 O3 23.4(6) 1_655 4_755
O3 O1 O3 69.4(4) 2_755 4_755
O2 O1 O3 81.8(8) 2_655 4_755
O3 O1 O3 72.6(8) 3_455 4_755
O3 O1 O3 30.1(5) 3 4_755
Ga4 O2 Ga2 115(3) 3_554 4_655
Ga4 O2 O5 62(3) 3_554 1_565
Ga2 O2 O5 135(4) 4_655 1_565
Ga4 O2 La1 106(3) 3_554 3_554
Ga2 O2 La1 97(3) 4_655 3_554
O5 O2 La1 128(3) 1_565 3_554
Ga4 O2 O7 39.4(16) 3_554 .
Ga2 O2 O7 151(3) 4_655 .
O5 O2 O7 55.5(19) 1_565 .
La1 O2 O7 82.7(19) 3_554 .
Ga4 O2 La1 126(4) 3_554 2_566
Ga2 O2 La1 103(3) 4_655 2_566
O5 O2 La1 64(2) 1_565 2_566
La1 O2 La1 106(2) 3_554 2_566
O7 O2 La1 105(3) . 2_566
Ga4 O2 O3 128(3) 3_554 4_655
Ga2 O2 O3 39.8(18) 4_655 4_655
O5 O2 O3 168(3) 1_565 4_655
La1 O2 O3 58.0(15) 3_554 4_655
O7 O2 O3 135(3) . 4_655
La1 O2 O3 105(2) 2_566 4_655
Ga4 O2 O4 130(4) 3_554 4
Ga2 O2 O4 53(2) 4_655 4
O5 O2 O4 92(4) 1_565 4
La1 O2 O4 123(3) 3_554 4
O7 O2 O4 148(4) . 4
La1 O2 O4 53(2) 2_566 4
O3 O2 O4 77(3) 4_655 4
Ga4 O2 O6 37.6(13) 3_554 1_565
Ga2 O2 O6 88(2) 4_655 1_565
O5 O2 O6 64(2) 1_565 1_565
La1 O2 O6 137(3) 3_554 1_565
O7 O2 O6 74.0(18) . 1_565
La1 O2 O6 114(3) 2_566 1_565
O3 O2 O6 120(3) 4_655 1_565
O4 O2 O6 93(3) 4 1_565
Ga4 O2 O1 153(3) 3_554 4
Ga2 O2 O1 88(3) 4_655 4
O5 O2 O1 113(3) 1_565 4
La1 O2 O1 54.1(17) 3_554 4
O7 O2 O1 114(3) . 4
La1 O2 O1 56.2(18) 2_566 4
O3 O2 O1 61(2) 4_655 4
O4 O2 O1 75(3) 4 4
O6 O2 O1 168(3) 1_565 4
Ga4 O2 O4 42(2) 3_554 1_655
Ga2 O2 O4 84(2) 4_655 1_655
O5 O2 O4 105(3) 1_565 1_655
La1 O2 O4 82(2) 3_554 1_655
O7 O2 O4 67(2) . 1_655
La1 O2 O4 169(3) 2_566 1_655
O3 O2 O4 86(2) 4_655 1_655
O4 O2 O4 130(3) 4 1_655
O6 O2 O4 56.4(16) 1_565 1_655
O1 O2 O4 134(3) 4 1_655
Ga4 O2 O6 98(3) 3_554 1_465
Ga2 O2 O6 147(3) 4_655 1_465
O5 O2 O6 58.4(18) 1_565 1_465
La1 O2 O6 75.4(16) 3_554 1_465
O7 O2 O6 61.1(16) . 1_465
La1 O2 O6 51.3(13) 2_566 1_465
O3 O2 O6 120(3) 4_655 1_465
O4 O2 O6 104(3) 4 1_465
O6 O2 O6 120(3) 1_565 1_465
O1 O2 O6 61.7(18) 4 1_465
O4 O2 O6 125(3) 1_655 1_465
Ga4 O2 O1 86(2) 3_554 4_655
Ga2 O2 O1 30.1(15) 4_655 4_655
O5 O2 O1 115(3) 1_565 4_655
La1 O2 O1 114(3) 3_554 4_655
O7 O2 O1 124(3) . 4_655
La1 O2 O1 118(3) 2_566 4_655
O3 O2 O1 64(2) 4_655 4_655
O4 O2 O1 66(3) 4 4_655
O6 O2 O1 58.1(16) 1_565 4_655
O1 O2 O1 118(3) 4 4_655
O4 O2 O1 63.8(19) 1_655 4_655
O6 O2 O1 169(3) 1_465 4_655
Ga4 O2 Ta 65(2) 3_554 1_565
Ga2 O2 Ta 167(3) 4_655 1_565
O5 O2 Ta 33.1(14) 1_565 1_565
La1 O2 Ta 94.8(17) 3_554 1_565
O7 O2 Ta 35.1(11) . 1_565
La1 O2 Ta 70.3(17) 2_566 1_565
O3 O2 Ta 151(2) 4_655 1_565
O4 O2 Ta 117(3) 4 1_565
O6 O2 Ta 86.1(19) 1_565 1_565
O1 O2 Ta 96(2) 4 1_565
O4 O2 Ta 101(2) 1_655 1_565
O6 O2 Ta 34.7(10) 1_465 1_565
O1 O2 Ta 144(2) 4_655 1_565
Ga4 O2 Ga1 65(2) 3_554 1_565
Ga2 O2 Ga1 167(3) 4_655 1_565
O5 O2 Ga1 33.1(14) 1_565 1_565
La1 O2 Ga1 94.8(17) 3_554 1_565
O7 O2 Ga1 35.1(11) . 1_565
La1 O2 Ga1 70.3(17) 2_566 1_565
O3 O2 Ga1 151(2) 4_655 1_565
O4 O2 Ga1 117(3) 4 1_565
O6 O2 Ga1 86.1(19) 1_565 1_565
O1 O2 Ga1 96(2) 4 1_565
O4 O2 Ga1 101(2) 1_655 1_565
O6 O2 Ga1 34.7(10) 1_465 1_565
O1 O2 Ga1 144(2) 4_655 1_565
Ta O2 Ga1 0.0(3) 1_565 1_565
Ga4 O2 O4 100(2) 3_554 .
Ga2 O2 O4 126(3) 4_655 .
O5 O2 O4 97(2) 1_565 .
La1 O2 O4 32.3(11) 3_554 .
O7 O2 O4 64.3(17) . .
La1 O2 O4 84.9(17) 2_566 .
O3 O2 O4 86.8(18) 4_655 .
O4 O2 O4 127(2) 4 .
O6 O2 O4 138(2) 1_565 .
O1 O2 O4 52.7(18) 4 .
O4 O2 O4 98(2) 1_655 .
O6 O2 O4 43.8(13) 1_465 .
O1 O2 O4 146(3) 4_655 .
Ta O2 O4 64.4(14) 1_565 .
Ga1 O2 O4 64.4(14) 1_565 .
Ga4 O2 O1 67(2) 3_554 .
Ga2 O2 O1 112(3) 4_655 .
O5 O2 O1 108(3) 1_565 .
La1 O2 O1 39.1(12) 3_554 .
O7 O2 O1 52.5(15) . .
La1 O2 O1 132(2) 2_566 .
O3 O2 O1 82.9(19) 4_655 .
O4 O2 O1 159(4) 4 .
O6 O2 O1 100.1(17) 1_565 .
O1 O2 O1 92(2) 4 .
O4 O2 O1 50.6(17) 1_655 .
O6 O2 O1 83.2(16) 1_465 .
O1 O2 O1 108(2) 4_655 .
Ta O2 O1 80.4(15) 1_565 .
Ga1 O2 O1 80.4(15) 1_565 .
O4 O2 O1 47.8(11) . .
Ga4 O2 Ga2 50.6(18) 3_554 .
Ga2 O2 Ga2 98(3) 4_655 .
O5 O2 Ga2 108(2) 1_565 .
La1 O2 Ga2 60.2(14) 3_554 .
O7 O2 Ga2 56.5(14) . .
La1 O2 Ga2 156(2) 2_566 .
O3 O2 Ga2 84.0(17) 4_655 .
O4 O2 Ga2 150(3) 4 .
O6 O2 Ga2 77.3(14) 1_565 .
O1 O2 Ga2 114(2) 4 .
O4 O2 Ga2 24.7(14) 1_655 .
O6 O2 Ga2 105.1(18) 1_465 .
O1 O2 Ga2 85.2(19) 4_655 .
Ta O2 Ga2 91.0(14) 1_565 .
Ga1 O2 Ga2 91.0(14) 1_565 .
O4 O2 Ga2 73.7(13) . .
O1 O2 Ga2 25.9(6) . .
Ga4 O2 Ga3 55.9(19) 3_554 1_565
Ga2 O2 Ga3 118(3) 4_655 1_565
O5 O2 Ga3 18.8(13) 1_565 1_565
La1 O2 Ga3 144(2) 3_554 1_565
O7 O2 Ga3 63.7(16) . 1_565
La1 O2 Ga3 73.3(18) 2_566 1_565
O3 O2 Ga3 158(2) 4_655 1_565
O4 O2 Ga3 86(3) 4 1_565
O6 O2 Ga3 46.8(12) 1_565 1_565
O1 O2 Ga3 128(3) 4 1_565
O4 O2 Ga3 96(2) 1_655 1_565
O6 O2 Ga3 77.1(17) 1_465 1_565
O1 O2 Ga3 96.7(18) 4_655 1_565
Ta O2 Ga3 50.2(10) 1_565 1_565
Ga1 O2 Ga3 50.2(10) 1_565 1_565
O4 O2 Ga3 114.6(19) . 1_565
O1 O2 Ga3 114.8(17) . 1_565
Ga2 O2 Ga3 106.2(14) . 1_565
Ga4 O2 O6 98(3) 3_554 4_655
Ga2 O2 O6 74(2) 4_655 4_655
O5 O2 O6 149(3) 1_565 4_655
La1 O2 O6 29.7(11) 3_554 4_655
O7 O2 O6 94.1(19) . 4_655
La1 O2 O6 129(2) 2_566 4_655
O3 O2 O6 41.3(10) 4_655 4_655
O4 O2 O6 118(3) 4 4_655
O6 O2 O6 117(2) 1_565 4_655
O1 O2 O6 72.4(19) 4 4_655
O4 O2 O6 61.7(19) 1_655 4_655
O6 O2 O6 104.9(18) 1_465 4_655
O1 O2 O6 85(2) 4_655 4_655
Ta O2 O6 118.4(17) 1_565 4_655
Ga1 O2 O6 118.4(17) 1_565 4_655
O4 O2 O6 61.3(12) . 4_655
O1 O2 O6 41.6(13) . 4_655
Ga2 O2 O6 47.9(9) . 4_655
Ga3 O2 O6 154.0(17) 1_565 4_655
Ga4 O2 La1 61.3(18) 3_554 3_654
Ga2 O2 La1 57.3(17) 4_655 3_654
O5 O2 La1 117(2) 1_565 3_654
La1 O2 La1 93(2) 3_554 3_654
O7 O2 La1 93.7(18) . 3_654
La1 O2 La1 154(2) 2_566 3_654
O3 O2 La1 70.4(17) 4_655 3_654
O4 O2 La1 102(3) 4 3_654
O6 O2 La1 54.4(12) 1_565 3_654
O1 O2 La1 130(3) 4 3_654
O4 O2 La1 27.8(13) 1_655 3_654
O6 O2 La1 153(2) 1_465 3_654
O1 O2 La1 36.4(13) 4_655 3_654
Ta O2 La1 125.7(16) 1_565 3_654
Ga1 O2 La1 125.7(16) 1_565 3_654
O4 O2 La1 119.2(18) . 3_654
O1 O2 La1 73.2(13) . 3_654
Ga2 O2 La1 49.1(8) . 3_654
Ga3 O2 La1 101.1(13) 1_565 3_654
O6 O2 La1 65.2(12) 4_655 3_654
Ga4 O2 La1 72.4(17) 3_554 2_666
Ga2 O2 La1 60.1(16) 4_655 2_666
O5 O2 La1 78(2) 1_565 2_666
La1 O2 La1 151(3) 3_554 2_666
O7 O2 La1 108(2) . 2_666
La1 O2 La1 98(2) 2_566 2_666
O3 O2 La1 99(2) 4_655 2_666
O4 O2 La1 60(2) 4 2_666
O6 O2 La1 34.9(9) 1_565 2_666
O1 O2 La1 134(3) 4 2_666
O4 O2 La1 77.7(15) 1_655 2_666
O6 O2 La1 134(2) 1_465 2_666
O1 O2 La1 37.7(13) 4_655 2_666
Ta O2 La1 109.6(18) 1_565 2_666
Ga1 O2 La1 109.6(18) 1_565 2_666
O4 O2 La1 172(2) . 2_666
O1 O2 La1 128.1(16) . 2_666
Ga2 O2 La1 102.3(13) . 2_666
Ga3 O2 La1 59.8(9) 1_565 2_666
O6 O2 La1 121.1(17) 4_655 2_666
La1 O2 La1 59.6(8) 3_654 2_666
Ga4 O2 O5 88(2) 3_554 4_655
Ga2 O2 O5 48(2) 4_655 4_655
O5 O2 O5 149(2) 1_565 4_655
La1 O2 O5 66.4(16) 3_554 4_655
O7 O2 O5 108(2) . 4_655
La1 O2 O5 144(2) 2_566 4_655
O3 O2 O5 39.8(12) 4_655 4_655
O4 O2 O5 100(3) 4 4_655
O6 O2 O5 87.6(17) 1_565 4_655
O1 O2 O5 97(2) 4 4_655
O4 O2 O5 46.3(16) 1_655 4_655
O6 O2 O5 142(2) 1_465 4_655
O1 O2 O5 48.6(16) 4_655 4_655
Ta O2 O5 142.6(19) 1_565 4_655
Ga1 O2 O5 142.6(19) 1_565 4_655
O4 O2 O5 97.7(16) . 4_655
O1 O2 O5 64.5(15) . 4_655
Ga2 O2 O5 51.7(10) . 4_655
Ga3 O2 O5 134.3(14) 1_565 4_655
O6 O2 O5 36.7(8) 4_655 4_655
La1 O2 O5 33.3(8) 3_654 4_655
La1 O2 O5 84.4(12) 2_666 4_655
Ga4 O2 Ga4 101(2) 3_554 3_454
Ga2 O2 Ga4 141(3) 4_655 3_454
O5 O2 Ga4 75.2(19) 1_565 3_454
La1 O2 Ga4 56.8(11) 3_554 3_454
O7 O2 Ga4 61.9(14) . 3_454
La1 O2 Ga4 63.8(13) 2_566 3_454
O3 O2 Ga4 105.2(19) 4_655 3_454
O4 O2 Ga4 114(3) 4 3_454
O6 O2 Ga4 132(2) 1_565 3_454
O1 O2 Ga4 53.6(16) 4 3_454
O4 O2 Ga4 116(2) 1_655 3_454
O6 O2 Ga4 18.7(8) 1_465 3_454
O1 O2 Ga4 169(3) 4_655 3_454
Ta O2 Ga4 46.4(8) 1_565 3_454
Ga1 O2 Ga4 46.4(8) 1_565 3_454
O4 O2 Ga4 25.2(9) . 3_454
O1 O2 Ga4 68.5(11) . 3_454
Ga2 O2 Ga4 92.9(13) . 3_454
Ga3 O2 Ga4 93.9(15) 1_565 3_454
O6 O2 Ga4 86.3(12) 4_655 3_454
La1 O2 Ga4 141.7(17) 3_654 3_454
La1 O2 Ga4 152(2) 2_666 3_454
O5 O2 Ga4 122.9(16) 4_655 3_454
Ga4 O2 O3 69(2) 3_554 1_565
Ga2 O2 O3 93(2) 4_655 1_565
O5 O2 O3 41.6(17) 1_565 1_565
La1 O2 O3 169(3) 3_554 1_565
O7 O2 O3 88(2) . 1_565
La1 O2 O3 72.3(17) 2_566 1_565
O3 O2 O3 133(2) 4_655 1_565
O4 O2 O3 64(2) 4 1_565
O6 O2 O3 42.1(12) 1_565 1_565
O1 O2 O3 127(3) 4 1_565
O4 O2 O3 98.5(18) 1_655 1_565
O6 O2 O3 96(2) 1_465 1_565
O1 O2 O3 75.6(16) 4_655 1_565
Ta O2 O3 74.6(15) 1_565 1_565
Ga1 O2 O3 74.6(15) 1_565 1_565
O4 O2 O3 138(2) . 1_565
O1 O2 O3 134.9(19) . 1_565
Ga2 O2 O3 117.6(15) . 1_565
Ga3 O2 O3 25.4(7) 1_565 1_565
O6 O2 O3 157.1(14) 4_655 1_565
La1 O2 O3 91.9(10) 3_654 1_565
La1 O2 O3 37.9(7) 2_666 1_565
O5 O2 O3 121.5(12) 4_655 1_565
Ga4 O2 O3 114.3(17) 3_454 1_565
Ga4 O2 La2 163(3) 3_554 3
Ga2 O2 La2 51.7(15) 4_655 3
O5 O2 La2 134(3) 1_565 3
La1 O2 La2 69.8(14) 3_554 3
O7 O2 La2 149(2) . 3
La1 O2 La2 69.8(13) 2_566 3
O3 O2 La2 35.5(11) 4_655 3
O4 O2 La2 54(2) 4 3
O6 O2 La2 137(2) 1_565 3
O1 O2 La2 36.2(16) 4 3
O4 O2 La2 121(2) 1_655 3
O6 O2 La2 96.5(16) 1_465 3
O1 O2 La2 81.7(19) 4_655 3
Ta O2 La2 130.7(16) 1_565 3
Ga1 O2 La2 130.7(16) 1_565 3
O4 O2 La2 84.3(14) . 3
O1 O2 La2 106.7(18) . 3
Ga2 O2 La2 116.8(18) . 3
Ga3 O2 La2 136.6(18) 1_565 3
O6 O2 La2 69.4(12) 4_655 3
La1 O2 La2 102.4(16) 3_654 3
La1 O2 La2 103.4(13) 2_666 3
O5 O2 La2 74.9(13) 4_655 3
Ga4 O2 La2 89.8(11) 3_454 3
O3 O2 La2 118.1(17) 1_565 3
Ga4 O2 Ga4 124(2) 3_554 2_666
Ga2 O2 Ga4 46.9(16) 4_655 2_666
O5 O2 Ga4 94(2) 1_565 2_666
La1 O2 Ga4 127(2) 3_554 2_666
O7 O2 Ga4 149(3) . 2_666
La1 O2 Ga4 60.9(13) 2_566 2_666
O3 O2 Ga4 75.3(16) 4_655 2_666
O4 O2 Ga4 8.6(17) 4 2_666
O6 O2 Ga4 86.5(16) 1_565 2_666
O1 O2 Ga4 82(2) 4 2_666
O4 O2 Ga4 121(2) 1_655 2_666
O6 O2 Ga4 112(2) 1_465 2_666
O1 O2 Ga4 57.7(16) 4_655 2_666
Ta O2 Ga4 122(2) 1_565 2_666
Ga1 O2 Ga4 122(2) 1_565 2_666
O4 O2 Ga4 134.3(17) . 2_666
O1 O2 Ga4 158(2) . 2_666
Ga2 O2 Ga4 142.5(18) . 2_666
Ga3 O2 Ga4 85.4(14) 1_565 2_666
O6 O2 Ga4 116.4(17) 4_655 2_666
La1 O2 Ga4 94.1(13) 3_654 2_666
La1 O2 Ga4 52.4(8) 2_666 2_666
O5 O2 Ga4 94.6(15) 4_655 2_666
Ga4 O2 Ga4 122.3(15) 3_454 2_666
O3 O2 Ga4 62.1(11) 1_565 2_666
La2 O2 Ga4 57.0(8) 3 2_666
Ga4 O2 Ga3 113(3) 3_554 3
Ga2 O2 Ga3 36.4(18) 4_655 3
O5 O2 Ga3 169(3) 1_565 3
La1 O2 Ga3 62.4(15) 3_554 3
O7 O2 Ga3 128(2) . 3
La1 O2 Ga3 120(2) 2_566 3
O3 O2 Ga3 15.8(9) 4_655 3
O4 O2 Ga3 84(3) 4 3
O6 O2 Ga3 106.0(19) 1_565 3
O1 O2 Ga3 76(2) 4 3
O4 O2 Ga3 70.7(19) 1_655 3
O6 O2 Ga3 133(2) 1_465 3
O1 O2 Ga3 53.6(15) 4_655 3
Ta O2 Ga3 156.2(19) 1_565 3
Ga1 O2 Ga3 156.2(19) 1_565 3
O4 O2 Ga3 94.0(16) . 3
O1 O2 Ga3 77.5(17) . 3
Ga2 O2 Ga3 72.5(13) . 3
Ga3 O2 Ga3 150.2(16) 1_565 3
O6 O2 Ga3 37.9(8) 4_655 3
La1 O2 Ga3 54.7(9) 3_654 3
La1 O2 Ga3 91.0(13) 2_666 3
O5 O2 Ga3 24.4(6) 4_655 3
Ga4 O2 Ga3 115.9(15) 3_454 3
O3 O2 Ga3 128.0(15) 1_565 3
La2 O2 Ga3 50.5(8) 3 3
Ga4 O2 Ga3 80.1(11) 2_666 3
Ga4 O2 O7 4.1(15) 3_554 2_655
Ga2 O2 O7 116(2) 4_655 2_655
O5 O2 O7 59(2) 1_565 2_655
La1 O2 O7 109.3(19) 3_554 2_655
O7 O2 O7 40.0(15) . 2_655
La1 O2 O7 123(2) 2_566 2_655
O3 O2 O7 131(2) 4_655 2_655
O4 O2 O7 127(3) 4 2_655
O6 O2 O7 35.3(10) 1_565 2_655
O1 O2 O7 154(3) 4 2_655
O4 O2 O7 45.9(16) 1_655 2_655
O6 O2 O7 96.8(19) 1_465 2_655
O1 O2 O7 86.0(16) 4_655 2_655
Ta O2 O7 63.2(12) 1_565 2_655
Ga1 O2 O7 63.2(12) 1_565 2_655
O4 O2 O7 102.3(17) . 2_655
O1 O2 O7 70.3(13) . 2_655
Ga2 O2 O7 54.7(9) . 2_655
Ga3 O2 O7 51.9(9) 1_565 2_655
O6 O2 O7 102.5(15) 4_655 2_655
La1 O2 O7 63.5(9) 3_654 2_655
La1 O2 O7 70.3(9) 2_666 2_655
O5 O2 O7 91.6(13) 4_655 2_655
Ga4 O2 O7 101.5(14) 3_454 2_655
O3 O2 O7 65.0(12) 1_565 2_655
La2 O2 O7 165.8(19) 3 2_655
Ga4 O2 O7 121.1(15) 2_666 2_655
Ga3 O2 O7 116.0(15) 3 2_655
Ga4 O2 La2 55.0(16) 3_554 .
Ga2 O2 La2 144(3) 4_655 .
O5 O2 La2 76(2) 1_565 .
La1 O2 La2 59.8(12) 3_554 .
O7 O2 La2 22.9(10) . .
La1 O2 La2 110.3(19) 2_566 .
O3 O2 La2 114.1(19) 4_655 .
O4 O2 La2 163(3) 4 .
O6 O2 La2 92.4(16) 1_565 .
O1 O2 La2 98(2) 4 .
O4 O2 La2 66.2(18) 1_655 .
O6 O2 La2 59.4(12) 1_465 .
O1 O2 La2 130(2) 4_655 .
Ta O2 La2 47.7(8) 1_565 .
Ga1 O2 La2 47.7(8) 1_565 .
O4 O2 La2 45.3(11) . .
O1 O2 La2 32.9(10) . .
Ga2 O2 La2 46.8(7) . .
Ga3 O2 La2 86.2(12) 1_565 .
O6 O2 La2 73.5(11) 4_655 .
La1 O2 La2 93.8(12) 3_654 .
La1 O2 La2 127.3(14) 2_666 .
O5 O2 La2 95.9(14) 4_655 .
Ga4 O2 La2 52.0(7) 3_454 .
O3 O2 La2 110.6(17) 1_565 .
La2 O2 La2 127.7(15) 3 .
Ga4 O2 La2 169(2) 2_666 .
Ga3 O2 La2 110.3(15) 3 .
O7 O2 La2 57.1(9) 2_655 .
Ga4 O2 Ga2 142(3) 3_554 4
Ga2 O2 Ga2 100(2) 4_655 4
O5 O2 Ga2 104(2) 1_565 4
La1 O2 Ga2 53.0(10) 3_554 4
O7 O2 Ga2 103.0(18) . 4
La1 O2 Ga2 53.4(11) 2_566 4
O3 O2 Ga2 71.2(16) 4_655 4
O4 O2 Ga2 83(2) 4 4
O6 O2 Ga2 167(3) 1_565 4
O1 O2 Ga2 12.0(14) 4 4
O4 O2 Ga2 135(2) 1_655 4
O6 O2 Ga2 50.0(10) 1_465 4
O1 O2 Ga2 130(2) 4_655 4
Ta O2 Ga2 84.6(12) 1_565 4
Ga1 O2 Ga2 84.6(12) 1_565 4
O4 O2 Ga2 43.9(10) . 4
O1 O2 Ga2 87.6(13) . 4
Ga2 O2 Ga2 112.2(15) . 4
Ga3 O2 Ga2 120.1(18) 1_565 4
O6 O2 Ga2 76.1(11) 4_655 4
La1 O2 Ga2 138.8(19) 3_654 4
La1 O2 Ga2 142.5(16) 2_666 4
O5 O2 Ga2 105.5(15) 4_655 4
Ga4 O2 Ga2 41.7(6) 3_454 4
O3 O2 Ga2 125.7(16) 1_565 4
La2 O2 Ga2 48.2(7) 3 4
Ga4 O2 Ga2 90.4(12) 2_666 4
Ga3 O2 Ga2 86.1(12) 3 4
O7 O2 Ga2 143.0(16) 2_655 4
La2 O2 Ga2 88.3(10) . 4
Ga4 O2 O2 65(2) 3_554 4_645
Ga2 O2 O2 75(3) 4_655 4_645
O5 O2 O2 127(3) 1_565 4_645
La1 O2 O2 62.4(12) 3_554 4_645
O7 O2 O2 79.7(17) . 4_645
La1 O2 O2 167(3) 2_566 4_645
O3 O2 O2 64.4(19) 4_655 4_645
O4 O2 O2 127(4) 4 4_645
O6 O2 O2 79(2) 1_565 4_645
O1 O2 O2 111(3) 4 4_645
O4 O2 O2 23.9(14) 1_655 4_645
O6 O2 O2 125(2) 1_465 4_645
O1 O2 O2 66(2) 4_655 4_645
Ta O2 O2 114.5(19) 1_565 4_645
Ga1 O2 O2 114.5(19) 1_565 4_645
O4 O2 O2 86.5(13) . 4_645
O1 O2 O2 42.1(9) . 4_645
Ga2 O2 O2 23.6(7) . 4_645
Ga3 O2 O2 119(2) 1_565 4_645
O6 O2 O2 38.4(10) 4_655 4_645
La1 O2 O2 32.7(13) 3_654 4_645
La1 O2 O2 92(2) 2_666 4_645
O5 O2 O2 28.4(14) 4_655 4_645
Ga4 O2 O2 109.9(14) 3_454 4_645
O3 O2 O2 120.3(19) 1_565 4_645
La2 O2 O2 100(2) 3 4_645
Ga4 O2 O2 120(2) 2_666 4_645
Ga3 O2 O2 50.9(17) 3 4_645
O7 O2 O2 68.7(15) 2_655 4_645
La2 O2 O2 69.6(11) . 4_645
Ga2 O2 O2 113.9(18) 4 4_645
Ga4 O2 O2 102(3) 3_554 4_655
Ga2 O2 O2 61(2) 4_655 4_655
O5 O2 O2 75(2) 1_565 4_655
La1 O2 O2 151(3) 3_554 4_655
O7 O2 O2 126(3) . 4_655
La1 O2 O2 64.5(10) 2_566 4_655
O3 O2 O2 96(2) 4_655 4_655
O4 O2 O2 28.3(15) 4 4_655
O6 O2 O2 65.5(19) 1_565 4_655
O1 O2 O2 103(2) 4 4_655
O4 O2 O2 112(2) 1_655 4_655
O6 O2 O2 111(2) 1_465 4_655
O1 O2 O2 58(2) 4_655 4_655
Ta O2 O2 106(2) 1_565 4_655
Ga1 O2 O2 106(2) 1_565 4_655
O4 O2 O2 149(2) . 4_655
O1 O2 O2 163(2) . 4_655
Ga2 O2 O2 137(2) . 4_655
Ga3 O2 O2 62.7(15) 1_565 4_655
O6 O2 O2 135(2) 4_655 4_655
La1 O2 O2 90.5(18) 3_654 4_655
La1 O2 O2 35.1(12) 2_666 4_655
O5 O2 O2 104(2) 4_655 4_655
Ga4 O2 O2 127.5(19) 3_454 4_655
O3 O2 O2 38.4(11) 1_565 4_655
La2 O2 O2 81.1(16) 3 4_655
Ga4 O2 O2 24.1(9) 2_666 4_655
Ga3 O2 O2 97(2) 3 4_655
O7 O2 O2 98(2) 2_655 4_655
La2 O2 O2 149(2) . 4_655
Ga2 O2 O2 108.3(16) 4 4_655
O2 O2 O2 123(3) 4_645 4_655
Ga4 O2 O1 107(3) 3_554 1_565
Ga2 O2 O1 96(2) 4_655 1_565
O5 O2 O1 51(2) 1_565 1_565
La1 O2 O1 134.9(19) 3_554 1_565
O7 O2 O1 105(2) . 1_565
La1 O2 O1 29.1(10) 2_566 1_565
O3 O2 O1 118(2) 4_655 1_565
O4 O2 O1 44(2) 4 1_565
O6 O2 O1 86.0(18) 1_565 1_565
O1 O2 O1 84(2) 4 1_565
O4 O2 O1 142(2) 1_655 1_565
O6 O2 O1 70.5(17) 1_465 1_565
O1 O2 O1 98(2) 4_655 1_565
Ta O2 O1 73.0(16) 1_565 1_565
Ga1 O2 O1 73.0(16) 1_565 1_565
O4 O2 O1 111.2(17) . 1_565
O1 O2 O1 152(2) . 1_565
Ga2 O2 O1 157.7(19) . 1_565
Ga3 O2 O1 51.6(12) 1_565 1_565
O6 O2 O1 154.0(17) 4_655 1_565
La1 O2 O1 129.4(15) 3_654 1_565
La1 O2 O1 69.9(11) 2_666 1_565
O5 O2 O1 143.1(18) 4_655 1_565
Ga4 O2 O1 87.2(14) 3_454 1_565
O3 O2 O1 43.9(9) 1_565 1_565
La2 O2 O1 85.5(14) 3 1_565
Ga4 O2 O1 48.8(11) 2_666 1_565
Ga3 O2 O1 127.1(16) 3 1_565
O7 O2 O1 103.4(17) 2_655 1_565
La2 O2 O1 120.6(18) . 1_565
Ga2 O2 O1 82.3(12) 4 1_565
O2 O2 O1 162(2) 4_645 1_565
O2 O2 O1 40.8(8) 4_655 1_565
Ga4 O2 O7 68(2) 3_554 2
Ga2 O2 O7 169(3) 4_655 2
O5 O2 O7 56.1(17) 1_565 2
La1 O2 O7 72.1(14) 3_554 2
O7 O2 O7 28.8(14) . 2
La1 O2 O7 82.4(17) 2_566 2
O3 O2 O7 130(2) 4_655 2
O4 O2 O7 135(3) 4 2
O6 O2 O7 99.2(18) 1_565 2
O1 O2 O7 87.2(19) 4 2
O4 O2 O7 93(2) 1_655 2
O6 O2 O7 33.2(10) 1_465 2
O1 O2 O7 153(2) 4_655 2
Ta O2 O7 23.4(7) 1_565 2
Ga1 O2 O7 23.4(7) 1_565 2
O4 O2 O7 43.8(13) . 2
O1 O2 O7 59.1(12) . 2
Ga2 O2 O7 75.2(11) . 2
Ga3 O2 O7 72.1(12) 1_565 2
O6 O2 O7 95.1(13) 4_655 2
La1 O2 O7 120.3(15) 3_654 2
La1 O2 O7 129.2(17) 2_666 2
O5 O2 O7 123.6(16) 4_655 2
Ga4 O2 O7 33.7(7) 3_454 2
O3 O2 O7 97.2(16) 1_565 2
La2 O2 O7 123.3(12) 3 2
Ga4 O2 O7 141.4(19) 2_666 2
Ga3 O2 O7 132.9(17) 3 2
O7 O2 O7 67.8(11) 2_655 2
La2 O2 O7 28.5(6) . 2
Ga2 O2 O7 75.4(10) 4 2
O2 O2 O7 98.1(15) 4_645 2
O2 O2 O7 129(2) 4_655 2
O1 O2 O7 93.3(17) 1_565 2
Ga4 O2 O5 122(3) 3_554 4
Ga2 O2 O5 85(2) 4_655 4
O5 O2 O5 138(2) 1_565 4
La1 O2 O5 17.1(8) 3_554 4
O7 O2 O5 99.3(18) . 4
La1 O2 O5 97.5(16) 2_566 4
O3 O2 O5 44.9(13) 4_655 4
O4 O2 O5 106(3) 4 4
O6 O2 O5 148(2) 1_565 4
O1 O2 O5 41.9(16) 4 4
O4 O2 O5 92(2) 1_655 4
O6 O2 O5 80.3(14) 1_465 4
O1 O2 O5 107(2) 4_655 4
Ta O2 O5 106.4(14) 1_565 4
Ga1 O2 O5 106.4(14) 1_565 4
O4 O2 O5 42.0(10) . 4
O1 O2 O5 55.3(12) . 4
Ga2 O2 O5 73.4(13) . 4
Ga3 O2 O5 156.4(17) 1_565 4
O6 O2 O5 31.7(7) 4_655 4
La1 O2 O5 96.1(16) 3_654 4
La1 O2 O5 143.9(19) 2_666 4
O5 O2 O5 64.6(11) 4_655 4
Ga4 O2 O5 62.7(8) 3_454 4
O3 O2 O5 169.0(17) 1_565 4
La2 O2 O5 52.7(9) 3 4
Ga4 O2 O5 109.6(15) 2_666 4
Ga3 O2 O5 53.2(10) 3 4
O7 O2 O5 125.5(17) 2_655 4
La2 O2 O5 76.5(10) . 4
Ga2 O2 O5 44.5(7) 4 4
O2 O2 O5 69.6(14) 4_645 4
O2 O2 O5 134(2) 4_655 4
O1 O2 O5 125.4(14) 1_565 4
O7 O2 O5 85.2(11) 2 4
Ga4 O2 Ta 27.7(13) 3_554 1_665
Ga2 O2 Ta 99(2) 4_655 1_665
O5 O2 Ta 56.0(18) 1_565 1_665
La1 O2 Ta 132(2) 3_554 1_665
O7 O2 Ta 62.1(14) . 1_665
La1 O2 Ta 113(2) 2_566 1_665
O3 O2 Ta 130(2) 4_655 1_665
O4 O2 Ta 102(2) 4 1_665
O6 O2 Ta 12.2(9) 1_565 1_665
O1 O2 Ta 169(3) 4 1_665
O4 O2 Ta 56.0(15) 1_655 1_665
O6 O2 Ta 109(2) 1_465 1_665
O1 O2 Ta 69.7(15) 4_655 1_665
Ta O2 Ta 74.8(12) 1_565 1_665
Ga1 O2 Ta 74.8(12) 1_565 1_665
O4 O2 Ta 126.2(17) . 1_665
O1 O2 Ta 93.4(13) . 1_665
Ga2 O2 Ta 73.4(9) . 1_665
Ga3 O2 Ta 41.2(6) 1_565 1_665
O6 O2 Ta 117.7(15) 4_655 1_665
La1 O2 Ta 60.8(7) 3_654 1_665
La1 O2 Ta 46.2(6) 2_666 1_665
O5 O2 Ta 93.9(12) 4_655 1_665
Ga4 O2 Ta 119.8(15) 3_454 1_665
O3 O2 Ta 44.2(7) 1_565 1_665
La2 O2 Ta 149.1(15) 3 1_665
Ga4 O2 Ta 96.4(12) 2_666 1_665
Ga3 O2 Ta 114.8(13) 3 1_665
O7 O2 Ta 24.7(5) 2_655 1_665
La2 O2 Ta 81.4(10) . 1_665
Ga2 O2 Ta 158.9(18) 4 1_665
O2 O2 Ta 79.6(16) 4_645 1_665
O2 O2 Ta 73.9(17) 4_655 1_665
O1 O2 Ta 87.2(13) 1_565 1_665
O7 O2 Ta 87.0(11) 2 1_665
O5 O2 Ta 146.8(17) 4 1_665
Ga4 O2 Ga1 27.7(13) 3_554 1_665
Ga2 O2 Ga1 99(2) 4_655 1_665
O5 O2 Ga1 56.0(18) 1_565 1_665
La1 O2 Ga1 132(2) 3_554 1_665
O7 O2 Ga1 62.1(14) . 1_665
La1 O2 Ga1 113(2) 2_566 1_665
O3 O2 Ga1 130(2) 4_655 1_665
O4 O2 Ga1 102(2) 4 1_665
O6 O2 Ga1 12.2(9) 1_565 1_665
O1 O2 Ga1 169(3) 4 1_665
O4 O2 Ga1 56.0(15) 1_655 1_665
O6 O2 Ga1 109(2) 1_465 1_665
O1 O2 Ga1 69.7(15) 4_655 1_665
Ta O2 Ga1 74.8(12) 1_565 1_665
Ga1 O2 Ga1 74.8(12) 1_565 1_665
O4 O2 Ga1 126.2(17) . 1_665
O1 O2 Ga1 93.4(13) . 1_665
Ga2 O2 Ga1 73.4(9) . 1_665
Ga3 O2 Ga1 41.2(6) 1_565 1_665
O6 O2 Ga1 117.7(15) 4_655 1_665
La1 O2 Ga1 60.8(7) 3_654 1_665
La1 O2 Ga1 46.2(6) 2_666 1_665
O5 O2 Ga1 93.9(12) 4_655 1_665
Ga4 O2 Ga1 119.8(15) 3_454 1_665
O3 O2 Ga1 44.2(7) 1_565 1_665
La2 O2 Ga1 149.1(15) 3 1_665
Ga4 O2 Ga1 96.4(12) 2_666 1_665
Ga3 O2 Ga1 114.8(13) 3 1_665
O7 O2 Ga1 24.7(5) 2_655 1_665
La2 O2 Ga1 81.4(10) . 1_665
Ga2 O2 Ga1 158.9(18) 4 1_665
O2 O2 Ga1 79.6(16) 4_645 1_665
O2 O2 Ga1 73.9(17) 4_655 1_665
O1 O2 Ga1 87.2(13) 1_565 1_665
O7 O2 Ga1 87.0(11) 2 1_665
O5 O2 Ga1 146.8(17) 4 1_665
Ta O2 Ga1 0.0(2) 1_665 1_665
Ga4 O2 O6 47.2(19) 3_554 2_665
Ga2 O2 O6 152(3) 4_655 2_665
O5 O2 O6 25.2(15) 1_565 2_665
La1 O2 O6 107.8(18) 3_554 2_665
O7 O2 O6 30.3(12) . 2_665
La1 O2 O6 82.2(18) 2_566 2_665
O3 O2 O6 165(2) 4_655 2_665
O4 O2 O6 118(3) 4 2_665
O6 O2 O6 66.0(16) 1_565 2_665
O1 O2 O6 116(2) 4 2_665
O4 O2 O6 88(2) 1_655 2_665
O6 O2 O6 54.8(14) 1_465 2_665
O1 O2 O6 124(2) 4_655 2_665
Ta O2 O6 20.2(6) 1_565 2_665
Ga1 O2 O6 20.2(6) 1_565 2_665
O4 O2 O6 80.9(15) . 2_665
O1 O2 O6 82.6(14) . 2_665
Ga2 O2 O6 84.5(12) . 2_665
Ga3 O2 O6 36.3(7) 1_565 2_665
O6 O2 O6 124.1(16) 4_655 2_665
La1 O2 O6 108.3(13) 3_654 2_665
La1 O2 O6 92.3(13) 2_666 2_665
O5 O2 O6 133.6(15) 4_655 2_665
Ga4 O2 O6 66.0(10) 3_454 2_665
O3 O2 O6 61.7(12) 1_565 2_665
La2 O2 O6 149.3(16) 3 2_665
Ga4 O2 O6 119.5(17) 2_666 2_665
Ga3 O2 O6 156.9(16) 3 2_665
O7 O2 O6 44.8(8) 2_655 2_665
La2 O2 O6 51.0(8) . 2_665
Ga2 O2 O6 104.8(13) 4 2_665
O2 O2 O6 106.1(19) 4_645 2_665
O2 O2 O6 98(2) 4_655 2_665
O1 O2 O6 75.2(15) 1_565 2_665
O7 O2 O6 37.1(8) 2 2_665
O5 O2 O6 122.2(14) 4 2_665
Ta O2 O6 54.6(8) 1_665 2_665
Ga1 O2 O6 54.6(8) 1_665 2_665
Ga4 O2 Ga2 94(2) 3_554 1_565
Ga2 O2 Ga2 84(2) 4_655 1_565
O5 O2 Ga2 52.5(18) 1_565 1_565
La1 O2 Ga2 157(2) 3_554 1_565
O7 O2 Ga2 107(2) . 1_565
La1 O2 Ga2 52.1(13) 2_566 1_565
O3 O2 Ga2 117.7(19) 4_655 1_565
O4 O2 Ga2 42(2) 4 1_565
O6 O2 Ga2 65.2(14) 1_565 1_565
O1 O2 Ga2 103(2) 4 1_565
O4 O2 Ga2 121(2) 1_655 1_565
O6 O2 Ga2 90.8(19) 1_465 1_565
O1 O2 Ga2 78.5(17) 4_655 1_565
Ta O2 Ga2 83.0(15) 1_565 1_565
Ga1 O2 Ga2 83.0(15) 1_565 1_565
O4 O2 Ga2 133.6(19) . 1_565
O1 O2 Ga2 158.5(19) . 1_565
Ga2 O2 Ga2 142.2(15) . 1_565
Ga3 O2 Ga2 43.7(8) 1_565 1_565
O6 O2 Ga2 158.3(17) 4_655 1_565
La1 O2 Ga2 106.4(12) 3_654 1_565
La1 O2 Ga2 46.8(7) 2_666 1_565
O5 O2 Ga2 126.8(15) 4_655 1_565
Ga4 O2 Ga2 108.7(16) 3_454 1_565
O3 O2 Ga2 25.2(6) 1_565 1_565
La2 O2 Ga2 94.4(12) 3 1_565
Ga4 O2 Ga2 42.4(7) 2_666 1_565
Ga3 O2 Ga2 120.5(14) 3 1_565
O7 O2 Ga2 90.0(13) 2_655 1_565
La2 O2 Ga2 128.1(17) . 1_565
Ga2 O2 Ga2 104.3(14) 4 1_565
O2 O2 Ga2 139(2) 4_645 1_565
O2 O2 Ga2 23.4(8) 4_655 1_565
O1 O2 Ga2 23.3(5) 1_565 1_565
O7 O2 Ga2 106.1(17) 2 1_565
O5 O2 Ga2 143.9(15) 4 1_565
Ta O2 Ga2 69.0(10) 1_665 1_565
Ga1 O2 Ga2 69.0(10) 1_665 1_565
O6 O2 Ga2 77.2(12) 2_665 1_565
Ga4 O2 Ga4 25.4(16) 3_554 4_655
Ga2 O2 Ga4 137(2) 4_655 4_655
O5 O2 Ga4 40.2(17) 1_565 4_655
La1 O2 Ga4 108.4(18) 3_554 4_655
O7 O2 Ga4 26.4(11) . 4_655
La1 O2 Ga4 103(2) 2_566 4_655
O3 O2 Ga4 151(2) 4_655 4_655
O4 O2 Ga4 126(3) 4 4_655
O6 O2 Ga4 50.3(12) 1_565 4_655
O1 O2 Ga4 135(2) 4 4_655
O4 O2 Ga4 66.6(18) 1_655 4_655
O6 O2 Ga4 74.5(15) 1_465 4_655
O1 O2 Ga4 106.8(18) 4_655 4_655
Ta O2 Ga4 40.3(7) 1_565 4_655
Ga1 O2 Ga4 40.3(7) 1_565 4_655
O4 O2 Ga4 89.9(15) . 4_655
O1 O2 Ga4 74.0(13) . 4_655
Ga2 O2 Ga4 67.9(9) . 4_655
Ga3 O2 Ga4 41.0(6) 1_565 4_655
O6 O2 Ga4 113.8(14) 4_655 4_655
La1 O2 Ga4 86.6(11) 3_654 4_655
La1 O2 Ga4 82.5(11) 2_666 4_655
O5 O2 Ga4 112.9(14) 4_655 4_655
Ga4 O2 Ga4 82.1(11) 3_454 4_655
O3 O2 Ga4 62.6(11) 1_565 4_655
La2 O2 Ga4 170.9(17) 3 4_655
Ga4 O2 Ga4 124.7(16) 2_666 4_655
Ga3 O2 Ga4 137.3(15) 3 4_655
O7 O2 Ga4 23.2(7) 2_655 4_655
La2 O2 Ga4 48.9(6) . 4_655
Ga2 O2 Ga4 123.3(14) 4 4_655
O2 O2 Ga4 87.0(16) 4_645 4_655
O2 O2 Ga4 101(2) 4_655 4_655
O1 O2 Ga4 90.1(16) 1_565 4_655
O7 O2 Ga4 48.9(8) 2 4_655
O5 O2 Ga4 125.4(14) 4 4_655
Ta O2 Ga4 38.1(5) 1_665 4_655
Ga1 O2 Ga4 38.1(5) 1_665 4_655
O6 O2 Ga4 21.8(5) 2_665 4_655
Ga2 O2 Ga4 84.5(12) 1_565 4_655
Ga4 O2 O3 105(3) 3_554 1_465
Ga2 O2 O3 127(3) 4_655 1_465
O5 O2 O3 44.3(17) 1_565 1_465
La1 O2 O3 105.4(16) 3_554 1_465
O7 O2 O3 80.6(19) . 1_465
La1 O2 O3 24.8(9) 2_566 1_465
O3 O2 O3 127(2) 4_655 1_465
O4 O2 O3 75(3) 4 1_465
O6 O2 O3 105(2) 1_565 1_465
O1 O2 O3 69.3(18) 4 1_465
O4 O2 O3 146(3) 1_655 1_465
O6 O2 O3 33.9(11) 1_465 1_465
O1 O2 O3 135(2) 4_655 1_465
Ta O2 O3 45.5(10) 1_565 1_465
Ga1 O2 O3 45.5(10) 1_565 1_465
O4 O2 O3 76.2(13) . 1_465
O1 O2 O3 116.6(16) . 1_465
Ga2 O2 O3 135.0(17) . 1_465
Ga3 O2 O3 58.7(11) 1_565 1_465
O6 O2 O3 134.5(13) 4_655 1_465
La1 O2 O3 159.4(16) 3_654 1_465
La1 O2 O3 103.2(15) 2_666 1_465
O5 O2 O3 166.4(15) 4_655 1_465
Ga4 O2 O3 51.3(8) 3_454 1_465
O3 O2 O3 68.3(10) 1_565 1_465
La2 O2 O3 92.2(12) 3 1_465
Ga4 O2 O3 81.7(13) 2_666 1_465
Ga3 O2 O3 142.5(15) 3 1_465
O7 O2 O3 101.5(16) 2_655 1_465
La2 O2 O3 88.5(13) . 1_465
Ga2 O2 O3 61.6(9) 4 1_465
O2 O2 O3 158(2) 4_645 1_465
O2 O2 O3 77.4(13) 4_655 1_465
O1 O2 O3 36.6(9) 1_565 1_465
O7 O2 O3 59.9(11) 2 1_465
O5 O2 O3 104.2(10) 4 1_465
Ta O2 O3 99.5(14) 1_665 1_465
Ga1 O2 O3 99.5(14) 1_665 1_465
O6 O2 O3 58.2(10) 2_665 1_465
Ga2 O2 O3 57.5(10) 1_565 1_465
Ga4 O2 O3 79.6(13) 4_655 1_465
Ga4 O2 O5 34.7(18) 3_554 2_665
Ga2 O2 O5 119(2) 4_655 2_665
O5 O2 O5 32.5(17) 1_565 2_665
La1 O2 O5 134(2) 3_554 2_665
O7 O2 O5 51.5(16) . 2_665
La1 O2 O5 94(2) 2_566 2_665
O3 O2 O5 154(2) 4_655 2_665
O4 O2 O5 102(3) 4 2_665
O6 O2 O5 33.6(12) 1_565 2_665
O1 O2 O5 145(3) 4 2_665
O4 O2 O5 74.6(19) 1_655 2_665
O6 O2 O5 86.3(18) 1_465 2_665
O1 O2 O5 91.0(16) 4_655 2_665
Ta O2 O5 53.0(11) 1_565 2_665
Ga1 O2 O5 53.0(11) 1_565 2_665
O4 O2 O5 113.1(19) . 2_665
O1 O2 O5 97.5(16) . 2_665
Ga2 O2 O5 85.3(12) . 2_665
Ga3 O2 O5 21.3(5) 1_565 2_665
O6 O2 O5 133.2(16) 4_655 2_665
La1 O2 O5 84.3(10) 3_654 2_665
La1 O2 O5 59.7(9) 2_666 2_665
O5 O2 O5 116.9(14) 4_655 2_665
Ga4 O2 O5 99.4(15) 3_454 2_665
O3 O2 O5 37.8(9) 1_565 2_665
La2 O2 O5 155.8(18) 3 2_665
Ga4 O2 O5 99.6(14) 2_666 2_665
Ga3 O2 O5 138.6(14) 3 2_665
O7 O2 O5 30.7(8) 2_655 2_665
La2 O2 O5 74.2(11) . 2_665
Ga2 O2 O5 135.2(18) 4 2_665
O2 O2 O5 98.3(18) 4_645 2_665
O2 O2 O5 75.5(17) 4_655 2_665
O1 O2 O5 72.7(14) 1_565 2_665
O7 O2 O5 69.7(12) 2 2_665
O5 O2 O5 150.7(17) 4 2_665
Ta O2 O5 23.8(5) 1_665 2_665
Ga1 O2 O5 23.8(5) 1_665 2_665
O6 O2 O5 33.5(7) 2_665 2_665
Ga2 O2 O5 61.4(10) 1_565 2_665
Ga4 O2 O5 25.3(7) 4_655 2_665
O3 O2 O5 76.7(13) 1_465 2_665
Ga4 O2 O2 122.5(19) 3_554 1_455
Ga2 O2 O2 120.7(18) 4_655 1_455
O5 O2 O2 87.2(18) 1_565 1_455
La1 O2 O2 55.2(15) 3_554 1_455
O7 O2 O2 83.1(15) . 1_455
La1 O2 O2 53.2(14) 2_566 1_455
O3 O2 O2 89.9(16) 4_655 1_455
O4 O2 O2 96(2) 4 1_455
O6 O2 O2 149.9(16) 1_565 1_455
O1 O2 O2 33.0(19) 4 1_455
O4 O2 O2 130.9(16) 1_655 1_455
O6 O2 O2 30.1(14) 1_465 1_455
O1 O2 O2 150.8(16) 4_655 1_455
Ta O2 O2 64.1(9) 1_565 1_455
Ga1 O2 O2 64.1(9) 1_565 1_455
O4 O2 O2 32.4(12) . 1_455
O1 O2 O2 80.3(9) . 1_455
Ga2 O2 O2 106.1(8) . 1_455
Ga3 O2 O2 105.4(9) 1_565 1_455
O6 O2 O2 83.7(8) 4_655 1_455
La1 O2 O2 148.5(9) 3_654 1_455
La1 O2 O2 150.8(10) 2_666 1_455
O5 O2 O2 118.5(8) 4_655 1_455
Ga4 O2 O2 21.2(8) 3_454 1_455
O3 O2 O2 119.2(8) 1_565 1_455
La2 O2 O2 69.1(8) 3 1_455
Ga4 O2 O2 104.7(8) 2_666 1_455
Ga3 O2 O2 103.4(7) 3 1_455
O7 O2 O2 122.7(9) 2_655 1_455
La2 O2 O2 71.4(7) . 1_455
Ga2 O2 O2 20.9(9) 4 1_455
O2 O2 O2 116.7(13) 4_645 1_455
O2 O2 O2 116.7(13) 4_655 1_455
O1 O2 O2 81.2(8) 1_565 1_455
O7 O2 O2 54.8(7) 2 1_455
O5 O2 O2 54.0(9) 4 1_455
Ta O2 O2 139.0(8) 1_665 1_455
Ga1 O2 O2 139.0(8) 1_665 1_455
O6 O2 O2 84.3(7) 2_665 1_455
Ga2 O2 O2 104.5(8) 1_565 1_455
Ga4 O2 O2 102.4(7) 4_655 1_455
O3 O2 O2 50.9(7) 1_465 1_455
O5 O2 O2 116.3(9) 2_665 1_455
Ga4 O2 O2 57.5(19) 3_554 1_655
Ga2 O2 O2 59.3(18) 4_655 1_655
O5 O2 O2 92.8(18) 1_565 1_655
La1 O2 O2 124.8(14) 3_554 1_655
O7 O2 O2 96.9(15) . 1_655
La1 O2 O2 126.8(14) 2_566 1_655
O3 O2 O2 90.1(16) 4_655 1_655
O4 O2 O2 84(2) 4 1_655
O6 O2 O2 30.1(16) 1_565 1_655
O1 O2 O2 147.0(19) 4 1_655
O4 O2 O2 49.1(16) 1_655 1_655
O6 O2 O2 149.9(14) 1_465 1_655
O1 O2 O2 29.2(16) 4_655 1_655
Ta O2 O2 115.9(9) 1_565 1_655
Ga1 O2 O2 115.9(9) 1_565 1_655
O4 O2 O2 147.6(12) . 1_655
O1 O2 O2 99.7(9) . 1_655
Ga2 O2 O2 73.9(8) . 1_655
Ga3 O2 O2 74.6(9) 1_565 1_655
O6 O2 O2 96.3(8) 4_655 1_655
La1 O2 O2 31.5(10) 3_654 1_655
La1 O2 O2 29.2(10) 2_666 1_655
O5 O2 O2 61.5(8) 4_655 1_655
Ga4 O2 O2 158.8(8) 3_454 1_655
O3 O2 O2 60.8(8) 1_565 1_655
La2 O2 O2 110.9(8) 3 1_655
Ga4 O2 O2 75.3(8) 2_666 1_655
Ga3 O2 O2 76.6(7) 3 1_655
O7 O2 O2 57.3(9) 2_655 1_655
La2 O2 O2 108.6(7) . 1_655
Ga2 O2 O2 159.1(9) 4 1_655
O2 O2 O2 63.3(13) 4_645 1_655
O2 O2 O2 63.3(13) 4_655 1_655
O1 O2 O2 98.8(8) 1_565 1_655
O7 O2 O2 125.2(7) 2 1_655
O5 O2 O2 126.0(9) 4 1_655
Ta O2 O2 41.0(8) 1_665 1_655
Ga1 O2 O2 41.0(8) 1_665 1_655
O6 O2 O2 95.7(7) 2_665 1_655
Ga2 O2 O2 75.5(8) 1_565 1_655
Ga4 O2 O2 77.6(7) 4_655 1_655
O3 O2 O2 129.1(7) 1_465 1_655
O5 O2 O2 63.7(9) 2_665 1_655
O2 O2 O2 179.999(12) 1_455 1_655
Ga4 O2 O7 117(2) 3_554 4_655
Ga2 O2 O7 26.1(16) 4_655 4_655
O5 O2 O7 111(2) 1_565 4_655
La1 O2 O7 119(2) 3_554 4_655
O7 O2 O7 155.1(19) . 4_655
La1 O2 O7 82.3(16) 2_566 4_655
O3 O2 O7 61.2(15) 4_655 4_655
O4 O2 O7 29(2) 4 4_655
O6 O2 O7 81.2(15) 1_565 4_655
O1 O2 O7 90(2) 4 4_655
O4 O2 O7 101.3(18) 1_655 4_655
O6 O2 O7 133(2) 1_465 4_655
O1 O2 O7 37.7(14) 4_655 4_655
Ta O2 O7 142(2) 1_565 4_655
Ga1 O2 O7 142(2) 1_565 4_655
O4 O2 O7 140.6(17) . 4_655
O1 O2 O7 137(2) . 4_655
Ga2 O2 O7 120.8(16) . 4_655
Ga3 O2 O7 97.1(13) 1_565 4_655
O6 O2 O7 99.6(16) 4_655 4_655
La1 O2 O7 73.6(10) 3_654 4_655
La1 O2 O7 47.1(8) 2_666 4_655
O5 O2 O7 73.1(13) 4_655 4_655
Ga4 O2 O7 139.4(14) 3_454 4_655
O3 O2 O7 71.7(12) 1_565 4_655
La2 O2 O7 56.3(9) 3 4_655
Ga4 O2 O7 22.0(6) 2_666 4_655
Ga3 O2 O7 61.7(10) 3 4_655
O7 O2 O7 116.0(12) 2_655 4_655
La2 O2 O7 167.4(16) . 4_655
Ga2 O2 O7 100.4(11) 4 4_655
O2 O2 O7 98(2) 4_645 4_655
O2 O2 O7 35.8(13) 4_655 4_655
O1 O2 O7 70.1(13) 1_565 4_655
O7 O2 O7 163(2) 2 4_655
O5 O2 O7 103.3(15) 4 4_655
Ta O2 O7 93.0(10) 1_665 4_655
Ga1 O2 O7 93.0(10) 1_665 4_655
O6 O2 O7 133.4(16) 2_665 4_655
Ga2 O2 O7 58.8(9) 1_565 4_655
Ga4 O2 O7 129.2(13) 4_655 4_655
O3 O2 O7 103.7(14) 1_465 4_655
O5 O2 O7 104.9(12) 2_665 4_655
O2 O2 O7 118.9(7) 1_455 4_655
O2 O2 O7 61.1(7) 1_655 4_655
Ga4 O2 Ga4 84(2) 3_554 2_656
Ga2 O2 Ga4 70(2) 4_655 2_656
O5 O2 Ga4 144(3) 1_565 2_656
La1 O2 Ga4 46.5(12) 3_554 2_656
O7 O2 Ga4 90.5(18) . 2_656
La1 O2 Ga4 147(2) 2_566 2_656
O3 O2 Ga4 47.8(11) 4_655 2_656
O4 O2 Ga4 121(3) 4 2_656
O6 O2 Ga4 98.0(17) 1_565 2_656
O1 O2 Ga4 91(2) 4 2_656
O4 O2 Ga4 44.1(16) 1_655 2_656
O6 O2 Ga4 119.0(19) 1_465 2_656
O1 O2 Ga4 71.7(18) 4_655 2_656
Ta O2 Ga4 121.9(16) 1_565 2_656
Ga1 O2 Ga4 121.9(16) 1_565 2_656
O4 O2 Ga4 75.6(13) . 2_656
O1 O2 Ga4 41.7(12) . 2_656
Ga2 O2 Ga4 36.2(7) . 2_656
Ga3 O2 Ga4 139.5(14) 1_565 2_656
O6 O2 Ga4 18.8(5) 4_655 2_656
La1 O2 Ga4 47.0(8) 3_654 2_656
La1 O2 Ga4 105.2(14) 2_666 2_656
O5 O2 Ga4 23.7(6) 4_655 2_656
Ga4 O2 Ga4 100.8(13) 3_454 2_656
O3 O2 Ga4 138.7(12) 1_565 2_656
La2 O2 Ga4 81.5(12) 3 2_656
Ga4 O2 Ga4 116.3(15) 2_666 2_656
Ga3 O2 Ga4 37.5(6) 3 2_656
O7 O2 Ga4 88.0(12) 2_655 2_656
La2 O2 Ga4 74.2(10) . 2_656
Ga2 O2 Ga4 94.9(13) 4 2_656
O2 O2 Ga4 20.3(9) 4_645 2_656
O2 O2 Ga4 128(2) 4_655 2_656
O1 O2 Ga4 164.6(17) 1_565 2_656
O7 O2 Ga4 100.7(13) 2 2_656
O5 O2 Ga4 50.4(9) 4 2_656
Ta O2 Ga4 99.9(11) 1_665 2_656
Ga1 O2 Ga4 99.9(11) 1_665 2_656
O6 O2 Ga4 120.0(13) 2_665 2_656
Ga2 O2 Ga4 150.2(14) 1_565 2_656
Ga4 O2 Ga4 103.9(11) 4_655 2_656
O3 O2 Ga4 151.6(12) 1_465 2_656
O5 O2 Ga4 118.2(13) 2_665 2_656
O2 O2 Ga4 101.5(6) 1_455 2_656
O2 O2 Ga4 78.5(7) 1_655 2_656
O7 O2 Ga4 95.8(13) 4_655 2_656
Ga4 O2 O2 99(2) 3_554 4_545
Ga2 O2 O2 106(3) 4_655 4_545
O5 O2 O2 119(3) 1_565 4_545
La1 O2 O2 9.1(4) 3_554 4_545
O7 O2 O2 73.7(16) . 4_545
La1 O2 O2 106(2) 2_566 4_545
O3 O2 O2 66.9(17) 4_655 4_545
O4 O2 O2 131(3) 4 4_545
O6 O2 O2 133.2(18) 1_565 4_545
O1 O2 O2 59(2) 4 4_545
O4 O2 O2 80.1(16) 1_655 4_545
O6 O2 O2 70.0(19) 1_465 4_545
O1 O2 O2 120(3) 4_655 4_545
Ta O2 O2 86.4(18) 1_565 4_545
Ga1 O2 O2 86.4(18) 1_565 4_545
O4 O2 O2 26.2(11) . 4_545
O1 O2 O2 33.2(6) . 4_545
Ga2 O2 O2 56.7(4) . 4_545
Ga3 O2 O2 135(2) 1_565 4_545
O6 O2 O2 35.2(9) 4_655 4_545
La1 O2 O2 95.3(13) 3_654 4_545
La1 O2 O2 155(2) 2_666 4_545
O5 O2 O2 71.5(13) 4_655 4_545
Ga4 O2 O2 51.4(13) 3_454 4_545
O3 O2 O2 160(3) 1_565 4_545
La2 O2 O2 78.1(18) 3 4_545
Ga4 O2 O2 135(2) 2_666 4_545
Ga3 O2 O2 70.3(15) 3 4_545
O7 O2 O2 102.2(14) 2_655 4_545
La2 O2 O2 50.8(10) . 4_545
Ga2 O2 O2 55.5(14) 4 4_545
O2 O2 O2 63.1(4) 4_645 4_545
O2 O2 O2 159(3) 4_655 4_545
O1 O2 O2 134.8(19) 1_565 4_545
O7 O2 O2 63.4(14) 2 4_545
O5 O2 O2 25.7(11) 4 4_545
Ta O2 O2 126.2(15) 1_665 4_545
Ga1 O2 O2 126.2(15) 1_665 4_545
O6 O2 O2 98.7(18) 2_665 4_545
Ga2 O2 O2 158.2(18) 1_565 4_545
Ga4 O2 O2 99.6(16) 4_655 4_545
O3 O2 O2 101.9(17) 1_465 4_545
O5 O2 O2 125(2) 2_665 4_545
O2 O2 O2 53.6(11) 1_455 4_545
O2 O2 O2 126.4(11) 1_655 4_545
O7 O2 O2 128(2) 4_655 4_545
Ga4 O2 O2 49.7(8) 2_656 4_545
Ga4 O2 O2 136(4) 3_554 4
Ga2 O2 O2 94(2) 4_655 4
O5 O2 O2 73(2) 1_565 4
La1 O2 O2 103(2) 3_554 4
O7 O2 O2 114(3) . 4
La1 O2 O2 9.69(18) 2_566 4
O3 O2 O2 96(2) 4_655 4
O4 O2 O2 46.9(16) 4 4
O6 O2 O2 119.3(19) 1_565 4
O1 O2 O2 50(2) 4 4
O4 O2 O2 175(2) 1_655 4
O6 O2 O2 57.6(18) 1_465 4
O1 O2 O2 113(2) 4_655 4
Ta O2 O2 79(2) 1_565 4
Ga1 O2 O2 79(2) 1_565 4
O4 O2 O2 86.1(19) . 4
O1 O2 O2 134(2) . 4
Ga2 O2 O2 159.8(19) . 4
Ga3 O2 O2 81.4(14) 1_565 4
O6 O2 O2 122.0(19) 4_655 4
La1 O2 O2 149(2) 3_654 4
La1 O2 O2 97.7(10) 2_666 4
O5 O2 O2 134(2) 4_655 4
Ga4 O2 O2 67.5(17) 3_454 4
O3 O2 O2 77.3(10) 1_565 4
La2 O2 O2 60.3(13) 3 4
Ga4 O2 O2 55.3(8) 2_666 4
Ga3 O2 O2 110.3(19) 3 4
O7 O2 O2 132(2) 2_655 4
La2 O2 O2 117(2) . 4
Ga2 O2 O2 49.5(13) 4 4
O2 O2 O2 159(3) 4_645 4
O2 O2 O2 63.1(4) 4_655 4
O1 O2 O2 33.4(6) 1_565 4
O7 O2 O2 90(2) 2 4
O5 O2 O2 92.0(16) 4 4
Ta O2 O2 120.2(16) 1_665 4
Ga1 O2 O2 120.2(16) 1_665 4
O6 O2 O2 91.9(19) 2_665 4
Ga2 O2 O2 54.8(5) 1_565 4
Ga4 O2 O2 112(2) 4_655 4
O3 O2 O2 34.2(11) 1_465 4
O5 O2 O2 102.6(17) 2_665 4
O2 O2 O2 53.6(11) 1_455 4
O2 O2 O2 126.4(11) 1_655 4
O7 O2 O2 75.6(12) 4_655 4
Ga4 O2 O2 139.1(19) 2_656 4
O2 O2 O2 105(2) 4_545 4
Ga4 O2 O3 39.7(19) 3_554 .
Ga2 O2 O3 103(2) 4_655 .
O5 O2 O3 98(2) 1_565 .
La1 O2 O3 69.9(14) 3_554 .
O7 O2 O3 49.8(15) . .
La1 O2 O3 155(2) 2_566 .
O3 O2 O3 93.7(16) 4_655 .
O4 O2 O3 151(3) 4 .
O6 O2 O3 67.8(13) 1_565 .
O1 O2 O3 124(2) 4 .
O4 O2 O3 21.3(15) 1_655 .
O6 O2 O3 104.5(17) 1_465 .
O1 O2 O3 85.0(17) 4_655 .
Ta O2 O3 84.8(13) 1_565 .
Ga1 O2 O3 84.8(13) 1_565 .
O4 O2 O3 79.2(13) . .
O1 O2 O3 32.8(8) . .
Ga2 O2 O3 11.0(5) . .
Ga3 O2 O3 95.3(12) 1_565 .
O6 O2 O3 58.9(9) 4_655 .
La1 O2 O3 48.8(7) 3_654 .
La1 O2 O3 95.8(10) 2_666 .
O5 O2 O3 58.7(9) 4_655 .
Ga4 O2 O3 95.2(12) 3_454 .
O3 O2 O3 107.1(12) 1_565 .
La2 O2 O3 127.5(16) 3 .
Ga4 O2 O3 142.4(13) 2_666 .
Ga3 O2 O3 81.2(11) 3 .
O7 O2 O3 43.7(9) 2_655 .
La2 O2 O3 45.1(8) . .
Ga2 O2 O3 120.5(13) 4 .
O2 O2 O3 30.5(10) 4_645 .
O2 O2 O3 130.9(17) 4_655 .
O1 O2 O3 146.9(16) 1_565 .
O7 O2 O3 72.3(11) 2 .
O5 O2 O3 84.0(12) 4 .
Ta O2 O3 63.0(8) 1_665 .
Ga1 O2 O3 63.0(8) 1_665 .
O6 O2 O3 75.7(11) 2_665 .
Ga2 O2 O3 132.0(12) 1_565 .
Ga4 O2 O3 57.8(8) 4_655 .
O3 O2 O3 130.2(17) 1_465 .
O5 O2 O3 74.3(10) 2_665 .
O2 O2 O3 111.2(6) 1_455 .
O2 O2 O3 68.8(6) 1_655 .
O7 O2 O3 122.4(12) 4_655 .
Ga4 O2 O3 46.2(6) 2_656 .
O2 O2 O3 65.5(8) 4_545 .
O2 O2 O3 162(2) 4 .
Ga4 O2 Ga2 92(2) 3_554 1_455
Ga2 O2 Ga2 125(3) 4_655 1_455
O5 O2 Ga2 100(2) 1_565 1_455
La1 O2 Ga2 27.7(9) 3_554 1_455
O7 O2 Ga2 59.2(13) . 1_455
La1 O2 Ga2 96.7(16) 2_566 1_455
O3 O2 Ga2 85.5(16) 4_655 1_455
O4 O2 Ga2 137(3) 4 1_455
O6 O2 Ga2 129.3(18) 1_565 1_455
O1 O2 Ga2 62.0(18) 4 1_455
O4 O2 Ga2 86.5(19) 1_655 1_455
O6 O2 Ga2 52.9(12) 1_465 1_455
O1 O2 Ga2 138(2) 4_655 1_455
Ta O2 Ga2 67.2(10) 1_565 1_455
Ga1 O2 Ga2 67.2(10) 1_565 1_455
O4 O2 Ga2 12.0(8) . 1_455
O1 O2 Ga2 35.9(6) . 1_455
Ga2 O2 Ga2 61.8(9) . 1_455
Ga3 O2 Ga2 116.5(14) 1_565 1_455
O6 O2 Ga2 53.9(9) 4_655 1_455
La1 O2 Ga2 107.8(14) 3_654 1_455
La1 O2 Ga2 163.0(15) 2_666 1_455
O5 O2 Ga2 89.2(12) 4_655 1_455
Ga4 O2 Ga2 35.2(5) 3_454 1_455
O3 O2 Ga2 141.7(17) 1_565 1_455
La2 O2 Ga2 90.1(11) 3 1_455
Ga4 O2 Ga2 144.2(14) 2_666 1_455
Ga3 O2 Ga2 89.7(12) 3 1_455
O7 O2 Ga2 94.3(12) 2_655 1_455
La2 O2 Ga2 37.7(5) . 1_455
Ga2 O2 Ga2 54.5(7) 4 1_455
O2 O2 Ga2 75.2(10) 4_645 1_455
O2 O2 Ga2 161.1(18) 4_655 1_455
O1 O2 Ga2 122.3(14) 1_565 1_455
O7 O2 Ga2 44.4(7) 2 1_455
O5 O2 Ga2 41.7(7) 4 1_455
Ta O2 Ga2 118.9(12) 1_665 1_455
Ga1 O2 Ga2 118.9(12) 1_665 1_455
O6 O2 Ga2 80.7(10) 2_665 1_455
Ga2 O2 Ga2 143.7(16) 1_565 1_455
Ga4 O2 Ga2 85.5(10) 4_655 1_455
O3 O2 Ga2 86.4(10) 1_465 1_455
O5 O2 Ga2 110.3(13) 2_665 1_455
O2 O2 Ga2 44.4(7) 1_455 1_455
O2 O2 Ga2 135.6(7) 1_655 1_455
O7 O2 Ga2 144.7(14) 4_655 1_455
Ga4 O2 Ga2 66.1(8) 2_656 1_455
O2 O2 Ga2 19.4(9) 4_545 1_455
O2 O2 Ga2 98.0(16) 4 1_455
O3 O2 Ga2 67.5(8) . 1_455
Ga4 O2 La2 104(2) 3_554 3_655
Ga2 O2 La2 11.6(12) 4_655 3_655
O5 O2 La2 126(2) 1_565 3_655
La1 O2 La2 106(2) 3_554 3_655
O7 O2 La2 142(2) . 3_655
La1 O2 La2 107.3(18) 2_566 3_655
O3 O2 La2 49.8(14) 4_655 3_655
O4 O2 La2 55(2) 4 3_655
O6 O2 La2 75.9(14) 1_565 3_655
O1 O2 La2 99(2) 4 3_655
O4 O2 La2 77.7(17) 1_655 3_655
O6 O2 La2 156.3(19) 1_465 3_655
O1 O2 La2 18.8(13) 4_655 3_655
Ta O2 La2 159.0(18) 1_565 3_655
Ga1 O2 La2 159.0(18) 1_565 3_655
O4 O2 La2 136.5(19) . 3_655
O1 O2 La2 112.9(18) . 3_655
Ga2 O2 La2 95.3(14) . 3_655
Ga3 O2 La2 108.9(13) 1_565 3_655
O6 O2 La2 80.0(13) 4_655 3_655
La1 O2 La2 50.0(7) 3_654 3_655
La1 O2 La2 49.5(7) 2_666 3_655
O5 O2 La2 48.6(9) 4_655 3_655
Ga4 O2 La2 152.4(15) 3_454 3_655
O3 O2 La2 84.8(11) 1_565 3_655
La2 O2 La2 63.0(9) 3 3_655
Ga4 O2 La2 47.6(7) 2_666 3_655
Ga3 O2 La2 43.4(6) 3 3_655
O7 O2 La2 104.8(11) 2_655 3_655
La2 O2 La2 142.1(16) . 3_655
Ga2 O2 La2 111.2(13) 4 3_655
O2 O2 La2 72.7(19) 4_645 3_655
O2 O2 La2 56.5(15) 4_655 3_655
O1 O2 La2 94.8(13) 1_565 3_655
O7 O2 La2 170.2(15) 2 3_655
O5 O2 La2 94.6(14) 4 3_655
Ta O2 La2 87.8(9) 1_665 3_655
Ga1 O2 La2 87.8(9) 1_665 3_655
O6 O2 La2 141.0(13) 2_665 3_655
Ga2 O2 La2 79.7(9) 1_565 3_655
Ga4 O2 La2 125.4(12) 4_655 3_655
O3 O2 La2 129.2(15) 1_465 3_655
O5 O2 La2 107.5(11) 2_665 3_655
O2 O2 La2 132.1(6) 1_455 3_655
O2 O2 La2 47.9(6) 1_655 3_655
O7 O2 La2 25.6(5) 4_655 3_655
Ga4 O2 La2 72.0(10) 2_656 3_655
O2 O2 La2 114(2) 4_545 3_655
O2 O2 La2 99.9(15) 4 3_655
O3 O2 La2 97.9(10) . 3_655
Ga2 O2 La2 133.1(15) 1_455 3_655
Ga4 O2 O3 66(2) 3_554 2_665
Ga2 O2 O3 127(3) 4_655 2_665
O5 O2 O3 7.7(15) 1_565 2_665
La1 O2 O3 134(2) 3_554 2_665
O7 O2 O3 62.9(17) . 2_665
La1 O2 O3 60.6(15) 2_566 2_665
O3 O2 O3 161(2) 4_655 2_665
O4 O2 O3 85(3) 4 2_665
O6 O2 O3 62.4(16) 1_565 2_665
O1 O2 O3 113(2) 4 2_665
O4 O2 O3 108(2) 1_655 2_665
O6 O2 O3 62.4(15) 1_465 2_665
O1 O2 O3 110(2) 4_655 2_665
Ta O2 O3 40.1(10) 1_565 2_665
Ga1 O2 O3 40.1(10) 1_565 2_665
O4 O2 O3 102.7(18) . 2_665
O1 O2 O3 115.3(17) . 2_665
Ga2 O2 O3 113.8(15) . 2_665
Ga3 O2 O3 15.6(5) 1_565 2_665
O6 O2 O3 156.8(16) 4_655 2_665
La1 O2 O3 116.5(15) 3_654 2_665
La1 O2 O3 72.7(12) 2_666 2_665
O5 O2 O3 149.8(15) 4_655 2_665
Ga4 O2 O3 80.0(13) 3_454 2_665
O3 O2 O3 35.3(10) 1_565 2_665
La2 O2 O3 128.7(15) 3 2_665
Ga4 O2 O3 86.9(12) 2_666 2_665
Ga3 O2 O3 163.2(16) 3 2_665
O7 O2 O3 62.6(12) 2_655 2_665
La2 O2 O3 83.3(12) . 2_665
Ga2 O2 O3 104.6(15) 4 2_665
O2 O2 O3 131(2) 4_645 2_665
O2 O2 O3 67.2(14) 4_655 2_665
O1 O2 O3 44.3(11) 1_565 2_665
O7 O2 O3 63.3(12) 2 2_665
O5 O2 O3 142.6(16) 4 2_665
Ta O2 O3 56.1(9) 1_665 2_665
Ga1 O2 O3 56.1(9) 1_665 2_665
O6 O2 O3 32.7(8) 2_665 2_665
Ga2 O2 O3 44.8(7) 1_565 2_665
Ga4 O2 O3 45.9(8) 4_655 2_665
O3 O2 O3 43.4(10) 1_465 2_665
O5 O2 O3 33.9(8) 2_665 2_665
O2 O2 O3 89.9(9) 1_455 2_665
O2 O2 O3 90.1(9) 1_655 2_665
O7 O2 O3 103.0(13) 4_655 2_665
Ga4 O2 O3 149.8(13) 2_656 2_665
O2 O2 O3 126(2) 4_545 2_665
O2 O2 O3 69.5(13) 4 2_665
O3 O2 O3 103.6(12) . 2_665
Ga2 O2 O3 107.0(13) 1_455 2_665
La2 O2 O3 119.8(13) 3_655 2_665
Ga4 O2 La2 18.4(17) 3_554 1_655
Ga2 O2 La2 102(2) 4_655 1_655
O5 O2 La2 81(2) 1_565 1_655
La1 O2 La2 95.2(16) 3_554 1_655
O7 O2 La2 49.2(13) . 1_655
La1 O2 La2 145(2) 2_566 1_655
O3 O2 La2 109.8(18) 4_655 1_655
O4 O2 La2 134(2) 4 1_655
O6 O2 La2 43.0(10) 1_565 1_655
O1 O2 La2 149(2) 4 1_655
O4 O2 La2 24.0(15) 1_655 1_655
O6 O2 La2 110.3(17) 1_465 1_655
O1 O2 La2 75.9(16) 4_655 1_655
Ta O2 La2 80.3(11) 1_565 1_655
Ga1 O2 La2 80.3(11) 1_565 1_655
O4 O2 La2 99.6(14) . 1_655
O1 O2 La2 57.1(9) . 1_655
Ga2 O2 La2 35.7(5) . 1_655
Ga3 O2 La2 73.2(9) 1_565 1_655
O6 O2 La2 82.1(11) 4_655 1_655
La1 O2 La2 45.6(6) 3_654 1_655
La1 O2 La2 74.2(9) 2_666 1_655
O5 O2 La2 70.2(10) 4_655 1_655
Ga4 O2 La2 108.5(12) 3_454 1_655
O3 O2 La2 81.9(10) 1_565 1_655
La2 O2 La2 145.1(17) 3 1_655
Ga4 O2 La2 125.9(12) 2_666 1_655
Ga3 O2 La2 94.7(12) 3 1_655
O7 O2 La2 22.0(6) 2_655 1_655
La2 O2 La2 57.1(7) . 1_655
Ga2 O2 La2 143.3(14) 4 1_655
O2 O2 La2 46.7(12) 4_645 1_655
O2 O2 La2 108.0(18) 4_655 1_655
O1 O2 La2 123.8(15) 1_565 1_655
O7 O2 La2 77.6(9) 2 1_655
O5 O2 La2 109.2(14) 4 1_655
Ta O2 La2 37.7(5) 1_665 1_655
Ga1 O2 La2 37.7(5) 1_665 1_655
O6 O2 La2 64.4(8) 2_665 1_655
Ga2 O2 La2 106.7(11) 1_565 1_655
Ga4 O2 La2 42.9(5) 4_655 1_655
O3 O2 La2 122.4(15) 1_465 1_655
O5 O2 La2 51.9(7) 2_665 1_655
O2 O2 La2 128.5(6) 1_455 1_655
O2 O2 La2 51.5(6) 1_655 1_655
O7 O2 La2 112.2(10) 4_655 1_655
Ga4 O2 La2 66.4(8) 2_656 1_655
O2 O2 La2 90.2(9) 4_545 1_655
O2 O2 La2 154(2) 4 1_655
O3 O2 La2 25.3(4) . 1_655
Ga2 O2 La2 88.8(9) 1_455 1_655
La2 O2 La2 93.3(9) 3_655 1_655
O3 O2 La2 84.5(11) 2_665 1_655
Ga4 O2 Ta 116(3) 3_554 3
Ga2 O2 Ta 69(2) 4_655 3
O5 O2 Ta 157(2) 1_565 3
La1 O2 Ta 28.8(10) 3_554 3
O7 O2 Ta 106.9(19) . 3
La1 O2 Ta 112.8(18) 2_566 3
O3 O2 Ta 30.0(10) 4_655 3
O4 O2 Ta 104(3) 4 3
O6 O2 Ta 131(2) 1_565 3
O1 O2 Ta 56.9(18) 4 3
O4 O2 Ta 78.0(19) 1_655 3
O6 O2 Ta 100.7(16) 1_465 3
O1 O2 Ta 87.0(19) 4_655 3
Ta O2 Ta 123.6(15) 1_565 3
Ga1 O2 Ta 123.6(15) 1_565 3
O4 O2 Ta 60.1(11) . 3
O1 O2 Ta 55.5(13) . 3
Ga2 O2 Ta 65.1(10) . 3
Ga3 O2 Ta 170.4(16) 1_565 3
O6 O2 Ta 17.2(5) 4_655 3
La1 O2 Ta 76.6(12) 3_654 3
La1 O2 Ta 124.7(16) 2_666 3
O5 O2 Ta 44.2(8) 4_655 3
Ga4 O2 Ta 82.7(10) 3_454 3
O3 O2 Ta 161.8(16) 1_565 3
La2 O2 Ta 52.7(8) 3 3
Ga4 O2 Ta 104.1(13) 2_666 3
Ga3 O2 Ta 33.9(6) 3 3
O7 O2 Ta 119.8(15) 2_655 3
La2 O2 Ta 84.6(11) . 3
Ga2 O2 Ta 62.6(9) 4 3
O2 O2 Ta 54.2(13) 4_645 3
O2 O2 Ta 126(2) 4_655 3
O1 O2 Ta 136.8(14) 1_565 3
O7 O2 Ta 100.7(12) 2 3
O5 O2 Ta 20.6(6) 4 3
Ta O2 Ta 133.8(15) 1_665 3
Ga1 O2 Ta 133.8(15) 1_665 3
O6 O2 Ta 135.2(13) 2_665 3
Ga2 O2 Ta 145.9(14) 1_565 3
Ga4 O2 Ta 129.4(13) 4_655 3
O3 O2 Ta 123.9(10) 1_465 3
O5 O2 Ta 150.4(15) 2_665 3
O2 O2 Ta 74.4(6) 1_455 3
O2 O2 Ta 105.6(6) 1_655 3
O7 O2 Ta 91.3(12) 4_655 3
Ga4 O2 Ta 33.9(5) 2_656 3
O2 O2 Ta 37.3(11) 4_545 3
O2 O2 Ta 105.4(17) 4 3
O3 O2 Ta 76.1(9) . 3
Ga2 O2 Ta 56.4(7) 1_455 3
La2 O2 Ta 77.0(10) 3_655 3
O3 O2 Ta 162.6(15) 2_665 3
La2 O2 Ta 99.2(11) 1_655 3
Ga4 O2 Ga1 116(3) 3_554 3
Ga2 O2 Ga1 69(2) 4_655 3
O5 O2 Ga1 157(2) 1_565 3
La1 O2 Ga1 28.8(10) 3_554 3
O7 O2 Ga1 106.9(19) . 3
La1 O2 Ga1 112.8(18) 2_566 3
O3 O2 Ga1 30.0(10) 4_655 3
O4 O2 Ga1 104(3) 4 3
O6 O2 Ga1 131(2) 1_565 3
O1 O2 Ga1 56.9(18) 4 3
O4 O2 Ga1 78.0(19) 1_655 3
O6 O2 Ga1 100.7(16) 1_465 3
O1 O2 Ga1 87.0(19) 4_655 3
Ta O2 Ga1 123.6(15) 1_565 3
Ga1 O2 Ga1 123.6(15) 1_565 3
O4 O2 Ga1 60.1(11) . 3
O1 O2 Ga1 55.5(13) . 3
Ga2 O2 Ga1 65.1(10) . 3
Ga3 O2 Ga1 170.4(16) 1_565 3
O6 O2 Ga1 17.2(5) 4_655 3
La1 O2 Ga1 76.6(12) 3_654 3
La1 O2 Ga1 124.7(16) 2_666 3
O5 O2 Ga1 44.2(8) 4_655 3
Ga4 O2 Ga1 82.7(10) 3_454 3
O3 O2 Ga1 161.8(16) 1_565 3
La2 O2 Ga1 52.7(8) 3 3
Ga4 O2 Ga1 104.1(13) 2_666 3
Ga3 O2 Ga1 33.9(6) 3 3
O7 O2 Ga1 119.8(15) 2_655 3
La2 O2 Ga1 84.6(11) . 3
Ga2 O2 Ga1 62.6(9) 4 3
O2 O2 Ga1 54.2(13) 4_645 3
O2 O2 Ga1 126(2) 4_655 3
O1 O2 Ga1 136.8(14) 1_565 3
O7 O2 Ga1 100.7(12) 2 3
O5 O2 Ga1 20.6(6) 4 3
Ta O2 Ga1 133.8(15) 1_665 3
Ga1 O2 Ga1 133.8(15) 1_665 3
O6 O2 Ga1 135.2(13) 2_665 3
Ga2 O2 Ga1 145.9(14) 1_565 3
Ga4 O2 Ga1 129.4(13) 4_655 3
O3 O2 Ga1 123.9(10) 1_465 3
O5 O2 Ga1 150.4(15) 2_665 3
O2 O2 Ga1 74.4(6) 1_455 3
O2 O2 Ga1 105.6(6) 1_655 3
O7 O2 Ga1 91.3(12) 4_655 3
Ga4 O2 Ga1 33.9(5) 2_656 3
O2 O2 Ga1 37.3(11) 4_545 3
O2 O2 Ga1 105.4(17) 4 3
O3 O2 Ga1 76.1(9) . 3
Ga2 O2 Ga1 56.4(7) 1_455 3
La2 O2 Ga1 77.0(10) 3_655 3
O3 O2 Ga1 162.6(15) 2_665 3
La2 O2 Ga1 99.2(11) 1_655 3
Ta O2 Ga1 0.00(12) 3 3
Ga4 O2 Ga3 96(2) 3_554 1_465
Ga2 O2 Ga3 144(3) 4_655 1_465
O5 O2 Ga3 44.6(16) 1_565 1_465
La1 O2 Ga3 92.5(15) 3_554 1_465
O7 O2 Ga3 65.0(15) . 1_465
La1 O2 Ga3 41.0(12) 2_566 1_465
O3 O2 Ga3 131(2) 4_655 1_465
O4 O2 Ga3 93(3) 4 1_465
O6 O2 Ga3 108(2) 1_565 1_465
O1 O2 Ga3 69.9(18) 4 1_465
O4 O2 Ga3 132(2) 1_655 1_465
O6 O2 Ga3 17.2(9) 1_465 1_465
O1 O2 Ga3 152(2) 4_655 1_465
Ta O2 Ga3 31.4(6) 1_565 1_465
Ga1 O2 Ga3 31.4(6) 1_565 1_465
O4 O2 Ga3 61.0(11) . 1_465
O1 O2 Ga3 98.1(13) . 1_465
Ga2 O2 Ga3 116.9(13) . 1_465
Ga3 O2 Ga3 62.6(10) 1_565 1_465
O6 O2 Ga3 122.1(12) 4_655 1_465
La1 O2 Ga3 157.0(15) 3_654 1_465
La1 O2 Ga3 116.7(16) 2_666 1_465
O5 O2 Ga3 158.8(14) 4_655 1_465
Ga4 O2 Ga3 35.9(6) 3_454 1_465
O3 O2 Ga3 79.2(12) 1_565 1_465
La2 O2 Ga3 100.5(11) 3 1_465
Ga4 O2 Ga3 100.2(14) 2_666 1_465
Ga3 O2 Ga3 145.6(13) 3 1_465
O7 O2 Ga3 93.6(13) 2_655 1_465
La2 O2 Ga3 70.1(9) . 1_465
Ga2 O2 Ga3 59.5(8) 4 1_465
O2 O2 Ga3 139.4(18) 4_645 1_465
O2 O2 Ga3 95.2(15) 4_655 1_465
O1 O2 Ga3 54.7(11) 1_565 1_465
O7 O2 Ga3 41.7(7) 2 1_465
O5 O2 Ga3 95.9(10) 4 1_465
Ta O2 Ga3 99.5(13) 1_665 1_465
Ga1 O2 Ga3 99.5(13) 1_665 1_465
O6 O2 Ga3 48.8(7) 2_665 1_465
Ga2 O2 Ga3 73.9(11) 1_565 1_465
Ga4 O2 Ga3 70.5(9) 4_655 1_465
O3 O2 Ga3 18.6(5) 1_465 1_465
O5 O2 Ga3 75.7(12) 2_665 1_465
O2 O2 Ga3 42.8(7) 1_455 1_465
O2 O2 Ga3 137.2(7) 1_655 1_465
O7 O2 Ga3 122.2(14) 4_655 1_465
Ga4 O2 Ga3 136.0(12) 2_656 1_465
O2 O2 Ga3 87.2(16) 4_545 1_465
O2 O2 Ga3 49.4(14) 4 1_465
O3 O2 Ga3 113.5(12) . 1_465
Ga2 O2 Ga3 69.9(7) 1_455 1_465
La2 O2 Ga3 147.7(14) 3_655 1_465
O3 O2 Ga3 47.2(8) 2_665 1_465
La2 O2 Ga3 111.7(11) 1_655 1_465
Ta O2 Ga3 116.5(10) 3 1_465
Ga1 O2 Ga3 116.5(10) 3 1_465
Ga4 O2 O3 116(2) 3_554 3
Ga2 O2 O3 18.8(18) 4_655 3
O5 O2 O3 153(2) 1_565 3
La1 O2 O3 79.1(16) 3_554 3
O7 O2 O3 142(2) . 3
La1 O2 O3 112.0(19) 2_566 3
O3 O2 O3 23.6(14) 4_655 3
O4 O2 O3 68(3) 4 3
O6 O2 O3 97.8(17) 1_565 3
O1 O2 O3 81(2) 4 3
O4 O2 O3 77.1(17) 1_655 3
O6 O2 O3 142.2(18) 1_465 3
O1 O2 O3 40.6(14) 4_655 3
Ta O2 O3 173.8(18) 1_565 3
Ga1 O2 O3 173.8(18) 1_565 3
O4 O2 O3 109.7(16) . 3
O1 O2 O3 94.2(17) . 3
Ga2 O2 O3 85.2(12) . 3
Ga3 O2 O3 135.7(13) 1_565 3
O6 O2 O3 55.5(9) 4_655 3
La1 O2 O3 54.5(8) 3_654 3
La1 O2 O3 76.1(10) 2_666 3
O5 O2 O3 33.6(7) 4_655 3
Ga4 O2 O3 128.8(14) 3_454 3
O3 O2 O3 111.5(13) 1_565 3
La2 O2 O3 48.1(9) 3 3
Ga4 O2 O3 63.5(10) 2_666 3
Ga3 O2 O3 17.6(4) 3 3
O7 O2 O3 117.8(13) 2_655 3
La2 O2 O3 127.0(15) . 3
Ga2 O2 O3 92.3(12) 4 3
O2 O2 O3 62.0(17) 4_645 3
O2 O2 O3 79.7(19) 4_655 3
O1 O2 O3 111.9(15) 1_565 3
O7 O2 O3 150.5(16) 2 3
O5 O2 O3 67.9(11) 4 3
Ta O2 O3 108.6(10) 1_665 3
Ga1 O2 O3 108.6(10) 1_665 3
O6 O2 O3 162.4(12) 2_665 3
Ga2 O2 O3 103.0(12) 1_565 3
Ga4 O2 O3 141.0(12) 4_655 3
O3 O2 O3 136.8(16) 1_465 3
O5 O2 O3 131.3(11) 2_665 3
O2 O2 O3 112.3(6) 1_455 3
O2 O2 O3 67.7(6) 1_655 3
O7 O2 O3 44.2(9) 4_655 3
Ga4 O2 O3 52.9(7) 2_656 3
O2 O2 O3 87.4(17) 4_545 3
O2 O2 O3 102.5(19) 4 3
O3 O2 O3 92.2(10) . 3
Ga2 O2 O3 106.7(12) 1_455 3
La2 O2 O3 26.9(5) 3_655 3
O3 O2 O3 146.1(13) 2_665 3
La2 O2 O3 99.3(10) 1_655 3
Ta O2 O3 50.3(7) 3 3
Ga1 O2 O3 50.3(7) 3 3
Ga3 O2 O3 148.5(12) 1_465 3
Ga4 O2 O1 43.1(19) 3_554 1_655
Ga2 O2 O1 79(2) 4_655 1_655
O5 O2 O1 104(2) 1_565 1_655
La1 O2 O1 88.5(17) 3_554 1_655
O7 O2 O1 72.3(16) . 1_655
La1 O2 O1 165(2) 2_566 1_655
O3 O2 O1 85.3(18) 4_655 1_655
O4 O2 O1 122(3) 4 1_655
O6 O2 O1 50.9(12) 1_565 1_655
O1 O2 O1 138(3) 4 1_655
O4 O2 O1 7.9(14) 1_655 1_655
O6 O2 O1 132.0(18) 1_465 1_655
O1 O2 O1 56.6(16) 4_655 1_655
Ta O2 O1 105.4(14) 1_565 1_655
Ga1 O2 O1 105.4(14) 1_565 1_655
O4 O2 O1 106.3(15) . 1_655
O1 O2 O1 58.4(11) . 1_655
Ga2 O2 O1 32.6(7) . 1_655
Ga3 O2 O1 93.0(12) 1_565 1_655
O6 O2 O1 66.1(11) 4_655 1_655
La1 O2 O1 21.5(7) 3_654 1_655
La1 O2 O1 70.1(10) 2_666 1_655
O5 O2 O1 45.5(10) 4_655 1_655
Ga4 O2 O1 124.1(14) 3_454 1_655
O3 O2 O1 92.9(10) 1_565 1_655
La2 O2 O1 120.1(17) 3 1_655
Ga4 O2 O1 113.5(14) 2_666 1_655
Ga3 O2 O1 69.8(12) 3 1_655
O7 O2 O1 46.2(10) 2_655 1_655
La2 O2 O1 73.3(10) . 1_655
Ga2 O2 O1 141.2(17) 4 1_655
O2 O2 O1 27.7(12) 4_645 1_655
O2 O2 O1 104.6(18) 4_655 1_655
O1 O2 O1 136.5(15) 1_565 1_655
O7 O2 O1 98.9(12) 2 1_655
O5 O2 O1 97.3(15) 4 1_655
Ta O2 O1 52.2(8) 1_665 1_655
Ga1 O2 O1 52.2(8) 1_665 1_655
O6 O2 O1 89.9(11) 2_665 1_655
Ga2 O2 O1 114.0(12) 1_565 1_655
Ga4 O2 O1 68.3(9) 4_655 1_655
O3 O2 O1 147.7(16) 1_465 1_655
O5 O2 O1 72.8(10) 2_665 1_655
O2 O2 O1 138.7(8) 1_455 1_655
O2 O2 O1 41.3(8) 1_655 1_655
O7 O2 O1 94.3(12) 4_655 1_655
Ga4 O2 O1 47.7(8) 2_656 1_655
O2 O2 O1 87.2(10) 4_545 1_655
O2 O2 O1 167.7(16) 4 1_655
O3 O2 O1 28.9(7) . 1_655
Ga2 O2 O1 94.3(11) 1_455 1_655
La2 O2 O1 71.4(10) 3_655 1_655
O3 O2 O1 106.7(13) 2_665 1_655
La2 O2 O1 25.5(7) 1_655 1_655
Ta O2 O1 81.6(12) 3 1_655
Ga1 O2 O1 81.6(12) 3 1_655
Ga3 O2 O1 136.8(13) 1_465 1_655
O3 O2 O1 73.8(10) 3 1_655
Ga4 O2 O3 81(2) 3_554 4_755
Ga2 O2 O3 34.3(15) 4_655 4_755
O5 O2 O3 122(2) 1_565 4_755
La1 O2 O3 103.4(19) 3_554 4_755
O7 O2 O3 117.3(19) . 4_755
La1 O2 O3 130.6(19) 2_566 4_755
O3 O2 O3 60.2(14) 4_655 4_755
O4 O2 O3 78(2) 4 4_755
O6 O2 O3 60.0(14) 1_565 4_755
O1 O2 O3 119(2) 4 4_755
O4 O2 O3 52.8(15) 1_655 4_755
O6 O2 O3 178(2) 1_465 4_755
O1 O2 O3 12.9(14) 4_655 4_755
Ta O2 O3 144.6(15) 1_565 4_755
Ga1 O2 O3 144.6(15) 1_565 4_755
O4 O2 O3 134.8(17) . 4_755
O1 O2 O3 94.9(14) . 4_755
Ga2 O2 O3 72.9(10) . 4_755
Ga3 O2 O3 103.4(12) 1_565 4_755
O6 O2 O3 73.8(10) 4_655 4_755
La1 O2 O3 24.9(5) 3_654 4_755
La1 O2 O3 47.4(8) 2_666 4_755
O5 O2 O3 37.1(6) 4_655 4_755
Ga4 O2 O3 160.0(17) 3_454 4_755
O3 O2 O3 85.1(10) 1_565 4_755
La2 O2 O3 84.5(11) 3 4_755
Ga4 O2 O3 69.7(10) 2_666 4_755
Ga3 O2 O3 47.1(6) 3 4_755
O7 O2 O3 82.0(10) 2_655 4_755
La2 O2 O3 118.7(12) . 4_755
Ga2 O2 O3 130.5(15) 4 4_755
O2 O2 O3 52.7(15) 4_645 4_755
O2 O2 O3 70.5(16) 4_655 4_755
O1 O2 O3 111.3(13) 1_565 4_755
O7 O2 O3 145.0(13) 2 4_755
O5 O2 O3 99.1(13) 4 4_755
Ta O2 O3 70.4(9) 1_665 4_755
Ga1 O2 O3 70.4(9) 1_665 4_755
O6 O2 O3 124.6(12) 2_665 4_755
Ga2 O2 O3 90.8(11) 1_565 4_755
Ga4 O2 O3 104.6(11) 4_655 4_755
O3 O2 O3 147.8(14) 1_465 4_755
O5 O2 O3 93.5(10) 2_665 4_755
O2 O2 O3 150.1(7) 1_455 4_755
O2 O2 O3 29.9(7) 1_655 4_755
O7 O2 O3 48.7(8) 4_655 4_755
Ga4 O2 O3 59.5(7) 2_656 4_755
O2 O2 O3 108.6(15) 4_545 4_755
O2 O2 O3 124.3(17) 4 4_755
O3 O2 O3 73.6(8) . 4_755
Ga2 O2 O3 125.5(13) 1_455 4_755
La2 O2 O3 25.4(5) 3_655 4_755
O3 O2 O3 118.3(14) 2_665 4_755
La2 O2 O3 68.2(7) 1_655 4_755
Ta O2 O3 78.6(9) 3 4_755
Ga1 O2 O3 78.6(9) 3 4_755
Ga3 O2 O3 164.1(14) 1_465 4_755
O3 O2 O3 38.2(7) 3 4_755
O1 O2 O3 46.2(8) 1_655 4_755
Ga4 O2 O3 74(2) 3_554 1_455
Ga2 O2 O3 129(3) 4_655 1_455
O5 O2 O3 95(2) 1_565 1_455
La1 O2 O3 37.3(10) 3_554 1_455
O7 O2 O3 45.3(13) . 1_455
La1 O2 O3 110.2(16) 2_566 1_455
O3 O2 O3 93.4(16) 4_655 1_455
O4 O2 O3 155(3) 4 1_455
O6 O2 O3 111.5(17) 1_565 1_455
O1 O2 O3 79.9(18) 4 1_455
O4 O2 O3 71.0(18) 1_655 1_455
O6 O2 O3 60.9(13) 1_465 1_455
O1 O2 O3 130(2) 4_655 1_455
Ta O2 O3 63.5(10) 1_565 1_455
Ga1 O2 O3 63.5(10) 1_565 1_455
O4 O2 O3 28.9(9) . 1_455
O1 O2 O3 22.4(8) . 1_455
Ga2 O2 O3 46.7(8) . 1_455
Ga3 O2 O3 107.9(14) 1_565 1_455
O6 O2 O3 55.0(9) 4_655 1_455
La1 O2 O3 95.3(12) 3_654 1_455
La1 O2 O3 145.1(13) 2_666 1_455
O5 O2 O3 85.0(12) 4_655 1_455
Ga4 O2 O3 46.4(7) 3_454 1_455
O3 O2 O3 132.7(18) 1_565 1_455
La2 O2 O3 105.8(12) 3 1_455
Ga4 O2 O3 161.9(14) 2_666 1_455
Ga3 O2 O3 92.9(12) 3 1_455
O7 O2 O3 76.9(11) 2_655 1_455
La2 O2 O3 22.5(5) . 1_455
Ga2 O2 O3 72.4(8) 4 1_455
O2 O2 O3 64.5(11) 4_645 1_455
O2 O2 O3 170(2) 4_655 1_455
O1 O2 O3 130.9(14) 1_565 1_455
O7 O2 O3 40.4(8) 2 1_455
O5 O2 O3 54.0(8) 4 1_455
Ta O2 O3 101.7(11) 1_665 1_455
Ga1 O2 O3 101.7(11) 1_665 1_455
O6 O2 O3 71.8(10) 2_665 1_455
Ga2 O2 O3 146.4(15) 1_565 1_455
Ga4 O2 O3 71.3(9) 4_655 1_455
O3 O2 O3 94.5(11) 1_465 1_455
O5 O2 O3 96.6(13) 2_665 1_455
O2 O2 O3 60.5(5) 1_455 1_455
O2 O2 O3 119.5(5) 1_655 1_455
O7 O2 O3 154.4(16) 4_655 1_455
Ga4 O2 O3 61.3(7) 2_656 1_455
O2 O2 O3 28.4(9) 4_545 1_455
O2 O2 O3 113.3(15) 4 1_455
O3 O2 O3 50.7(6) . 1_455
Ga2 O2 O3 18.0(3) 1_455 1_455
La2 O2 O3 133.3(14) 3_655 1_455
O3 O2 O3 102.6(12) 2_665 1_455
La2 O2 O3 70.9(8) 1_655 1_455
Ta O2 O3 63.4(7) 3 1_455
Ga1 O2 O3 63.4(7) 3 1_455
Ga3 O2 O3 76.2(7) 1_465 1_455
O3 O2 O3 110.5(12) 3 1_455
O1 O2 O3 78.8(10) 1_655 1_455
O3 O2 O3 117.2(11) 4_755 1_455
Ga4 O2 O3 141(2) 3_554 4
Ga2 O2 O3 93(2) 4_655 4
O5 O2 O3 116(2) 1_565 4
La1 O2 O3 40.7(9) 3_554 4
O7 O2 O3 104.5(18) . 4
La1 O2 O3 67.2(14) 2_566 4
O3 O2 O3 60.0(13) 4_655 4
O4 O2 O3 89(2) 4 4
O6 O2 O3 178(2) 1_565 4
O1 O2 O3 13.9(16) 4 4
O4 O2 O3 122(2) 1_655 4
O6 O2 O3 59.9(13) 1_465 4
O1 O2 O3 123(2) 4_655 4
Ta O2 O3 93.3(13) 1_565 4
Ga1 O2 O3 93.3(13) 1_565 4
O4 O2 O3 40.7(10) . 4
O1 O2 O3 78.0(11) . 4
Ga2 O2 O3 100.9(12) . 4
Ga3 O2 O3 133.8(16) 1_565 4
O6 O2 O3 62.0(8) 4_655 4
La1 O2 O3 124.9(16) 3_654 4
La1 O2 O3 146.8(14) 2_666 4
O5 O2 O3 91.8(11) 4_655 4
Ga4 O2 O3 47.4(8) 3_454 4
O3 O2 O3 139.4(14) 1_565 4
La2 O2 O3 44.4(6) 3 4
Ga4 O2 O3 95.4(11) 2_666 4
Ga3 O2 O3 73.9(9) 3 4
O7 O2 O3 142.9(14) 2_655 4
La2 O2 O3 85.8(10) . 4
Ga2 O2 O3 14.3(5) 4 4
O2 O2 O3 100.0(15) 4_645 4
O2 O2 O3 116.5(17) 4_655 4
O1 O2 O3 95.6(12) 1_565 4
O7 O2 O3 79.6(10) 2 4
O5 O2 O3 30.4(5) 4 4
Ta O2 O3 166.5(14) 1_665 4
Ga1 O2 O3 166.5(14) 1_665 4
O6 O2 O3 113.3(13) 2_665 4
Ga2 O2 O3 116.6(12) 1_565 4
Ga4 O2 O3 128.5(13) 4_655 4
O3 O2 O3 75.6(9) 1_465 4
O5 O2 O3 146.1(16) 2_665 4
O2 O2 O3 29.9(8) 1_455 4
O2 O2 O3 150.1(8) 1_655 4
O7 O2 O3 100.3(10) 4_655 4
Ga4 O2 O3 80.7(9) 2_656 4
O2 O2 O3 44.9(12) 4_545 4
O2 O2 O3 62.4(14) 4 4
O3 O2 O3 110.3(11) . 4
Ga2 O2 O3 48.8(6) 1_455 4
La2 O2 O3 105.1(11) 3_655 4
O3 O2 O3 118.1(15) 2_665 4
La2 O2 O3 135.1(12) 1_655 4
Ta O2 O3 48.4(5) 3 4
Ga1 O2 O3 48.4(5) 3 4
Ga3 O2 O3 71.8(9) 1_465 4
O3 O2 O3 82.6(10) 3 4
O1 O2 O3 127.6(14) 1_655 4
O3 O2 O3 120.2(13) 4_755 4
O3 O2 O3 66.6(7) 1_455 4
Ga4 O2 La1 77(2) 3_554 2_556
Ga2 O2 La1 104(3) 4_655 2_556
O5 O2 La1 117(2) 1_565 2_556
La1 O2 La1 29.0(9) 3_554 2_556
O7 O2 La1 62.7(14) . 2_556
La1 O2 La1 129.3(18) 2_566 2_556
O3 O2 La1 72.8(13) 4_655 2_556
O4 O2 La1 148(3) 4 2_556
O6 O2 La1 108.9(16) 1_565 2_556
O1 O2 La1 83(2) 4 2_556
O4 O2 La1 55.9(16) 1_655 2_556
O6 O2 La1 84.7(15) 1_465 2_556
O1 O2 La1 106(2) 4_655 2_556
Ta O2 La1 87.9(12) 1_565 2_556
Ga1 O2 La1 87.9(12) 1_565 2_556
O4 O2 La1 44.6(10) . 2_556
O1 O2 La1 11.1(9) . 2_556
Ga2 O2 La1 32.1(5) . 2_556
Ga3 O2 La1 125.7(13) 1_565 2_556
O6 O2 La1 31.8(7) 4_655 2_556
La1 O2 La1 74.7(11) 3_654 2_556
La1 O2 La1 133.1(14) 2_666 2_556
O5 O2 La1 59.6(9) 4_655 2_556
Ga4 O2 La1 68.0(9) 3_454 2_556
O3 O2 La1 145.8(15) 1_565 2_556
La2 O2 La1 95.6(12) 3 2_556
Ga4 O2 La1 148.1(17) 2_666 2_556
Ga3 O2 La1 69.0(10) 3 2_556
O7 O2 La1 81.0(11) 2_655 2_556
La2 O2 La1 41.7(6) . 2_556
Ga2 O2 La1 80.1(10) 4 2_556
O2 O2 La1 42.1(8) 4_645 2_556
O2 O2 La1 164(2) 4_655 2_556
O1 O2 La1 155.2(15) 1_565 2_556
O7 O2 La1 65.4(9) 2 2_556
O5 O2 La1 44.6(7) 4 2_556
Ta O2 La1 103.3(11) 1_665 2_556
Ga1 O2 La1 103.3(11) 1_665 2_556
O6 O2 La1 92.4(10) 2_665 2_556
Ga2 O2 La1 169.4(15) 1_565 2_556
Ga4 O2 La1 85.0(9) 4_655 2_556
O3 O2 La1 118.7(11) 1_465 2_556
O5 O2 La1 108.6(12) 2_665 2_556
O2 O2 La1 76.1(6) 1_455 2_556
O2 O2 La1 103.9(6) 1_655 2_556
O7 O2 La1 130.5(15) 4_655 2_556
Ga4 O2 La1 35.9(5) 2_656 2_556
O2 O2 La1 24.6(5) 4_545 2_556
O2 O2 La1 128.8(16) 4 2_556
O3 O2 La1 41.1(5) . 2_556
Ga2 O2 La1 33.1(4) 1_455 2_556
La2 O2 La1 107.9(13) 3_655 2_556
O3 O2 La1 125.0(12) 2_665 2_556
La2 O2 La1 66.2(7) 1_655 2_556
Ta O2 La1 44.6(5) 3 2_556
Ga1 O2 La1 44.6(5) 3 2_556
Ga3 O2 La1 100.9(9) 1_465 2_556
O3 O2 La1 86.3(10) 3 2_556
O1 O2 La1 63.3(9) 1_655 2_556
O3 O2 La1 93.5(10) 4_755 2_556
O3 O2 La1 25.4(4) 1_455 2_556
O3 O2 La1 69.2(7) 4 2_556
Ga4 O2 La2 91(3) 3_554 1_565
Ga2 O2 La2 118(3) 4_655 1_565
O5 O2 La2 29.8(17) 1_565 1_565
La1 O2 La2 129.3(18) 3_554 1_565
O7 O2 La2 81.8(18) . 1_565
La1 O2 La2 35.7(12) 2_566 1_565
O3 O2 La2 138.6(18) 4_655 1_565
O4 O2 La2 67(3) 4 1_565
O6 O2 La2 82.3(17) 1_565 1_565
O1 O2 La2 90(2) 4 1_565
O4 O2 La2 133(2) 1_655 1_565
O6 O2 La2 54.9(13) 1_465 1_565
O1 O2 La2 115(2) 4_655 1_565
Ta O2 La2 50.0(10) 1_565 1_565
Ga1 O2 La2 50.0(10) 1_565 1_565
O4 O2 La2 98.6(15) . 1_565
O1 O2 La2 130.2(17) . 1_565
Ga2 O2 La2 137.1(15) . 1_565
Ga3 O2 La2 37.8(7) 1_565 1_565
O6 O2 La2 158.8(13) 4_655 1_565
La1 O2 La2 135.6(14) 3_654 1_565
La1 O2 La2 79.7(12) 2_666 1_565
O5 O2 La2 163.4(14) 4_655 1_565
Ga4 O2 La2 73.4(10) 3_454 1_565
O3 O2 La2 44.0(8) 1_565 1_565
La2 O2 La2 103.9(12) 3 1_565
Ga4 O2 La2 71.8(11) 2_666 1_565
Ga3 O2 La2 150.2(14) 3 1_565
O7 O2 La2 87.7(13) 2_655 1_565
La2 O2 La2 97.7(12) . 1_565
Ga2 O2 La2 84.5(11) 4 1_565
O2 O2 La2 156(2) 4_645 1_565
O2 O2 La2 59.4(12) 4_655 1_565
O1 O2 La2 23.3(9) 1_565 1_565
O7 O2 La2 71.3(11) 2 1_565
O5 O2 La2 128.3(12) 4 1_565
Ta O2 La2 78.7(11) 1_665 1_565
Ga1 O2 La2 78.7(11) 1_665 1_565
O6 O2 La2 52.7(8) 2_665 1_565
Ga2 O2 La2 36.7(6) 1_565 1_565
Ga4 O2 La2 70.0(10) 4_655 1_565
O3 O2 La2 24.3(5) 1_465 1_565
O5 O2 La2 58.4(10) 2_665 1_565
O2 O2 La2 75.2(6) 1_455 1_565
O2 O2 La2 104.8(6) 1_655 1_565
O7 O2 La2 92.3(12) 4_655 1_565
Ga4 O2 La2 171.9(13) 2_656 1_565
O2 O2 La2 124.8(18) 4_545 1_565
O2 O2 La2 44.4(10) 4 1_565
O3 O2 La2 127.6(13) . 1_565
Ga2 O2 La2 107.4(11) 1_455 1_565
La2 O2 La2 115.7(12) 3_655 1_565
O3 O2 La2 25.1(4) 2_665 1_565
La2 O2 La2 109.6(11) 1_655 1_565
Ta O2 La2 147.0(11) 3 1_565
Ga1 O2 La2 147.0(11) 3 1_565
Ga3 O2 La2 37.7(5) 1_465 1_565
O3 O2 La2 135.2(13) 3 1_565
O1 O2 La2 130.8(12) 1_655 1_565
O3 O2 La2 126.6(11) 4_755 1_565
O3 O2 La2 111.0(10) 1_455 1_565
O3 O2 La2 98.8(10) 4 1_565
La1 O2 La2 136.4(11) 2_556 1_565
Ga4 O2 O3 150(3) 3_554 3_455
Ga2 O2 O3 64(2) 4_655 3_455
O5 O2 O3 142(2) 1_565 3_455
La1 O2 O3 48.0(10) 3_554 3_455
O7 O2 O3 128.6(19) . 3_455
La1 O2 O3 80.2(15) 2_566 3_455
O3 O2 O3 31.6(15) 4_655 3_455
O4 O2 O3 75(2) 4 3_455
O6 O2 O3 151(2) 1_565 3_455
O1 O2 O3 29.2(16) 4 3_455
O4 O2 O3 111(2) 1_655 3_455
O6 O2 O3 89.2(13) 1_465 3_455
O1 O2 O3 92.8(19) 4_655 3_455
Ta O2 O3 123.1(12) 1_565 3_455
Ga1 O2 O3 123.1(12) 1_565 3_455
O4 O2 O3 65.4(12) . 3_455
O1 O2 O3 85.5(14) . 3_455
Ga2 O2 O3 99.4(13) . 3_455
Ga3 O2 O3 153.3(15) 1_565 3_455
O6 O2 O3 51.6(7) 4_655 3_455
La1 O2 O3 101.3(14) 3_654 3_455
La1 O2 O3 122.0(15) 2_666 3_455
O5 O2 O3 68.9(10) 4_655 3_455
Ga4 O2 O3 77.1(8) 3_454 3_455
O3 O2 O3 139.6(17) 1_565 3_455
La2 O2 O3 21.8(6) 3 3_455
Ga4 O2 O3 78.8(11) 2_666 3_455
Ga3 O2 O3 46.8(7) 3 3_455
O7 O2 O3 154.1(17) 2_655 3_455
La2 O2 O3 106.5(11) . 3_455
Ga2 O2 O3 39.7(6) 4 3_455
O2 O2 O3 87.3(17) 4_645 3_455
O2 O2 O3 103(2) 4_655 3_455
O1 O2 O3 102.4(13) 1_565 3_455
O7 O2 O3 108.1(10) 2 3_455
O5 O2 O3 30.9(6) 4 3_455
Ta O2 O3 161.4(14) 1_665 3_455
Ga1 O2 O3 161.4(14) 1_665 3_455
O6 O2 O3 143.1(11) 2_665 3_455
Ga2 O2 O3 115.1(13) 1_565 3_455
Ga4 O2 O3 155.0(13) 4_655 3_455
O3 O2 O3 97.6(9) 1_465 3_455
O5 O2 O3 174.2(15) 2_665 3_455
O2 O2 O3 59.2(6) 1_455 3_455
O2 O2 O3 120.8(6) 1_655 3_455
O7 O2 O3 75.7(11) 4_655 3_455
Ga4 O2 O3 67.2(8) 2_656 3_455
O2 O2 O3 56.3(13) 4_545 3_455
O2 O2 O3 71.9(14) 4 3_455
O3 O2 O3 110.4(11) . 3_455
Ga2 O2 O3 69.5(7) 1_455 3_455
La2 O2 O3 75.6(10) 3_655 3_455
O3 O2 O3 140.3(13) 2_665 3_455
La2 O2 O3 133.4(13) 1_655 3_455
Ta O2 O3 34.4(4) 3 3_455
Ga1 O2 O3 34.4(4) 3 3_455
Ga3 O2 O3 99.1(8) 1_465 3_455
O3 O2 O3 53.0(7) 3 3_455
O1 O2 O3 113.0(13) 1_655 3_455
O3 O2 O3 91.1(10) 4_755 3_455
O3 O2 O3 84.2(8) 1_455 3_455
O3 O2 O3 29.8(7) 4 3_455
La1 O2 O3 74.5(8) 2_556 3_455
La2 O2 O3 115.9(10) 1_565 3_455
Ga4 O2 O3 40.0(15) 3_554 2_655
Ga2 O2 O3 130(3) 4_655 2_655
O5 O2 O3 79.1(19) 1_565 2_655
La1 O2 O3 67.6(14) 3_554 2_655
O7 O2 O3 24.4(12) . 2_655
La1 O2 O3 127(2) 2_566 2_655
O3 O2 O3 112.3(17) 4_655 2_655
O4 O2 O3 169(3) 4 2_655
O6 O2 O3 77.2(14) 1_565 2_655
O1 O2 O3 114(2) 4 2_655
O4 O2 O3 48.2(16) 1_655 2_655
O6 O2 O3 77.2(13) 1_465 2_655
O1 O2 O3 111(2) 4_655 2_655
Ta O2 O3 58.4(9) 1_565 2_655
Ga1 O2 O3 58.4(9) 1_565 2_655
O4 O2 O3 61.7(12) . 2_655
O1 O2 O3 30.9(11) . 2_655
Ga2 O2 O3 32.5(7) . 2_655
Ga3 O2 O3 84.0(9) 1_565 2_655
O6 O2 O3 71.5(11) 4_655 2_655
La1 O2 O3 76.0(11) 3_654 2_655
La1 O2 O3 111.4(12) 2_666 2_655
O5 O2 O3 84.2(12) 4_655 2_655
Ga4 O2 O3 70.8(9) 3_454 2_655
O3 O2 O3 104.8(13) 1_565 2_655
La2 O2 O3 137.1(15) 3 2_655
Ga4 O2 O3 163.8(15) 2_666 2_655
Ga3 O2 O3 103.6(13) 3 2_655
O7 O2 O3 42.9(8) 2_655 2_655
La2 O2 O3 18.8(4) . 2_655
Ga2 O2 O3 105.6(12) 4 2_655
O2 O2 O3 56.1(13) 4_645 2_655
O2 O2 O3 141(2) 4_655 2_655
O1 O2 O3 129.2(16) 1_565 2_655
O7 O2 O3 44.6(7) 2 2_655
O5 O2 O3 84.6(11) 4 2_655
Ta O2 O3 67.6(8) 1_665 2_655
Ga1 O2 O3 67.6(8) 1_665 2_655
O6 O2 O3 54.1(7) 2_665 2_655
Ga2 O2 O3 127.6(13) 1_565 2_655
Ga4 O2 O3 43.1(5) 4_655 2_655
O3 O2 O3 103.0(12) 1_465 2_655
O5 O2 O3 67.0(9) 2_665 2_655
O2 O2 O3 90.0(7) 1_455 2_655
O2 O2 O3 90.0(7) 1_655 2_655
O7 O2 O3 149.2(14) 4_655 2_655
Ga4 O2 O3 66.1(8) 2_656 2_655
O2 O2 O3 59.7(11) 4_545 2_655
O2 O2 O3 134(2) 4 2_655
O3 O2 O3 27.8(8) . 2_655
Ga2 O2 O3 52.1(7) 1_455 2_655
La2 O2 O3 125.6(13) 3_655 2_655
O3 O2 O3 86.2(10) 2_665 2_655
La2 O2 O3 38.7(5) 1_655 2_655
Ta O2 O3 86.4(10) 3 2_655
Ga1 O2 O3 86.4(10) 3 2_655
Ga3 O2 O3 85.7(9) 1_465 2_655
O3 O2 O3 117.6(13) 3 2_655
O1 O2 O3 55.0(9) 1_655 2_655
O3 O2 O3 100.9(11) 4_755 2_655
O3 O2 O3 34.3(7) 1_455 2_655
O3 O2 O3 100.8(11) 4 2_655
La1 O2 O3 42.0(5) 2_556 2_655
La2 O2 O3 106.2(10) 1_565 2_655
O3 O2 O3 115.5(11) 3_455 2_655
Ga4 O2 O1 77(2) 3_554 1_665
Ga2 O2 O1 69(2) 4_655 1_665
O5 O2 O1 66(2) 1_565 1_665
La1 O2 O1 166(2) 3_554 1_665
O7 O2 O1 106.3(19) . 1_665
La1 O2 O1 82.9(17) 2_566 1_665
O3 O2 O1 109.2(19) 4_655 1_665
O4 O2 O1 53(2) 4 1_665
O6 O2 O1 40.4(12) 1_565 1_665
O1 O2 O1 128(2) 4 1_665
O4 O2 O1 91.1(17) 1_655 1_665
O6 O2 O1 119(2) 1_465 1_665
O1 O2 O1 52.0(16) 4_655 1_665
Ta O2 O1 98.8(16) 1_565 1_665
Ga1 O2 O1 98.8(16) 1_565 1_665
O4 O2 O1 162(2) . 1_665
O1 O2 O1 139.9(15) . 1_665
Ga2 O2 O1 115.1(12) . 1_665
Ga3 O2 O1 48.9(9) 1_565 1_665
O6 O2 O1 136.5(15) 4_655 1_665
La1 O2 O1 75.3(9) 3_654 1_665
La1 O2 O1 15.9(6) 2_666 1_665
O5 O2 O1 99.9(12) 4_655 1_665
Ga4 O2 O1 137.2(17) 3_454 1_665
O3 O2 O1 24.4(9) 1_565 1_665
La2 O2 O1 103.8(13) 3 1_665
Ga4 O2 O1 47.6(9) 2_666 1_665
Ga3 O2 O1 103.6(12) 3 1_665
O7 O2 O1 73.7(11) 2_655 1_665
La2 O2 O1 128.5(14) . 1_665
Ga2 O2 O1 132.4(15) 4 1_665
O2 O2 O1 107.6(18) 4_645 1_665
O2 O2 O1 25.2(12) 4_655 1_665
O1 O2 O1 54.5(9) 1_565 1_665
O7 O2 O1 121.0(16) 2 1_665
O5 O2 O1 153.4(16) 4 1_665
Ta O2 O1 49.0(8) 1_665 1_665
Ga1 O2 O1 49.0(8) 1_665 1_665
O6 O2 O1 84.3(12) 2_665 1_665
Ga2 O2 O1 31.2(6) 1_565 1_665
Ga4 O2 O1 79.9(11) 4_655 1_665
O3 O2 O1 87.3(12) 1_465 1_665
O5 O2 O1 54.9(9) 2_665 1_665
O2 O2 O1 135.7(8) 1_455 1_665
O2 O2 O1 44.3(8) 1_655 1_665
O7 O2 O1 50.2(9) 4_655 1_665
Ga4 O2 O1 121.1(12) 2_656 1_665
O2 O2 O1 170.6(17) 4_545 1_665
O2 O2 O1 84.2(9) 4 1_665
O3 O2 O1 107.0(9) . 1_665
Ga2 O2 O1 164.9(15) 1_455 1_665
La2 O2 O1 60.4(8) 3_655 1_665
O3 O2 O1 59.7(10) 2_665 1_665
La2 O2 O1 83.1(9) 1_655 1_665
Ta O2 O1 137.4(13) 3 1_665
Ga1 O2 O1 137.4(13) 3 1_665
Ga3 O2 O1 101.3(13) 1_465 1_665
O3 O2 O1 87.2(10) 3 1_665
O1 O2 O1 83.9(8) 1_655 1_665
O3 O2 O1 62.8(8) 4_755 1_665
O3 O2 O1 150.3(13) 1_455 1_665
O3 O2 O1 141.6(13) 4 1_665
La1 O2 O1 147.0(12) 2_556 1_665
La2 O2 O1 64.0(9) 1_565 1_665
O3 O2 O1 125.0(13) 3_455 1_665
O3 O2 O1 116.6(11) 2_655 1_665
Ga4 O2 O2 26(2) 3_554 2_655
Ga2 O2 O2 130(3) 4_655 2_655
O5 O2 O2 35.9(19) 1_565 2_655
La1 O2 O2 118.1(17) 3_554 2_655
O7 O2 O2 36.1(15) . 2_655
La1 O2 O2 100.0(19) 2_566 2_655
O3 O2 O2 154(2) 4_655 2_655
O4 O2 O2 117(2) 4 2_655
O6 O2 O2 42.7(11) 1_565 2_655
O1 O2 O2 141(3) 4 2_655
O4 O2 O2 68.9(18) 1_655 2_655
O6 O2 O2 79.2(17) 1_465 2_655
O1 O2 O2 100.5(19) 4_655 2_655
Ta O2 O2 44.5(9) 1_565 2_655
Ga1 O2 O2 44.5(9) 1_565 2_655
O4 O2 O2 99.1(17) . 2_655
O1 O2 O2 82.9(13) . 2_655
Ga2 O2 O2 74.1(10) . 2_655
Ga3 O2 O2 32.8(9) 1_565 2_655
O6 O2 O2 121.4(9) 4_655 2_655
La1 O2 O2 85.2(11) 3_654 2_655
La1 O2 O2 73.4(10) 2_666 2_655
O5 O2 O2 114.6(12) 4_655 2_655
Ga4 O2 O2 89.0(15) 3_454 2_655
O3 O2 O2 53.0(11) 1_565 2_655
La2 O2 O2 169.1(12) 3 2_655
Ga4 O2 O2 115.1(11) 2_666 2_655
Ga3 O2 O2 138.9(14) 3 2_655
O7 O2 O2 23.0(9) 2_655 2_655
La2 O2 O2 58.7(10) . 2_655
Ga2 O2 O2 129.1(19) 4 2_655
O2 O2 O2 91.1(16) 4_645 2_655
O2 O2 O2 91.1(16) 4_655 2_655
O1 O2 O2 83.6(12) 1_565 2_655
O7 O2 O2 56.9(12) 2 2_655
O5 O2 O2 135.1(12) 4 2_655
Ta O2 O2 30.8(5) 1_665 2_655
Ga1 O2 O2 30.8(5) 1_665 2_655
O6 O2 O2 24.5(7) 2_665 2_655
Ga2 O2 O2 75.7(8) 1_565 2_655
Ga4 O2 O2 9.8(8) 4_655 2_655
O3 O2 O2 78.6(13) 1_465 2_655
O5 O2 O2 15.6(9) 2_665 2_655
O2 O2 O2 108.4(11) 1_455 2_655
O2 O2 O2 71.6(11) 1_655 2_655
O7 O2 O2 119.8(12) 4_655 2_655
Ga4 O2 O2 109.4(8) 2_656 2_655
O2 O2 O2 109.4(18) 4_545 2_655
O2 O2 O2 109.4(18) 4 2_655
O3 O2 O2 63.5(7) . 2_655
Ga2 O2 O2 95.2(12) 1_455 2_655
La2 O2 O2 118.6(14) 3_655 2_655
O3 O2 O2 40.4(8) 2_665 2_655
La2 O2 O2 44.8(7) 1_655 2_655
Ta O2 O2 137.8(6) 3 2_655
Ga1 O2 O2 137.8(6) 3 2_655
Ga3 O2 O2 72.5(11) 1_465 2_655
O3 O2 O2 138.1(14) 3 2_655
O1 O2 O2 69.2(10) 1_655 2_655
O3 O2 O2 100.1(13) 4_755 2_655
O3 O2 O2 81.1(10) 1_455 2_655
O3 O2 O2 136.3(17) 4 2_655
La1 O2 O2 94.0(7) 2_556 2_655
La2 O2 O2 65.4(7) 1_565 2_655
O3 O2 O2 164.5(14) 3_455 2_655
O3 O2 O2 52.1(7) 2_655 2_655
O1 O2 O2 70.2(10) 1_665 2_655
Ga4 O2 O1 146(3) 3_554 3
Ga2 O2 O1 37.3(15) 4_655 3
O5 O2 O1 147(3) 1_565 3
La1 O2 O1 70.2(15) 3_554 3
O7 O2 O1 153(2) . 3
La1 O2 O1 85.7(16) 2_566 3
O3 O2 O1 20.9(10) 4_655 3
O4 O2 O1 58(2) 4 3
O6 O2 O1 124.8(19) 1_565 3
O1 O2 O1 51.2(19) 4 3
O4 O2 O1 105(2) 1_655 3
O6 O2 O1 112.7(16) 1_465 3
O1 O2 O1 67.0(16) 4_655 3
Ta O2 O1 147.4(15) 1_565 3
Ga1 O2 O1 147.4(15) 1_565 3
O4 O2 O1 92.5(14) . 3
O1 O2 O1 101.6(18) . 3
Ga2 O2 O1 104.9(15) . 3
Ga3 O2 O1 143.4(16) 1_565 3
O6 O2 O1 60.6(10) 4_655 3
La1 O2 O1 85.0(12) 3_654 3
La1 O2 O1 94.9(12) 2_666 3
O5 O2 O1 58.5(10) 4_655 3
Ga4 O2 O1 103.4(11) 3_454 3
O3 O2 O1 119.7(16) 1_565 3
La2 O2 O1 17.4(6) 3 3
Ga4 O2 O1 58.1(10) 2_666 3
Ga3 O2 O1 34.3(6) 3 3
O7 O2 O1 148.5(16) 2_655 3
La2 O2 O1 129.8(14) . 3
Ga2 O2 O1 63.1(8) 4 3
O2 O2 O1 85(2) 4_645 3
O2 O2 O1 81.3(18) 4_655 3
O1 O2 O1 96.8(15) 1_565 3
O7 O2 O1 135.3(12) 2 3
O5 O2 O1 53.9(9) 4 3
Ta O2 O1 136.7(13) 1_665 3
Ga1 O2 O1 136.7(13) 1_665 3
O6 O2 O1 166.7(14) 2_665 3
Ga2 O2 O1 99.8(13) 1_565 3
Ga4 O2 O1 171.4(15) 4_655 3
O3 O2 O1 109.1(13) 1_465 3
O5 O2 O1 154.4(14) 2_665 3
O2 O2 O1 83.9(6) 1_455 3
O2 O2 O1 96.1(6) 1_655 3
O7 O2 O1 49.6(9) 4_655 3
Ga4 O2 O1 68.7(10) 2_656 3
O2 O2 O1 79.2(17) 4_545 3
O2 O2 O1 76.0(16) 4 3
O3 O2 O1 114.6(13) . 3
Ga2 O2 O1 95.2(10) 1_455 3
La2 O2 O1 48.9(6) 3_655 3
O3 O2 O1 141.0(14) 2_665 3
La2 O2 O1 128.5(14) 1_655 3
Ta O2 O1 46.2(7) 3 3
Ga1 O2 O1 46.2(7) 3 3
Ga3 O2 O1 117.9(11) 1_465 3
O3 O2 O1 30.8(6) 3 3
O1 O2 O1 103.1(14) 1_655 3
O3 O2 O1 68.0(8) 4_755 3
O3 O2 O1 107.5(11) 1_455 3
O3 O2 O1 56.2(6) 4 3
La1 O2 O1 90.8(11) 2_556 3
La2 O2 O1 117.8(12) 1_565 3
O3 O2 O1 27.3(6) 3_455 3
O3 O2 O1 132.1(14) 2_655 3
O1 O2 O1 99.8(12) 1_665 3
O2 O2 O1 167.5(16) 2_655 3
Ga4 O2 O2 63(2) 3_554 2
Ga2 O2 O2 171(3) 4_655 2
O5 O2 O2 36.6(18) 1_565 2
La1 O2 O2 91.5(16) 3_554 2
O7 O2 O2 31.3(16) . 2
La1 O2 O2 73.9(15) 2_566 2
O3 O2 O2 149(2) 4_655 2
O4 O2 O2 121(3) 4 2
O6 O2 O2 86.6(18) 1_565 2
O1 O2 O2 97(2) 4 2
O4 O2 O2 98(2) 1_655 2
O6 O2 O2 35.4(9) 1_465 2
O1 O2 O2 145(2) 4_655 2
Ta O2 O2 4.4(12) 1_565 2
Ga1 O2 O2 4.4(12) 1_565 2
O4 O2 O2 61.8(13) . 2
O1 O2 O2 76.0(14) . 2
Ga2 O2 O2 86.9(11) . 2
Ga3 O2 O2 53.1(9) 1_565 2
O6 O2 O2 114.3(10) 4_655 2
La1 O2 O2 123.3(14) 3_654 2
La1 O2 O2 111.9(15) 2_666 2
O5 O2 O2 138.3(11) 4_655 2
Ga4 O2 O2 45.3(8) 3_454 2
O3 O2 O2 77.9(13) 1_565 2
La2 O2 O2 131.9(16) 3 2
Ga4 O2 O2 126.1(11) 2_666 2
Ga3 O2 O2 152.2(10) 3 2
O7 O2 O2 61.7(12) 2_655 2
La2 O2 O2 43.3(10) . 2
Ga2 O2 O2 84.8(12) 4 2
O2 O2 O2 110.4(18) 4_645 2
O2 O2 O2 110.4(18) 4_655 2
O1 O2 O2 77.4(12) 1_565 2
O7 O2 O2 19.6(10) 2 2
O5 O2 O2 103.7(12) 4 2
Ta O2 O2 75.0(12) 1_665 2
Ga1 O2 O2 75.0(12) 1_665 2
O6 O2 O2 20.7(6) 2_665 2
Ga2 O2 O2 87.2(10) 1_565 2
Ga4 O2 O2 39.1(7) 4_655 2
O3 O2 O2 49.2(9) 1_465 2
O5 O2 O2 54.1(10) 2_665 2
O2 O2 O2 64.0(10) 1_455 2
O2 O2 O2 116.0(10) 1_655 2
O7 O2 O2 145.9(11) 4_655 2
Ga4 O2 O2 117.6(7) 2_656 2
O2 O2 O2 83.0(16) 4_545 2
O2 O2 O2 83.0(16) 4 2
O3 O2 O2 81.0(10) . 2
Ga2 O2 O2 63.8(8) 1_455 2
La2 O2 O2 161.4(15) 3_655 2
O3 O2 O2 43.8(8) 2_665 2
La2 O2 O2 77.7(10) 1_655 2
Ta O2 O2 120.2(10) 3 2
Ga1 O2 O2 120.2(10) 3 2
Ga3 O2 O2 34.3(6) 1_465 2
O3 O2 O2 169.9(8) 3 2
O1 O2 O2 102.5(12) 1_655 2
O3 O2 O2 143.7(15) 4_755 2
O3 O2 O2 59.4(7) 1_455 2
O3 O2 O2 92.6(13) 4 2
La1 O2 O2 83.6(7) 2_556 2
La2 O2 O2 54.3(6) 1_565 2
O3 O2 O2 122.4(12) 3_455 2
O3 O2 O2 54.3(7) 2_655 2
O1 O2 O2 101.9(12) 1_665 2
O2 O2 O2 44.4(9) 2_655 2
O1 O2 O2 147.9(14) 3 2
Ga4 O2 O1 52.8(17) 3_554 2
Ga2 O2 O1 154(3) 4_655 2
O5 O2 O1 64.9(19) 1_565 2
La1 O2 O1 68.7(14) 3_554 2
O7 O2 O1 15.2(12) . 2
La1 O2 O1 102.7(17) 2_566 2
O3 O2 O1 124.5(18) 4_655 2
O4 O2 O1 154(3) 4 2
O6 O2 O1 88.8(15) 1_565 2
O1 O2 O1 100.3(19) 4 2
O4 O2 O1 72.2(18) 1_655 2
O6 O2 O1 53.3(12) 1_465 2
O1 O2 O1 135(2) 4_655 2
Ta O2 O1 37.1(9) 1_565 2
Ga1 O2 O1 37.1(9) 1_565 2
O4 O2 O1 49.3(12) . 2
O1 O2 O1 43.7(14) . 2
Ga2 O2 O1 55.5(9) . 2
Ga3 O2 O1 76.3(11) 1_565 2
O6 O2 O1 84.2(12) 4_655 2
La1 O2 O1 100.0(12) 3_654 2
La1 O2 O1 123.1(13) 2_666 2
O5 O2 O1 106.0(14) 4_655 2
Ga4 O2 O1 49.7(7) 3_454 2
O3 O2 O1 101.2(15) 1_565 2
La2 O2 O1 133.5(12) 3 2
Ga4 O2 O1 158.7(18) 2_666 2
Ga3 O2 O1 121.2(14) 3 2
O7 O2 O1 54.0(9) 2_655 2
La2 O2 O1 10.9(6) . 2
Ga2 O2 O1 89.5(9) 4 2
O2 O2 O1 78.9(14) 4_645 2
O2 O2 O1 139(2) 4_655 2
O1 O2 O1 110.1(14) 1_565 2
O7 O2 O1 20.4(6) 2 2
O5 O2 O1 84.9(10) 4 2
Ta O2 O1 77.0(9) 1_665 2
Ga1 O2 O1 77.0(9) 1_665 2
O6 O2 O1 40.6(8) 2_665 2
Ga2 O2 O1 117.4(14) 1_565 2
Ga4 O2 O1 41.4(6) 4_655 2
O3 O2 O1 79.5(11) 1_465 2
O5 O2 O1 66.3(10) 2_665 2
O2 O2 O1 70.5(5) 1_455 2
O2 O2 O1 109.5(5) 1_655 2
O7 O2 O1 170.0(11) 4_655 2
Ga4 O2 O1 84.9(10) 2_656 2
O2 O2 O1 59.6(13) 4_545 2
O2 O2 O1 110.3(19) 4 2
O3 O2 O1 52.0(8) . 2
Ga2 O2 O1 44.1(6) 1_455 2
La2 O2 O1 149.8(13) 3_655 2
O3 O2 O1 72.6(10) 2_665 2
La2 O2 O1 58.9(6) 1_655 2
Ta O2 O1 94.7(10) 3 2
Ga1 O2 O1 94.7(10) 3 2
Ga3 O2 O1 61.7(7) 1_465 2
O3 O2 O1 137.8(13) 3 2
O1 O2 O1 78.7(11) 1_655 2
O3 O2 O1 124.9(11) 4_755 2
O3 O2 O1 31.6(7) 1_455 2
O3 O2 O1 89.6(9) 4 2
La1 O2 O1 52.5(7) 2_556 2
La2 O2 O1 87.0(10) 1_565 2
O3 O2 O1 113.6(10) 3_455 2
O3 O2 O1 24.2(5) 2_655 2
O1 O2 O1 121.2(11) 1_665 2
O2 O2 O1 51.1(9) 2_655 2
O1 O2 O1 138.8(13) 3 2
O2 O2 O1 32.7(8) 2 2
Ga4 O2 O1 100(2) 3_554 1_455
Ga2 O2 O1 126(3) 4_655 1_455
O5 O2 O1 98(2) 1_565 1_455
La1 O2 O1 30.8(12) 3_554 1_455
O7 O2 O1 64.3(15) . 1_455
La1 O2 O1 86.6(15) 2_566 1_455
O3 O2 O1 85.9(17) 4_655 1_455
O4 O2 O1 128(2) 4 1_455
O6 O2 O1 137.1(18) 1_565 1_455
O1 O2 O1 53.4(18) 4 1_455
O4 O2 O1 97(2) 1_655 1_455
O6 O2 O1 45.5(12) 1_465 1_455
O1 O2 O1 144(2) 4_655 1_455
Ta O2 O1 65.5(10) 1_565 1_455
Ga1 O2 O1 65.5(10) 1_565 1_455
O4 O2 O1 1.8(9) . 1_455
O1 O2 O1 46.2(7) . 1_455
Ga2 O2 O1 72.1(10) . 1_455
Ga3 O2 O1 115.7(14) 1_565 1_455
O6 O2 O1 59.6(10) 4_655 1_455
La1 O2 O1 117.4(15) 3_654 1_455
La1 O2 O1 172.1(14) 2_666 1_455
O5 O2 O1 96.1(13) 4_655 1_455
Ga4 O2 O1 27.0(7) 3_454 1_455
O3 O2 O1 139.3(16) 1_565 1_455
La2 O2 O1 84.4(10) 3 1_455
Ga4 O2 O1 135.3(13) 2_666 1_455
Ga3 O2 O1 92.7(12) 3 1_455
O7 O2 O1 101.8(12) 2_655 1_455
La2 O2 O1 44.7(7) . 1_455
Ga2 O2 O1 44.9(7) 4 1_455
O2 O2 O1 84.7(12) 4_645 1_455
O2 O2 O1 150.7(17) 4_655 1_455
O1 O2 O1 113.0(13) 1_565 1_455
O7 O2 O1 44.5(8) 2 1_455
O5 O2 O1 41.0(8) 4 1_455
Ta O2 O1 125.9(12) 1_665 1_455
Ga1 O2 O1 125.9(12) 1_665 1_455
O6 O2 O1 81.6(10) 2_665 1_455
Ga2 O2 O1 135.4(14) 1_565 1_455
Ga4 O2 O1 90.1(10) 4_655 1_455
O3 O2 O1 78.0(9) 1_465 1_455
O5 O2 O1 113.5(13) 2_665 1_455
O2 O2 O1 34.0(7) 1_455 1_455
O2 O2 O1 146.0(7) 1_655 1_455
O7 O2 O1 140.6(12) 4_655 1_455
Ga4 O2 O1 73.9(10) 2_656 1_455
O2 O2 O1 24.5(12) 4_545 1_455
O2 O2 O1 87.7(15) 4 1_455
O3 O2 O1 77.8(9) . 1_455
Ga2 O2 O1 10.4(5) 1_455 1_455
La2 O2 O1 135.5(14) 3_655 1_455
O3 O2 O1 104.0(13) 2_665 1_455
La2 O2 O1 98.5(10) 1_655 1_455
Ta O2 O1 58.8(8) 3 1_455
Ga1 O2 O1 58.8(8) 3 1_455
Ga3 O2 O1 62.7(8) 1_465 1_455
O3 O2 O1 108.6(11) 3 1_455
O1 O2 O1 104.7(13) 1_655 1_455
O3 O2 O1 133.1(13) 4_755 1_455
O3 O2 O1 27.6(5) 1_455 1_455
O3 O2 O1 41.1(7) 4 1_455
La1 O2 O1 42.8(6) 2_556 1_455
La2 O2 O1 100.3(10) 1_565 1_455
O3 O2 O1 65.2(8) 3_455 1_455
O3 O2 O1 60.8(8) 2_655 1_455
O1 O2 O1 163.5(17) 1_665 1_455
O2 O2 O1 99.3(13) 2_655 1_455
O1 O2 O1 92.1(10) 3 1_455
O2 O2 O1 62.7(10) 2 1_455
O1 O2 O1 49.1(9) 2 1_455
Ga4 O2 O1 13.5(15) 3_554 2_655
Ga2 O2 O1 121(2) 4_655 2_655
O5 O2 O1 68(2) 1_565 2_655
La1 O2 O1 92.7(16) 3_554 2_655
O7 O2 O1 30.4(13) . 2_655
La1 O2 O1 130(2) 2_566 2_655
O3 O2 O1 123.9(18) 4_655 2_655
O4 O2 O1 143(3) 4 2_655
O6 O2 O1 50.8(11) 1_565 2_655
O1 O2 O1 140(2) 4 2_655
O4 O2 O1 40.4(17) 1_655 2_655
O6 O2 O1 91.4(15) 1_465 2_655
O1 O2 O1 94.2(15) 4_655 2_655
Ta O2 O1 61.7(10) 1_565 2_655
Ga1 O2 O1 61.7(10) 1_565 2_655
O4 O2 O1 87.4(14) . 2_655
O1 O2 O1 53.9(12) . 2_655
Ga2 O2 O1 41.2(8) . 2_655
Ga3 O2 O1 65.2(9) 1_565 2_655
O6 O2 O1 88.8(12) 4_655 2_655
La1 O2 O1 64.4(8) 3_654 2_655
La1 O2 O1 85.4(9) 2_666 2_655
O5 O2 O1 86.1(12) 4_655 2_655
Ga4 O2 O1 91.3(11) 3_454 2_655
O3 O2 O1 81.2(11) 1_565 2_655
La2 O2 O1 158.1(17) 3 2_655
Ga4 O2 O1 137.3(13) 2_666 2_655
Ga3 O2 O1 110.1(13) 3 2_655
O7 O2 O1 16.7(7) 2_655 2_655
La2 O2 O1 42.4(6) . 2_655
Ga2 O2 O1 130.5(12) 4 2_655
O2 O2 O1 59.6(14) 4_645 2_655
O2 O2 O1 115.0(19) 4_655 2_655
O1 O2 O1 116.5(14) 1_565 2_655
O7 O2 O1 59.1(8) 2 2_655
O5 O2 O1 109.1(13) 4 2_655
Ta O2 O1 41.1(6) 1_665 2_655
Ga1 O2 O1 41.1(6) 1_665 2_655
O6 O2 O1 47.5(8) 2_665 2_655
Ga2 O2 O1 105.9(12) 1_565 2_655
Ga4 O2 O1 27.5(6) 4_655 2_655
O3 O2 O1 105.5(14) 1_465 2_655
O5 O2 O1 44.9(8) 2_665 2_655
O2 O2 O1 112.3(6) 1_455 2_655
O2 O2 O1 67.7(6) 1_655 2_655
O7 O2 O1 128.7(10) 4_655 2_655
Ga4 O2 O1 76.8(9) 2_656 2_655
O2 O2 O1 85.5(12) 4_545 2_655
O2 O2 O1 139(2) 4 2_655
O3 O2 O1 30.6(7) . 2_655
Ga2 O2 O1 78.5(8) 1_455 2_655
La2 O2 O1 112.0(10) 3_655 2_655
O3 O2 O1 73.0(10) 2_665 2_655
La2 O2 O1 19.0(4) 1_655 2_655
Ta O2 O1 105.7(11) 3 2_655
Ga1 O2 O1 105.7(11) 3 2_655
Ga3 O2 O1 93.1(10) 1_465 2_655
O3 O2 O1 117.4(11) 3 2_655
O1 O2 O1 43.7(11) 1_655 2_655
O3 O2 O1 87.1(8) 4_755 2_655
O3 O2 O1 60.8(8) 1_455 2_655
O3 O2 O1 127.3(11) 4 2_655
La1 O2 O1 64.7(8) 2_556 2_655
La2 O2 O1 97.4(10) 1_565 2_655
O3 O2 O1 138.9(13) 3_455 2_655
O3 O2 O1 26.5(5) 2_655 2_655
O1 O2 O1 90.1(8) 1_665 2_655
O2 O2 O1 32.9(8) 2_655 2_655
O1 O2 O1 144.4(15) 3 2_655
O2 O2 O1 58.9(9) 2 2_655
O1 O2 O1 41.7(6) 2 2_655
O1 O2 O1 86.7(10) 1_455 2_655
Ga4 O2 O1 79(2) 3_554 2_565
Ga2 O2 O1 137(3) 4_655 2_565
O5 O2 O1 18.0(16) 1_565 2_565
La1 O2 O1 119.2(18) 3_554 2_565
O7 O2 O1 63.1(16) . 2_565
La1 O2 O1 47.9(14) 2_566 2_565
O3 O2 O1 152.9(19) 4_655 2_565
O4 O2 O1 86(3) 4 2_565
O6 O2 O1 81.0(17) 1_565 2_565
O1 O2 O1 95(2) 4 2_565
O4 O2 O1 121(2) 1_655 2_565
O6 O2 O1 44.5(13) 1_465 2_565
O1 O2 O1 127(2) 4_655 2_565
Ta O2 O1 31.2(10) 1_565 2_565
Ga1 O2 O1 31.2(10) 1_565 2_565
O4 O2 O1 86.9(14) . 2_565
O1 O2 O1 111.6(14) . 2_565
Ga2 O2 O1 119.3(15) . 2_565
Ga3 O2 O1 34.4(7) 1_565 2_565
O6 O2 O1 147.3(14) 4_655 2_565
La1 O2 O1 134.6(13) 3_654 2_565
La1 O2 O1 89.5(12) 2_666 2_565
O5 O2 O1 167.1(13) 4_655 2_565
Ga4 O2 O1 62.8(10) 3_454 2_565
O3 O2 O1 51.5(9) 1_565 2_565
La2 O2 O1 117.6(13) 3 2_565
Ga4 O2 O1 90.6(13) 2_666 2_565
Ga3 O2 O1 167.8(14) 3 2_565
O7 O2 O1 75.6(12) 2_655 2_565
La2 O2 O1 78.9(11) . 2_565
Ga2 O2 O1 86.2(11) 4 2_565
O2 O2 O1 141(2) 4_645 2_565
O2 O2 O1 76.2(15) 4_655 2_565
O1 O2 O1 42.2(13) 1_565 2_565
O7 O2 O1 53.4(10) 2 2_565
O5 O2 O1 124.5(11) 4 2_565
Ta O2 O1 73.8(10) 1_665 2_565
Ga1 O2 O1 73.8(10) 1_665 2_565
O6 O2 O1 35.2(8) 2_665 2_565
Ga2 O2 O1 52.8(9) 1_565 2_565
Ga4 O2 O1 54.9(9) 4_655 2_565
O3 O2 O1 26.4(7) 1_465 2_565
O5 O2 O1 50.5(9) 2_665 2_565
O2 O2 O1 71.2(5) 1_455 2_565
O2 O2 O1 108.8(5) 1_655 2_565
O7 O2 O1 110.6(14) 4_655 2_565
Ga4 O2 O1 153.0(13) 2_656 2_565
O2 O2 O1 112.5(18) 4_545 2_565
O2 O2 O1 57.6(14) 4 2_565
O3 O2 O1 110.9(13) . 2_565
Ga2 O2 O1 93.5(10) 1_455 2_565
La2 O2 O1 132.5(13) 3_655 2_565
O3 O2 O1 18.8(6) 2_665 2_565
La2 O2 O1 97.2(11) 1_655 2_565
Ta O2 O1 145.0(10) 3 2_565
Ga1 O2 O1 145.0(10) 3 2_565
Ga3 O2 O1 28.6(5) 1_465 2_565
O3 O2 O1 154.1(14) 3 2_565
O1 O2 O1 121.7(10) 1_655 2_565
O3 O2 O1 136.3(11) 4_755 2_565
O3 O2 O1 93.7(10) 1_455 2_565
O3 O2 O1 99.5(10) 4 2_565
La1 O2 O1 118.8(11) 2_556 2_565
La2 O2 O1 18.9(6) 1_565 2_565
O3 O2 O1 123.8(9) 3_455 2_565
O3 O2 O1 87.6(10) 2_655 2_565
O1 O2 O1 75.1(11) 1_665 2_565
O2 O2 O1 52.6(9) 2_655 2_565
O1 O2 O1 133.6(14) 3 2_565
O2 O2 O1 35.6(8) 2 2_565
O1 O2 O1 68.1(9) 2 2_565
O1 O2 O1 88.5(8) 1_455 2_565
O1 O2 O1 82.1(10) 2_655 2_565
Ga4 O2 O1 124(3) 3_554 1_465
Ga2 O2 O1 115(2) 4_655 1_465
O5 O2 O1 65.3(19) 1_565 1_465
La1 O2 O1 91.4(14) 3_554 1_465
O7 O2 O1 94.0(18) . 1_465
La1 O2 O1 17.4(10) 2_566 1_465
O3 O2 O1 106.2(17) 4_655 1_465
O4 O2 O1 69(2) 4 1_465
O6 O2 O1 125(2) 1_565 1_465
O1 O2 O1 48.5(18) 4 1_465
O4 O2 O1 161(2) 1_655 1_465
O6 O2 O1 35.4(12) 1_465 1_465
O1 O2 O1 135(2) 4_655 1_465
Ta O2 O1 60.9(11) 1_565 1_465
Ga1 O2 O1 60.9(11) 1_565 1_465
O4 O2 O1 67.8(12) . 1_465
O1 O2 O1 114.7(13) . 1_465
Ga2 O2 O1 139.3(14) . 1_465
Ga3 O2 O1 79.1(12) 1_565 1_465
O6 O2 O1 117.9(11) 4_655 1_465
La1 O2 O1 171.4(15) 3_654 1_465
La1 O2 O1 114.2(14) 2_666 1_465
O5 O2 O1 145.4(13) 4_655 1_465
Ga4 O2 O1 46.4(8) 3_454 1_465
O3 O2 O1 84.7(11) 1_565 1_465
La2 O2 O1 72.5(10) 3 1_465
Ga4 O2 O1 77.3(11) 2_666 1_465
Ga3 O2 O1 122.0(12) 3 1_465
O7 O2 O1 121.5(15) 2_655 1_465
La2 O2 O1 94.8(11) . 1_465
Ga2 O2 O1 42.1(8) 4 1_465
O2 O2 O1 153.5(17) 4_645 1_465
O2 O2 O1 81.9(12) 4_655 1_465
O1 O2 O1 44.4(7) 1_565 1_465
O7 O2 O1 68.1(10) 2 1_465
O5 O2 O1 86.3(9) 4 1_465
Ta O2 O1 120.3(14) 1_665 1_465
Ga1 O2 O1 120.3(14) 1_665 1_465
O6 O2 O1 77.0(11) 2_665 1_465
Ga2 O2 O1 67.7(10) 1_565 1_465
Ga4 O2 O1 98.8(12) 4_655 1_465
O3 O2 O1 21.0(7) 1_465 1_465
O5 O2 O1 97.7(13) 2_665 1_465
O2 O2 O1 36.8(7) 1_455 1_465
O2 O2 O1 143.2(7) 1_655 1_465
O7 O2 O1 97.8(11) 4_655 1_465
Ga4 O2 O1 136.6(12) 2_656 1_465
O2 O2 O1 90.5(15) 4_545 1_465
O2 O2 O1 22.2(12) 4 1_465
O3 O2 O1 139.9(12) . 1_465
Ga2 O2 O1 79.5(9) 1_455 1_465
La2 O2 O1 121.7(11) 3_655 1_465
O3 O2 O1 64.2(10) 2_665 1_465
La2 O2 O1 141.0(13) 1_655 1_465
Ta O2 O1 104.6(9) 3 1_465
Ga1 O2 O1 104.6(9) 3 1_465
Ga3 O2 O1 29.5(6) 1_465 1_465
O3 O2 O1 119.6(11) 3 1_465
O1 O2 O1 166.3(16) 1_655 1_465
O3 O2 O1 146.5(12) 4_755 1_465
O3 O2 O1 92.8(8) 1_455 1_465
O3 O2 O1 56.3(8) 4 1_465
La1 O2 O1 112.4(10) 2_556 1_465
La2 O2 O1 42.4(6) 1_565 1_465
O3 O2 O1 76.6(7) 3_455 1_465
O3 O2 O1 112.5(11) 2_655 1_465
O1 O2 O1 98.9(13) 1_665 1_465
O2 O2 O1 99.0(12) 2_655 1_465
O1 O2 O1 89.8(9) 3 1_465
O2 O2 O1 63.7(9) 2 1_465
O1 O2 O1 88.5(8) 2 1_465
O1 O2 O1 69.5(6) 1_455 1_465
O1 O2 O1 122.6(10) 2_655 1_465
O1 O2 O1 47.4(9) 2_565 1_465
Ga4 O2 O3 48.5(19) 3_554 2_765
Ga2 O2 O3 95(2) 4_655 2_765
O5 O2 O3 47.4(16) 1_565 2_765
La1 O2 O3 154.2(18) 3_554 2_765
O7 O2 O3 76.0(16) . 2_765
La1 O2 O3 93.8(17) 2_566 2_765
O3 O2 O3 133(2) 4_655 2_765
O4 O2 O3 82(2) 4 2_765
O6 O2 O3 20.7(12) 1_565 2_765
O1 O2 O3 150(2) 4 2_765
O4 O2 O3 76.5(18) 1_655 2_765
O6 O2 O3 105.7(18) 1_465 2_765
O1 O2 O3 68.9(16) 4_655 2_765
Ta O2 O3 75.8(11) 1_565 2_765
Ga1 O2 O3 75.8(11) 1_565 2_765
O4 O2 O3 138.2(17) . 2_765
O1 O2 O3 115.1(13) . 2_765
Ga2 O2 O3 95.5(11) . 2_765
Ga3 O2 O3 28.8(5) 1_565 2_765
O6 O2 O3 137.4(13) 4_655 2_765
La1 O2 O3 74.1(10) 3_654 2_765
La1 O2 O3 34.7(7) 2_666 2_765
O5 O2 O3 106.7(11) 4_655 2_765
Ga4 O2 O3 121.7(14) 3_454 2_765
O3 O2 O3 22.3(5) 1_565 2_765
La2 O2 O3 134.2(12) 3 2_765
Ga4 O2 O3 77.5(10) 2_666 2_765
Ga3 O2 O3 121.7(12) 3 2_765
O7 O2 O3 45.0(8) 2_655 2_765
La2 O2 O3 98.0(10) . 2_765
Ga2 O2 O3 146.3(15) 4 2_765
O2 O2 O3 99.2(17) 4_645 2_765
O2 O2 O3 53.8(14) 4_655 2_765
O1 O2 O3 66.0(9) 1_565 2_765
O7 O2 O3 94.6(11) 2 2_765
O5 O2 O3 168.6(14) 4 2_765
Ta O2 O3 22.2(5) 1_665 2_765
Ga1 O2 O3 22.2(5) 1_665 2_765
O6 O2 O3 57.7(8) 2_665 2_765
Ga2 O2 O3 46.9(6) 1_565 2_765
Ga4 O2 O3 49.6(7) 4_655 2_765
O3 O2 O3 85.3(10) 1_465 2_765
O5 O2 O3 25.2(6) 2_665 2_765
O2 O2 O3 134.1(7) 1_455 2_765
O2 O2 O3 45.9(7) 1_655 2_765
O7 O2 O3 79.9(9) 4_655 2_765
Ga4 O2 O3 118.7(11) 2_656 2_765
O2 O2 O3 147.0(17) 4_545 2_765
O2 O2 O3 99.3(11) 4 2_765
O3 O2 O3 85.2(7) . 2_765
Ga2 O2 O3 135.1(11) 1_455 2_765
La2 O2 O3 83.7(9) 3_655 2_765
O3 O2 O3 44.2(6) 2_665 2_765
La2 O2 O3 59.9(7) 1_655 2_765
Ta O2 O3 150.8(12) 3 2_765
Ga1 O2 O3 150.8(12) 3 2_765
Ga3 O2 O3 91.4(10) 1_465 2_765
O3 O2 O3 109.4(9) 3 2_765
O1 O2 O3 71.5(9) 1_655 2_765
O3 O2 O3 74.7(8) 4_755 2_765
O3 O2 O3 120.0(10) 1_455 2_765
O3 O2 O3 160.5(14) 4 2_765
La1 O2 O3 125.4(10) 2_556 2_765
La2 O2 O3 61.9(6) 1_565 2_765
O3 O2 O3 155.4(12) 3_455 2_765
O3 O2 O3 87.3(8) 2_655 2_765
O1 O2 O3 30.5(7) 1_665 2_765
O2 O2 O3 40.0(6) 2_655 2_765
O1 O2 O3 129.2(11) 3 2_765
O2 O2 O3 77.7(9) 2 2_765
O1 O2 O3 91.0(9) 2 2_765
O1 O2 O3 138.7(12) 1_455 2_765
O1 O2 O3 61.7(7) 2_655 2_765
O1 O2 O3 62.9(7) 2_565 2_765
O1 O2 O3 104.2(11) 1_465 2_765
Ga4 O2 O1 56(2) 3_554 2_665
Ga2 O2 O1 111(2) 4_655 2_665
O5 O2 O1 25.7(16) 1_565 2_665
La1 O2 O1 150(2) 3_554 2_665
O7 O2 O1 68.8(16) . 2_665
La1 O2 O1 75.6(17) 2_566 2_665
O3 O2 O1 151(2) 4_655 2_665
O4 O2 O1 82(3) 4 2_665
O6 O2 O1 41.8(14) 1_565 2_665
O1 O2 O1 131(2) 4 2_665
O4 O2 O1 93.6(19) 1_655 2_665
O6 O2 O1 83.7(17) 1_465 2_665
O1 O2 O1 89.7(16) 4_655 2_665
Ta O2 O1 57.2(11) 1_565 2_665
Ga1 O2 O1 57.2(11) 1_565 2_665
O4 O2 O1 121.6(17) . 2_665
O1 O2 O1 118.5(14) . 2_665
Ga2 O2 O1 106.9(13) . 2_665
Ga3 O2 O1 7.0(5) 1_565 2_665
O6 O2 O1 154.5(14) 4_655 2_665
La1 O2 O1 96.2(10) 3_654 2_665
La1 O2 O1 52.7(9) 2_666 2_665
O5 O2 O1 129.2(11) 4_655 2_665
Ga4 O2 O1 100.8(13) 3_454 2_665
O3 O2 O1 19.2(8) 1_565 2_665
La2 O2 O1 134.4(15) 3 2_665
Ga4 O2 O1 80.6(12) 2_666 2_665
Ga3 O2 O1 143.3(12) 3 2_665
O7 O2 O1 52.2(10) 2_655 2_665
La2 O2 O1 91.6(12) . 2_665
Ga2 O2 O1 124.9(14) 4 2_665
O2 O2 O1 117.4(18) 4_645 2_665
O2 O2 O1 57.2(15) 4_655 2_665
O1 O2 O1 51.4(12) 1_565 2_665
O7 O2 O1 78.9(12) 2 2_665
O5 O2 O1 163.4(14) 4 2_665
Ta O2 O1 37.9(7) 1_665 2_665
Ga1 O2 O1 37.9(7) 1_665 2_665
O6 O2 O1 42.6(8) 2_665 2_665
Ga2 O2 O1 40.1(8) 1_565 2_665
Ga4 O2 O1 44.6(8) 4_655 2_665
O3 O2 O1 63.3(9) 1_465 2_665
O5 O2 O1 21.8(8) 2_665 2_665
O2 O2 O1 111.5(5) 1_455 2_665
O2 O2 O1 68.5(5) 1_655 2_665
O7 O2 O1 90.9(11) 4_655 2_665
Ga4 O2 O1 137.7(11) 2_656 2_665
O2 O2 O1 141(2) 4_545 2_665
O2 O2 O1 83.0(12) 4 2_665
O3 O2 O1 95.9(10) . 2_665
Ga2 O2 O1 123.2(12) 1_455 2_665
La2 O2 O1 101.8(10) 3_655 2_665
O3 O2 O1 21.6(6) 2_665 2_665
La2 O2 O1 72.4(8) 1_655 2_665
Ta O2 O1 171.6(12) 3 2_665
Ga1 O2 O1 171.6(12) 3 2_665
Ga3 O2 O1 68.8(9) 1_465 2_665
O3 O2 O1 128.7(10) 3 2_665
O1 O2 O1 90.1(8) 1_655 2_665
O3 O2 O1 96.8(9) 4_755 2_665
O3 O2 O1 113.6(12) 1_455 2_665
O3 O2 O1 139.0(12) 4 2_665
La1 O2 O1 129.6(12) 2_556 2_665
La2 O2 O1 41.0(5) 1_565 2_665
O3 O2 O1 153.7(13) 3_455 2_665
O3 O2 O1 87.6(9) 2_655 2_665
O1 O2 O1 42.0(11) 1_665 2_665
O2 O2 O1 35.6(8) 2_655 2_665
O1 O2 O1 138.5(14) 3 2_665
O2 O2 O1 60.0(9) 2 2_665
O1 O2 O1 82.0(10) 2 2_665
O1 O2 O1 122.7(10) 1_455 2_665
O1 O2 O1 66.7(8) 2_655 2_665
O1 O2 O1 40.3(5) 2_565 2_665
O1 O2 O1 83.2(10) 1_465 2_665
O3 O2 O1 22.6(4) 2_765 2_665
Ga4 O2 O3 95(2) 3_554 2_565
Ga2 O2 O3 142(2) 4_655 2_565
O5 O2 O3 41.9(16) 1_565 2_565
La1 O2 O3 95.9(16) 3_554 2_565
O7 O2 O3 65.8(16) . 2_565
La1 O2 O3 39.7(12) 2_566 2_565
O3 O2 O3 133(2) 4_655 2_565
O4 O2 O3 91(3) 4 2_565
O6 O2 O3 105.7(19) 1_565 2_565
O1 O2 O3 72.0(19) 4 2_565
O4 O2 O3 133(2) 1_655 2_565
O6 O2 O3 20.7(12) 1_465 2_565
O1 O2 O3 149(2) 4_655 2_565
Ta O2 O3 31.5(8) 1_565 2_565
Ga1 O2 O3 31.5(8) 1_565 2_565
O4 O2 O3 64.5(13) . 2_565
O1 O2 O3 100.9(14) . 2_565
Ga2 O2 O3 118.9(13) . 2_565
Ga3 O2 O3 59.7(9) 1_565 2_565
O6 O2 O3 125.6(13) 4_655 2_565
La1 O2 O3 156.1(14) 3_654 2_565
La1 O2 O3 113.2(14) 2_666 2_565
O5 O2 O3 162.2(13) 4_655 2_565
Ga4 O2 O3 39.3(8) 3_454 2_565
O3 O2 O3 75.8(11) 1_565 2_565
La2 O2 O3 101.5(11) 3 2_565
Ga4 O2 O3 97.9(12) 2_666 2_565
Ga3 O2 O3 148.0(12) 3 2_565
O7 O2 O3 92.6(13) 2_655 2_565
La2 O2 O3 72.2(10) . 2_565
Ga2 O2 O3 62.0(9) 4 2_565
O2 O2 O3 141.8(19) 4_645 2_565
O2 O2 O3 92.0(14) 4_655 2_565
O1 O2 O3 51.7(9) 1_565 2_565
O7 O2 O3 43.7(9) 2 2_565
O5 O2 O3 99.2(11) 4 2_565
Ta O2 O3 97.2(12) 1_665 2_565
Ga1 O2 O3 97.2(12) 1_665 2_565
O6 O2 O3 47.8(8) 2_665 2_565
Ga2 O2 O3 70.5(9) 1_565 2_565
Ga4 O2 O3 69.6(9) 4_655 2_565
O3 O2 O3 16.2(6) 1_465 2_565
O5 O2 O3 73.4(11) 2_665 2_565
O2 O2 O3 45.8(6) 1_455 2_565
O2 O2 O3 134.2(6) 1_655 2_565
O7 O2 O3 119.9(12) 4_655 2_565
Ga4 O2 O3 139.3(12) 2_656 2_565
O2 O2 O3 90.7(16) 4_545 2_565
O2 O2 O3 48.4(14) 4 2_565
O3 O2 O3 114.9(11) . 2_565
Ga2 O2 O3 73.3(9) 1_455 2_565
La2 O2 O3 145.5(12) 3_655 2_565
O3 O2 O3 44.1(6) 2_665 2_565
La2 O2 O3 111.4(11) 1_655 2_565
Ta O2 O3 119.8(10) 3 2_565
Ga1 O2 O3 119.8(10) 3 2_565
Ga3 O2 O3 3.5(3) 1_465 2_565
O3 O2 O3 149.2(11) 3 2_565
O1 O2 O3 136.8(12) 1_655 2_565
O3 O2 O3 160.6(13) 4_755 2_565
O3 O2 O3 79.2(7) 1_455 2_565
O3 O2 O3 74.6(9) 4 2_565
La1 O2 O3 104.1(9) 2_556 2_565
La2 O2 O3 34.2(3) 1_565 2_565
O3 O2 O3 101.3(8) 3_455 2_565
O3 O2 O3 87.3(9) 2_655 2_565
O1 O2 O3 97.9(11) 1_665 2_565
O2 O2 O3 71.0(10) 2_655 2_565
O1 O2 O3 118.9(10) 3 2_565
O2 O2 O3 34.7(6) 2 2_565
O1 O2 O3 63.5(8) 2 2_565
O1 O2 O3 66.2(8) 1_455 2_565
O1 O2 O3 93.1(9) 2_655 2_565
O1 O2 O3 25.4(3) 2_565 2_565
O1 O2 O3 29.6(6) 1_465 2_565
O3 O2 O3 88.4(8) 2_765 2_565
O1 O2 O3 65.7(7) 2_665 2_565
Ga4 O2 O1 109(2) 3_554 3_655
Ga2 O2 O1 7.1(16) 4_655 3_655
O5 O2 O1 136(2) 1_565 3_655
La1 O2 O1 95.8(18) 3_554 3_655
O7 O2 O1 144(2) . 3_655
La1 O2 O1 109.7(18) 2_566 3_655
O3 O2 O1 40.0(14) 4_655 3_655
O4 O2 O1 59(2) 4 3_655
O6 O2 O1 83.9(16) 1_565 3_655
O1 O2 O1 92.5(19) 4 3_655
O4 O2 O1 77.0(18) 1_655 3_655
O6 O2 O1 153.2(17) 1_465 3_655
O1 O2 O1 25.8(16) 4_655 3_655
Ta O2 O1 168.9(16) 1_565 3_655
Ga1 O2 O1 168.9(16) 1_565 3_655
O4 O2 O1 126.6(17) . 3_655
O1 O2 O1 106.1(18) . 3_655
Ga2 O2 O1 91.5(13) . 3_655
Ga3 O2 O1 118.8(12) 1_565 3_655
O6 O2 O1 70.7(11) 4_655 3_655
La1 O2 O1 50.4(8) 3_654 3_655
La1 O2 O1 59.3(9) 2_666 3_655
O5 O2 O1 41.8(9) 4_655 3_655
Ga4 O2 O1 144.1(13) 3_454 3_655
O3 O2 O1 94.7(12) 1_565 3_655
La2 O2 O1 56.9(8) 3 3_655
Ga4 O2 O1 52.9(9) 2_666 3_655
Ga3 O2 O1 33.6(6) 3 3_655
O7 O2 O1 109.9(11) 2_655 3_655
La2 O2 O1 137.5(15) . 3_655
Ga2 O2 O1 104.4(12) 4 3_655
O2 O2 O1 68.1(18) 4_645 3_655
O2 O2 O1 65.0(17) 4_655 3_655
O1 O2 O1 101.4(14) 1_565 3_655
O7 O2 O1 165.2(17) 2 3_655
O5 O2 O1 84.7(12) 4 3_655
Ta O2 O1 95.5(10) 1_665 3_655
Ga1 O2 O1 95.5(10) 1_665 3_655
O6 O2 O1 149.8(11) 2_665 3_655
Ga2 O2 O1 88.4(11) 1_565 3_655
Ga4 O2 O1 132.0(11) 4_655 3_655
O3 O2 O1 133.4(14) 1_465 3_655
O5 O2 O1 116.5(10) 2_665 3_655
O2 O2 O1 125.3(5) 1_455 3_655
O2 O2 O1 54.7(5) 1_655 3_655
O7 O2 O1 31.4(8) 4_655 3_655
Ga4 O2 O1 64.5(8) 2_656 3_655
O2 O2 O1 103.9(18) 4_545 3_655
O2 O2 O1 101.3(17) 4 3_655
O3 O2 O1 95.8(10) . 3_655
Ga2 O2 O1 123.3(13) 1_455 3_655
La2 O2 O1 10.0(5) 3_655 3_655
O3 O2 O1 129.7(13) 2_665 3_655
La2 O2 O1 95.6(9) 1_655 3_655
Ta O2 O1 67.1(8) 3 3_655
Ga1 O2 O1 67.1(8) 3 3_655
Ga3 O2 O1 150.6(12) 1_465 3_655
O3 O2 O1 16.9(5) 3 3_655
O1 O2 O1 71.7(9) 1_655 3_655
O3 O2 O1 28.0(5) 4_755 3_655
O3 O2 O1 125.0(12) 1_455 3_655
O3 O2 O1 96.8(10) 4 3_655
La1 O2 O1 99.9(11) 2_556 3_655
La2 O2 O1 123.5(11) 1_565 3_655
O3 O2 O1 67.1(8) 3_455 3_655
O3 O2 O1 123.4(12) 2_655 3_655
O1 O2 O1 70.4(8) 1_665 3_655
O2 O2 O1 126.3(14) 2_655 3_655
O1 O2 O1 41.4(5) 3 3_655
O2 O2 O1 170.5(14) 2 3_655
O1 O2 O1 147.0(14) 2 3_655
O1 O2 O1 125.5(13) 1_455 3_655
O1 O2 O1 114.5(10) 2_655 3_655
O1 O2 O1 141.2(14) 2_565 3_655
O1 O2 O1 121.9(12) 1_465 3_655
O3 O2 O1 93.2(9) 2_765 3_655
O1 O2 O1 111.8(11) 2_665 3_655
O3 O2 O1 149.3(11) 2_565 3_655
Ga4 O2 O1 133(2) 3_554 4_455
Ga2 O2 O1 109(2) 4_655 4_455
O5 O2 O1 96(2) 1_565 4_455
La1 O2 O1 53.2(12) 3_554 4_455
O7 O2 O1 94.1(17) . 4_455
La1 O2 O1 52.7(12) 2_566 4_455
O3 O2 O1 79.5(17) 4_655 4_455
O4 O2 O1 89(2) 4 4_455
O6 O2 O1 160(2) 1_565 4_455
O1 O2 O1 21.4(12) 4 4_455
O4 O2 O1 134(2) 1_655 4_455
O6 O2 O1 41.0(12) 1_465 4_455
O1 O2 O1 139(2) 4_655 4_455
Ta O2 O1 75.4(11) 1_565 4_455
Ga1 O2 O1 75.4(11) 1_565 4_455
O4 O2 O1 37.9(11) . 4_455
O1 O2 O1 84.2(11) . 4_455
Ga2 O2 O1 109.8(12) . 4_455
Ga3 O2 O1 113.8(14) 1_565 4_455
O6 O2 O1 79.3(10) 4_655 4_455
La1 O2 O1 144.1(16) 3_654 4_455
La1 O2 O1 147.5(15) 2_666 4_455
O5 O2 O1 111.5(12) 4_655 4_455
Ga4 O2 O1 32.5(7) 3_454 4_455
O3 O2 O1 123.4(13) 1_565 4_455
La2 O2 O1 57.5(8) 3 4_455
Ga4 O2 O1 96.9(12) 2_666 4_455
Ga3 O2 O1 93.8(11) 3 4_455
O7 O2 O1 134.0(14) 2_655 4_455
La2 O2 O1 80.7(9) . 4_455
Ga2 O2 O1 9.3(6) 4 4_455
O2 O2 O1 115.6(15) 4_645 4_455
O2 O2 O1 112.4(15) 4_655 4_455
O1 O2 O1 81.7(10) 1_565 4_455
O7 O2 O1 66.2(9) 2 4_455
O5 O2 O1 48.0(7) 4 4_455
Ta O2 O1 150.2(15) 1_665 4_455
Ga1 O2 O1 150.2(15) 1_665 4_455
O6 O2 O1 95.7(11) 2_665 4_455
Ga2 O2 O1 104.7(12) 1_565 4_455
Ga4 O2 O1 114.0(12) 4_655 4_455
O3 O2 O1 56.4(7) 1_465 4_455
O5 O2 O1 126.9(14) 2_665 4_455
O2 O2 O1 11.6(8) 1_455 4_455
O2 O2 O1 168.4(8) 1_655 4_455
O7 O2 O1 108.8(11) 4_655 4_455
Ga4 O2 O1 97.9(10) 2_656 4_455
O2 O2 O1 53.9(12) 4_545 4_455
O2 O2 O1 50.7(13) 4 4_455
O3 O2 O1 116.7(11) . 4_455
Ga2 O2 O1 49.3(7) 1_455 4_455
La2 O2 O1 120.5(12) 3_655 4_455
O3 O2 O1 98.1(12) 2_665 4_455
La2 O2 O1 137.2(12) 1_655 4_455
Ta O2 O1 67.5(8) 3 4_455
Ga1 O2 O1 67.5(8) 3 4_455
Ga3 O2 O1 51.8(7) 1_465 4_455
O3 O2 O1 101.2(10) 3 4_455
O1 O2 O1 141.2(15) 1_655 4_455
O3 O2 O1 139.4(13) 4_755 4_455
O3 O2 O1 66.8(7) 1_455 4_455
O3 O2 O1 20.1(7) 4 4_455
La1 O2 O1 78.1(8) 2_556 4_455
La2 O2 O1 80.3(9) 1_565 4_455
O3 O2 O1 48.3(6) 3_455 4_455
O3 O2 O1 98.6(11) 2_655 4_455
O1 O2 O1 134.9(14) 1_665 4_455
O2 O2 O1 119.9(16) 2_655 4_455
O1 O2 O1 72.4(9) 3 4_455
O2 O2 O1 75.5(11) 2 4_455
O1 O2 O1 81.0(7) 2 4_455
O1 O2 O1 39.2(5) 1_455 4_455
O1 O2 O1 122.5(12) 2_655 4_455
O1 O2 O1 79.4(7) 2_565 4_455
O1 O2 O1 38.7(5) 1_465 4_455
O3 O2 O1 141.7(12) 2_765 4_455
O1 O2 O1 119.3(12) 2_665 4_455
O3 O2 O1 54.5(7) 2_565 4_455
O1 O2 O1 113.7(9) 3_655 4_455
Ga2 O3 Ga3 115.6(18) . .
Ga2 O3 La2 100.0(12) . 1_655
Ga3 O3 La2 116.8(17) . 1_655
Ga2 O3 La1 93.7(14) . 2_656
Ga3 O3 La1 121.5(14) . 2_656
La2 O3 La1 104.9(13) 1_655 2_656
Ga2 O3 O6 122.0(16) . .
Ga3 O3 O6 71.1(12) . .
La2 O3 O6 129.6(14) 1_655 .
La1 O3 O6 50.7(9) 2_656 .
Ga2 O3 O1 83.9(15) . 1_655
Ga3 O3 O1 160.5(18) . 1_655
La2 O3 O1 56.3(14) 1_655 1_655
La1 O3 O1 52.6(15) 2_656 1_655
O6 O3 O1 98.8(18) . 1_655
Ga2 O3 O2 38.1(14) . 4_645
Ga3 O3 O2 138(2) . 4_645
La2 O3 O2 102.0(18) 1_655 4_645
La1 O3 O2 56.2(13) 2_656 4_645
O6 O3 O2 96.3(15) . 4_645
O1 O3 O2 57.7(19) 1_655 4_645
Ga2 O3 O4 30.6(10) . 1_655
Ga3 O3 O4 136.8(18) . 1_655
La2 O3 O4 70.4(13) 1_655 1_655
La1 O3 O4 93.8(15) 2_656 1_655
O6 O3 O4 140.1(19) . 1_655
O1 O3 O4 61.2(15) 1_655 1_655
O2 O3 O4 43.9(16) 4_645 1_655
Ga2 O3 O5 91.8(15) . .
Ga3 O3 O5 38.2(10) . .
La2 O3 O5 154.5(16) 1_655 .
La1 O3 O5 96.7(11) 2_656 .
O6 O3 O5 57.3(9) . .
O1 O3 O5 148(2) 1_655 .
O2 O3 O5 101.1(18) 4_645 .
O4 O3 O5 122.0(17) 1_655 .
Ga2 O3 O5 152.2(18) . 2_655
Ga3 O3 O5 36.7(9) . 2_655
La2 O3 O5 95.8(12) 1_655 2_655
La1 O3 O5 104.1(11) 2_656 2_655
O6 O3 O5 59.9(11) . 2_655
O1 O3 O5 123.8(16) 1_655 2_655
O2 O3 O5 156.1(16) 4_645 2_655
O4 O3 O5 159.9(18) 1_655 2_655
O5 O3 O5 65.5(14) . 2_655
Ga2 O3 O1 28.6(12) . .
Ga3 O3 O1 87.0(16) . .
La2 O3 O1 116.6(14) 1_655 .
La1 O3 O1 109.5(17) 2_656 .
O6 O3 O1 113.5(17) . .
O1 O3 O1 112(2) 1_655 .
O2 O3 O1 61.0(18) 4_645 .
O4 O3 O1 55.9(14) 1_655 .
O5 O3 O1 66.9(15) . .
O5 O3 O1 123.7(16) 2_655 .
Ga2 O3 O3 96.9(16) . 2_655
Ga3 O3 O3 33.9(11) . 2_655
La2 O3 O3 95.3(13) 1_655 2_655
La1 O3 O3 155.1(7) 2_656 2_655
O6 O3 O3 105.0(10) . 2_655
O1 O3 O3 151.0(19) 1_655 2_655
O2 O3 O3 134(2) 4_645 2_655
O4 O3 O3 106.7(13) 1_655 2_655
O5 O3 O3 60.6(12) . 2_655
O5 O3 O3 58.8(11) 2_655 2_655
O1 O3 O3 72.7(16) . 2_655
Ga2 O3 O5 137.5(17) . 1_655
Ga3 O3 O5 99.1(12) . 1_655
La2 O3 O5 84.1(10) 1_655 1_655
La1 O3 O5 45.3(8) 2_656 1_655
O6 O3 O5 46.4(9) . 1_655
O1 O3 O5 63.2(13) 1_655 1_655
O2 O3 O5 99.5(18) 4_645 1_655
O4 O3 O5 124.1(15) 1_655 1_655
O5 O3 O5 102.3(12) . 1_655
O5 O3 O5 66.6(13) 2_655 1_655
O1 O3 O5 153.1(18) . 1_655
O3 O3 O5 125.1(13) 2_655 1_655
Ga2 O3 Ta 157.1(15) . 1_655
Ga3 O3 Ta 65.8(8) . 1_655
La2 O3 Ta 99.0(9) 1_655 1_655
La1 O3 Ta 69.0(7) 2_656 1_655
O6 O3 Ta 35.2(6) . 1_655
O1 O3 Ta 96.2(14) 1_655 1_655
O2 O3 Ta 124.6(17) 4_645 1_655
O4 O3 Ta 157.4(16) 1_655 1_655
O5 O3 Ta 76.1(8) . 1_655
O5 O3 Ta 35.5(7) 2_655 1_655
O1 O3 Ta 142.6(14) . 1_655
O3 O3 Ta 93.9(9) 2_655 1_655
O5 O3 Ta 33.3(7) 1_655 1_655
Ga2 O3 Ga1 157.1(15) . 1_655
Ga3 O3 Ga1 65.8(8) . 1_655
La2 O3 Ga1 99.0(9) 1_655 1_655
La1 O3 Ga1 69.0(7) 2_656 1_655
O6 O3 Ga1 35.2(6) . 1_655
O1 O3 Ga1 96.2(14) 1_655 1_655
O2 O3 Ga1 124.6(17) 4_645 1_655
O4 O3 Ga1 157.4(16) 1_655 1_655
O5 O3 Ga1 76.1(8) . 1_655
O5 O3 Ga1 35.5(7) 2_655 1_655
O1 O3 Ga1 142.6(14) . 1_655
O3 O3 Ga1 93.9(9) 2_655 1_655
O5 O3 Ga1 33.3(7) 1_655 1_655
Ta O3 Ga1 0.00(15) 1_655 1_655
Ga2 O3 O1 119.9(15) . 2_655
Ga3 O3 O1 72.9(13) . 2_655
La2 O3 O1 43.9(10) 1_655 2_655
La1 O3 O1 134.5(12) 2_656 2_655
O6 O3 O1 116.9(14) . 2_655
O1 O3 O1 98(2) 1_655 2_655
O2 O3 O1 142.7(18) 4_645 2_655
O4 O3 O1 100.9(18) 1_655 2_655
O5 O3 O1 110.7(14) . 2_655
O5 O3 O1 60.0(13) 2_655 2_655
O1 O3 O1 114.5(18) . 2_655
O3 O3 O1 56.1(10) 2_655 2_655
O5 O3 O1 92.3(10) 1_655 2_655
Ta O3 O1 82.8(11) 1_655 2_655
Ga1 O3 O1 82.8(11) 1_655 2_655
Ga2 O3 Ga2 104.1(13) . 2_655
Ga3 O3 Ga2 56.8(11) . 2_655
La2 O3 Ga2 65.2(8) 1_655 2_655
La1 O3 Ga2 160.7(11) 2_656 2_655
O6 O3 Ga2 121.5(11) . 2_655
O1 O3 Ga2 121.4(16) 1_655 2_655
O2 O3 Ga2 139.9(16) 4_645 2_655
O4 O3 Ga2 97.8(13) 1_655 2_655
O5 O3 Ga2 90.1(12) . 2_655
O5 O3 Ga2 62.6(10) 2_655 2_655
O1 O3 Ga2 89.8(15) . 2_655
O3 O3 Ga2 30.3(7) 2_655 2_655
O5 O3 Ga2 115.6(10) 1_655 2_655
Ta O3 Ga2 95.4(8) 1_655 2_655
Ga1 O3 Ga2 95.4(8) 1_655 2_655
O1 O3 Ga2 27.7(4) 2_655 2_655
Ga2 O3 O3 140.6(12) . 2_755
Ga3 O3 O3 96.0(14) . 2_755
La2 O3 O3 42.1(7) 1_655 2_755
La1 O3 O3 88.6(13) 2_656 2_755
O6 O3 O3 89.2(10) . 2_755
O1 O3 O3 66.6(15) 1_655 2_755
O2 O3 O3 124(2) 4_645 2_755
O4 O3 O3 110.0(13) 1_655 2_755
O5 O3 O3 127.1(12) . 2_755
O5 O3 O3 62.2(10) 2_655 2_755
O1 O3 O3 156.8(16) . 2_755
O3 O3 O3 97.2(18) 2_655 2_755
O5 O3 O3 49.2(9) 1_655 2_755
Ta O3 O3 56.9(5) 1_655 2_755
Ga1 O3 O3 56.9(5) 1_655 2_755
O1 O3 O3 45.9(9) 2_655 2_755
Ga2 O3 O3 73.0(10) 2_655 2_755
Ga2 O3 Ga4 110.2(12) . 3_544
Ga3 O3 Ga4 53.3(8) . 3_544
La2 O3 Ga4 149.5(10) 1_655 3_544
La1 O3 Ga4 69.8(7) 2_656 3_544
O6 O3 Ga4 25.2(8) . 3_544
O1 O3 Ga4 121.6(17) 1_655 3_544
O2 O3 Ga4 99.2(14) 4_645 3_544
O4 O3 Ga4 138.5(16) 1_655 3_544
O5 O3 Ga4 32.2(7) . 3_544
O5 O3 Ga4 58.6(8) 2_655 3_544
O1 O3 Ga4 92.8(13) . 3_544
O3 O3 Ga4 85.4(7) 2_655 3_544
O5 O3 Ga4 70.9(7) 1_655 3_544
Ta O3 Ga4 50.6(4) 1_655 3_544
Ga1 O3 Ga4 50.6(4) 1_655 3_544
O1 O3 Ga4 118.1(12) 2_655 3_544
Ga2 O3 Ga4 109.7(8) 2_655 3_544
O3 O3 Ga4 107.4(5) 2_755 3_544
Ga2 O3 La2 59.5(9) . .
Ga3 O3 La2 64.6(11) . .
La2 O3 La2 97.5(10) 1_655 .
La1 O3 La2 148.0(11) 2_656 .
O6 O3 La2 126.4(13) . .
O1 O3 La2 131.7(13) 1_655 .
O2 O3 La2 97.2(16) 4_645 .
O4 O3 La2 72.3(11) 1_655 .
O5 O3 La2 69.2(11) . .
O5 O3 La2 96.0(12) 2_655 .
O1 O3 La2 38.8(12) . .
O3 O3 La2 37.5(8) 2_655 .
O5 O3 La2 162.5(11) 1_655 .
Ta O3 La2 129.9(10) 1_655 .
Ga1 O3 La2 129.9(10) 1_655 .
O1 O3 La2 77.3(8) 2_655 .
Ga2 O3 La2 51.1(5) 2_655 .
O3 O3 La2 123.1(13) 2_755 .
Ga4 O3 La2 101.3(8) 3_544 .
Ga2 O3 O7 75.2(11) . 2_655
Ga3 O3 O7 109.1(16) . 2_655
La2 O3 O7 33.0(7) 1_655 2_655
La1 O3 O7 127.5(12) 2_656 2_655
O6 O3 O7 161.6(13) . 2_655
O1 O3 O7 75.1(15) 1_655 2_655
O2 O3 O7 94.9(16) 4_645 2_655
O4 O3 O7 52.1(14) 1_655 2_655
O5 O3 O7 134.1(14) . 2_655
O5 O3 O7 108.6(13) 2_655 2_655
O1 O3 O7 84.8(14) . 2_655
O3 O3 O7 77.2(9) 2_655 2_655
O5 O3 O7 117.1(11) 1_655 2_655
Ta O3 O7 127.1(11) 1_655 2_655
Ga1 O3 O7 127.1(11) 1_655 2_655
O1 O3 O7 48.8(12) 2_655 2_655
Ga2 O3 O7 52.9(8) 2_655 2_655
O3 O3 O7 72.4(7) 2_755 2_655
Ga4 O3 O7 162.4(13) 3_544 2_655
La2 O3 O7 66.3(8) . 2_655
Ga2 O3 La1 56.3(9) . 2_556
Ga3 O3 La1 69.6(10) . 2_556
La2 O3 La1 152.5(10) 1_655 2_556
La1 O3 La1 91.6(8) 2_656 2_556
O6 O3 La1 77.9(10) . 2_556
O1 O3 La1 125.8(16) 1_655 2_556
O2 O3 La1 68.9(14) 4_645 2_556
O4 O3 La1 86.9(13) 1_655 2_556
O5 O3 La1 36.1(9) . 2_556
O5 O3 La1 101.4(10) 2_655 2_556
O1 O3 La1 36.0(11) . 2_556
O3 O3 La1 76.0(12) 2_655 2_556
O5 O3 La1 122.4(9) 1_655 2_556
Ta O3 La1 107.5(7) 1_655 2_556
Ga1 O3 La1 107.5(7) 1_655 2_556
O1 O3 La1 131.7(11) 2_655 2_556
Ga2 O3 La1 104.3(9) 2_655 2_556
O3 O3 La1 163.0(7) 2_755 2_556
Ga4 O3 La1 57.0(4) 3_544 2_556
La2 O3 La1 59.7(5) . 2_556
O7 O3 La1 119.9(9) 2_655 2_556
Ga2 O3 La1 50.0(8) . 3_654
Ga3 O3 La1 165.3(14) . 3_654
La2 O3 La1 68.1(7) 1_655 3_654
La1 O3 La1 67.3(7) 2_656 3_654
O6 O3 La1 117.6(13) . 3_654
O1 O3 La1 34.1(10) 1_655 3_654
O2 O3 La1 34.0(14) 4_645 3_654
O4 O3 La1 29.3(10) 1_655 3_654
O5 O3 La1 134.4(12) . 3_654
O5 O3 La1 157.4(12) 2_655 3_654
O1 O3 La1 78.6(12) . 3_654
O3 O3 La1 135.4(6) 2_655 3_654
O5 O3 La1 95.2(10) 1_655 3_654
Ta O3 La1 128.5(10) 1_655 3_654
Ga1 O3 La1 128.5(10) 1_655 3_654
O1 O3 La1 110.2(11) 2_655 3_654
Ga2 O3 La1 119.4(7) 2_655 3_654
O3 O3 La1 96.1(10) 2_755 3_654
Ga4 O3 La1 129.9(9) 3_544 3_654
La2 O3 La1 101.5(6) . 3_654
O7 O3 La1 66.8(8) 2_655 3_654
La1 O3 La1 99.7(6) 2_556 3_654
Ga2 O3 Ga4 40.3(8) . 2_656
Ga3 O3 Ga4 118.9(13) . 2_656
La2 O3 Ga4 121.8(10) 1_655 2_656
La1 O3 Ga4 56.8(6) 2_656 2_656
O6 O3 Ga4 84.1(10) . 2_656
O1 O3 Ga4 75.1(14) 1_655 2_656
O2 O3 Ga4 19.9(13) 4_645 2_656
O4 O3 Ga4 58.4(12) 1_655 2_656
O5 O3 Ga4 81.3(11) . 2_656
O5 O3 Ga4 140.1(10) 2_655 2_656
O1 O3 Ga4 53.1(13) . 2_656
O3 O3 Ga4 123.1(15) 2_655 2_656
O5 O3 Ga4 102.0(10) 1_655 2_656
Ta O3 Ga4 117.5(9) 1_655 2_656
Ga1 O3 Ga4 117.5(9) 1_655 2_656
O1 O3 Ga4 159.0(12) 2_655 2_656
Ga2 O3 Ga4 142.4(9) 2_655 2_656
O3 O3 Ga4 139.6(16) 2_755 2_656
Ga4 O3 Ga4 81.5(6) 3_544 2_656
La2 O3 Ga4 91.9(6) . 2_656
O7 O3 Ga4 110.4(9) 2_655 2_656
La1 O3 Ga4 50.7(4) 2_556 2_656
La1 O3 Ga4 53.8(4) 3_654 2_656
Ga2 O3 Ga4 39.4(7) . 3_554
Ga3 O3 Ga4 118.5(15) . 3_554
La2 O3 Ga4 63.5(6) 1_655 3_554
La1 O3 Ga4 115.9(9) 2_656 3_554
O6 O3 Ga4 160.6(13) . 3_554
O1 O3 Ga4 76.4(12) 1_655 3_554
O2 O3 Ga4 65.1(14) 4_645 3_554
O4 O3 Ga4 22.3(10) 1_655 3_554
O5 O3 Ga4 118.5(12) . 3_554
O5 O3 Ga4 138.2(13) 2_655 3_554
O1 O3 Ga4 53.8(11) . 3_554
O3 O3 Ga4 85.9(6) 2_655 3_554
O5 O3 Ga4 138.1(10) 1_655 3_554
Ta O3 Ga4 162.4(9) 1_655 3_554
Ga1 O3 Ga4 162.4(9) 1_655 3_554
O1 O3 Ga4 82.5(11) 2_655 3_554
Ga2 O3 Ga4 75.7(6) 2_655 3_554
O3 O3 Ga4 105.6(4) 2_755 3_554
Ga4 O3 Ga4 146.6(9) 3_544 3_554
La2 O3 Ga4 55.3(4) . 3_554
O7 O3 Ga4 35.8(6) 2_655 3_554
La1 O3 Ga4 89.6(6) 2_556 3_554
La1 O3 Ga4 49.5(3) 3_654 3_554
Ga4 O3 Ga4 76.5(5) 2_656 3_554
Ga2 O3 O2 84.2(14) . 1_545
Ga3 O3 O2 66.2(14) . 1_545
La2 O3 O2 172.4(11) 1_655 1_545
La1 O3 O2 68.2(10) 2_656 1_545
O6 O3 O2 43.6(12) . 1_545
O1 O3 O2 118(2) 1_655 1_545
O2 O3 O2 77.3(13) 4_645 1_545
O4 O3 O2 112.6(17) 1_655 1_545
O5 O3 O2 30.1(12) . 1_545
O5 O3 O2 82.9(12) 2_655 1_545
O1 O3 O2 69.9(15) . 1_545
O3 O3 O2 90.5(11) 2_655 1_545
O5 O3 O2 88.5(10) 1_655 1_545
Ta O3 O2 75.6(10) 1_655 1_545
Ga1 O3 O2 75.6(10) 1_655 1_545
O1 O3 O2 138.7(15) 2_655 1_545
Ga2 O3 O2 120.2(13) 2_655 1_545
O3 O3 O2 132.2(8) 2_755 1_545
Ga4 O3 O2 26.1(9) 3_544 1_545
La2 O3 O2 90.2(10) . 1_545
O7 O3 O2 154.3(12) 2_655 1_545
La1 O3 O2 34.4(9) 2_556 1_545
La1 O3 O2 110.9(13) 3_654 1_545
Ga4 O3 O2 57.9(10) 2_656 1_545
Ga4 O3 O2 122.0(11) 3_554 1_545
Ga2 O3 Ga3 140.0(15) . 1_655
Ga3 O3 Ga3 104.4(11) . 1_655
La2 O3 Ga3 59.0(7) 1_655 1_655
La1 O3 Ga3 64.2(7) 2_656 1_655
O6 O3 Ga3 70.7(9) . 1_655
O1 O3 Ga3 56.1(11) 1_655 1_655
O2 O3 Ga3 108.5(18) 4_645 1_655
O4 O3 Ga3 113.7(14) 1_655 1_655
O5 O3 Ga3 122.1(10) . 1_655
O5 O3 Ga3 67.7(9) 2_655 1_655
O1 O3 Ga3 168.5(15) . 1_655
O3 O3 Ga3 117.3(14) 2_655 1_655
O5 O3 Ga3 25.8(6) 1_655 1_655
Ta O3 Ga3 46.1(4) 1_655 1_655
Ga1 O3 Ga3 46.1(4) 1_655 1_655
O1 O3 Ga3 70.5(7) 2_655 1_655
Ga2 O3 Ga3 97.0(7) 2_655 1_655
O3 O3 Ga3 24.8(6) 2_755 1_655
Ga4 O3 Ga3 93.6(6) 3_544 1_655
La2 O3 Ga3 147.8(9) . 1_655
O7 O3 Ga3 91.9(8) 2_655 1_655
La1 O3 Ga3 148.1(8) 2_556 1_655
La1 O3 Ga3 90.0(7) 3_654 1_655
Ga4 O3 Ga3 118.6(9) 2_656 1_655
Ga4 O3 Ga3 118.9(7) 3_554 1_655
O2 O3 Ga3 113.8(9) 1_545 1_655
Ga2 O3 O7 48.0(10) . .
Ga3 O3 O7 93.3(14) . .
La2 O3 O7 73.3(9) 1_655 .
La1 O3 O7 138.7(11) 2_656 .
O6 O3 O7 156.1(16) . .
O1 O3 O7 101.0(15) 1_655 .
O2 O3 O7 83.3(16) 4_645 .
O4 O3 O7 45.8(12) 1_655 .
O5 O3 O7 99.2(14) . .
O5 O3 O7 117.2(14) 2_655 .
O1 O3 O7 45.9(13) . .
O3 O3 O7 61.0(8) 2_655 .
O5 O3 O7 157.3(11) 1_655 .
Ta O3 O7 152.1(12) 1_655 .
Ga1 O3 O7 152.1(12) 1_655 .
O1 O3 O7 73.1(11) 2_655 .
Ga2 O3 O7 56.8(7) 2_655 .
O3 O3 O7 110.9(9) 2_755 .
Ga4 O3 O7 131.2(11) 3_544 .
La2 O3 O7 31.1(6) . .
O7 O3 O7 40.3(11) 2_655 .
La1 O3 O7 79.8(8) 2_556 .
La1 O3 O7 74.5(7) 3_654 .
Ga4 O3 O7 88.3(8) 2_656 .
Ga4 O3 O7 25.3(6) 3_554 .
O2 O3 O7 114.0(10) 1_545 .
Ga3 O3 O7 132.2(10) 1_655 .
Ga2 O3 O4 54.2(10) . 4_545
Ga3 O3 O4 94.2(14) . 4_545
La2 O3 O4 147.3(13) 1_655 4_545
La1 O3 O4 62.6(12) 2_656 4_545
O6 O3 O4 68.1(14) . 4_545
O1 O3 O4 97.4(17) 1_655 4_545
O2 O3 O4 45.3(13) 4_645 4_545
O4 O3 O4 80.0(10) 1_655 4_545
O5 O3 O4 56.2(11) . 4_545
O5 O3 O4 116.2(12) 2_655 4_545
O1 O3 O4 51.4(15) . 4_545
O3 O3 O4 106.6(15) 2_655 4_545
O5 O3 O4 101.8(14) 1_655 4_545
Ta O3 O4 103.3(12) 1_655 4_545
Ga1 O3 O4 103.3(12) 1_655 4_545
O1 O3 O4 162.3(14) 2_655 4_545
Ga2 O3 O4 134.7(12) 2_655 4_545
O3 O3 O4 150.5(17) 2_755 4_545
Ga4 O3 O4 58.5(9) 3_544 4_545
La2 O3 O4 86.3(10) . 4_545
O7 O3 O4 129.4(12) 2_655 4_545
La1 O3 O4 30.7(8) 2_556 4_545
La1 O3 O4 79.3(9) 3_654 4_545
Ga4 O3 O4 25.5(8) 2_656 4_545
Ga4 O3 O4 93.6(9) 3_554 4_545
O2 O3 O4 33.3(11) 1_545 4_545
Ga3 O3 O4 125.7(13) 1_655 4_545
O7 O3 O4 96.1(11) . 4_545
Ga2 O3 Ga2 97.8(12) . 1_655
Ga3 O3 Ga2 146.6(13) . 1_655
La2 O3 Ga2 52.5(7) 1_655 1_655
La1 O3 Ga2 52.6(6) 2_656 1_655
O6 O3 Ga2 92.3(11) . 1_655
O1 O3 Ga2 13.9(10) 1_655 1_655
O2 O3 Ga2 70.4(16) 4_645 1_655
O4 O3 Ga2 73.9(12) 1_655 1_655
O5 O3 Ga2 148.1(12) . 1_655
O5 O3 Ga2 109.9(11) 2_655 1_655
O1 O3 Ga2 126.4(14) . 1_655
O3 O3 Ga2 146.5(14) 2_655 1_655
O5 O3 Ga2 51.7(7) 1_655 1_655
Ta O3 Ga2 83.8(7) 1_655 1_655
Ga1 O3 Ga2 83.8(7) 1_655 1_655
O1 O3 Ga2 90.6(8) 2_655 1_655
Ga2 O3 Ga2 116.5(8) 2_655 1_655
O3 O3 Ga2 53.9(9) 2_755 1_655
Ga4 O3 Ga2 116.9(8) 3_544 1_655
La2 O3 Ga2 141.0(7) . 1_655
O7 O3 Ga2 77.8(7) 2_655 1_655
La1 O3 Ga2 136.6(9) 2_556 1_655
La1 O3 Ga2 47.9(4) 3_654 1_655
Ga4 O3 Ga2 86.5(7) 2_656 1_655
Ga4 O3 Ga2 86.6(6) 3_554 1_655
O2 O3 Ga2 120.8(11) 1_545 1_655
Ga3 O3 Ga2 42.2(4) 1_655 1_655
O7 O3 Ga2 109.9(8) . 1_655
O4 O3 Ga2 106.4(12) 4_545 1_655
Ga2 O3 O6 117.3(13) . 2_655
Ga3 O3 O6 2.4(8) . 2_655
La2 O3 O6 117.6(11) 1_655 2_655
La1 O3 O6 119.3(9) 2_656 2_655
O6 O3 O6 68.8(12) . 2_655
O1 O3 O6 158.7(14) 1_655 2_655
O2 O3 O6 138.4(17) 4_645 2_655
O4 O3 O6 139.1(14) 1_655 2_655
O5 O3 O6 37.7(9) . 2_655
O5 O3 O6 35.1(7) 2_655 2_655
O1 O3 O6 88.7(13) . 2_655
O3 O3 O6 36.3(5) 2_655 2_655
O5 O3 O6 96.8(8) 1_655 2_655
Ta O3 O6 63.5(6) 1_655 2_655
Ga1 O3 O6 63.5(6) 1_655 2_655
O1 O3 O6 73.8(10) 2_655 2_655
Ga2 O3 O6 58.5(7) 2_655 2_655
O3 O3 O6 95.2(11) 2_755 2_655
Ga4 O3 O6 51.3(5) 3_544 2_655
La2 O3 O6 66.9(7) . 2_655
O7 O3 O6 111.0(11) 2_655 2_655
La1 O3 O6 70.0(6) 2_556 2_655
La1 O3 O6 167.2(8) 3_654 2_655
Ga4 O3 O6 118.8(8) 2_656 2_655
Ga4 O3 O6 121.0(9) 3_554 2_655
O2 O3 O6 65.1(11) 1_545 2_655
Ga3 O3 O6 102.8(6) 1_655 2_655
O7 O3 O6 95.7(8) . 2_655
O4 O3 O6 93.9(10) 4_545 2_655
Ga2 O3 O6 144.9(8) 1_655 2_655
Ga2 O3 O1 88.0(13) . 4_645
Ga3 O3 O1 101.0(13) . 4_645
La2 O3 O1 132.1(13) 1_655 4_645
La1 O3 O1 27.2(5) 2_656 4_645
O6 O3 O1 38.2(11) . 4_645
O1 O3 O1 78.2(12) 1_655 4_645
O2 O3 O1 58.1(16) 4_645 4_645
O4 O3 O1 101.9(15) 1_655 4_645
O5 O3 O1 70.3(10) . 4_645
O5 O3 O1 98.1(12) 2_655 4_645
O1 O3 O1 92.4(12) . 4_645
O3 O3 O1 130.8(11) 2_655 4_645
O5 O3 O1 60.7(9) 1_655 4_645
Ta O3 O1 69.8(9) 1_655 4_645
Ga1 O3 O1 69.8(9) 1_655 4_645
O1 O3 O1 151.6(15) 2_655 4_645
Ga2 O3 O1 157.5(10) 2_655 4_645
O3 O3 O1 109.5(11) 2_755 4_645
Ga4 O3 O1 47.8(9) 3_544 4_645
La2 O3 O1 126.0(8) . 4_645
O7 O3 O1 149.6(13) 2_655 4_645
La1 O3 O1 66.4(5) 2_556 4_645
La1 O3 O1 83.0(10) 3_654 4_645
Ga4 O3 O1 47.8(8) 2_656 4_645
Ga4 O3 O1 123.0(10) 3_554 4_645
O2 O3 O1 41.1(10) 1_545 4_645
Ga3 O3 O1 84.9(7) 1_655 4_645
O7 O3 O1 135.3(10) . 4_645
O4 O3 O1 41.1(10) 4_545 4_645
Ga2 O3 O1 79.7(7) 1_655 4_645
O6 O3 O1 99.1(10) 2_655 4_645
Ga2 O3 O7 84.5(10) . 1_655
Ga3 O3 O7 133.8(15) . 1_655
La2 O3 O7 18.5(7) 1_655 1_655
La1 O3 O7 96.1(11) 2_656 1_655
O6 O3 O7 134.8(15) . 1_655
O1 O3 O7 43.9(14) 1_655 1_655
O2 O3 O7 83.6(16) 4_645 1_655
O4 O3 O7 54.0(12) 1_655 1_655
O5 O3 O7 166.9(15) . 1_655
O5 O3 O7 114.0(11) 2_655 1_655
O1 O3 O7 105.9(13) . 1_655
O3 O3 O7 107.2(10) 2_655 1_655
O5 O3 O7 88.8(9) 1_655 1_655
Ta O3 O7 111.4(10) 1_655 1_655
Ga1 O3 O7 111.4(10) 1_655 1_655
O1 O3 O7 61.2(12) 2_655 1_655
Ga2 O3 O7 78.6(8) 2_655 1_655
O3 O3 O7 56.2(7) 2_755 1_655
Ga4 O3 O7 159.7(11) 3_544 1_655
La2 O3 O7 98.2(7) . 1_655
O7 O3 O7 32.8(10) 2_655 1_655
La1 O3 O7 140.5(8) 2_556 1_655
La1 O3 O7 49.7(6) 3_654 1_655
Ga4 O3 O7 103.4(8) 2_656 1_655
Ga4 O3 O7 52.3(5) 3_554 1_655
O2 O3 O7 160.0(15) 1_545 1_655
Ga3 O3 O7 66.7(7) 1_655 1_655
O7 O3 O7 69.0(7) . 1_655
O4 O3 O7 128.8(11) 4_545 1_655
Ga2 O3 O7 45.0(7) 1_655 1_655
O6 O3 O7 134.9(10) 2_655 1_655
O1 O3 O7 122.0(11) 4_645 1_655
Ga2 O3 Ga2 76.6(10) . 4_645
Ga3 O3 Ga2 88.8(11) . 4_645
La2 O3 Ga2 152.0(13) 1_655 4_645
La1 O3 Ga2 48.5(5) 2_656 4_645
O6 O3 Ga2 45.4(8) . 4_645
O1 O3 Ga2 95.8(17) 1_655 4_645
O2 O3 Ga2 58.1(13) 4_645 4_645
O4 O3 Ga2 99.3(14) 1_655 4_645
O5 O3 Ga2 52.9(9) . 4_645
O5 O3 Ga2 99.3(9) 2_655 4_645
O1 O3 Ga2 73.3(14) . 4_645
O3 O3 Ga2 112.7(11) 2_655 4_645
O5 O3 Ga2 80.5(8) 1_655 4_645
Ta O3 Ga2 80.6(6) 1_655 4_645
Ga1 O3 Ga2 80.6(6) 1_655 4_645
O1 O3 Ga2 159.2(12) 2_655 4_645
Ga2 O3 Ga2 142.8(9) 2_655 4_645
O3 O3 Ga2 129.6(10) 2_755 4_645
Ga4 O3 Ga2 41.1(4) 3_544 4_645
La2 O3 Ga2 104.2(7) . 4_645
O7 O3 Ga2 151.1(10) 2_655 4_645
La1 O3 Ga2 44.4(3) 2_556 4_645
La1 O3 Ga2 90.1(7) 3_654 4_645
Ga4 O3 Ga2 41.0(3) 2_656 4_645
Ga4 O3 Ga2 115.7(7) 3_554 4_645
O2 O3 Ga2 22.9(9) 1_545 4_645
Ga3 O3 Ga2 105.8(7) 1_655 4_645
O7 O3 Ga2 118.9(9) . 4_645
O4 O3 Ga2 23.1(9) 4_545 4_645
Ga2 O3 Ga2 100.0(7) 1_655 4_645
O6 O3 Ga2 87.5(6) 2_655 4_645
O1 O3 Ga2 22.1(3) 4_645 4_645
O7 O3 Ga2 137.4(10) 1_655 4_645
Ga2 O3 O6 176.4(17) . 2_755
Ga3 O3 O6 67.7(9) . 2_755
La2 O3 O6 79.1(8) 1_655 2_755
La1 O3 O6 83.2(8) 2_656 2_755
O6 O3 O6 57.2(10) . 2_755
O1 O3 O6 92.7(13) 1_655 2_755
O2 O3 O6 138.6(18) 4_645 2_755
O4 O3 O6 147.5(15) 1_655 2_755
O5 O3 O6 90.4(10) . 2_755
O5 O3 O6 31.2(7) 2_655 2_755
O1 O3 O6 154.7(15) . 2_755
O3 O3 O6 86.6(12) 2_655 2_755
O5 O3 O6 39.1(8) 1_655 2_755
Ta O3 O6 22.0(4) 1_655 2_755
Ga1 O3 O6 22.0(4) 1_655 2_755
O1 O3 O6 61.7(10) 2_655 2_755
Ga2 O3 O6 78.7(7) 2_655 2_755
O3 O3 O6 37.8(5) 2_755 2_755
Ga4 O3 O6 70.5(6) 3_544 2_755
La2 O3 O6 123.9(9) . 2_755
O7 O3 O6 105.2(9) 2_655 2_755
La1 O3 O6 125.4(7) 2_556 2_755
La1 O3 O6 126.7(9) 3_654 2_755
Ga4 O3 O6 137.5(9) 2_656 2_755
Ga4 O3 O6 140.9(8) 3_554 2_755
O2 O3 O6 96.4(11) 1_545 2_755
Ga3 O3 O6 36.7(5) 1_655 2_755
O7 O3 O6 134.3(10) . 2_755
O4 O3 O6 125.3(12) 4_545 2_755
Ga2 O3 O6 78.9(7) 1_655 2_755
O6 O3 O6 66.0(5) 2_655 2_755
O1 O3 O6 90.1(10) 4_645 2_755
O7 O3 O6 94.0(8) 1_655 2_755
Ga2 O3 O6 102.5(6) 4_645 2_755
Ga2 O3 La1 152.3(14) . 1_654
Ga3 O3 La1 59.9(9) . 1_654
La2 O3 La1 64.5(7) 1_655 1_654
La1 O3 La1 112.0(9) 2_656 1_654
O6 O3 La1 83.8(9) . 1_654
O1 O3 La1 103.2(14) 1_655 1_654
O2 O3 La1 160.7(19) 4_645 1_654
O4 O3 La1 132.2(15) 1_655 1_654
O5 O3 La1 95.2(10) . 1_654
O5 O3 La1 31.4(8) 2_655 1_654
O1 O3 La1 136.4(16) . 1_654
O3 O3 La1 64.0(11) 2_655 1_654
O5 O3 La1 66.7(8) 1_655 1_654
Ta O3 La1 49.9(4) 1_655 1_654
Ga1 O3 La1 49.9(4) 1_655 1_654
O1 O3 La1 33.1(9) 2_655 1_654
Ga2 O3 La1 49.2(4) 2_655 1_654
O3 O3 La1 36.6(8) 2_755 1_654
Ga4 O3 La1 89.1(5) 3_544 1_654
La2 O3 La1 98.2(8) . 1_654
O7 O3 La1 80.8(9) 2_655 1_654
La1 O3 La1 129.5(8) 2_556 1_654
La1 O3 La1 130.4(7) 3_654 1_654
Ga4 O3 La1 167.4(8) 2_656 1_654
Ga4 O3 La1 115.5(7) 3_554 1_654
O2 O3 La1 114.2(12) 1_545 1_654
Ga3 O3 La1 53.3(4) 1_655 1_654
O7 O3 La1 104.3(9) . 1_654
O4 O3 La1 147.4(11) 4_545 1_654
Ga2 O3 La1 90.3(6) 1_655 1_654
O6 O3 La1 59.4(5) 2_655 1_654
O1 O3 La1 119.6(9) 4_645 1_654
O7 O3 La1 82.7(8) 1_655 1_654
Ga2 O3 La1 128.1(6) 4_645 1_654
O6 O3 La1 30.0(4) 2_755 1_654
Ga2 O3 Ga1 97.6(12) . .
Ga3 O3 Ga1 24.2(7) . .
La2 O3 Ga1 139.5(12) 1_655 .
La1 O3 Ga1 110.0(8) 2_656 .
O6 O3 Ga1 65.5(9) . .
O1 O3 Ga1 162.6(17) 1_655 .
O2 O3 Ga1 114.1(16) 4_645 .
O4 O3 Ga1 125.6(13) 1_655 .
O5 O3 Ga1 15.1(8) . .
O5 O3 Ga1 56.5(8) 2_655 .
O1 O3 Ga1 70.0(12) . .
O3 O3 Ga1 46.3(6) 2_655 .
O5 O3 Ga1 106.3(8) 1_655 .
Ta O3 Ga1 75.6(5) 1_655 .
Ga1 O3 Ga1 75.6(5) 1_655 .
O1 O3 Ga1 95.8(10) 2_655 .
Ga2 O3 Ga1 75.2(6) 2_655 .
O3 O3 Ga1 118.4(10) 2_755 .
Ga4 O3 Ga1 41.6(3) 3_544 .
La2 O3 Ga1 61.6(5) . .
O7 O3 Ga1 122.2(11) 2_655 .
La1 O3 Ga1 46.0(3) 2_556 .
La1 O3 Ga1 145.5(8) 3_654 .
Ga4 O3 Ga1 94.7(6) 2_656 .
Ga4 O3 Ga1 115.6(8) 3_554 .
O2 O3 Ga1 45.1(10) 1_545 .
Ga3 O3 Ga1 120.7(6) 1_655 .
O7 O3 Ga1 92.7(9) . .
O4 O3 Ga1 70.2(9) 4_545 .
Ga2 O3 Ga1 157.5(7) 1_655 .
O6 O3 Ga1 24.2(4) 2_655 .
O1 O3 Ga1 84.5(8) 4_645 .
O7 O3 Ga1 153.5(10) 1_655 .
Ga2 O3 Ga1 67.9(4) 4_645 .
O6 O3 Ga1 85.2(6) 2_755 .
La1 O3 Ga1 83.5(5) 1_654 .
Ga2 O3 Ta 97.6(12) . .
Ga3 O3 Ta 24.2(7) . .
La2 O3 Ta 139.5(12) 1_655 .
La1 O3 Ta 110.0(8) 2_656 .
O6 O3 Ta 65.5(9) . .
O1 O3 Ta 162.6(17) 1_655 .
O2 O3 Ta 114.1(16) 4_645 .
O4 O3 Ta 125.6(13) 1_655 .
O5 O3 Ta 15.1(8) . .
O5 O3 Ta 56.5(8) 2_655 .
O1 O3 Ta 70.0(12) . .
O3 O3 Ta 46.3(6) 2_655 .
O5 O3 Ta 106.3(8) 1_655 .
Ta O3 Ta 75.6(5) 1_655 .
Ga1 O3 Ta 75.6(5) 1_655 .
O1 O3 Ta 95.8(10) 2_655 .
Ga2 O3 Ta 75.2(6) 2_655 .
O3 O3 Ta 118.4(10) 2_755 .
Ga4 O3 Ta 41.6(3) 3_544 .
La2 O3 Ta 61.6(5) . .
O7 O3 Ta 122.2(11) 2_655 .
La1 O3 Ta 46.0(3) 2_556 .
La1 O3 Ta 145.5(8) 3_654 .
Ga4 O3 Ta 94.7(6) 2_656 .
Ga4 O3 Ta 115.6(8) 3_554 .
O2 O3 Ta 45.1(10) 1_545 .
Ga3 O3 Ta 120.7(6) 1_655 .
O7 O3 Ta 92.7(9) . .
O4 O3 Ta 70.2(9) 4_545 .
Ga2 O3 Ta 157.5(7) 1_655 .
O6 O3 Ta 24.2(4) 2_655 .
O1 O3 Ta 84.5(8) 4_645 .
O7 O3 Ta 153.5(10) 1_655 .
Ga2 O3 Ta 67.9(4) 4_645 .
O6 O3 Ta 85.2(6) 2_755 .
La1 O3 Ta 83.5(5) 1_654 .
Ga1 O3 Ta 0.00(16) . .
Ga2 O3 O7 143.7(13) . 2_645
Ga3 O3 O7 47.1(9) . 2_645
La2 O3 O7 116.2(10) 1_655 2_645
La1 O3 O7 78.9(8) 2_656 2_645
O6 O3 O7 31.2(9) . 2_645
O1 O3 O7 116.6(14) 1_655 2_645
O2 O3 O7 127.3(15) 4_645 2_645
O4 O3 O7 171.1(17) 1_655 2_645
O5 O3 O7 54.6(10) . 2_645
O5 O3 O7 28.9(9) 2_655 2_645
O1 O3 O7 121.5(13) . 2_645
O3 O3 O7 79.2(8) 2_655 2_645
O5 O3 O7 53.6(7) 1_655 2_645
Ta O3 O7 21.9(5) 1_655 2_645
Ga1 O3 O7 21.9(5) 1_655 2_645
O1 O3 O7 88.0(12) 2_655 2_645
Ga2 O3 O7 90.6(9) 2_655 2_645
O3 O3 O7 75.2(6) 2_755 2_645
Ga4 O3 O7 33.9(5) 3_544 2_645
La2 O3 O7 111.3(9) . 2_645
O7 O3 O7 136.7(14) 2_655 2_645
La1 O3 O7 88.1(6) 2_556 2_645
La1 O3 O7 145.4(11) 3_654 2_645
Ga4 O3 O7 112.9(9) 2_656 2_645
Ga4 O3 O7 165.0(11) 3_554 2_645
O2 O3 O7 60.0(10) 1_545 2_645
Ga3 O3 O7 67.9(6) 1_655 2_645
O7 O3 O7 140.1(9) . 2_645
O4 O3 O7 92.0(11) 4_545 2_645
Ga2 O3 O7 105.1(8) 1_655 2_645
O6 O3 O7 44.7(5) 2_655 2_645
O1 O3 O7 69.3(11) 4_645 2_645
O7 O3 O7 131.4(7) 1_655 2_645
Ga2 O3 O7 72.0(7) 4_645 2_645
O6 O3 O7 37.5(6) 2_755 2_645
La1 O3 O7 56.2(6) 1_654 2_645
Ga1 O3 O7 53.8(5) . 2_645
Ta O3 O7 53.8(5) . 2_645
Ga2 O3 O4 87.2(14) . 2
Ga3 O3 O4 70.7(13) . 2
La2 O3 O4 60.5(8) 1_655 2
La1 O3 O4 165.2(11) 2_656 2
O6 O3 O4 139.4(13) . 2
O1 O3 O4 113.0(16) 1_655 2
O2 O3 O4 121.6(18) 4_645 2
O4 O3 O4 79.5(17) 1_655 2
O5 O3 O4 98.1(14) . 2
O5 O3 O4 81.0(12) 2_655 2
O1 O3 O4 77.8(16) . 2
O3 O3 O4 38.5(7) 2_655 2
O5 O3 O4 129.0(10) 1_655 2
Ta O3 O4 113.4(9) 1_655 2
Ga1 O3 O4 113.4(9) 1_655 2
O1 O3 O4 36.7(8) 2_655 2
Ga2 O3 O4 18.5(6) 2_655 2
O3 O3 O4 81.5(10) 2_755 2
Ga4 O3 O4 123.7(10) 3_544 2
La2 O3 O4 42.0(8) . 2
O7 O3 O4 38.7(9) 2_655 2
La1 O3 O4 101.1(10) 2_556 2
La1 O3 O4 102.8(8) 3_654 2
Ga4 O3 O4 127.1(9) 2_656 2
Ga4 O3 O4 57.3(8) 3_554 2
O2 O3 O4 126.5(12) 1_545 2
Ga3 O3 O4 106.3(8) 1_655 2
O7 O3 O4 39.2(10) . 2
O4 O3 O4 128.1(15) 4_545 2
Ga2 O3 O4 112.7(8) 1_655 2
O6 O3 O4 72.8(8) 2_655 2
O1 O3 O4 167.2(10) 4_645 2
O7 O3 O4 69.2(8) 1_655 2
Ga2 O3 O4 145.3(10) 4_645 2
O6 O3 O4 95.3(9) 2_755 2
La1 O3 O4 65.3(7) 1_654 2
Ga1 O3 O4 84.4(8) . 2
Ta O3 O4 84.4(8) . 2
O7 O3 O4 108.7(10) 2_645 2
Ga2 O3 O4 93.1(13) . 4_645
Ga3 O3 O4 132.2(15) . 4_645
La2 O3 O4 92.5(12) 1_655 4_645
La1 O3 O4 12.8(7) 2_656 4_645
O6 O3 O4 61.3(11) . 4_645
O1 O3 O4 39.9(16) 1_655 4_645
O2 O3 O4 55.1(14) 4_645 4_645
O4 O3 O4 86.8(12) 1_655 4_645
O5 O3 O4 109.5(11) . 4_645
O5 O3 O4 108.9(12) 2_655 4_645
O1 O3 O4 113.8(16) . 4_645
O3 O3 O4 166.1(7) 2_655 4_645
O5 O3 O4 44.4(11) 1_655 4_645
Ta O3 O4 73.4(10) 1_655 4_645
Ga1 O3 O4 73.4(10) 1_655 4_645
O1 O3 O4 125.9(12) 2_655 4_645
Ga2 O3 O4 153.6(11) 2_655 4_645
O3 O3 O4 81.0(14) 2_755 4_645
Ga4 O3 O4 82.0(9) 3_544 4_645
La2 O3 O4 152.1(9) . 4_645
O7 O3 O4 115.0(11) 2_655 4_645
La1 O3 O4 101.8(9) 2_556 4_645
La1 O3 O4 58.4(8) 3_654 4_645
Ga4 O3 O4 60.9(8) 2_656 4_645
Ga4 O3 O4 107.9(9) 3_554 4_645
O2 O3 O4 80.8(11) 1_545 4_645
Ga3 O3 O4 57.9(9) 1_655 4_645
O7 O3 O4 132.6(11) . 4_645
O4 O3 O4 71.7(11) 4_545 4_645
Ga2 O3 O4 40.0(8) 1_655 4_645
O6 O3 O4 129.9(10) 2_655 4_645
O1 O3 O4 39.7(8) 4_645 4_645
O7 O3 O4 83.4(11) 1_655 4_645
Ga2 O3 O4 60.3(7) 4_645 4_645
O6 O3 O4 83.5(10) 2_755 4_645
La1 O3 O4 109.7(10) 1_654 4_645
Ga1 O3 O4 122.7(9) . 4_645
Ta O3 O4 122.7(9) . 4_645
O7 O3 O4 87.0(10) 2_645 4_645
O4 O3 O4 152.5(13) 2 4_645
Ga2 O3 O2 115.9(17) . 1_645
Ga3 O3 O2 104.3(14) . 1_645
La2 O3 O2 104.1(11) 1_655 1_645
La1 O3 O2 22.7(7) 2_656 1_645
O6 O3 O2 35.1(12) . 1_645
O1 O3 O2 63.8(16) 1_655 1_645
O2 O3 O2 78.8(14) 4_645 1_645
O4 O3 O2 115.3(16) 1_655 1_645
O5 O3 O2 90.6(12) . 1_645
O5 O3 O2 81.6(12) 2_655 1_645
O1 O3 O2 126.8(18) . 1_645
O3 O3 O2 137.5(11) 2_655 1_645
O5 O3 O2 26.2(10) 1_655 1_645
Ta O3 O2 46.3(9) 1_655 1_645
Ga1 O3 O2 46.3(9) 1_655 1_645
O1 O3 O2 118.5(12) 2_655 1_645
Ga2 O3 O2 140.0(12) 2_655 1_645
O3 O3 O2 74.8(9) 2_755 1_645
Ga4 O3 O2 59.1(9) 3_544 1_645
La2 O3 O2 158.4(9) . 1_645
O7 O3 O2 134.9(11) 2_655 1_645
La1 O3 O2 99.5(9) 2_556 1_645
La1 O3 O2 87.0(11) 3_654 1_645
Ga4 O3 O2 77.1(10) 2_656 1_645
Ga4 O3 O2 136.6(12) 3_554 1_645
O2 O3 O2 68.3(10) 1_545 1_645
Ga3 O3 O2 50.3(8) 1_655 1_645
O7 O3 O2 161.0(14) . 1_645
O4 O3 O2 75.8(13) 4_545 1_645
Ga2 O3 O2 57.9(8) 1_655 1_645
O6 O3 O2 101.9(10) 2_655 1_645
O1 O3 O2 34.7(9) 4_645 1_645
O7 O3 O2 102.3(10) 1_655 1_645
Ga2 O3 O2 55.6(8) 4_645 1_645
O6 O3 O2 61.2(10) 2_755 1_645
La1 O3 O2 90.9(10) 1_654 1_645
Ga1 O3 O2 100.4(9) . 1_645
Ta O3 O2 100.4(9) . 1_645
O7 O3 O2 58.4(10) 2_645 1_645
O4 O3 O2 155.2(12) 2 1_645
O4 O3 O2 28.6(9) 4_645 1_645
Ga2 O3 Ga4 136.9(14) . 4_645
Ga3 O3 Ga4 24.7(7) . 4_645
La2 O3 Ga4 113.8(10) 1_655 4_645
La1 O3 Ga4 102.0(7) 2_656 4_645
O6 O3 Ga4 52.3(8) . 4_645
O1 O3 Ga4 136.9(13) 1_655 4_645
O2 O3 Ga4 142.4(15) 4_645 4_645
O4 O3 Ga4 161.4(14) 1_655 4_645
O5 O3 Ga4 47.1(8) . 4_645
O5 O3 Ga4 18.5(7) 2_655 4_645
O1 O3 Ga4 108.9(13) . 4_645
O3 O3 Ga4 55.7(5) 2_655 4_645
O5 O3 Ga4 74.4(7) 1_655 4_645
Ta O3 Ga4 41.1(4) 1_655 4_645
Ga1 O3 Ga4 41.1(4) 1_655 4_645
O1 O3 Ga4 74.8(11) 2_655 4_645
Ga2 O3 Ga4 69.8(6) 2_655 4_645
O3 O3 Ga4 80.2(8) 2_755 4_645
Ga4 O3 Ga4 43.4(4) 3_544 4_645
La2 O3 Ga4 89.2(7) . 4_645
O7 O3 Ga4 121.2(11) 2_655 4_645
La1 O3 Ga4 83.1(6) 2_556 4_645
La1 O3 Ga4 168.9(9) 3_654 4_645
Ga4 O3 Ga4 123.6(7) 2_656 4_645
Ga4 O3 Ga4 141.5(9) 3_554 4_645
O2 O3 Ga4 65.7(11) 1_545 4_645
Ga3 O3 Ga4 82.2(5) 1_655 4_645
O7 O3 Ga4 116.6(10) . 4_645
O4 O3 Ga4 98.7(10) 4_545 4_645
Ga2 O3 Ga4 123.6(7) 1_655 4_645
O6 O3 Ga4 22.4(4) 2_655 4_645
O1 O3 Ga4 88.4(9) 4_645 4_645
O7 O3 Ga4 132.2(9) 1_655 4_645
Ga2 O3 Ga4 84.4(5) 4_645 4_645
O6 O3 Ga4 46.0(5) 2_755 4_645
La1 O3 Ga4 49.4(3) 1_654 4_645
Ga1 O3 Ga4 39.3(3) . 4_645
Ta O3 Ga4 39.3(3) . 4_645
O7 O3 Ga4 23.5(5) 2_645 4_645
O4 O3 Ga4 87.1(8) 2 4_645
O4 O3 Ga4 110.5(9) 4_645 4_645
O2 O3 Ga4 81.9(9) 1_645 4_645
Ga2 O3 O6 22.9(8) . 4_655
Ga3 O3 O6 110.7(12) . 4_655
La2 O3 O6 119.7(9) 1_655 4_655
La1 O3 O6 77.6(8) 2_656 4_655
O6 O3 O6 99.1(10) . 4_655
O1 O3 O6 87.0(14) 1_655 4_655
O2 O3 O6 30.0(14) 4_645 4_655
O4 O3 O6 49.5(12) 1_655 4_655
O5 O3 O6 77.7(10) . 4_655
O5 O3 O6 143.2(11) 2_655 4_655
O1 O3 O6 32.9(13) . 4_655
O3 O3 O6 105.0(13) 2_655 4_655
O5 O3 O6 122.8(12) 1_655 4_655
Ta O3 O6 134.2(9) 1_655 4_655
Ga1 O3 O6 134.2(9) 1_655 4_655
O1 O3 O6 142.1(12) 2_655 4_655
Ga2 O3 O6 121.6(8) 2_655 4_655
O3 O3 O6 153.3(14) 2_755 4_655
Ga4 O3 O6 89.2(7) 3_544 4_655
La2 O3 O6 71.5(6) . 4_655
O7 O3 O6 97.9(9) 2_655 4_655
La1 O3 O6 42.1(5) 2_556 4_655
La1 O3 O6 57.6(5) 3_654 4_655
Ga4 O3 O6 20.8(4) 2_656 4_655
Ga4 O3 O6 62.2(5) 3_554 4_655
O2 O3 O6 63.2(10) 1_545 4_655
Ga3 O3 O6 137.7(10) 1_655 4_655
O7 O3 O6 69.0(8) . 4_655
O4 O3 O6 31.5(8) 4_545 4_655
Ga2 O3 O6 100.2(8) 1_655 4_655
O6 O3 O6 111.5(8) 2_655 4_655
O1 O3 O6 66.3(8) 4_645 4_655
O7 O3 O6 102.2(8) 1_655 4_655
Ga2 O3 O6 53.7(5) 4_645 4_655
O6 O3 O6 156.0(10) 2_755 4_655
La1 O3 O6 168.9(10) 1_654 4_655
Ga1 O3 O6 87.9(6) . 4_655
Ta O3 O6 87.9(6) . 4_655
O7 O3 O6 123.1(9) 2_645 4_655
O4 O3 O6 106.9(10) 2 4_655
O4 O3 O6 80.9(9) 4_645 4_655
O2 O3 O6 97.6(11) 1_645 4_655
Ga4 O3 O6 124.7(7) 4_645 4_655
Ga2 O3 O7 111.3(13) . 1_545
Ga3 O3 O7 33.4(10) . 1_545
La2 O3 O7 144.3(11) 1_655 1_545
La1 O3 O7 90.1(8) 2_656 1_545
O6 O3 O7 42.7(8) . 1_545
O1 O3 O7 141.3(17) 1_655 1_545
O2 O3 O7 113.0(15) 4_645 1_545
O4 O3 O7 141.8(15) 1_655 1_545
O5 O3 O7 20.2(7) . 1_545
O5 O3 O7 48.7(9) 2_655 1_545
O1 O3 O7 87.0(13) . 1_545
O3 O3 O7 65.1(7) 2_655 1_545
O5 O3 O7 84.1(9) 1_655 1_545
Ta O3 O7 56.0(5) 1_655 1_545
Ga1 O3 O7 56.0(5) 1_655 1_545
O1 O3 O7 103.2(11) 2_655 1_545
Ga2 O3 O7 90.2(8) 2_655 1_545
O3 O3 O7 108.0(7) 2_755 1_545
Ga4 O3 O7 20.3(5) 3_544 1_545
La2 O3 O7 84.6(8) . 1_545
O7 O3 O7 142.1(9) 2_655 1_545
La1 O3 O7 55.0(6) 2_556 1_545
La1 O3 O7 146.6(9) 3_654 1_545
Ga4 O3 O7 93.5(8) 2_656 1_545
Ga4 O3 O7 137.6(10) 3_554 1_545
O2 O3 O7 35.8(11) 1_545 1_545
Ga3 O3 O7 102.1(7) 1_655 1_545
O7 O3 O7 115.7(12) . 1_545
O4 O3 O7 68.3(11) 4_545 1_545
Ga2 O3 O7 134.4(8) 1_655 1_545
O6 O3 O7 31.7(6) 2_655 1_545
O1 O3 O7 67.6(10) 4_645 1_545
O7 O3 O7 162.7(12) 1_655 1_545
Ga2 O3 O7 56.8(6) 4_645 1_545
O6 O3 O7 70.7(7) 2_755 1_545
La1 O3 O7 80.0(6) 1_654 1_545
Ga1 O3 O7 23.1(5) . 1_545
Ta O3 O7 23.1(5) . 1_545
O7 O3 O7 34.5(8) 2_645 1_545
O4 O3 O7 103.4(10) 2 1_545
O4 O3 O7 102.2(9) 4_645 1_545
O2 O3 O7 77.7(9) 1_645 1_545
Ga4 O3 O7 30.6(5) 4_645 1_545
O6 O3 O7 94.8(8) 4_655 1_545
Ga2 O3 O5 36.4(9) . 4_655
Ga3 O3 O5 141.7(13) . 4_655
La2 O3 O5 97.4(9) 1_655 4_655
La1 O3 O5 59.1(7) 2_656 4_655
O6 O3 O5 100.9(11) . 4_655
O1 O3 O5 55.2(12) 1_655 4_655
O2 O3 O5 5.1(15) 4_645 4_655
O4 O3 O5 39.2(13) 1_655 4_655
O5 O3 O5 105.3(10) . 4_655
O5 O3 O5 160.9(14) 2_655 4_655
O1 O3 O5 61.2(13) . 4_655
O3 O3 O5 133.1(13) 2_655 4_655
O5 O3 O5 101.1(10) 1_655 4_655
Ta O3 O5 128.0(10) 1_655 4_655
Ga1 O3 O5 128.0(10) 1_655 4_655
O1 O3 O5 137.6(12) 2_655 4_655
Ga2 O3 O5 136.1(7) 2_655 4_655
O3 O3 O5 121.8(13) 2_755 4_655
Ga4 O3 O5 104.3(8) 3_544 4_655
La2 O3 O5 95.9(7) . 4_655
O7 O3 O5 89.9(9) 2_655 4_655
La1 O3 O5 72.1(6) 2_556 4_655
La1 O3 O5 29.4(5) 3_654 4_655
Ga4 O3 O5 24.5(5) 2_656 4_655
Ga4 O3 O5 60.7(5) 3_554 4_655
O2 O3 O5 82.2(12) 1_545 4_655
Ga3 O3 O5 107.9(8) 1_655 4_655
O7 O3 O5 79.9(8) . 4_655
O4 O3 O5 49.9(10) 4_545 4_655
Ga2 O3 O5 68.4(6) 1_655 4_655
O6 O3 O5 142.1(9) 2_655 4_655
O1 O3 O5 62.7(10) 4_645 4_655
O7 O3 O5 78.9(8) 1_655 4_655
Ga2 O3 O5 63.2(6) 4_645 4_655
O6 O3 O5 140.1(11) 2_755 4_655
La1 O3 O5 158.3(8) 1_654 4_655
Ga1 O3 O5 117.9(7) . 4_655
Ta O3 O5 117.9(7) . 4_655
O7 O3 O5 132.0(10) 2_645 4_655
O4 O3 O5 117.6(8) 2 4_655
O4 O3 O5 56.8(9) 4_645 4_655
O2 O3 O5 81.8(12) 1_645 4_655
Ga4 O3 O5 147.5(8) 4_645 4_655
O6 O3 O5 31.8(5) 4_655 4_655
O7 O3 O5 117.9(8) 1_545 4_655
Ga2 O3 O3 119.7(11) . 1_655
Ga3 O3 O3 124.7(10) . 1_655
La2 O3 O3 53.2(8) 1_655 1_655
La1 O3 O3 56.1(7) 2_656 1_655
O6 O3 O3 80.5(10) . 1_655
O1 O3 O3 35.8(11) 1_655 1_655
O2 O3 O3 90.1(16) 4_645 1_655
O4 O3 O3 94.6(12) 1_655 1_655
O5 O3 O3 137.2(9) . 1_655
O5 O3 O3 88.0(9) 2_655 1_655
O1 O3 O3 148.2(12) . 1_655
O3 O3 O3 133.3(12) 2_655 1_655
O5 O3 O3 34.8(7) 1_655 1_655
Ta O3 O3 63.8(6) 1_655 1_655
Ga1 O3 O3 63.8(6) 1_655 1_655
O1 O3 O3 79.7(7) 2_655 1_655
Ga2 O3 O3 107.4(5) 2_655 1_655
O3 O3 O3 36.2(12) 2_755 1_655
Ga4 O3 O3 105.5(5) 3_544 1_655
La2 O3 O3 150.7(4) . 1_655
O7 O3 O3 84.9(7) 2_655 1_655
La1 O3 O3 147.7(5) 2_556 1_655
La1 O3 O3 69.8(4) 3_654 1_655
Ga4 O3 O3 103.5(5) 2_656 1_655
Ga4 O3 O3 103.9(5) 3_554 1_655
O2 O3 O3 119.2(8) 1_545 1_655
Ga3 O3 O3 20.3(4) 1_655 1_655
O7 O3 O3 123.3(7) . 1_655
O4 O3 O3 117.9(10) 4_545 1_655
Ga2 O3 O3 21.9(4) 1_655 1_655
O6 O3 O3 123.0(5) 2_655 1_655
O1 O3 O3 81.8(5) 4_645 1_655
O7 O3 O3 54.3(7) 1_655 1_655
Ga2 O3 O3 103.8(4) 4_645 1_655
O6 O3 O3 57.0(6) 2_755 1_655
La1 O3 O3 70.9(5) 1_654 1_655
Ga1 O3 O3 139.5(4) . 1_655
Ta O3 O3 139.5(4) . 1_655
O7 O3 O3 85.7(6) 2_645 1_655
O4 O3 O3 110.9(7) 2 1_655
O4 O3 O3 46.2(7) 4_645 1_655
O2 O3 O3 50.9(7) 1_645 1_655
Ga4 O3 O3 102.2(4) 4_645 1_655
O6 O3 O3 120.1(6) 4_655 1_655
O7 O3 O3 118.5(6) 1_545 1_655
O5 O3 O3 88.8(5) 4_655 1_655
Ga2 O3 O3 60.3(11) . 1_455
Ga3 O3 O3 55.3(10) . 1_455
La2 O3 O3 126.8(8) 1_655 1_455
La1 O3 O3 123.9(7) 2_656 1_455
O6 O3 O3 99.5(10) . 1_455
O1 O3 O3 144.2(11) 1_655 1_455
O2 O3 O3 89.9(16) 4_645 1_455
O4 O3 O3 85.4(12) 1_655 1_455
O5 O3 O3 42.8(9) . 1_455
O5 O3 O3 92.0(9) 2_655 1_455
O1 O3 O3 31.8(12) . 1_455
O3 O3 O3 46.7(12) 2_655 1_455
O5 O3 O3 145.2(7) 1_655 1_455
Ta O3 O3 116.2(6) 1_655 1_455
Ga1 O3 O3 116.2(6) 1_655 1_455
O1 O3 O3 100.3(7) 2_655 1_455
Ga2 O3 O3 72.6(5) 2_655 1_455
O3 O3 O3 143.8(12) 2_755 1_455
Ga4 O3 O3 74.5(5) 3_544 1_455
La2 O3 O3 29.3(4) . 1_455
O7 O3 O3 95.1(7) 2_655 1_455
La1 O3 O3 32.3(5) 2_556 1_455
La1 O3 O3 110.2(4) 3_654 1_455
Ga4 O3 O3 76.5(5) 2_656 1_455
Ga4 O3 O3 76.1(5) 3_554 1_455
O2 O3 O3 60.8(8) 1_545 1_455
Ga3 O3 O3 159.7(4) 1_655 1_455
O7 O3 O3 56.7(7) . 1_455
O4 O3 O3 62.1(10) 4_545 1_455
Ga2 O3 O3 158.1(4) 1_655 1_455
O6 O3 O3 57.0(5) 2_655 1_455
O1 O3 O3 98.2(5) 4_645 1_455
O7 O3 O3 125.7(7) 1_655 1_455
Ga2 O3 O3 76.2(4) 4_645 1_455
O6 O3 O3 123.0(6) 2_755 1_455
La1 O3 O3 109.1(5) 1_654 1_455
Ga1 O3 O3 40.5(4) . 1_455
Ta O3 O3 40.5(4) . 1_455
O7 O3 O3 94.3(6) 2_645 1_455
O4 O3 O3 69.1(7) 2 1_455
O4 O3 O3 133.8(7) 4_645 1_455
O2 O3 O3 129.1(7) 1_645 1_455
Ga4 O3 O3 77.8(4) 4_645 1_455
O6 O3 O3 59.9(6) 4_655 1_455
O7 O3 O3 61.5(6) 1_545 1_455
O5 O3 O3 91.2(5) 4_655 1_455
O3 O3 O3 180.0(12) 1_655 1_455
Ga2 O3 O6 64.8(11) . 4_755
Ga3 O3 O6 157.6(14) . 4_755
La2 O3 O6 84.0(9) 1_655 4_755
La1 O3 O6 39.3(6) 2_656 4_755
O6 O3 O6 89.6(10) . 4_755
O1 O3 O6 30.0(13) 1_655 4_755
O2 O3 O6 30.2(15) 4_645 4_755
O4 O3 O6 55.3(12) 1_655 4_755
O5 O3 O6 121.5(12) . 4_755
O5 O3 O6 140.0(12) 2_655 4_755
O1 O3 O6 90.7(14) . 4_755
O3 O3 O6 161.1(10) 2_655 4_755
O5 O3 O6 73.7(9) 1_655 4_755
Ta O3 O6 104.8(9) 1_655 4_755
Ga1 O3 O6 104.8(9) 1_655 4_755
O1 O3 O6 127.6(11) 2_655 4_755
Ga2 O3 O6 145.5(8) 2_655 4_755
O3 O3 O6 94.9(13) 2_755 4_755
Ga4 O3 O6 104.7(8) 3_544 4_755
La2 O3 O6 123.8(7) . 4_755
O7 O3 O6 92.8(9) 2_655 4_755
La1 O3 O6 96.0(7) 2_556 4_755
La1 O3 O6 28.0(4) 3_654 4_755
Ga4 O3 O6 45.4(5) 2_656 4_755
Ga4 O3 O6 76.9(6) 3_554 4_755
O2 O3 O6 92.1(12) 1_545 4_755
Ga3 O3 O6 78.5(7) 1_655 4_755
O7 O3 O6 101.1(9) . 4_755
O4 O3 O6 67.4(10) 4_545 4_755
Ga2 O3 O6 41.1(4) 1_655 4_755
O6 O3 O6 156.0(10) 2_655 4_755
O1 O3 O6 56.9(8) 4_645 4_755
O7 O3 O6 68.1(8) 1_655 4_755
Ga2 O3 O6 69.3(6) 4_645 4_755
O6 O3 O6 111.6(9) 2_755 4_755
La1 O3 O6 130.8(8) 1_654 4_755
Ga1 O3 O6 136.5(8) . 4_755
Ta O3 O6 136.5(8) . 4_755
O7 O3 O6 118.1(10) 2_645 4_755
O4 O3 O6 130.4(9) 2 4_755
O4 O3 O6 31.6(7) 4_645 4_755
O2 O3 O6 60.0(10) 1_645 4_755
Ga4 O3 O6 141.3(8) 4_645 4_755
O6 O3 O6 60.1(5) 4_655 4_755
O7 O3 O6 124.3(9) 1_545 4_755
O5 O3 O6 29.5(5) 4_655 4_755
O3 O3 O6 60.0(5) 1_655 4_755
O3 O3 O6 120.0(5) 1_455 4_755
Ga2 O3 O7 56.3(11) . 4_645
Ga3 O3 O7 126.7(13) . 4_645
La2 O3 O7 116.4(11) 1_655 4_645
La1 O3 O7 38.4(6) 2_656 4_645
O6 O3 O7 73.7(9) . 4_645
O1 O3 O7 62.6(15) 1_655 4_645
O2 O3 O7 22.6(13) 4_645 4_645
O4 O3 O7 66.4(13) 1_655 4_645
O5 O3 O7 88.9(10) . 4_645
O5 O3 O7 133.6(12) 2_655 4_645
O1 O3 O7 71.8(14) . 4_645
O3 O3 O7 140.2(15) 2_655 4_645
O5 O3 O7 83.7(10) 1_655 4_645
Ta O3 O7 103.4(9) 1_655 4_645
Ga1 O3 O7 103.4(9) 1_655 4_645
O1 O3 O7 160.4(11) 2_655 4_645
Ga2 O3 O7 160.3(8) 2_655 4_645
O3 O3 O7 122.3(15) 2_755 4_645
Ga4 O3 O7 78.9(7) 3_544 4_645
La2 O3 O7 110.6(7) . 4_645
O7 O3 O7 116.6(11) 2_655 4_645
La1 O3 O7 64.8(6) 2_556 4_645
La1 O3 O7 51.4(5) 3_654 4_645
Ga4 O3 O7 18.7(4) 2_656 4_645
Ga4 O3 O7 87.6(7) 3_554 4_645
O2 O3 O7 60.6(11) 1_545 4_645
Ga3 O3 O7 100.1(8) 1_655 4_645
O7 O3 O7 104.0(9) . 4_645
O4 O3 O7 34.8(10) 4_545 4_645
Ga2 O3 O7 71.8(6) 1_655 4_645
O6 O3 O7 125.7(8) 2_655 4_645
O1 O3 O7 35.5(8) 4_645 4_645
O7 O3 O7 99.4(8) 1_655 4_645
Ga2 O3 O7 38.7(5) 4_645 4_645
O6 O3 O7 120.9(10) 2_755 4_645
La1 O3 O7 150.4(9) 1_654 4_645
Ga1 O3 O7 103.8(6) . 4_645
Ta O3 O7 103.8(6) . 4_645
O7 O3 O7 104.8(10) 2_645 4_645
O4 O3 O7 143.1(10) 2 4_645
O4 O3 O7 42.3(8) 4_645 4_645
O2 O3 O7 59.7(10) 1_645 4_645
Ga4 O3 O7 122.0(7) 4_645 4_645
O6 O3 O7 39.3(5) 4_655 4_645
O7 O3 O7 95.5(8) 1_545 4_645
O5 O3 O7 27.3(5) 4_655 4_645
O3 O3 O7 86.3(5) 1_655 4_645
O3 O3 O7 93.7(5) 1_455 4_645
O6 O3 O7 32.9(4) 4_755 4_645
Ga2 O3 Ga4 75.5(9) . 4_655
Ga3 O3 Ga4 91.5(13) . 4_655
La2 O3 Ga4 48.1(6) 1_655 4_655
La1 O3 Ga4 146.3(10) 2_656 4_655
O6 O3 Ga4 159.1(12) . 4_655
O1 O3 Ga4 94.1(14) 1_655 4_655
O2 O3 Ga4 104.5(15) 4_645 4_655
O4 O3 Ga4 60.8(12) 1_655 4_655
O5 O3 Ga4 115.2(12) . 4_655
O5 O3 Ga4 99.2(11) 2_655 4_655
O1 O3 Ga4 75.9(13) . 4_655
O3 O3 Ga4 58.5(5) 2_655 4_655
O5 O3 Ga4 129.7(10) 1_655 4_655
Ta O3 Ga4 127.1(8) 1_655 4_655
Ga1 O3 Ga4 127.1(8) 1_655 4_655
O1 O3 Ga4 44.4(9) 2_655 4_655
Ga2 O3 Ga4 37.8(3) 2_655 4_655
O3 O3 Ga4 81.0(7) 2_755 4_655
Ga4 O3 Ga4 143.9(9) 3_544 4_655
La2 O3 Ga4 49.4(4) . 4_655
O7 O3 Ga4 19.1(7) 2_655 4_655
La1 O3 Ga4 107.5(7) 2_556 4_655
La1 O3 Ga4 82.0(5) 3_654 4_655
Ga4 O3 Ga4 115.2(6) 2_656 4_655
Ga4 O3 Ga4 39.6(3) 3_554 4_655
O2 O3 Ga4 139.6(9) 1_545 4_655
Ga3 O3 Ga4 104.0(7) 1_655 4_655
O7 O3 Ga4 30.3(6) . 4_655
O4 O3 Ga4 126.4(10) 4_545 4_655
Ga2 O3 Ga4 96.6(6) 1_655 4_655
O6 O3 Ga4 93.6(8) 2_655 4_655
O1 O3 Ga4 162.5(10) 4_645 4_655
O7 O3 Ga4 51.7(6) 1_655 4_655
Ga2 O3 Ga4 149.2(7) 4_645 4_655
O6 O3 Ga4 106.0(7) 2_755 4_655
La1 O3 Ga4 77.3(5) 1_654 4_655
Ga1 O3 Ga4 103.1(7) . 4_655
Ta O3 Ga4 103.1(7) . 4_655
O7 O3 Ga4 127.9(10) 2_645 4_655
O4 O3 Ga4 20.9(6) 2 4_655
O4 O3 Ga4 134.0(10) 4_645 4_655
O2 O3 Ga4 152.1(8) 1_645 4_655
Ga4 O3 Ga4 107.5(7) 4_645 4_655
O6 O3 Ga4 97.9(6) 4_655 4_655
O7 O3 Ga4 123.6(9) 1_545 4_655
O5 O3 Ga4 99.9(6) 4_655 4_655
O3 O3 Ga4 101.3(4) 1_655 4_655
O3 O3 Ga4 78.7(4) 1_455 4_655
O6 O3 Ga4 109.5(6) 4_755 4_655
O7 O3 Ga4 127.1(7) 4_645 4_655
Ga2 O3 O7 147.1(15) . 1_645
Ga3 O3 O7 75.0(10) . 1_645
La2 O3 O7 102.1(10) 1_655 1_645
La1 O3 O7 57.0(7) 2_656 1_645
O6 O3 O7 28.4(8) . 1_645
O1 O3 O7 88.3(14) 1_655 1_645
O2 O3 O7 112.6(16) 4_645 1_645
O4 O3 O7 147.9(15) 1_655 1_645
O5 O3 O7 78.4(8) . 1_645
O5 O3 O7 47.3(9) 2_655 1_645
O1 O3 O7 141.4(15) . 1_645
O3 O3 O7 105.0(8) 2_655 1_645
O5 O3 O7 25.5(8) 1_655 1_645
Ta O3 O7 12.0(6) 1_655 1_645
Ga1 O3 O7 12.0(6) 1_655 1_645
O1 O3 O7 92.8(10) 2_655 1_645
Ga2 O3 O7 107.3(8) 2_655 1_645
O3 O3 O7 60.9(6) 2_755 1_645
Ga4 O3 O7 49.0(6) 3_544 1_645
La2 O3 O7 139.5(9) . 1_645
O7 O3 O7 133.2(7) 2_655 1_645
La1 O3 O7 105.4(7) 2_556 1_645
La1 O3 O7 118.6(9) 3_654 1_645
Ga4 O3 O7 106.8(8) 2_656 1_645
Ga4 O3 O7 163.1(10) 3_554 1_645
O2 O3 O7 71.5(10) 1_545 1_645
Ga3 O3 O7 44.6(5) 1_655 1_645
O7 O3 O7 164.0(13) . 1_645
O4 O3 O7 95.5(12) 4_545 1_645
Ga2 O3 O7 77.1(7) 1_655 1_645
O6 O3 O7 72.6(8) 2_655 1_645
O1 O3 O7 59.1(10) 4_645 1_645
O7 O3 O7 111.3(10) 1_655 1_645
Ga2 O3 O7 72.4(6) 4_645 1_645
O6 O3 O7 31.1(6) 2_755 1_645
La1 O3 O7 60.6(6) 1_654 1_645
Ga1 O3 O7 81.0(6) . 1_645
Ta O3 O7 81.0(6) . 1_645
O7 O3 O7 28.3(9) 2_645 1_645
O4 O3 O7 125.1(9) 2 1_645
O4 O3 O7 61.9(9) 4_645 1_645
O2 O3 O7 34.4(10) 1_645 1_645
Ga4 O3 O7 50.5(6) 4_645 1_645
O6 O3 O7 124.9(9) 4_655 1_645
O7 O3 O7 59.2(5) 1_545 1_645
O5 O3 O7 116.0(10) 4_655 1_645
O3 O3 O7 59.3(6) 1_655 1_645
O3 O3 O7 120.7(6) 1_455 1_645
O6 O3 O7 93.5(7) 4_755 1_645
O7 O3 O7 91.8(9) 4_645 1_645
Ga4 O3 O7 137.1(8) 4_655 1_645
Ga2 O3 O4 113.1(13) . 2_655
Ga3 O3 O4 102.2(13) . 2_655
La2 O3 O4 15.7(8) 1_655 2_655
La1 O3 O4 111.1(10) 2_656 2_655
O6 O3 O4 121.6(11) . 2_655
O1 O3 O4 68.2(15) 1_655 2_655
O2 O3 O4 117.6(18) 4_645 2_655
O4 O3 O4 84.8(17) 1_655 2_655
O5 O3 O4 140.4(13) . 2_655
O5 O3 O4 80.3(11) 2_655 2_655
O1 O3 O4 124.3(15) . 2_655
O3 O3 O4 85.2(12) 2_655 2_655
O5 O3 O4 80.2(9) 1_655 2_655
Ta O3 O4 87.8(7) 1_655 2_655
Ga1 O3 O4 87.8(7) 1_655 2_655
O1 O3 O4 30.3(9) 2_655 2_655
Ga2 O3 O4 55.2(7) 2_655 2_655
O3 O3 O4 32.6(7) 2_755 2_655
Ga4 O3 O4 136.4(8) 3_544 2_655
La2 O3 O4 96.6(9) . 2_655
O7 O3 O4 40.0(9) 2_655 2_655
La1 O3 O4 156.3(10) 2_556 2_655
La1 O3 O4 83.6(7) 3_654 2_655
Ga4 O3 O4 137.5(9) 2_656 2_655
Ga4 O3 O4 74.6(8) 3_554 2_655
O2 O3 O4 162.5(13) 1_545 2_655
Ga3 O3 O4 54.5(6) 1_655 2_655
O7 O3 O4 78.6(10) . 2_655
O4 O3 O4 162.9(14) 4_545 2_655
Ga2 O3 O4 61.4(6) 1_655 2_655
O6 O3 O4 102.7(8) 2_655 2_655
O1 O3 O4 137.1(9) 4_645 2_655
O7 O3 O4 34.2(9) 1_655 2_655
Ga2 O3 O4 159.1(10) 4_645 2_655
O6 O3 O4 66.5(7) 2_755 2_655
La1 O3 O4 48.9(6) 1_654 2_655
Ga1 O3 O4 125.8(9) . 2_655
Ta O3 O4 125.8(9) . 2_655
O7 O3 O4 102.5(9) 2_645 2_655
O4 O3 O4 55.5(7) 2 2_655
O4 O3 O4 99.8(10) 4_645 2_655
O2 O3 O4 104.1(9) 1_645 2_655
Ga4 O3 O4 98.2(7) 4_645 2_655
O6 O3 O4 134.3(8) 4_655 2_655
O7 O3 O4 128.7(8) 1_545 2_655
O5 O3 O4 113.0(7) 4_655 2_655
O3 O3 O4 55.4(7) 1_655 2_655
O3 O3 O4 124.6(7) 1_455 2_655
O6 O3 O4 97.4(8) 4_755 2_655
O7 O3 O4 130.4(8) 4_645 2_655
Ga4 O3 O4 49.4(7) 4_655 2_655
O7 O3 O4 93.2(8) 1_645 2_655
Ga2 O3 La1 12.1(8) . 3_554
Ga3 O3 La1 103.7(12) . 3_554
La2 O3 La1 105.4(8) 1_655 3_554
La1 O3 La1 102.4(8) 2_656 3_554
O6 O3 La1 121.6(11) . 3_554
O1 O3 La1 95.8(12) 1_655 3_554
O2 O3 La1 48.5(14) 4_645 3_554
O4 O3 La1 39.6(11) 1_655 3_554
O5 O3 La1 82.5(10) . 3_554
O5 O3 La1 140.2(12) 2_655 3_554
O1 O3 La1 16.9(10) . 3_554
O3 O3 La1 85.6(11) 2_655 3_554
O5 O3 La1 147.5(11) 1_655 3_554
Ta O3 La1 155.6(8) 1_655 3_554
Ga1 O3 La1 155.6(8) 1_655 3_554
O1 O3 La1 116.3(10) 2_655 3_554
Ga2 O3 La1 96.3(6) 2_655 3_554
O3 O3 La1 147.4(3) 2_755 3_554
Ga4 O3 La1 105.1(6) 3_544 3_554
La2 O3 La1 48.7(3) . 3_554
O7 O3 La1 76.7(7) 2_655 3_554
La1 O3 La1 48.7(3) 2_556 3_554
La1 O3 La1 61.8(3) 3_654 3_554
Ga4 O3 La1 46.4(3) 2_656 3_554
Ga4 O3 La1 42.0(3) 3_554 3_554
O2 O3 La1 80.0(10) 1_545 3_554
Ga3 O3 La1 151.8(8) 1_655 3_554
O7 O3 La1 43.2(6) . 3_554
O4 O3 La1 54.0(8) 4_545 3_554
Ga2 O3 La1 109.7(6) 1_655 3_554
O6 O3 La1 105.4(7) 2_655 3_554
O1 O3 La1 92.1(8) 4_645 3_554
O7 O3 La1 91.9(6) 1_655 3_554
Ga2 O3 La1 77.1(5) 4_645 3_554
O6 O3 La1 171.4(9) 2_755 3_554
La1 O3 La1 145.5(8) 1_654 3_554
Ga1 O3 La1 86.8(5) . 3_554
Ta O3 La1 86.8(5) . 3_554
O7 O3 La1 136.7(7) 2_645 3_554
O4 O3 La1 80.9(9) 2 3_554
O4 O3 La1 103.4(8) 4_645 3_554
O2 O3 La1 123.5(11) 1_645 3_554
Ga4 O3 La1 125.8(7) 4_645 3_554
O6 O3 La1 26.1(4) 4_655 3_554
O7 O3 La1 102.6(7) 1_545 3_554
O5 O3 La1 47.5(5) 4_655 3_554
O3 O3 La1 131.6(4) 1_655 3_554
O3 O3 La1 48.4(4) 1_455 3_554
O6 O3 La1 76.5(5) 4_755 3_554
O7 O3 La1 64.1(5) 4_645 3_554
Ga4 O3 La1 72.9(4) 4_655 3_554
O7 O3 La1 149.5(8) 1_645 3_554
O4 O3 La1 116.4(8) 2_655 3_554
Ga2 O3 O2 23.7(12) . .
Ga3 O3 O2 119.2(12) . .
La2 O3 O2 77.9(8) 1_655 .
La1 O3 O2 107.7(12) 2_656 .
O6 O3 O2 145.4(13) . .
O1 O3 O2 78.8(13) 1_655 .
O2 O3 O2 53.0(17) 4_645 .
O4 O3 O2 17.7(11) 1_655 .
O5 O3 O2 108.4(10) . .
O5 O3 O2 148.1(13) 2_655 .
O1 O3 O2 41.6(12) . .
O3 O3 O2 90.4(8) 2_655 .
O5 O3 O2 141.7(11) 1_655 .
Ta O3 O2 175.0(10) 1_655 .
Ga1 O3 O2 175.0(10) 1_655 .
O1 O3 O2 97.5(12) 2_655 .
Ga2 O3 O2 87.0(7) 2_655 .
O3 O3 O2 119.9(6) 2_755 .
Ga4 O3 O2 132.6(9) 3_544 .
La2 O3 O2 54.8(5) . .
O7 O3 O2 51.5(8) 2_655 .
La1 O3 O2 76.1(7) 2_556 .
La1 O3 O2 46.7(8) 3_654 .
Ga4 O3 O2 61.8(9) 2_656 .
Ga4 O3 O2 15.7(7) 3_554 .
O2 O3 O2 107.1(12) 1_545 .
Ga3 O3 O2 129.2(7) 1_655 .
O7 O3 O2 30.9(9) . .
O4 O3 O2 77.9(12) 4_545 .
Ga2 O3 O2 91.2(8) 1_655 .
O6 O3 O2 121.4(8) 2_655 .
O1 O3 O2 109.2(12) 4_645 .
O7 O3 O2 64.6(8) 1_655 .
Ga2 O3 O2 100.2(9) 4_645 .
O6 O3 O2 156.4(9) 2_755 .
La1 O3 O2 130.6(8) 1_654 .
Ga1 O3 O2 109.3(6) . .
Ta O3 O2 109.3(6) . .
O7 O3 O2 162.9(9) 2_645 .
O4 O3 O2 68.7(9) 2 .
O4 O3 O2 102.6(12) 4_645 .
O2 O3 O2 130.2(17) 1_645 .
Ga4 O3 O2 143.8(8) 4_645 .
O6 O3 O2 46.6(9) 4_655 .
O7 O3 O2 128.5(8) 1_545 .
O5 O3 O2 49.3(10) 4_655 .
O3 O3 O2 111.2(6) 1_655 .
O3 O3 O2 68.8(6) 1_455 .
O6 O3 O2 71.0(9) 4_755 .
O7 O3 O2 74.8(10) 4_645 .
Ga4 O3 O2 53.5(7) 4_655 .
O7 O3 O2 164.5(11) 1_645 .
O4 O3 O2 89.9(9) 2_655 .
La1 O3 O2 27.5(7) 3_554 .
Ga2 O3 Ga2 130.0(12) . 2_755
Ga3 O3 Ga2 99.0(11) . 2_755
La2 O3 Ga2 30.1(5) 1_655 2_755
La1 O3 Ga2 97.8(9) 2_656 2_755
O6 O3 Ga2 102.3(10) . 2_755
O1 O3 Ga2 66.1(13) 1_655 2_755
O2 O3 Ga2 122.8(18) 4_645 2_755
O4 O3 Ga2 99.9(13) 1_655 2_755
O5 O3 Ga2 134.4(11) . 2_755
O5 O3 Ga2 69.1(9) 2_655 2_755
O1 O3 Ga2 143.7(14) . 2_755
O3 O3 Ga2 92.5(13) 2_655 2_755
O5 O3 Ga2 61.5(7) 1_655 2_755
Ta O3 Ga2 69.3(5) 1_655 2_755
Ga1 O3 Ga2 69.3(5) 1_655 2_755
O1 O3 Ga2 37.5(5) 2_655 2_755
Ga2 O3 Ga2 65.2(5) 2_655 2_755
O3 O3 Ga2 13.1(4) 2_755 2_755
Ga4 O3 Ga2 119.5(6) 3_544 2_755
La2 O3 Ga2 112.8(7) . 2_755
O7 O3 Ga2 59.3(7) 2_655 2_755
La1 O3 Ga2 168.0(9) 2_556 2_755
La1 O3 Ga2 90.9(6) 3_654 2_755
Ga4 O3 Ga2 141.3(8) 2_656 2_755
Ga4 O3 Ga2 93.1(5) 3_554 2_755
O2 O3 Ga2 144.9(10) 1_545 2_755
Ga3 O3 Ga2 36.2(3) 1_655 2_755
O7 O3 Ga2 97.9(8) . 2_755
O4 O3 Ga2 160.2(13) 4_545 2_755
Ga2 O3 Ga2 55.4(4) 1_655 2_755
O6 O3 Ga2 98.7(7) 2_655 2_755
O1 O3 Ga2 121.0(8) 4_645 2_755
O7 O3 Ga2 46.0(6) 1_655 2_755
Ga2 O3 Ga2 142.0(8) 4_645 2_755
O6 O3 Ga2 49.0(5) 2_755 2_755
La1 O3 Ga2 39.5(3) 1_654 2_755
Ga1 O3 Ga2 122.9(7) . 2_755
Ta O3 Ga2 122.9(7) . 2_755
O7 O3 Ga2 86.3(7) 2_645 2_755
O4 O3 Ga2 70.8(6) 2 2_755
O4 O3 Ga2 88.5(9) 4_645 2_755
O2 O3 Ga2 86.5(8) 1_645 2_755
Ga4 O3 Ga2 87.5(5) 4_645 2_755
O6 O3 Ga2 147.8(7) 4_655 2_755
O7 O3 Ga2 117.2(7) 1_545 2_755
O5 O3 Ga2 119.2(7) 4_655 2_755
O3 O3 Ga2 42.2(4) 1_655 2_755
O3 O3 Ga2 137.8(4) 1_455 2_755
O6 O3 Ga2 96.0(6) 4_755 2_755
O7 O3 Ga2 127.0(8) 4_645 2_755
Ga4 O3 Ga2 68.2(5) 4_655 2_755
O7 O3 Ga2 73.9(6) 1_645 2_755
O4 O3 Ga2 19.4(5) 2_655 2_755
La1 O3 Ga2 135.1(6) 3_554 2_755
O2 O3 Ga2 107.9(6) . 2_755
Ga2 O3 O2 149.6(19) . 2_645
Ga3 O3 O2 35.1(8) . 2_645
La2 O3 O2 92.8(9) 1_655 2_645
La1 O3 O2 109.5(11) 2_656 2_645
O6 O3 O2 65.5(12) . 2_645
O1 O3 O2 125.7(16) 1_655 2_645
O2 O3 O2 161(2) 4_645 2_645
O4 O3 O2 154.4(17) 1_655 2_645
O5 O3 O2 66.9(11) . 2_645
O5 O3 O2 5.7(11) 2_655 2_645
O1 O3 O2 121.6(17) . 2_645
O3 O3 O2 54.2(9) 2_655 2_645
O5 O3 O2 70.9(11) 1_655 2_645
Ta O3 O2 40.7(8) 1_655 2_645
Ga1 O3 O2 40.7(8) 1_655 2_645
O1 O3 O2 55.2(12) 2_655 2_645
Ga2 O3 O2 56.9(7) 2_655 2_645
O3 O3 O2 61.8(8) 2_755 2_645
Ga4 O3 O2 63.0(9) 3_544 2_645
La2 O3 O2 91.7(10) . 2_645
O7 O3 O2 103.5(11) 2_655 2_645
La1 O3 O2 102.3(11) 2_556 2_645
La1 O3 O2 157.9(12) 3_654 2_645
Ga4 O3 O2 144.3(10) 2_656 2_645
Ga4 O3 O2 132.6(10) 3_554 2_645
O2 O3 O2 86.5(17) 1_545 2_645
Ga3 O3 O2 69.9(8) 1_655 2_645
O7 O3 O2 111.8(11) . 2_645
O4 O3 O2 119.7(14) 4_545 2_645
Ga2 O3 O2 111.8(11) 1_655 2_645
O6 O3 O2 33.9(8) 2_655 2_645
O1 O3 O2 103.7(11) 4_645 2_645
O7 O3 O2 111.2(11) 1_655 2_645
Ga2 O3 O2 104.0(9) 4_645 2_645
O6 O3 O2 34.0(8) 2_755 2_645
La1 O3 O2 28.6(6) 1_654 2_645
Ga1 O3 O2 56.6(8) . 2_645
Ta O3 O2 56.6(8) . 2_645
O7 O3 O2 34.4(10) 2_645 2_645
O4 O3 O2 75.3(8) 2 2_645
O4 O3 O2 113.9(13) 4_645 2_645
O2 O3 O2 87.0(16) 1_645 2_645
Ga4 O3 O2 21.0(7) 4_645 2_645
O6 O3 O2 144.4(11) 4_655 2_645
O7 O3 O2 51.5(9) 1_545 2_645
O5 O3 O2 166.4(9) 4_655 2_645
O3 O3 O2 90.1(9) 1_655 2_645
O3 O3 O2 89.9(9) 1_455 2_645
O6 O3 O2 144.6(11) 4_755 2_645
O7 O3 O2 139.1(10) 4_645 2_645
Ga4 O3 O2 93.6(8) 4_655 2_645
O7 O3 O2 52.6(9) 1_645 2_645
O4 O3 O2 77.2(8) 2_655 2_645
La1 O3 O2 137.5(12) 3_554 2_645
O2 O3 O2 142.7(9) . 2_645
Ga2 O3 O2 67.4(7) 2_755 2_645
Ga2 O3 Ta 72.5(9) . 1_665
Ga3 O3 Ta 124.1(14) . 1_665
La2 O3 Ta 28.2(4) 1_655 1_665
La1 O3 Ta 112.3(9) 2_656 1_665
O6 O3 Ta 154.7(13) . 1_665
O1 O3 Ta 60.0(14) 1_655 1_665
O2 O3 Ta 84.1(15) 4_645 1_665
O4 O3 Ta 44.6(12) 1_655 1_665
O5 O3 Ta 147.5(12) . 1_665
O5 O3 Ta 118.1(11) 2_655 1_665
O1 O3 Ta 88.9(12) . 1_665
O3 O3 Ta 92.4(6) 2_655 1_665
O5 O3 Ta 108.5(9) 1_655 1_665
Ta O3 Ta 127.2(8) 1_655 1_665
Ga1 O3 Ta 127.2(8) 1_655 1_665
O1 O3 Ta 58.6(11) 2_655 1_665
Ga2 O3 Ta 67.5(5) 2_655 1_665
O3 O3 Ta 70.3(3) 2_755 1_665
Ga4 O3 Ta 176.7(8) 3_544 1_665
La2 O3 Ta 78.4(5) . 1_665
O7 O3 Ta 15.3(6) 2_655 1_665
La1 O3 Ta 124.9(6) 2_556 1_665
La1 O3 Ta 53.2(3) 3_654 1_665
Ga4 O3 Ta 101.8(5) 2_656 1_665
Ga4 O3 Ta 35.4(2) 3_554 1_665
O2 O3 Ta 156.7(12) 1_545 1_665
Ga3 O3 Ta 85.2(5) 1_655 1_665
O7 O3 Ta 49.2(6) . 1_665
O4 O3 Ta 124.6(10) 4_545 1_665
Ga2 O3 Ta 63.9(4) 1_655 1_665
O6 O3 Ta 125.9(8) 2_655 1_665
O1 O3 Ta 134.9(10) 4_645 1_665
O7 O3 Ta 20.0(5) 1_655 1_665
Ga2 O3 Ta 142.2(7) 4_645 1_665
O6 O3 Ta 106.9(7) 2_755 1_665
La1 O3 Ta 87.7(5) 1_654 1_665
Ga1 O3 Ta 137.0(8) . 1_665
Ta O3 Ta 137.0(8) . 1_665
O7 O3 Ta 143.1(8) 2_645 1_665
O4 O3 Ta 54.0(6) 2 1_665
O4 O3 Ta 99.9(9) 4_645 1_665
O2 O3 Ta 121.8(9) 1_645 1_665
Ga4 O3 Ta 133.3(7) 4_645 1_665
O6 O3 Ta 93.8(5) 4_655 1_665
O7 O3 Ta 157.3(9) 1_545 1_665
O5 O3 Ta 79.0(5) 4_655 1_665
O3 O3 Ta 74.2(4) 1_655 1_665
O3 O3 Ta 105.8(4) 1_455 1_665
O6 O3 Ta 78.1(5) 4_755 1_665
O7 O3 Ta 104.4(6) 4_645 1_665
Ga4 O3 Ta 34.1(2) 4_655 1_665
O7 O3 Ta 129.5(8) 1_645 1_665
O4 O3 Ta 40.7(6) 2_655 1_665
La1 O3 Ta 77.2(3) 3_554 1_665
O2 O3 Ta 49.8(6) . 1_665
Ga2 O3 Ta 58.0(3) 2_755 1_665
O2 O3 Ta 113.7(8) 2_645 1_665
Ga2 O3 Ga1 72.5(9) . 1_665
Ga3 O3 Ga1 124.1(14) . 1_665
La2 O3 Ga1 28.2(4) 1_655 1_665
La1 O3 Ga1 112.3(9) 2_656 1_665
O6 O3 Ga1 154.7(13) . 1_665
O1 O3 Ga1 60.0(14) 1_655 1_665
O2 O3 Ga1 84.1(15) 4_645 1_665
O4 O3 Ga1 44.6(12) 1_655 1_665
O5 O3 Ga1 147.5(12) . 1_665
O5 O3 Ga1 118.1(11) 2_655 1_665
O1 O3 Ga1 88.9(12) . 1_665
O3 O3 Ga1 92.4(6) 2_655 1_665
O5 O3 Ga1 108.5(9) 1_655 1_665
Ta O3 Ga1 127.2(8) 1_655 1_665
Ga1 O3 Ga1 127.2(8) 1_655 1_665
O1 O3 Ga1 58.6(11) 2_655 1_665
Ga2 O3 Ga1 67.5(5) 2_655 1_665
O3 O3 Ga1 70.3(3) 2_755 1_665
Ga4 O3 Ga1 176.7(8) 3_544 1_665
La2 O3 Ga1 78.4(5) . 1_665
O7 O3 Ga1 15.3(6) 2_655 1_665
La1 O3 Ga1 124.9(6) 2_556 1_665
La1 O3 Ga1 53.2(3) 3_654 1_665
Ga4 O3 Ga1 101.8(5) 2_656 1_665
Ga4 O3 Ga1 35.4(2) 3_554 1_665
O2 O3 Ga1 156.7(12) 1_545 1_665
Ga3 O3 Ga1 85.2(5) 1_655 1_665
O7 O3 Ga1 49.2(6) . 1_665
O4 O3 Ga1 124.6(10) 4_545 1_665
Ga2 O3 Ga1 63.9(4) 1_655 1_665
O6 O3 Ga1 125.9(8) 2_655 1_665
O1 O3 Ga1 134.9(10) 4_645 1_665
O7 O3 Ga1 20.0(5) 1_655 1_665
Ga2 O3 Ga1 142.2(7) 4_645 1_665
O6 O3 Ga1 106.9(7) 2_755 1_665
La1 O3 Ga1 87.7(5) 1_654 1_665
Ga1 O3 Ga1 137.0(8) . 1_665
Ta O3 Ga1 137.0(8) . 1_665
O7 O3 Ga1 143.1(8) 2_645 1_665
O4 O3 Ga1 54.0(6) 2 1_665
O4 O3 Ga1 99.9(9) 4_645 1_665
O2 O3 Ga1 121.8(9) 1_645 1_665
Ga4 O3 Ga1 133.3(7) 4_645 1_665
O6 O3 Ga1 93.8(5) 4_655 1_665
O7 O3 Ga1 157.3(9) 1_545 1_665
O5 O3 Ga1 79.0(5) 4_655 1_665
O3 O3 Ga1 74.2(4) 1_655 1_665
O3 O3 Ga1 105.8(4) 1_455 1_665
O6 O3 Ga1 78.1(5) 4_755 1_665
O7 O3 Ga1 104.4(6) 4_645 1_665
Ga4 O3 Ga1 34.1(2) 4_655 1_665
O7 O3 Ga1 129.5(8) 1_645 1_665
O4 O3 Ga1 40.7(6) 2_655 1_665
La1 O3 Ga1 77.2(3) 3_554 1_665
O2 O3 Ga1 49.8(6) . 1_665
Ga2 O3 Ga1 58.0(3) 2_755 1_665
O2 O3 Ga1 113.7(8) 2_645 1_665
Ta O3 Ga1 0.0 1_665 1_665
Ga2 O3 Ga4 134.5(14) . 3_644
Ga3 O3 Ga4 95.4(10) . 3_644
La2 O3 Ga4 93.9(9) 1_655 3_644
La1 O3 Ga4 40.7(5) 2_656 3_644
O6 O3 Ga4 37.0(8) . 3_644
O1 O3 Ga4 68.5(13) 1_655 3_644
O2 O3 Ga4 96.7(16) 4_645 3_644
O4 O3 Ga4 127.5(14) 1_655 3_644
O5 O3 Ga4 93.7(9) . 3_644
O5 O3 Ga4 66.2(9) 2_655 3_644
O1 O3 Ga4 144.5(15) . 3_644
O3 O3 Ga4 124.8(8) 2_655 3_644
O5 O3 Ga4 9.8(6) 1_655 3_644
Ta O3 Ga4 30.9(4) 1_655 3_644
Ga1 O3 Ga4 30.9(4) 1_655 3_644
O1 O3 Ga4 100.0(9) 2_655 3_644
Ga2 O3 Ga4 121.0(7) 2_655 3_644
O3 O3 Ga4 58.4(7) 2_755 3_644
Ga4 O3 Ga4 61.9(4) 3_544 3_644
La2 O3 Ga4 159.8(7) . 3_644
O7 O3 Ga4 126.9(8) 2_655 3_644
La1 O3 Ga4 112.6(6) 2_556 3_644
La1 O3 Ga4 98.2(7) 3_654 3_644
Ga4 O3 Ga4 96.2(7) 2_656 3_644
Ga4 O3 Ga4 144.8(8) 3_554 3_644
O2 O3 Ga4 78.7(8) 1_545 3_644
Ga3 O3 Ga4 35.5(3) 1_655 3_644
O7 O3 Ga4 166.9(9) . 3_644
O4 O3 Ga4 93.1(11) 4_545 3_644
Ga2 O3 Ga4 58.3(4) 1_655 3_644
O6 O3 Ga4 93.0(6) 2_655 3_644
O1 O3 Ga4 52.3(6) 4_645 3_644
O7 O3 Ga4 97.9(8) 1_655 3_644
Ga2 O3 Ga4 71.3(5) 4_645 3_644
O6 O3 Ga4 42.5(5) 2_755 3_644
La1 O3 Ga4 71.8(4) 1_654 3_644
Ga1 O3 Ga4 99.2(5) . 3_644
Ta O3 Ga4 99.2(5) . 3_644
O7 O3 Ga4 48.5(6) 2_645 3_644
O4 O3 Ga4 136.3(8) 2 3_644
O4 O3 Ga4 42.8(8) 4_645 3_644
O2 O3 Ga4 19.1(8) 1_645 3_644
Ga4 O3 Ga4 70.9(4) 4_645 3_644
O6 O3 Ga4 116.7(8) 4_655 3_644
O7 O3 Ga4 76.5(6) 1_545 3_644
O5 O3 Ga4 99.1(7) 4_655 3_644
O3 O3 Ga4 43.6(3) 1_655 3_644
O3 O3 Ga4 136.4(3) 1_455 3_644
O6 O3 Ga4 74.0(6) 4_755 3_644
O7 O3 Ga4 78.6(6) 4_645 3_644
Ga4 O3 Ga4 139.2(7) 4_655 3_644
O7 O3 Ga4 20.4(5) 1_645 3_644
O4 O3 Ga4 89.9(7) 2_655 3_644
La1 O3 Ga4 142.6(7) 3_554 3_644
O2 O3 Ga4 144.7(10) . 3_644
Ga2 O3 Ga4 71.0(4) 2_755 3_644
O2 O3 Ga4 71.1(8) 2_645 3_644
Ta O3 Ga4 117.7(6) 1_665 3_644
Ga1 O3 Ga4 117.7(6) 1_665 3_644
Ga2 O3 O2 106.8(12) . 3_544
Ga3 O3 O2 47.7(13) . 3_544
La2 O3 O2 73.6(10) 1_655 3_544
La1 O3 O2 159.4(11) 2_656 3_544
O6 O3 O2 113.9(14) . 3_544
O1 O3 O2 129.9(16) 1_655 3_544
O2 O3 O2 144.4(19) 4_645 3_544
O4 O3 O2 104.6(15) 1_655 3_544
O5 O3 O2 81.5(12) . 3_544
O5 O3 O2 56.4(13) 2_655 3_544
O1 O3 O2 88.8(14) . 3_544
O3 O3 O2 22.8(11) 2_655 3_544
O5 O3 O2 114.8(12) 1_655 3_544
Ta O3 O2 90.7(11) 1_655 3_544
Ga1 O3 O2 90.7(11) 1_655 3_544
O1 O3 O2 33.4(9) 2_655 3_544
Ga2 O3 O2 9.1(8) 2_655 3_544
O3 O3 O2 76.6(14) 2_755 3_544
Ga4 O3 O2 100.8(10) 3_544 3_544
La2 O3 O2 50.1(6) . 3_544
O7 O3 O2 61.8(10) 2_655 3_544
La1 O3 O2 98.4(7) 2_556 3_544
La1 O3 O2 127.8(8) 3_654 3_544
Ga4 O3 O2 141.8(7) 2_656 3_544
Ga4 O3 O2 82.3(8) 3_554 3_544
O2 O3 O2 111.5(13) 1_545 3_544
Ga3 O3 O2 99.3(9) 1_655 3_544
O7 O3 O2 61.4(9) . 3_544
O4 O3 O2 129.1(10) 4_545 3_544
Ga2 O3 O2 123.8(8) 1_655 3_544
O6 O3 O2 49.5(9) 2_655 3_544
O1 O3 O2 148.6(11) 4_645 3_544
O7 O3 O2 87.6(9) 1_655 3_544
Ga2 O3 O2 134.3(8) 4_645 3_544
O6 O3 O2 76.3(10) 2_755 3_544
La1 O3 O2 48.3(8) 1_654 3_544
Ga1 O3 O2 66.5(8) . 3_544
Ta O3 O2 66.5(8) . 3_544
O7 O3 O2 83.4(11) 2_645 3_544
O4 O3 O2 25.4(8) 2 3_544
O4 O3 O2 157.2(10) 4_645 3_544
O2 O3 O2 136.8(16) 1_645 3_544
Ga4 O3 O2 61.7(9) 4_645 3_544
O6 O3 O2 121.5(8) 4_655 3_544
O7 O3 O2 81.2(10) 1_545 3_544
O5 O3 O2 141.3(8) 4_655 3_544
O3 O3 O2 112.3(6) 1_655 3_544
O3 O3 O2 67.7(6) 1_455 3_544
O6 O3 O2 154.5(9) 4_755 3_544
O7 O3 O2 160.5(9) 4_645 3_544
Ga4 O3 O2 45.9(7) 4_655 3_544
O7 O3 O2 102.7(11) 1_645 3_544
O4 O3 O2 62.5(9) 2_655 3_544
La1 O3 O2 97.7(7) 3_554 3_544
O2 O3 O2 92.2(10) . 3_544
Ga2 O3 O2 70.4(7) 2_755 3_544
O2 O3 O2 50.8(7) 2_645 3_544
Ta O3 O2 76.4(7) 1_665 3_544
Ga1 O3 O2 76.4(7) 1_665 3_544
Ga4 O3 O2 118.7(9) 3_644 3_544
Ga2 O3 La1 105.7(13) . 1_554
Ga3 O3 La1 22.5(9) . 1_554
La2 O3 La1 101.1(10) 1_655 1_554
La1 O3 La1 144.1(8) 2_656 1_554
O6 O3 La1 93.5(10) . 1_554
O1 O3 La1 157.1(16) 1_655 1_554
O2 O3 La1 140.0(18) 4_645 1_554
O4 O3 La1 118.2(13) 1_655 1_554
O5 O3 La1 53.7(9) . 1_554
O5 O3 La1 48.5(9) 2_655 1_554
O1 O3 La1 79.5(13) . 1_554
O3 O3 La1 11.8(4) 2_655 1_554
O5 O3 La1 115.0(9) 1_655 1_554
Ta O3 La1 82.9(6) 1_655 1_554
Ga1 O3 La1 82.9(6) 1_655 1_554
O1 O3 La1 58.7(8) 2_655 1_554
Ga2 O3 La1 36.6(4) 2_655 1_554
O3 O3 La1 94.6(12) 2_755 1_554
Ga4 O3 La1 75.2(5) 3_544 1_554
La2 O3 La1 47.5(4) . 1_554
O7 O3 La1 87.2(9) 2_655 1_554
La1 O3 La1 75.5(6) 2_556 1_554
La1 O3 La1 147.2(7) 3_654 1_554
Ga4 O3 La1 125.6(7) 2_656 1_554
Ga4 O3 La1 97.7(7) 3_554 1_554
O2 O3 La1 83.7(11) 1_545 1_554
Ga3 O3 La1 111.4(6) 1_655 1_554
O7 O3 La1 72.7(8) . 1_554
O4 O3 La1 105.1(10) 4_545 1_554
Ga2 O3 La1 147.8(7) 1_655 1_554
O6 O3 La1 24.8(4) 2_655 1_554
O1 O3 La1 122.1(8) 4_645 1_554
O7 O3 La1 115.3(8) 1_655 1_554
Ga2 O3 La1 106.6(6) 4_645 1_554
O6 O3 La1 77.9(6) 2_755 1_554
La1 O3 La1 58.9(4) 1_654 1_554
Ga1 O3 La1 38.7(3) . 1_554
Ta O3 La1 38.7(3) . 1_554
O7 O3 La1 67.4(7) 2_645 1_554
O4 O3 La1 48.5(7) 2 1_554
O4 O3 La1 154.3(9) 4_645 1_554
O2 O3 La1 125.8(10) 1_645 1_554
Ga4 O3 La1 43.9(3) 4_645 1_554
O6 O3 La1 110.1(7) 4_655 1_554
O7 O3 La1 54.9(6) 1_545 1_554
O5 O3 La1 140.7(7) 4_655 1_554
O3 O3 La1 129.8(3) 1_655 1_554
O3 O3 La1 50.2(3) 1_455 1_554
O6 O3 La1 170.1(7) 4_755 1_554
O7 O3 La1 139.9(7) 4_645 1_554
Ga4 O3 La1 69.1(5) 4_655 1_554
O7 O3 La1 93.7(7) 1_645 1_554
O4 O3 La1 88.9(8) 2_655 1_554
La1 O3 La1 93.9(5) 3_554 1_554
O2 O3 La1 101.5(7) . 1_554
Ga2 O3 La1 92.5(5) 2_755 1_554
O2 O3 La1 44.4(7) 2_645 1_554
Ta O3 La1 102.4(6) 1_665 1_554
Ga1 O3 La1 102.4(6) 1_665 1_554
Ga4 O3 La1 113.8(5) 3_644 1_554
O2 O3 La1 27.8(7) 3_544 1_554
Ga2 O3 O1 83.3(13) . 2
Ga3 O3 O1 46.0(12) . 2
La2 O3 O1 93.8(11) 1_655 2
La1 O3 O1 161.3(11) 2_656 2
O6 O3 O1 116.0(13) . 2
O1 O3 O1 145(2) 1_655 2
O2 O3 O1 120.8(17) 4_645 2
O4 O3 O1 92.9(14) 1_655 2
O5 O3 O1 65.1(12) . 2
O5 O3 O1 73.0(11) 2_655 2
O1 O3 O1 60.9(18) . 2
O3 O3 O1 14.2(9) 2_655 2
O5 O3 O1 139.0(11) 1_655 2
Ta O3 O1 108.1(9) 1_655 2
Ga1 O3 O1 108.1(9) 1_655 2
O1 O3 O1 60.8(9) 2_655 2
Ga2 O3 O1 33.1(6) 2_655 2
O3 O3 O1 105.5(13) 2_755 2
Ga4 O3 O1 93.8(9) 3_544 2
La2 O3 O1 23.7(7) . 2
O7 O3 O1 69.7(10) 2_655 2
La1 O3 O1 71.4(7) 2_556 2
La1 O3 O1 122.0(8) 3_654 2
Ga4 O3 O1 113.3(8) 2_656 2
Ga4 O3 O1 72.8(8) 3_554 2
O2 O3 O1 93.0(11) 1_545 2
Ga3 O3 O1 128.0(8) 1_655 2
O7 O3 O1 47.6(9) . 2
O4 O3 O1 101.5(11) 4_545 2
Ga2 O3 O1 146.1(9) 1_655 2
O6 O3 O1 48.4(8) 2_655 2
O1 O3 O1 134.1(10) 4_645 2
O7 O3 O1 102.0(10) 1_655 2
Ga2 O3 O1 113.1(8) 4_645 2
O6 O3 O1 100.2(9) 2_755 2
La1 O3 O1 75.5(7) 1_654 2
Ga1 O3 O1 52.5(7) . 2
Ta O3 O1 52.5(7) . 2
O7 O3 O1 92.5(10) 2_645 2
O4 O3 O1 33.5(9) 2 2
O4 O3 O1 173.2(10) 4_645 2
O2 O3 O1 150.3(11) 1_645 2
Ga4 O3 O1 69.1(8) 4_645 2
O6 O3 O1 93.7(8) 4_655 2
O7 O3 O1 74.0(9) 1_545 2
O5 O3 O1 119.7(9) 4_655 2
O3 O3 O1 140.5(6) 1_655 2
O3 O3 O1 39.5(6) 1_455 2
O6 O3 O1 147.0(9) 4_755 2
O7 O3 O1 131.8(8) 4_645 2
Ga4 O3 O1 50.6(7) 4_655 2
O7 O3 O1 119.0(9) 1_645 2
O4 O3 O1 86.9(9) 2_655 2
La1 O3 O1 72.4(7) 3_554 2
O2 O3 O1 76.3(9) . 2
Ga2 O3 O1 98.3(7) 2_755 2
O2 O3 O1 68.3(10) 2_645 2
Ta O3 O1 84.6(7) 1_665 2
Ga1 O3 O1 84.6(7) 1_665 2
Ga4 O3 O1 139.0(8) 3_644 2
O2 O3 O1 28.9(7) 3_544 2
La1 O3 O1 25.4(7) 1_554 2
Ga2 O3 Ga4 82.3(11) . 2_756
Ga3 O3 Ga4 148.4(13) . 2_756
La2 O3 Ga4 82.6(9) 1_655 2_756
La1 O3 Ga4 27.3(4) 2_656 2_756
O6 O3 Ga4 77.4(10) . 2_756
O1 O3 Ga4 26.7(14) 1_655 2_756
O2 O3 Ga4 46.0(14) 4_645 2_756
O4 O3 Ga4 71.4(12) 1_655 2_756
O5 O3 Ga4 121.6(11) . 2_756
O5 O3 Ga4 122.5(11) 2_655 2_756
O1 O3 Ga4 107.1(14) . 2_756
O3 O3 Ga4 177.6(5) 2_655 2_756
O5 O3 Ga4 56.1(8) 1_655 2_756
Ta O3 Ga4 87.7(7) 1_655 2_756
Ga1 O3 Ga4 87.7(7) 1_655 2_756
O1 O3 Ga4 122.4(9) 2_655 2_756
Ga2 O3 Ga4 147.7(8) 2_655 2_756
O3 O3 Ga4 82.1(12) 2_755 2_756
Ga4 O3 Ga4 97.0(7) 3_544 2_756
La2 O3 Ga4 141.3(6) . 2_756
O7 O3 Ga4 100.4(8) 2_655 2_756
La1 O3 Ga4 105.3(7) 2_556 2_756
La1 O3 Ga4 42.5(3) 3_654 2_756
Ga4 O3 Ga4 57.5(4) 2_656 2_756
Ga4 O3 Ga4 92.0(6) 3_554 2_756
O2 O3 Ga4 91.7(10) 1_545 2_756
Ga3 O3 Ga4 62.7(5) 1_655 2_756
O7 O3 Ga4 117.0(8) . 2_756
O4 O3 Ga4 74.8(10) 4_545 2_756
Ga2 O3 Ga4 31.8(3) 1_655 2_756
O6 O3 Ga4 146.1(7) 2_655 2_756
O1 O3 Ga4 51.6(7) 4_645 2_756
O7 O3 Ga4 70.4(8) 1_655 2_756
Ga2 O3 Ga4 69.4(5) 4_645 2_756
O6 O3 Ga4 94.2(7) 2_755 2_756
La1 O3 Ga4 116.0(6) 1_654 2_756
Ga1 O3 Ga4 136.1(7) . 2_756
Ta O3 Ga4 136.1(7) . 2_756
O7 O3 Ga4 102.9(8) 2_645 2_756
O4 O3 Ga4 139.0(8) 2 2_756
O4 O3 Ga4 16.2(6) 4_645 2_756
O2 O3 Ga4 44.6(9) 1_645 2_756
Ga4 O3 Ga4 126.4(6) 4_645 2_756
O6 O3 Ga4 75.1(6) 4_655 2_756
O7 O3 Ga4 117.3(8) 1_545 2_756
O5 O3 Ga4 46.3(5) 4_655 2_756
O3 O3 Ga4 46.0(3) 1_655 2_756
O3 O3 Ga4 134.0(3) 1_455 2_756
O6 O3 Ga4 17.6(4) 4_755 2_756
O7 O3 Ga4 40.8(5) 4_645 2_756
Ga4 O3 Ga4 119.0(6) 4_655 2_756
O7 O3 Ga4 76.7(7) 1_645 2_756
O4 O3 Ga4 93.0(7) 2_655 2_756
La1 O3 Ga4 93.7(5) 3_554 2_756
O2 O3 Ga4 88.0(9) . 2_756
Ga2 O3 Ga4 86.3(5) 2_755 2_756
O2 O3 Ga4 127.0(11) 2_645 2_756
Ta O3 Ga4 85.1(5) 1_665 2_756
Ga1 O3 Ga4 85.1(5) 1_665 2_756
Ga4 O3 Ga4 56.8(4) 3_644 2_756
O2 O3 Ga4 155.5(7) 3_544 2_756
La1 O3 Ga4 170.3(5) 1_554 2_756
O1 O3 Ga4 164.2(8) 2 2_756
Ga2 O3 O2 92.1(12) . 4_745
Ga3 O3 O2 150.0(13) . 4_745
La2 O3 O2 65.4(11) 1_655 4_745
La1 O3 O2 40.4(7) 2_656 4_745
O6 O3 O2 85.0(12) . 4_745
O1 O3 O2 13.9(15) 1_655 4_745
O2 O3 O2 60.2(14) 4_645 4_745
O4 O3 O2 73.2(12) 1_655 4_745
O5 O3 O2 137.1(12) . 4_745
O5 O3 O2 115.2(12) 2_655 4_745
O1 O3 O2 119.7(14) . 4_745
O3 O3 O2 160.0(14) 2_655 4_745
O5 O3 O2 50.9(11) 1_655 4_745
Ta O3 O2 84.3(10) 1_655 4_745
Ga1 O3 O2 84.3(10) 1_655 4_745
O1 O3 O2 104.0(11) 2_655 4_745
Ga2 O3 O2 129.9(10) 2_655 4_745
O3 O3 O2 65.1(14) 2_755 4_745
Ga4 O3 O2 108.2(9) 3_544 4_745
La2 O3 O2 145.0(8) . 4_745
O7 O3 O2 88.0(10) 2_655 4_745
La1 O3 O2 123.6(8) 2_556 4_745
La1 O3 O2 44.5(8) 3_654 4_745
Ga4 O3 O2 74.5(7) 2_656 4_745
Ga4 O3 O2 89.9(8) 3_554 4_745
O2 O3 O2 108.2(10) 1_545 4_745
Ga3 O3 O2 49.0(9) 1_655 4_745
O7 O3 O2 114.8(10) . 4_745
O4 O3 O2 93.2(11) 4_545 4_745
Ga2 O3 O2 13.5(7) 1_655 4_745
O6 O3 O2 147.8(9) 2_655 4_745
O1 O3 O2 67.2(8) 4_645 4_745
O7 O3 O2 55.8(10) 1_655 4_745
Ga2 O3 O2 86.8(7) 4_645 4_745
O6 O3 O2 84.3(10) 2_755 4_745
La1 O3 O2 100.7(9) 1_654 4_745
Ga1 O3 O2 149.7(8) . 4_745
Ta O3 O2 149.7(8) . 4_745
O7 O3 O2 103.7(10) 2_645 4_745
O4 O3 O2 124.8(11) 2 4_745
O4 O3 O2 27.6(8) 4_645 4_745
O2 O3 O2 49.9(4) 1_645 4_745
Ga4 O3 O2 125.3(9) 4_645 4_745
O6 O3 O2 90.2(8) 4_655 4_745
O7 O3 O2 127.5(9) 1_545 4_745
O5 O3 O2 59.1(9) 4_655 4_745
O3 O3 O2 29.9(7) 1_655 4_745
O3 O3 O2 150.1(7) 1_455 4_745
O6 O3 O2 30.1(7) 4_755 4_745
O7 O3 O2 58.9(8) 4_645 4_745
Ga4 O3 O2 107.1(9) 4_655 4_745
O7 O3 O2 75.4(9) 1_645 4_745
O4 O3 O2 74.8(10) 2_655 4_745
La1 O3 O2 104.2(8) 3_554 4_745
O2 O3 O2 90.8(10) . 4_745
Ga2 O3 O2 68.1(8) 2_755 4_745
O2 O3 O2 118.3(14) 2_645 4_745
Ta O3 O2 73.3(8) 1_665 4_745
Ga1 O3 O2 73.3(8) 1_665 4_745
Ga4 O3 O2 55.2(8) 3_644 4_745
O2 O3 O2 137.2(8) 3_544 4_745
La1 O3 O2 159.6(9) 1_554 4_745
O1 O3 O2 157.7(9) 2 4_745
Ga4 O3 O2 18.4(6) 2_756 4_745
Ga2 O3 O2 63.7(12) . 1_655
Ga3 O3 O2 158.1(14) . 1_655
La2 O3 O2 46.2(6) 1_655 1_655
La1 O3 O2 79.7(11) 2_656 1_655
O6 O3 O2 129.2(13) . 1_655
O1 O3 O2 31.2(14) 1_655 1_655
O2 O3 O2 55.9(17) 4_645 1_655
O4 O3 O2 34.6(12) 1_655 1_655
O5 O3 O2 154.6(12) . 1_655
O5 O3 O2 139.9(12) 2_655 1_655
O1 O3 O2 90.5(13) . 1_655
O3 O3 O2 125.2(7) 2_655 1_655
O5 O3 O2 92.9(9) 1_655 1_655
Ta O3 O2 124.3(8) 1_655 1_655
Ga1 O3 O2 124.3(8) 1_655 1_655
O1 O3 O2 88.5(12) 2_655 1_655
Ga2 O3 O2 101.5(7) 2_655 1_655
O3 O3 O2 78.2(7) 2_755 1_655
Ga4 O3 O2 148.6(11) 3_544 1_655
La2 O3 O2 100.7(6) . 1_655
O7 O3 O2 49.0(9) 2_655 1_655
La1 O3 O2 118.6(9) 2_556 1_655
La1 O3 O2 22.0(7) 3_654 1_655
Ga4 O3 O2 75.7(9) 2_656 1_655
Ga4 O3 O2 45.6(7) 3_554 1_655
O2 O3 O2 132.7(18) 1_545 1_655
Ga3 O3 O2 79.1(6) 1_655 1_655
O7 O3 O2 69.9(9) . 1_655
O4 O3 O2 101.1(13) 4_545 1_655
Ga2 O3 O2 41.2(7) 1_655 1_655
O6 O3 O2 160.0(10) 2_655 1_655
O1 O3 O2 100.9(11) 4_645 1_655
O7 O3 O2 27.7(8) 1_655 1_655
Ga2 O3 O2 111.3(10) 4_645 1_655
O6 O3 O2 113.8(7) 2_755 1_655
La1 O3 O2 109.6(7) 1_654 1_655
Ga1 O3 O2 160.0(7) . 1_655
Ta O3 O2 160.0(7) . 1_655
O7 O3 O2 146.1(9) 2_645 1_655
O4 O3 O2 87.5(9) 2 1_655
O4 O3 O2 68.2(11) 4_645 1_655
O2 O3 O2 94.5(11) 1_645 1_655
Ga4 O3 O2 158.3(8) 4_645 1_655
O6 O3 O2 77.0(9) 4_655 1_655
O7 O3 O2 168.0(11) 1_545 1_655
O5 O3 O2 51.2(8) 4_655 1_655
O3 O3 O2 60.5(5) 1_655 1_655
O3 O3 O2 119.5(5) 1_455 1_655
O6 O3 O2 44.0(9) 4_755 1_655
O7 O3 O2 72.6(10) 4_645 1_655
Ga4 O3 O2 66.8(7) 4_655 1_655
O7 O3 O2 118.4(8) 1_645 1_655
O4 O3 O2 61.8(8) 2_655 1_655
La1 O3 O2 73.9(7) 3_554 1_655
O2 O3 O2 50.7(6) . 1_655
Ga2 O3 O2 70.8(5) 2_755 1_655
O2 O3 O2 138.1(8) 2_645 1_655
Ta O3 O2 34.1(7) 1_665 1_655
Ga1 O3 O2 34.1(7) 1_665 1_655
Ga4 O3 O2 99.2(7) 3_644 1_655
O2 O3 O2 110.5(12) 3_544 1_655
La1 O3 O2 136.0(7) 1_554 1_655
O1 O3 O2 114.8(9) 2 1_655
Ga4 O3 O2 52.4(8) 2_756 1_655
O2 O3 O2 45.0(6) 4_745 1_655
Ga2 O3 O2 34.8(11) . 4_545
Ga3 O3 O2 83.0(14) . 4_545
La2 O3 O2 128.5(10) 1_655 4_545
La1 O3 O2 101.9(9) 2_656 4_545
O6 O3 O2 101.4(11) . 4_545
O1 O3 O2 115.9(14) 1_655 4_545
O2 O3 O2 60.0(13) 4_645 4_545
O4 O3 O2 64.6(14) 1_655 4_545
O5 O3 O2 57.4(12) . 4_545
O5 O3 O2 119.0(14) 2_655 4_545
O1 O3 O2 12.1(14) . 4_545
O3 O3 O2 75.5(15) 2_655 4_545
O5 O3 O2 142.5(11) 1_655 4_545
Ta O3 O2 131.7(9) 1_655 4_545
Ga1 O3 O2 131.7(9) 1_655 4_545
O1 O3 O2 123.4(11) 2_655 4_545
Ga2 O3 O2 97.0(10) 2_655 4_545
O3 O3 O2 168.4(11) 2_755 4_545
Ga4 O3 O2 81.3(8) 3_544 4_545
La2 O3 O2 46.1(8) . 4_545
O7 O3 O2 96.9(10) 2_655 4_545
La1 O3 O2 24.3(7) 2_556 4_545
La1 O3 O2 83.5(8) 3_654 4_545
Ga4 O3 O2 47.9(7) 2_656 4_545
Ga4 O3 O2 65.3(8) 3_554 4_545
O2 O3 O2 57.9(5) 1_545 4_545
Ga3 O3 O2 166.0(11) 1_655 4_545
O7 O3 O2 57.7(9) . 4_545
O4 O3 O2 40.9(10) 4_545 4_545
Ga2 O3 O2 129.6(9) 1_655 4_545
O6 O3 O2 84.2(10) 2_655 4_545
O1 O3 O2 82.0(8) 4_645 4_545
O7 O3 O2 116.8(9) 1_655 4_545
Ga2 O3 O2 62.0(6) 4_645 4_545
O6 O3 O2 147.7(10) 2_755 4_545
La1 O3 O2 138.9(11) 1_654 4_545
Ga1 O3 O2 63.0(9) . 4_545
Ta O3 O2 63.0(9) . 4_545
O7 O3 O2 111.5(9) 2_645 4_545
O4 O3 O2 87.3(11) 2 4_545
O4 O3 O2 108.3(9) 4_645 4_545
O2 O3 O2 116.7(9) 1_645 4_545
Ga4 O3 O2 102.2(10) 4_645 4_545
O6 O3 O2 30.1(8) 4_655 4_545
O7 O3 O2 77.4(10) 1_545 4_545
O5 O3 O2 61.4(8) 4_655 4_545
O3 O3 O2 150.1(8) 1_655 4_545
O3 O3 O2 29.9(8) 1_455 4_545
O6 O3 O2 90.2(8) 4_755 4_545
O7 O3 O2 66.2(8) 4_645 4_545
Ga4 O3 O2 87.5(8) 4_655 4_545
O7 O3 O2 129.4(9) 1_645 4_545
O4 O3 O2 136.3(10) 2_655 4_545
La1 O3 O2 25.2(7) 3_554 4_545
O2 O3 O2 52.2(7) . 4_545
Ga2 O3 O2 155.6(9) 2_755 4_545
O2 O3 O2 118.1(15) 2_645 4_545
Ta O3 O2 100.6(8) 1_665 4_545
Ga1 O3 O2 100.6(8) 1_665 4_545
Ga4 O3 O2 133.3(8) 3_644 4_545
O2 O3 O2 94.4(10) 3_544 4_545
La1 O3 O2 80.0(9) 1_554 4_545
O1 O3 O2 65.6(9) 2 4_545
Ga4 O3 O2 104.8(8) 2_756 4_545
O2 O3 O2 120.2(13) 4_745 4_545
O2 O3 O2 98.5(11) 1_655 4_545
Ga2 O3 La1 109.5(12) . 3_644
Ga3 O3 La1 87.0(10) . 3_644
La2 O3 La1 128.7(10) 1_655 3_644
La1 O3 La1 34.6(4) 2_656 3_644
O6 O3 La1 17.3(8) . 3_644
O1 O3 La1 85.8(15) 1_655 3_644
O2 O3 La1 79.8(13) 4_645 3_644
O4 O3 La1 123.2(14) 1_655 3_644
O5 O3 La1 66.1(9) . 3_644
O5 O3 La1 76.7(8) 2_655 3_644
O1 O3 La1 108.9(14) . 3_644
O3 O3 La1 120.5(4) 2_655 3_644
O5 O3 La1 46.0(7) 1_655 3_644
Ta O3 La1 47.9(4) 1_655 3_644
Ga1 O3 La1 47.9(4) 1_655 3_644
O1 O3 La1 130.5(10) 2_655 3_644
Ga2 O3 La1 138.8(7) 2_655 3_644
O3 O3 La1 94.3(7) 2_755 3_644
Ga4 O3 La1 35.9(4) 3_544 3_644
La2 O3 La1 133.5(7) . 3_644
O7 O3 La1 159.8(10) 2_655 3_644
La1 O3 La1 76.5(5) 2_556 3_644
La1 O3 La1 100.6(7) 3_654 3_644
Ga4 O3 La1 69.7(5) 2_656 3_644
Ga4 O3 La1 144.9(8) 3_554 3_644
O2 O3 La1 43.6(8) 1_545 3_644
Ga3 O3 La1 71.8(5) 1_655 3_644
O7 O3 La1 154.6(9) . 3_644
O4 O3 La1 58.6(10) 4_545 3_644
Ga2 O3 La1 82.1(5) 1_655 3_644
O6 O3 La1 84.7(5) 2_655 3_644
O1 O3 La1 22.1(8) 4_645 3_644
O7 O3 La1 127.0(9) 1_655 3_644
Ga2 O3 La1 35.7(3) 4_645 3_644
O6 O3 La1 68.9(5) 2_755 3_644
La1 O3 La1 97.8(5) 1_654 3_644
Ga1 O3 La1 77.3(4) . 3_644
Ta O3 La1 77.3(4) . 3_644
O7 O3 La1 48.3(6) 2_645 3_644
O4 O3 La1 156.6(8) 2 3_644
O4 O3 La1 46.3(7) 4_645 3_644
O2 O3 La1 25.1(7) 1_645 3_644
Ga4 O3 La1 69.5(4) 4_645 3_644
O6 O3 La1 87.2(6) 4_655 3_644
O7 O3 La1 55.9(5) 1_545 3_644
O5 O3 La1 84.2(6) 4_655 3_644
O3 O3 La1 75.7(3) 1_655 3_644
O3 O3 La1 104.3(3) 1_455 3_644
O6 O3 La1 72.7(6) 4_755 3_644
O7 O3 La1 57.3(5) 4_645 3_644
Ga4 O3 La1 174.9(6) 4_655 3_644
O7 O3 La1 37.8(5) 1_645 3_644
O4 O3 La1 126.2(8) 2_655 3_644
La1 O3 La1 112.2(6) 3_554 3_644
O2 O3 La1 131.3(10) . 3_644
Ga2 O3 La1 107.2(5) 2_755 3_644
O2 O3 La1 82.4(8) 2_645 3_644
Ta O3 La1 145.6(7) 1_665 3_644
Ga1 O3 La1 145.6(7) 1_665 3_644
Ga4 O3 La1 36.3(2) 3_644 3_644
O2 O3 La1 131.2(9) 3_544 3_644
La1 O3 La1 109.5(5) 1_554 3_644
O1 O3 La1 129.7(8) 2 3_644
Ga4 O3 La1 61.9(4) 2_756 3_644
O2 O3 La1 72.4(7) 4_745 3_644
O2 O3 La1 114.3(8) 1_655 3_644
O2 O3 La1 97.2(7) 4_545 3_644
Ga2 O3 O2 134.1(12) . 3_644
Ga3 O3 O2 82.4(13) . 3_644
La2 O3 O2 38.7(7) 1_655 3_644
La1 O3 O2 112.8(9) 2_656 3_644
O6 O3 O2 103.6(12) . 3_644
O1 O3 O2 83.9(14) 1_655 3_644
O2 O3 O2 139.1(18) 4_645 3_644
O4 O3 O2 107.7(15) 1_655 3_644
O5 O3 O2 119.7(13) . 3_644
O5 O3 O2 57.1(12) 2_655 3_644
O1 O3 O2 135.6(15) . 3_644
O3 O3 O2 74.7(14) 2_655 3_644
O5 O3 O2 71.4(10) 1_655 3_644
Ta O3 O2 68.3(9) 1_655 3_644
Ga1 O3 O2 68.3(9) 1_655 3_644
O1 O3 O2 21.7(9) 2_655 3_644
Ga2 O3 O2 48.9(8) 2_655 3_644
O3 O3 O2 24.2(11) 2_755 3_644
Ga4 O3 O2 113.8(9) 3_544 3_644
La2 O3 O2 99.0(8) . 3_644
O7 O3 O2 58.9(9) 2_655 3_644
La1 O3 O2 150.0(10) 2_556 3_644
La1 O3 O2 105.7(8) 3_654 3_644
Ga4 O3 O2 158.6(10) 2_656 3_644
Ga4 O3 O2 94.7(8) 3_554 3_644
O2 O3 O2 139.6(17) 1_545 3_644
Ga3 O3 O2 48.8(7) 1_655 3_644
O7 O3 O2 91.7(9) . 3_644
O4 O3 O2 171.7(12) 4_545 3_644
Ga2 O3 O2 73.4(6) 1_655 3_644
O6 O3 O2 82.4(9) 2_655 3_644
O1 O3 O2 131.9(9) 4_645 3_644
O7 O3 O2 57.1(8) 1_655 3_644
Ga2 O3 O2 148.7(8) 4_645 3_644
O6 O3 O2 46.4(8) 2_755 3_644
La1 O3 O2 25.7(7) 1_654 3_644
Ga1 O3 O2 106.6(9) . 3_644
Ta O3 O2 106.6(9) . 3_644
O7 O3 O2 80.1(10) 2_645 3_644
O4 O3 O2 58.0(10) 2 3_644
O4 O3 O2 105.0(10) 4_645 3_644
O2 O3 O2 97.6(9) 1_645 3_644
Ga4 O3 O2 75.1(9) 4_645 3_644
O6 O3 O2 156.7(9) 4_655 3_644
O7 O3 O2 105.7(10) 1_545 3_644
O5 O3 O2 135.0(9) 4_655 3_644
O3 O3 O2 59.2(6) 1_655 3_644
O3 O3 O2 120.8(6) 1_455 3_644
O6 O3 O2 113.9(8) 4_755 3_644
O7 O3 O2 145.0(9) 4_645 3_644
Ga4 O3 O2 61.5(7) 4_655 3_644
O7 O3 O2 76.3(9) 1_645 3_644
O4 O3 O2 23.3(7) 2_655 3_644
La1 O3 O2 134.2(7) 3_554 3_644
O2 O3 O2 110.4(11) . 3_644
Ga2 O3 O2 18.1(6) 2_755 3_644
O2 O3 O2 54.1(7) 2_645 3_644
Ta O3 O2 63.1(7) 1_665 3_644
Ga1 O3 O2 63.1(7) 1_665 3_644
Ga4 O3 O2 79.7(7) 3_644 3_644
O2 O3 O2 53.0(7) 3_544 3_644
La1 O3 O2 74.4(8) 1_554 3_644
O1 O3 O2 81.6(9) 2 3_644
Ga4 O3 O2 104.2(7) 2_756 3_644
O2 O3 O2 86.2(11) 4_745 3_644
O2 O3 O2 84.2(8) 1_655 3_644
O2 O3 O2 145.1(8) 4_545 3_644
La1 O3 O2 113.5(7) 3_644 3_644
Ga2 O3 La1 111.4(11) . 4_655
Ga3 O3 La1 84.8(12) . 4_655
La2 O3 La1 32.5(6) 1_655 4_655
La1 O3 La1 131.5(10) 2_656 4_655
O6 O3 La1 126.5(10) . 4_655
O1 O3 La1 88.4(15) 1_655 4_655
O2 O3 La1 130.2(15) 4_645 4_655
O4 O3 La1 89.3(13) 1_655 4_655
O5 O3 La1 122.0(12) . 4_655
O5 O3 La1 72.1(9) 2_655 4_655
O1 O3 La1 112.0(14) . 4_655
O3 O3 La1 64.2(9) 2_655 4_655
O5 O3 La1 94.7(8) 1_655 4_655
Ta O3 La1 91.5(6) 1_655 4_655
Ga1 O3 La1 91.5(6) 1_655 4_655
O1 O3 La1 12.6(10) 2_655 4_655
Ga2 O3 La1 34.1(3) 2_655 4_655
O3 O3 La1 45.7(7) 2_755 4_655
Ga4 O3 La1 130.5(7) 3_544 4_655
La2 O3 La1 78.3(5) . 4_655
O7 O3 La1 37.5(7) 2_655 4_655
La1 O3 La1 137.0(8) 2_556 4_655
La1 O3 La1 97.6(5) 3_654 4_655
Ga4 O3 La1 147.6(6) 2_656 4_655
Ga4 O3 La1 72.6(4) 3_554 4_655
O2 O3 La1 151.0(13) 1_545 4_655
Ga3 O3 La1 70.4(5) 1_655 4_655
O7 O3 La1 67.4(7) . 4_655
O4 O3 La1 163.3(11) 4_545 4_655
Ga2 O3 La1 82.4(5) 1_655 4_655
O6 O3 La1 85.9(6) 2_655 4_655
O1 O3 La1 155.3(8) 4_645 4_655
O7 O3 La1 49.0(6) 1_655 4_655
Ga2 O3 La1 171.4(6) 4_645 4_655
O6 O3 La1 69.6(5) 2_755 4_655
La1 O3 La1 43.3(3) 1_654 4_655
Ga1 O3 La1 106.9(7) . 4_655
Ta O3 La1 106.9(7) . 4_655
O7 O3 La1 99.4(8) 2_645 4_655
O4 O3 La1 36.3(6) 2 4_655
O4 O3 La1 120.7(9) 4_645 4_655
O2 O3 La1 120.5(9) 1_645 4_655
Ga4 O3 La1 87.4(5) 4_645 4_655
O6 O3 La1 134.3(6) 4_655 4_655
O7 O3 La1 115.8(8) 1_545 4_655
O5 O3 La1 125.1(6) 4_655 4_655
O3 O3 La1 75.4(4) 1_655 4_655
O3 O3 La1 104.6(4) 1_455 4_655
O6 O3 La1 116.5(6) 4_755 4_655
O7 O3 La1 148.4(7) 4_645 4_655
Ga4 O3 La1 37.2(3) 4_655 4_655
O7 O3 La1 100.3(7) 1_645 4_655
O4 O3 La1 21.1(6) 2_655 4_655
La1 O3 La1 110.0(5) 3_554 4_655
O2 O3 La1 88.0(7) . 4_655
Ga2 O3 La1 34.5(2) 2_755 4_655
O2 O3 La1 67.5(7) 2_645 4_655
Ta O3 La1 46.2(3) 1_665 4_655
Ga1 O3 La1 46.2(3) 1_665 4_655
Ga4 O3 La1 103.5(5) 3_644 4_655
O2 O3 La1 41.7(7) 3_544 4_655
La1 O3 La1 68.8(4) 1_554 4_655
O1 O3 La1 66.0(6) 2 4_655
Ga4 O3 La1 113.9(6) 2_756 4_655
O2 O3 La1 95.9(8) 4_745 4_655
O2 O3 La1 76.0(6) 1_655 4_655
O2 O3 La1 122.7(9) 4_545 4_655
La1 O3 La1 137.7(5) 3_644 4_655
O2 O3 La1 24.3(7) 3_644 4_655
Ga2 O3 O1 37.7(8) . 4_655
Ga3 O3 O1 148.9(13) . 4_655
La2 O3 O1 68.4(8) 1_655 4_655
La1 O3 O1 82.8(8) 2_656 4_655
O6 O3 O1 131.6(13) . 4_655
O1 O3 O1 49.5(10) 1_655 4_655
O2 O3 O1 38.0(15) 4_645 4_655
O4 O3 O1 12.3(11) 1_655 4_655
O5 O3 O1 128.7(11) . 4_655
O5 O3 O1 164.0(11) 2_655 4_655
O1 O3 O1 65.3(11) . 4_655
O3 O3 O1 118.7(7) 2_655 4_655
O5 O3 O1 112.0(9) 1_655 4_655
Ta O3 O1 145.3(10) 1_655 4_655
Ga1 O3 O1 145.3(10) 1_655 4_655
O1 O3 O1 104.8(13) 2_655 4_655
Ga2 O3 O1 106.8(8) 2_655 4_655
O3 O3 O1 104.2(8) 2_755 4_655
Ga4 O3 O1 137.0(9) 3_544 4_655
La2 O3 O1 84.5(6) . 4_655
O7 O3 O1 57.0(9) 2_655 4_655
La1 O3 O1 92.7(6) 2_556 4_655
La1 O3 O1 17.1(4) 3_654 4_655
Ga4 O3 O1 55.6(6) 2_656 4_655
Ga4 O3 O1 33.2(6) 3_554 4_655
O2 O3 O1 113.0(13) 1_545 4_655
Ga3 O3 O1 103.7(6) 1_655 4_655
O7 O3 O1 57.6(8) . 4_655
O4 O3 O1 79.7(10) 4_545 4_655
Ga2 O3 O1 62.6(4) 1_655 4_655
O6 O3 O1 151.2(8) 2_655 4_655
O1 O3 O1 94.4(11) 4_645 4_655
O7 O3 O1 50.4(7) 1_655 4_655
Ga2 O3 O1 96.0(8) 4_645 4_655
O6 O3 O1 139.6(8) 2_755 4_655
La1 O3 O1 132.7(8) 1_654 4_655
Ga1 O3 O1 135.2(6) . 4_655
Ta O3 O1 135.2(6) . 4_655
O7 O3 O1 161.8(11) 2_645 4_655
O4 O3 O1 89.0(9) 2 4_655
O4 O3 O1 75.0(9) 4_645 4_655
O2 O3 O1 103.6(11) 1_645 4_655
Ga4 O3 O1 173.6(8) 4_645 4_655
O6 O3 O1 51.9(6) 4_655 4_655
O7 O3 O1 146.8(9) 1_545 4_655
O5 O3 O1 33.0(7) 4_655 4_655
O3 O3 O1 84.0(4) 1_655 4_655
O3 O3 O1 96.0(4) 1_455 4_655
O6 O3 O1 43.7(6) 4_755 4_655
O7 O3 O1 59.7(7) 4_645 4_655
Ga4 O3 O1 69.1(7) 4_655 4_655
O7 O3 O1 135.7(9) 1_645 4_655
O4 O3 O1 83.8(8) 2_655 4_655
La1 O3 O1 48.4(3) 3_554 4_655
O2 O3 O1 29.8(7) . 4_655
Ga2 O3 O1 96.0(6) 2_755 4_655
O2 O3 O1 160.0(10) 2_645 4_655
Ta O3 O1 46.3(6) 1_665 4_655
Ga1 O3 O1 46.3(6) 1_665 4_655
Ga4 O3 O1 115.3(7) 3_644 4_655
O2 O3 O1 114.4(10) 3_544 4_655
La1 O3 O1 130.3(7) 1_554 4_655
O1 O3 O1 105.0(9) 2 4_655
Ga4 O3 O1 59.4(5) 2_756 4_655
O2 O3 O1 61.0(8) 4_745 4_655
O2 O3 O1 26.1(7) 1_655 4_655
O2 O3 O1 72.5(8) 4_545 4_655
La1 O3 O1 114.3(8) 3_644 4_655
O2 O3 O1 107.0(9) 3_644 4_655
La1 O3 O1 92.5(7) 4_655 4_655
Ga2 O3 O2 87.4(10) . 2_655
Ga3 O3 O2 91.9(16) . 2_655
La2 O3 O2 37.5(6) 1_655 2_655
La1 O3 O2 141.4(12) 2_656 2_655
O6 O3 O2 150.0(13) . 2_655
O1 O3 O2 89.3(16) 1_655 2_655
O2 O3 O2 112.3(17) 4_645 2_655
O4 O3 O2 68.6(14) 1_655 2_655
O5 O3 O2 121.9(15) . 2_655
O5 O3 O2 91.5(13) 2_655 2_655
O1 O3 O2 89.3(15) . 2_655
O3 O3 O2 61.8(8) 2_655 2_655
O5 O3 O2 116.4(11) 1_655 2_655
Ta O3 O2 115.4(10) 1_655 2_655
Ga1 O3 O2 115.4(10) 1_655 2_655
O1 O3 O2 33.1(12) 2_655 2_655
Ga2 O3 O2 35.2(8) 2_655 2_655
O3 O3 O2 67.6(8) 2_755 2_655
Ga4 O3 O2 144.9(11) 3_544 2_655
La2 O3 O2 60.9(7) . 2_655
O7 O3 O2 18.1(10) 2_655 2_655
La1 O3 O2 120.1(10) 2_556 2_655
La1 O3 O2 84.8(6) 3_654 2_655
Ga4 O3 O2 125.9(7) 2_656 2_655
Ga4 O3 O2 49.4(6) 3_554 2_655
O2 O3 O2 149.9(8) 1_545 2_655
Ga3 O3 O2 90.9(8) 1_655 2_655
O7 O3 O2 43.7(7) . 2_655
O4 O3 O2 139.7(12) 4_545 2_655
Ga2 O3 O2 89.0(7) 1_655 2_655
O6 O3 O2 93.7(10) 2_655 2_655
O1 O3 O2 167.1(12) 4_645 2_655
O7 O3 O2 45.5(7) 1_655 2_655
Ga2 O3 O2 162.6(9) 4_645 2_655
O6 O3 O2 93.8(9) 2_755 2_655
La1 O3 O2 66.2(8) 1_654 2_655
Ga1 O3 O2 108.1(10) . 2_655
Ta O3 O2 108.1(10) . 2_655
O7 O3 O2 120.3(11) 2_645 2_655
O4 O3 O2 23.9(8) 2 2_655
O4 O3 O2 128.6(11) 4_645 2_655
O2 O3 O2 140.3(8) 1_645 2_655
Ga4 O3 O2 103.2(10) 4_645 2_655
O6 O3 O2 110.2(7) 4_655 2_655
O7 O3 O2 125.3(11) 1_545 2_655
O5 O3 O2 107.4(7) 4_655 2_655
O3 O3 O2 90.0(7) 1_655 2_655
O3 O3 O2 90.0(7) 1_455 2_655
O6 O3 O2 110.3(8) 4_755 2_655
O7 O3 O2 134.4(8) 4_645 2_655
Ga4 O3 O2 13.4(5) 4_655 2_655
O7 O3 O2 124.5(10) 1_645 2_655
O4 O3 O2 36.4(8) 2_655 2_655
La1 O3 O2 85.8(6) 3_554 2_655
O2 O3 O2 64.5(13) . 2_655
Ga2 O3 O2 54.9(7) 2_755 2_655
O2 O3 O2 86.2(10) 2_645 2_655
Ta O3 O2 32.2(6) 1_665 2_655
Ga1 O3 O2 32.2(6) 1_665 2_655
Ga4 O3 O2 125.9(9) 3_644 2_655
O2 O3 O2 44.2(8) 3_544 2_655
La1 O3 O2 70.8(9) 1_554 2_655
O1 O3 O2 57.2(9) 2 2_655
Ga4 O3 O2 115.8(8) 2_756 2_655
O2 O3 O2 100.9(11) 4_745 2_655
O2 O3 O2 66.3(13) 1_655 2_655
O2 O3 O2 100.8(11) 4_545 2_655
La1 O3 O2 161.7(9) 3_644 2_655
O2 O3 O2 48.3(7) 3_644 2_655
La1 O3 O2 24.2(6) 4_655 2_655
O1 O3 O2 74.8(8) 4_655 2_655
Ga2 O3 O1 65.0(11) . 4_545
Ga3 O3 O1 71.4(12) . 4_545
La2 O3 O1 165.0(10) 1_655 4_545
La1 O3 O1 78.5(8) 2_656 4_545
O6 O3 O1 64.0(10) . 4_545
O1 O3 O1 120.0(12) 1_655 4_545
O2 O3 O1 67.4(15) 4_645 4_545
O4 O3 O1 94.9(14) 1_655 4_545
O5 O3 O1 33.8(11) . 4_545
O5 O3 O1 97.5(10) 2_655 4_545
O1 O3 O1 49.4(8) . 4_545
O3 O3 O1 85.6(12) 2_655 4_545
O5 O3 O1 107.6(10) 1_655 4_545
Ta O3 O1 95.9(8) 1_655 4_545
Ga1 O3 O1 95.9(8) 1_655 4_545
O1 O3 O1 141.3(13) 2_655 4_545
Ga2 O3 O1 115.5(9) 2_655 4_545
O3 O3 O1 152.7(6) 2_755 4_545
Ga4 O3 O1 45.5(7) 3_544 4_545
La2 O3 O1 74.2(6) . 4_545
O7 O3 O1 134.2(10) 2_655 4_545
La1 O3 O1 14.9(5) 2_556 4_545
La1 O3 O1 100.9(8) 3_654 4_545
Ga4 O3 O1 47.6(7) 2_656 4_545
Ga4 O3 O1 101.7(7) 3_554 4_545
O2 O3 O1 20.6(10) 1_545 4_545
Ga3 O3 O1 133.3(8) 1_655 4_545
O7 O3 O1 94.3(8) . 4_545
O4 O3 O1 23.0(9) 4_545 4_545
Ga2 O3 O1 127.8(8) 1_655 4_545
O6 O3 O1 71.2(8) 2_655 4_545
O1 O3 O1 52.4(6) 4_645 4_545
O7 O3 O1 148.4(9) 1_655 4_545
Ga2 O3 O1 30.4(5) 4_645 4_545
O6 O3 O1 115.9(8) 2_755 4_545
La1 O3 O1 128.4(8) 1_654 4_545
Ga1 O3 O1 47.3(7) . 4_545
Ta O3 O1 47.3(7) . 4_545
O7 O3 O1 78.7(8) 2_645 4_545
O4 O3 O1 114.9(10) 2 4_545
O4 O3 O1 89.8(8) 4_645 4_545
O2 O3 O1 84.8(9) 1_645 4_545
Ga4 O3 O1 79.1(7) 4_645 4_545
O6 O3 O1 46.1(7) 4_655 4_545
O7 O3 O1 48.8(8) 1_545 4_545
O5 O3 O1 71.6(8) 4_655 4_545
O3 O3 O1 134.1(5) 1_655 4_545
O3 O3 O1 45.9(5) 1_455 4_545
O6 O3 O1 90.3(7) 4_755 4_545
O7 O3 O1 57.4(7) 4_645 4_545
Ga4 O3 O1 122.4(7) 4_655 4_545
O7 O3 O1 92.1(8) 1_645 4_545
O4 O3 O1 170.4(10) 2_655 4_545
La1 O3 O1 59.7(6) 3_554 4_545
O2 O3 O1 87.1(9) . 4_545
Ga2 O3 O1 164.9(7) 2_755 4_545
O2 O3 O1 99.8(10) 2_645 4_545
Ta O3 O1 136.9(7) 1_665 4_545
Ga1 O3 O1 136.9(7) 1_665 4_545
Ga4 O3 O1 97.8(6) 3_644 4_545
O2 O3 O1 108.4(8) 3_544 4_545
La1 O3 O1 82.7(7) 1_554 4_545
O1 O3 O1 83.5(5) 2 4_545
Ga4 O3 O1 96.0(7) 2_756 4_545
O2 O3 O1 114.4(9) 4_745 4_545
O2 O3 O1 122.1(10) 1_655 4_545
O2 O3 O1 37.3(8) 4_545 4_545
La1 O3 O1 61.7(5) 3_644 4_545
O2 O3 O1 153.4(10) 3_644 4_545
La1 O3 O1 149.4(8) 4_655 4_545
O1 O3 O1 98.0(9) 4_655 4_545
O2 O3 O1 134.9(10) 2_655 4_545
Ga2 O3 O3 11.7(5) . 4_655
Ga3 O3 O3 126.9(15) . 4_655
La2 O3 O3 95.5(6) 1_655 4_655
La1 O3 O3 84.5(9) 2_656 4_655
O6 O3 O3 119.8(12) . 4_655
O1 O3 O3 72.6(12) 1_655 4_655
O2 O3 O3 28.3(13) 4_645 4_655
O4 O3 O3 25.3(11) 1_655 4_655
O5 O3 O3 99.9(12) . 4_655
O5 O3 O3 163.5(14) 2_655 4_655
O1 O3 O3 39.9(11) . 4_655
O3 O3 O3 108.1(12) 2_655 4_655
O5 O3 O3 126.6(13) 1_655 4_655
Ta O3 O3 152.3(11) 1_655 4_655
Ga1 O3 O3 152.3(11) 1_655 4_655
O1 O3 O3 123.3(11) 2_655 4_655
Ga2 O3 O3 112.2(7) 2_655 4_655
O3 O3 O3 133.0(10) 2_755 4_655
Ga4 O3 O3 113.3(8) 3_544 4_655
La2 O3 O3 70.7(5) . 4_655
O7 O3 O3 75.5(6) 2_655 4_655
La1 O3 O3 63.8(6) 2_556 4_655
La1 O3 O3 39.0(3) 3_654 4_655
Ga4 O3 O3 35.7(5) 2_656 4_655
Ga4 O3 O3 40.81(17) 3_554 4_655
O2 O3 O3 87.4(12) 1_545 4_655
Ga3 O3 O3 128.6(10) 1_655 4_655
O7 O3 O3 55.3(7) . 4_655
O4 O3 O3 55.0(9) 4_545 4_655
Ga2 O3 O3 86.5(7) 1_655 4_655
O6 O3 O3 128.4(10) 2_655 4_655
O1 O3 O3 83.0(10) 4_645 4_655
O7 O3 O3 78.4(6) 1_655 4_655
Ga2 O3 O3 75.6(6) 4_645 4_655
O6 O3 O3 164.8(12) 2_755 4_655
La1 O3 O3 156.3(6) 1_654 4_655
Ga1 O3 O3 107.5(8) . 4_655
Ta O3 O3 107.5(8) . 4_655
O7 O3 O3 147.0(9) 2_645 4_655
O4 O3 O3 94.3(9) 2 4_655
O4 O3 O3 82.5(9) 4_645 4_655
O2 O3 O3 107.1(13) 1_645 4_655
Ga4 O3 O3 146.6(9) 4_645 4_655
O6 O3 O3 24.2(5) 4_655 4_655
O7 O3 O3 118.3(9) 1_545 4_655
O5 O3 O3 25.8(5) 4_655 4_655
O3 O3 O3 108.4(6) 1_655 4_655
O3 O3 O3 71.6(6) 1_455 4_655
O6 O3 O3 53.4(6) 4_755 4_655
O7 O3 O3 48.9(6) 4_645 4_655
Ga4 O3 O3 79.7(3) 4_655 4_655
O7 O3 O3 140.6(10) 1_645 4_655
O4 O3 O3 110.1(7) 2_655 4_655
La1 O3 O3 23.7(3) 3_554 4_655
O2 O3 O3 26.3(7) . 4_655
Ga2 O3 O3 124.4(5) 2_755 4_655
O2 O3 O3 161.3(14) 2_645 4_655
Ta O3 O3 69.78(13) 1_665 4_655
Ga1 O3 O3 69.78(13) 1_665 4_655
Ga4 O3 O3 124.8(9) 3_644 4_655
O2 O3 O3 116.1(8) 3_544 4_655
La1 O3 O3 117.3(8) 1_554 4_655
O1 O3 O3 94.3(9) 2 4_655
Ga4 O3 O3 70.9(6) 2_756 4_655
O2 O3 O3 80.5(9) 4_745 4_655
O2 O3 O3 54.9(8) 1_655 4_655
O2 O3 O3 44.7(7) 4_545 4_655
La1 O3 O3 105.1(7) 3_644 4_655
O2 O3 O3 132.9(7) 3_644 4_655
La1 O3 O3 113.0(3) 4_655 4_655
O1 O3 O3 28.8(4) 4_655 4_655
O2 O3 O3 90.2(7) 2_655 4_655
O1 O3 O3 70.1(7) 4_545 4_655
Ga2 O3 O3 75.5(12) . 4_645
Ga3 O3 O3 85.2(9) . 4_645
La2 O3 O3 156.4(15) 1_655 4_645
La1 O3 O3 53.2(6) 2_656 4_645
O6 O3 O3 46.8(7) . 4_645
O1 O3 O3 100.1(18) 1_655 4_645
O2 O3 O3 60.0(13) 4_645 4_645
O4 O3 O3 99.8(15) 1_655 4_645
O5 O3 O3 48.7(8) . 4_645
O5 O3 O3 98.2(8) 2_655 4_645
O1 O3 O3 70.1(14) . 4_645
O3 O3 O3 108.1(12) 2_655 4_645
O5 O3 O3 84.2(8) 1_655 4_645
Ta O3 O3 82.0(3) 1_655 4_645
Ga1 O3 O3 82.0(3) 1_655 4_645
O1 O3 O3 157.1(12) 2_655 4_645
Ga2 O3 O3 138.4(11) 2_655 4_645
O3 O3 O3 133.0(10) 2_755 4_645
Ga4 O3 O3 39.6(2) 3_544 4_645
La2 O3 O3 99.8(8) . 4_645
O7 O3 O3 150.6(10) 2_655 4_645
La1 O3 O3 40.1(4) 2_556 4_645
La1 O3 O3 92.7(8) 3_654 4_645
Ga4 O3 O3 41.9(6) 2_656 4_645
Ga4 O3 O3 114.9(8) 3_554 4_645
O2 O3 O3 19.1(10) 1_545 4_645
Ga3 O3 O3 109.6(8) 1_655 4_645
O7 O3 O3 115.9(10) . 4_645
O4 O3 O3 21.4(10) 4_545 4_645
Ga2 O3 O3 104.6(9) 1_655 4_645
O6 O3 O3 84.1(6) 2_655 4_645
O1 O3 O3 26.6(4) 4_645 4_645
O7 O3 O3 141.0(11) 1_655 4_645
Ga2 O3 O3 4.7(2) 4_645 4_645
O6 O3 O3 103.9(5) 2_755 4_645
La1 O3 O3 128.0(4) 1_654 4_645
Ga1 O3 O3 63.8(4) . 4_645
Ta O3 O3 63.8(4) . 4_645
O7 O3 O3 71.7(5) 2_645 4_645
O4 O3 O3 140.7(11) 2 4_645
O4 O3 O3 65.0(8) 4_645 4_645
O2 O3 O3 59.7(9) 1_645 4_645
Ga4 O3 O3 82.5(3) 4_645 4_645
O6 O3 O3 52.7(6) 4_655 4_645
O7 O3 O3 53.9(6) 1_545 4_645
O5 O3 O3 65.0(7) 4_655 4_645
O3 O3 O3 108.4(6) 1_655 4_645
O3 O3 O3 71.6(6) 1_455 4_645
O6 O3 O3 73.1(8) 4_755 4_645
O7 O3 O3 41.8(6) 4_645 4_645
Ga4 O3 O3 146.0(8) 4_655 4_645
O7 O3 O3 74.5(5) 1_645 4_645
O4 O3 O3 163.6(11) 2_655 4_645
La1 O3 O3 75.1(6) 3_554 4_645
O2 O3 O3 99.2(9) . 4_645
Ga2 O3 O3 145.7(8) 2_755 4_645
O2 O3 O3 102.6(9) 2_645 4_645
Ta O3 O3 143.7(7) 1_665 4_645
Ga1 O3 O3 143.7(7) 1_665 4_645
Ga4 O3 O3 74.7(4) 3_644 4_645
O2 O3 O3 130.0(9) 3_544 4_645
La1 O3 O3 102.4(7) 1_554 4_645
O1 O3 O3 108.4(9) 2 4_645
Ga4 O3 O3 73.9(7) 2_756 4_645
O2 O3 O3 91.4(8) 4_745 4_645
O2 O3 O3 114.3(11) 1_655 4_645
O2 O3 O3 58.5(8) 4_545 4_645
La1 O3 O3 38.7(3) 3_644 4_645
O2 O3 O3 150.3(8) 3_644 4_645
La1 O3 O3 169.7(7) 4_655 4_645
O1 O3 O3 97.4(8) 4_655 4_645
O2 O3 O3 159.4(11) 2_655 4_645
O1 O3 O3 25.8(6) 4_545 4_645
O3 O3 O3 75.4(7) 4_655 4_645
Ga2 O3 La2 76.0(11) . 3_645
Ga3 O3 La2 118.4(12) . 3_645
La2 O3 La2 119.9(11) 1_655 3_645
La1 O3 La2 21.7(4) 2_656 3_645
O6 O3 La2 55.4(9) . 3_645
O1 O3 La2 63.7(15) 1_655 3_645
O2 O3 La2 41.7(13) 4_645 3_645
O4 O3 La2 84.8(13) 1_655 3_645
O5 O3 La2 84.7(10) . 3_645
O5 O3 La2 115.1(10) 2_655 3_645
O1 O3 La2 88.1(14) . 3_645
O3 O3 La2 144.7(12) 2_655 3_645
O5 O3 La2 65.8(8) 1_655 3_645
Ta O3 La2 83.5(6) 1_655 3_645
Ga1 O3 La2 83.5(6) 1_655 3_645
O1 O3 La2 156.1(9) 2_655 3_645
Ga2 O3 La2 174.9(8) 2_655 3_645
O3 O3 La2 110.3(12) 2_755 3_645
Ga4 O3 La2 65.8(5) 3_544 3_645
La2 O3 La2 126.3(6) . 3_645
O7 O3 La2 131.4(10) 2_655 3_645
La1 O3 La2 71.4(5) 2_556 3_645
La1 O3 La2 64.7(5) 3_654 3_645
Ga4 O3 La2 36.5(3) 2_656 3_645
Ga4 O3 La2 106.7(6) 3_554 3_645
O2 O3 La2 54.7(10) 1_545 3_645
Ga3 O3 La2 85.9(6) 1_655 3_645
O7 O3 La2 123.9(8) . 3_645
O4 O3 La2 41.4(9) 4_545 3_645
Ga2 O3 La2 68.4(5) 1_655 3_645
O6 O3 La2 116.7(6) 2_655 3_645
O1 O3 La2 18.3(8) 4_645 3_645
O7 O3 La2 106.4(8) 1_655 3_645
Ga2 O3 La2 32.1(3) 4_645 3_645
O6 O3 La2 101.4(7) 2_755 3_645
La1 O3 La2 131.3(6) 1_654 3_645
Ga1 O3 La2 99.7(5) . 3_645
Ta O3 La2 99.7(5) . 3_645
O7 O3 La2 86.6(8) 2_645 3_645
O4 O3 La2 163.0(8) 2 3_645
O4 O3 La2 30.5(7) 4_645 3_645
O2 O3 La2 40.6(9) 1_645 3_645
Ga4 O3 La2 106.6(5) 4_645 3_645
O6 O3 La2 57.1(5) 4_655 3_645
O7 O3 La2 85.0(6) 1_545 3_645
O5 O3 La2 46.0(5) 4_655 3_645
O3 O3 La2 76.6(3) 1_655 3_645
O3 O3 La2 103.4(3) 1_455 3_645
O6 O3 La2 39.2(4) 4_755 3_645
O7 O3 La2 19.9(4) 4_645 3_645
Ga4 O3 La2 145.5(6) 4_655 3_645
O7 O3 La2 71.9(6) 1_645 3_645
O4 O3 La2 129.7(8) 2_655 3_645
La1 O3 La2 82.9(4) 3_554 3_645
O2 O3 La2 94.5(10) . 3_645
Ga2 O3 La2 118.8(6) 2_755 3_645
O2 O3 La2 120.7(9) 2_645 3_645
Ta O3 La2 117.1(6) 1_665 3_645
Ga1 O3 La2 117.1(6) 1_665 3_645
Ga4 O3 La2 59.6(4) 3_644 3_645
O2 O3 La2 166.0(8) 3_544 3_645
La1 O3 La2 138.3(5) 1_554 3_645
O1 O3 La2 142.7(7) 2 3_645
Ga4 O3 La2 37.3(3) 2_756 3_645
O2 O3 La2 55.0(6) 4_745 3_645
O2 O3 La2 83.2(9) 1_655 3_645
O2 O3 La2 80.1(7) 4_545 3_645
La1 O3 La2 38.4(2) 3_644 3_645
O2 O3 La2 134.5(7) 3_644 3_645
La1 O3 La2 150.8(6) 4_655 3_645
O1 O3 La2 76.4(7) 4_655 3_645
O2 O3 La2 149.3(8) 2_655 3_645
O1 O3 La2 59.8(6) 4_545 3_645
O3 O3 La2 68.8(6) 4_655 3_645
O3 O3 La2 36.6(5) 4_645 3_645
Ga2 O3 O3 55.5(8) . 4_755
Ga3 O3 O3 170.7(15) . 4_755
La2 O3 O3 69.6(6) 1_655 4_755
La1 O3 O3 60.0(8) 2_656 4_755
O6 O3 O3 110.6(13) . 4_755
O1 O3 O3 28.5(10) 1_655 4_755
O2 O3 O3 33.4(14) 4_645 4_755
O4 O3 O3 36.9(10) 1_655 4_755
O5 O3 O3 134.5(13) . 4_755
O5 O3 O3 152.3(13) 2_655 4_755
O1 O3 O3 84.0(12) . 4_755
O3 O3 O3 143.0(6) 2_655 4_755
O5 O3 O3 88.0(10) 1_655 4_755
Ta O3 O3 121.1(11) 1_655 4_755
Ga1 O3 O3 121.1(11) 1_655 4_755
O1 O3 O3 113.0(11) 2_655 4_755
Ga2 O3 O3 125.3(5) 2_655 4_755
O3 O3 O3 93.2(11) 2_755 4_755
Ga4 O3 O3 124.8(9) 3_544 4_755
La2 O3 O3 108.9(5) . 4_755
O7 O3 O3 72.4(7) 2_655 4_755
La1 O3 O3 101.6(7) 2_556 4_755
La1 O3 O3 7.6(3) 3_654 4_755
Ga4 O3 O3 53.2(5) 2_656 4_755
Ga4 O3 O3 57.1(2) 3_554 4_755
O2 O3 O3 108.3(14) 1_545 4_755
Ga3 O3 O3 84.6(8) 1_655 4_755
O7 O3 O3 82.1(6) . 4_755
O4 O3 O3 78.3(10) 4_545 4_755
Ga2 O3 O3 42.5(5) 1_655 4_755
O6 O3 O3 171.6(9) 2_655 4_755
O1 O3 O3 77.2(10) 4_645 4_755
O7 O3 O3 51.8(6) 1_655 4_755
Ga2 O3 O3 86.5(7) 4_645 4_755
O6 O3 O3 121.1(10) 2_755 4_755
La1 O3 O3 129.0(8) 1_654 4_755
Ga1 O3 O3 147.4(9) . 4_755
Ta O3 O3 147.4(9) . 4_755
O7 O3 O3 137.8(10) 2_645 4_755
O4 O3 O3 109.4(7) 2 4_755
O4 O3 O3 50.9(8) 4_645 4_755
O2 O3 O3 79.5(11) 1_645 4_755
Ga4 O3 O3 161.3(8) 4_645 4_755
O6 O3 O3 60.1(6) 4_655 4_755
O7 O3 O3 143.2(9) 1_545 4_755
O5 O3 O3 29.6(5) 4_655 4_755
O3 O3 O3 64.3(5) 1_655 4_755
O3 O3 O3 115.7(5) 1_455 4_755
O6 O3 O3 21.0(5) 4_755 4_755
O7 O3 O3 47.8(6) 4_645 4_755
Ga4 O3 O3 88.5(2) 4_655 4_755
O7 O3 O3 111.0(9) 1_645 4_755
O4 O3 O3 84.8(7) 2_655 4_755
La1 O3 O3 67.5(4) 3_554 4_755
O2 O3 O3 54.1(7) . 4_755
Ga2 O3 O3 89.7(6) 2_755 4_755
O2 O3 O3 154.1(13) 2_645 4_755
Ta O3 O3 58.15(16) 1_665 4_755
Ga1 O3 O3 58.15(16) 1_665 4_755
Ga4 O3 O3 90.7(7) 3_644 4_755
O2 O3 O3 134.0(7) 3_544 4_755
La1 O3 O3 154.8(6) 1_554 4_755
O1 O3 O3 129.6(8) 2 4_755
Ga4 O3 O3 34.9(4) 2_756 4_755
O2 O3 O3 37.6(7) 4_745 4_755
O2 O3 O3 24.9(7) 1_655 4_755
O2 O3 O3 87.7(8) 4_545 4_755
La1 O3 O3 93.8(7) 3_644 4_755
O2 O3 O3 105.7(7) 3_644 4_755
La1 O3 O3 100.7(5) 4_655 4_755
O1 O3 O3 24.7(4) 4_655 4_755
O2 O3 O3 90.3(7) 2_655 4_755
O1 O3 O3 100.8(8) 4_545 4_755
O3 O3 O3 44.1(4) 4_655 4_755
O3 O3 O3 89.5(9) 4_645 4_755
La2 O3 O3 59.1(5) 3_645 4_755
Ga2 O3 O3 97.2(14) . 4_745
Ga3 O3 O3 109.8(9) . 4_745
La2 O3 O3 115.5(13) 1_655 4_745
La1 O3 O3 12.2(5) 2_656 4_745
O6 O3 O3 39.6(8) . 4_745
O1 O3 O3 64.7(16) 1_655 4_745
O2 O3 O3 61.7(14) 4_645 4_745
O4 O3 O3 102.8(15) 1_655 4_745
O5 O3 O3 84.9(9) . 4_745
O5 O3 O3 96.3(8) 2_655 4_745
O1 O3 O3 107.5(16) . 4_745
O3 O3 O3 143.0(6) 2_655 4_745
O5 O3 O3 45.7(7) 1_655 4_745
Ta O3 O3 62.9(4) 1_655 4_745
Ga1 O3 O3 62.9(4) 1_655 4_745
O1 O3 O3 138.0(11) 2_655 4_745
Ga2 O3 O3 158.3(7) 2_655 4_745
O3 O3 O3 93.2(11) 2_755 4_745
Ga4 O3 O3 57.6(3) 3_544 4_745
La2 O3 O3 143.2(9) . 4_745
O7 O3 O3 139.6(11) 2_655 4_745
La1 O3 O3 83.9(6) 2_556 4_745
La1 O3 O3 78.0(8) 3_654 4_745
Ga4 O3 O3 57.6(6) 2_656 4_745
Ga4 O3 O3 125.1(9) 3_554 4_745
O2 O3 O3 57.3(10) 1_545 4_745
Ga3 O3 O3 68.4(6) 1_655 4_745
O7 O3 O3 144.9(10) . 4_745
O4 O3 O3 57.3(11) 4_545 4_745
Ga2 O3 O3 63.8(7) 1_655 4_745
O6 O3 O3 107.6(5) 2_655 4_745
O1 O3 O3 17.5(3) 4_645 4_745
O7 O3 O3 108.0(10) 1_655 4_745
Ga2 O3 O3 39.5(3) 4_645 4_745
O6 O3 O3 80.2(6) 2_755 4_745
La1 O3 O3 110.1(6) 1_654 4_745
Ga1 O3 O3 97.9(4) . 4_745
Ta O3 O3 97.9(4) . 4_745
O7 O3 O3 69.3(6) 2_645 4_745
O4 O3 O3 174.7(10) 2 4_745
O4 O3 O3 24.8(7) 4_645 4_745
O2 O3 O3 19.7(8) 1_645 4_745
Ga4 O3 O3 91.7(2) 4_645 4_745
O6 O3 O3 78.0(8) 4_655 4_745
O7 O3 O3 77.9(5) 1_545 4_745
O5 O3 O3 65.4(7) 4_655 4_745
O3 O3 O3 64.3(5) 1_655 4_745
O3 O3 O3 115.7(5) 1_455 4_745
O6 O3 O3 50.0(7) 4_755 4_745
O7 O3 O3 40.9(6) 4_645 4_745
Ga4 O3 O3 158.4(8) 4_655 4_745
O7 O3 O3 51.0(6) 1_645 4_745
O4 O3 O3 119.6(9) 2_655 4_745
La1 O3 O3 104.0(7) 3_554 4_745
O2 O3 O3 114.7(11) . 4_745
Ga2 O3 O3 104.0(8) 2_755 4_745
O2 O3 O3 101.9(9) 2_645 4_745
Ta O3 O3 124.4(8) 1_665 4_745
Ga1 O3 O3 124.4(8) 1_665 4_745
Ga4 O3 O3 38.7(3) 3_644 4_745
O2 O3 O3 152.6(9) 3_544 4_745
La1 O3 O3 132.3(4) 1_554 4_745
O1 O3 O3 149.9(8) 2 4_745
Ga4 O3 O3 39.4(5) 2_756 4_745
O2 O3 O3 52.2(7) 4_745 4_745
O2 O3 O3 91.7(9) 1_655 4_745
O2 O3 O3 98.1(8) 4_545 4_745
La1 O3 O3 22.89(16) 3_644 4_745
O2 O3 O3 116.7(8) 3_644 4_745
La1 O3 O3 138.5(8) 4_655 4_745
O1 O3 O3 92.6(8) 4_655 4_745
O2 O3 O3 152.8(11) 2_655 4_745
O1 O3 O3 69.9(6) 4_545 4_745
O3 O3 O3 89.5(9) 4_655 4_745
O3 O3 O3 44.1(4) 4_645 4_745
La2 O3 O3 21.2(3) 3_645 4_745
O3 O3 O3 71.0(7) 4_755 4_745
Ga2 O3 O1 162.4(15) . 3_644
Ga3 O3 O1 56.9(9) . 3_644
La2 O3 O1 73.3(8) 1_655 3_644
La1 O3 O1 103.7(8) 2_656 3_644
O6 O3 O1 72.6(10) . 3_644
O1 O3 O1 104.6(11) 1_655 3_644
O2 O3 O1 158.2(18) 4_645 3_644
O4 O3 O1 142.7(16) 1_655 3_644
O5 O3 O1 88.7(10) . 3_644
O5 O3 O1 23.3(9) 2_655 3_644
O1 O3 O1 140.4(17) . 3_644
O3 O3 O1 68.1(11) 2_655 3_644
O5 O3 O1 59.1(8) 1_655 3_644
Ta O3 O1 38.9(6) 1_655 3_644
Ga1 O3 O1 38.9(6) 1_655 3_644
O1 O3 O1 44.3(5) 2_655 3_644
Ga2 O3 O1 58.3(7) 2_655 3_644
O3 O3 O1 39.5(8) 2_755 3_644
Ga4 O3 O1 78.8(6) 3_544 3_644
La2 O3 O1 104.5(8) . 3_644
O7 O3 O1 91.9(10) 2_655 3_644
La1 O3 O1 124.5(7) 2_556 3_644
La1 O3 O1 135.6(7) 3_654 3_644
Ga4 O3 O1 156.4(8) 2_656 3_644
Ga4 O3 O1 126.8(9) 3_554 3_644
O2 O3 O1 104.4(11) 1_545 3_644
Ga3 O3 O1 50.5(4) 1_655 3_644
O7 O3 O1 114.5(10) . 3_644
O4 O3 O1 137.3(11) 4_545 3_644
Ga2 O3 O1 90.9(6) 1_655 3_644
O6 O3 O1 55.9(5) 2_655 3_644
O1 O3 O1 108.7(13) 4_645 3_644
O7 O3 O1 91.1(9) 1_655 3_644
Ga2 O3 O1 117.0(7) 4_645 3_644
O6 O3 O1 20.5(6) 2_755 3_644
La1 O3 O1 11.3(6) 1_654 3_644
Ga1 O3 O1 78.9(5) . 3_644
Ta O3 O1 78.9(5) . 3_644
O7 O3 O1 45.4(8) 2_645 3_644
O4 O3 O1 75.4(9) 2 3_644
O4 O3 O1 103.3(9) 4_645 3_644
O2 O3 O1 81.7(10) 1_645 3_644
Ga4 O3 O1 41.8(5) 4_645 3_644
O6 O3 O1 166.5(8) 4_655 3_644
O7 O3 O1 71.8(7) 1_545 3_644
O5 O3 O1 158.4(8) 4_655 3_644
O3 O3 O1 69.9(4) 1_655 3_644
O3 O3 O1 110.1(4) 1_455 3_644
O6 O3 O1 128.9(7) 4_755 3_644
O7 O3 O1 141.3(9) 4_645 3_644
Ga4 O3 O1 88.4(8) 4_655 3_644
O7 O3 O1 50.0(7) 1_645 3_644
O4 O3 O1 58.2(7) 2_655 3_644
La1 O3 O1 153.2(8) 3_554 3_644
O2 O3 O1 141.8(11) . 3_644
Ga2 O3 O1 45.8(5) 2_755 3_644
O2 O3 O1 22.3(7) 2_645 3_644
Ta O3 O1 98.1(7) 1_665 3_644
Ga1 O3 O1 98.1(7) 1_665 3_644
Ga4 O3 O1 63.0(5) 3_644 3_644
O2 O3 O1 55.9(10) 3_544 3_644
La1 O3 O1 61.0(5) 1_554 3_644
O1 O3 O1 81.0(5) 2 3_644
Ga4 O3 O1 112.3(6) 2_756 3_644
O2 O3 O1 99.5(9) 4_745 3_644
O2 O3 O1 116.6(8) 1_655 3_644
O2 O3 O1 139.5(10) 4_545 3_644
La1 O3 O1 86.7(6) 3_644 3_644
O2 O3 O1 35.1(9) 3_644 3_644
La1 O3 O1 54.5(6) 4_655 3_644
O1 O3 O1 141.5(8) 4_655 3_644
O2 O3 O1 77.4(9) 2_655 3_644
O1 O3 O1 120.5(10) 4_545 3_644
O3 O3 O1 167.4(8) 4_655 3_644
O3 O3 O1 117.1(6) 4_645 3_644
La2 O3 O1 121.5(7) 3_645 3_644
O3 O3 O1 132.4(8) 4_755 3_644
O3 O3 O1 100.4(6) 4_745 3_644
Ga2 O3 O1 124.9(14) . 3_544
Ga3 O3 O1 18.0(9) . 3_544
La2 O3 O1 99.0(10) 1_655 3_544
La1 O3 O1 129.7(8) 2_656 3_544
O6 O3 O1 80.0(11) . 3_544
O1 O3 O1 147.0(16) 1_655 3_544
O2 O3 O1 155.2(18) 4_645 3_544
O4 O3 O1 136.1(14) 1_655 3_544
O5 O3 O1 56.2(10) . 3_544
O5 O3 O1 29.0(8) 2_655 3_544
O1 O3 O1 97.7(13) . 3_544
O3 O3 O1 30.0(7) 2_655 3_544
O5 O3 O1 95.5(8) 1_655 3_544
Ta O3 O1 63.9(6) 1_655 3_544
Ga1 O3 O1 63.9(6) 1_655 3_544
O1 O3 O1 55.2(6) 2_655 3_544
Ga2 O3 O1 42.9(7) 2_655 3_544
O3 O3 O1 80.4(11) 2_755 3_544
Ga4 O3 O1 67.3(7) 3_544 3_544
La2 O3 O1 67.0(6) . 3_544
O7 O3 O1 95.6(11) 2_655 3_544
La1 O3 O1 86.5(6) 2_556 3_544
La1 O3 O1 162.2(9) 3_654 3_544
Ga4 O3 O1 136.7(8) 2_656 3_544
Ga4 O3 O1 114.3(9) 3_554 3_544
O2 O3 O1 83.6(11) 1_545 3_544
Ga3 O3 O1 93.5(5) 1_655 3_544
O7 O3 O1 90.3(9) . 3_544
O4 O3 O1 112.2(11) 4_545 3_544
Ga2 O3 O1 133.9(7) 1_655 3_544
O6 O3 O1 18.6(5) 2_655 3_544
O1 O3 O1 114.7(14) 4_645 3_544
O7 O3 O1 116.4(10) 1_655 3_544
Ga2 O3 O1 105.7(7) 4_645 3_544
O6 O3 O1 58.7(6) 2_755 3_544
La1 O3 O1 43.8(4) 1_654 3_544
Ga1 O3 O1 42.0(5) . 3_544
Ta O3 O1 42.0(5) . 3_544
O7 O3 O1 50.8(8) 2_645 3_544
O4 O3 O1 59.5(9) 2 3_544
O4 O3 O1 137.0(9) 4_645 3_544
O2 O3 O1 108.6(10) 1_645 3_544
Ga4 O3 O1 27.8(6) 4_645 3_544
O6 O3 O1 125.9(7) 4_655 3_544
O7 O3 O1 49.1(7) 1_545 3_544
O5 O3 O1 157.7(8) 4_655 3_544
O3 O3 O1 113.1(3) 1_655 3_544
O3 O3 O1 66.9(3) 1_455 3_544
O6 O3 O1 168.6(8) 4_755 3_544
O7 O3 O1 144.2(8) 4_645 3_544
Ga4 O3 O1 80.2(7) 4_655 3_544
O7 O3 O1 75.1(7) 1_645 3_544
O4 O3 O1 84.2(8) 2_655 3_544
La1 O3 O1 113.0(6) 3_554 3_544
O2 O3 O1 120.3(9) . 3_544
Ga2 O3 O1 81.8(6) 2_755 3_544
O2 O3 O1 24.9(8) 2_645 3_544
Ta O3 O1 109.7(8) 1_665 3_544
Ga1 O3 O1 109.7(8) 1_665 3_544
Ga4 O3 O1 94.8(5) 3_644 3_544
O2 O3 O1 34.3(10) 3_544 3_544
La1 O3 O1 19.5(3) 1_554 3_544
O1 O3 O1 44.2(4) 2 3_544
Ga4 O3 O1 151.5(6) 2_756 3_544
O2 O3 O1 142.5(9) 4_745 3_544
O2 O3 O1 142.9(10) 1_655 3_544
O2 O3 O1 96.4(10) 4_545 3_544
La1 O3 O1 97.1(6) 3_644 3_544
O2 O3 O1 64.7(9) 3_644 3_544
La1 O3 O1 67.4(6) 4_655 3_544
O1 O3 O1 147.5(10) 4_655 3_544
O2 O3 O1 77.6(10) 2_655 3_544
O1 O3 O1 89.4(10) 4_545 3_544
O3 O3 O1 136.6(9) 4_655 3_544
O3 O3 O1 102.5(7) 4_645 3_544
La2 O3 O1 132.9(7) 3_645 3_544
O3 O3 O1 167.7(8) 4_755 3_544
O3 O3 O1 119.5(6) 4_745 3_544
O1 O3 O1 43.3(5) 3_644 3_544
Ga4 O4 Ga2 115(3) 3_454 1_455
Ga4 O4 La1 131(3) 3_454 3_554
Ga2 O4 La1 113(2) 1_455 3_554
Ga4 O4 La2 94(2) 3_454 .
Ga2 O4 La2 73.6(18) 1_455 .
La1 O4 La2 92.0(17) 3_554 .
Ga4 O4 O1 136(3) 3_454 .
Ga2 O4 O1 76(2) 1_455 .
La1 O4 O1 52.2(14) 3_554 .
La2 O4 O1 45.8(15) . .
Ga4 O4 O3 115(3) 3_454 1_455
Ga2 O4 O3 30.5(11) 1_455 1_455
La1 O4 O3 102.3(18) 3_554 1_455
La2 O4 O3 43.9(9) . 1_455
O1 O4 O3 53.1(16) . 1_455
Ga4 O4 O2 161(4) 3_454 4_545
Ga2 O4 O2 50(2) 1_455 4_545
La1 O4 O2 67(2) 3_554 4_545
La2 O4 O2 93(2) . 4_545
O1 O4 O2 59(2) . 4_545
O3 O4 O2 59(3) 1_455 4_545
Ga4 O4 O2 43(2) 3_454 1_455
Ga2 O4 O2 118(3) 1_455 1_455
La1 O4 O2 116(3) 3_554 1_455
La2 O4 O2 137(2) . 1_455
O1 O4 O2 165(3) . 1_455
O3 O4 O2 141(3) 1_455 1_455
O2 O4 O2 128(3) 4_545 1_455
Ga4 O4 O1 92(2) 3_454 1_455
Ga2 O4 O1 33.1(13) 1_455 1_455
La1 O4 O1 136(3) 3_554 1_455
La2 O4 O1 98(2) . 1_455
O1 O4 O1 109(3) . 1_455
O3 O4 O1 60.7(17) 1_455 1_455
O2 O4 O1 69(3) 4_545 1_455
O2 O4 O1 85(2) 1_455 1_455
Ga4 O4 O1 86(2) 3_454 4
Ga2 O4 O1 152(3) 1_455 4
La1 O4 O1 52.5(14) 3_554 4
La2 O4 O1 126.2(19) . 4
O1 O4 O1 102.5(17) . 4
O3 O4 O1 155(2) 1_455 4
O2 O4 O1 105(3) 4_545 4
O2 O4 O1 63.9(18) 1_455 4
O1 O4 O1 136(2) 1_455 4
Ga4 O4 O2 92(2) 3_454 .
Ga2 O4 O2 143(2) 1_455 .
La1 O4 O2 41.0(14) 3_554 .
La2 O4 O2 80.7(14) . .
O1 O4 O2 67.0(15) . .
O3 O4 O2 116.5(18) 1_455 .
O2 O4 O2 107(2) 4_545 .
O2 O4 O2 98(2) 1_455 .
O1 O4 O2 176(2) 1_455 .
O1 O4 O2 45.6(13) 4 .
Ga4 O4 O3 92(2) 3_454 4
Ga2 O4 O3 105(2) 1_455 4
La1 O4 O3 83.8(18) 3_554 4
La2 O4 O3 174.3(17) . 4
O1 O4 O3 129(2) . 4
O3 O4 O3 133(2) 1_455 4
O2 O4 O3 82(2) 4_545 4
O2 O4 O3 48.9(16) 1_455 4
O1 O4 O3 82.5(19) 1_455 4
O1 O4 O3 53.5(12) 4 4
O2 O4 O3 98.4(16) . 4
Ga3 O5 Ga1 106.9(19) . .
Ga3 O5 Ta 106.9(19) . .
Ga1 O5 Ta 0.0(4) . .
Ga3 O5 La1 126.7(19) . 2_556
Ga1 O5 La1 101.5(14) . 2_556
Ta O5 La1 101.5(14) . 2_556
Ga3 O5 O2 139(3) . 1_545
Ga1 O5 O2 109(2) . 1_545
Ta O5 O2 109(2) . 1_545
La1 O5 O2 63.0(19) 2_556 1_545
Ga3 O5 O3 36.2(9) . .
Ga1 O5 O3 142.1(18) . .
Ta O5 O3 142.1(18) . .
La1 O5 O3 100.0(13) 2_556 .
O2 O5 O3 108(2) 1_545 .
Ga3 O5 O3 34.8(10) . 2_655
Ga1 O5 O3 82.8(15) . 2_655
Ta O5 O3 82.8(15) . 2_655
La1 O5 O3 110.0(13) 2_556 2_655
O2 O5 O3 167(3) 1_545 2_655
O3 O5 O3 60.5(15) . 2_655
Ga3 O5 O1 80.1(15) . .
Ga1 O5 O1 118.5(16) . .
Ta O5 O1 118.5(16) . .
La1 O5 O1 46.7(11) 2_556 .
O2 O5 O1 99(3) 1_545 .
O3 O5 O1 60.0(9) . .
O3 O5 O1 69.9(14) 2_655 .
Ga3 O5 O3 100.5(14) . 1_455
Ga1 O5 O3 69.8(12) . 1_455
Ta O5 O3 69.8(12) . 1_455
La1 O5 O3 49.9(9) 2_556 1_455
O2 O5 O3 109(2) 1_545 1_455
O3 O5 O3 102.3(12) . 1_455
O3 O5 O3 68.7(12) 2_655 1_455
O1 O5 O3 49.2(9) . 1_455
Ga3 O5 O1 157.6(18) . 4_545
Ga1 O5 O1 90.7(13) . 4_545
Ta O5 O1 90.7(13) . 4_545
La1 O5 O1 33.2(10) 2_556 4_545
O2 O5 O1 37.8(18) 1_545 4_545
O3 O5 O1 123.2(15) . 4_545
O3 O5 O1 140.2(14) 2_655 4_545
O1 O5 O1 79.3(11) . 4_545
O3 O5 O1 72.2(11) 1_455 4_545
Ga3 O5 O2 74.8(14) . 4_645
Ga1 O5 O2 161.7(17) . 4_645
Ta O5 O2 161.7(17) . 4_645
La1 O5 O2 65.2(11) 2_556 4_645
O2 O5 O2 76.8(15) 1_545 4_645
O3 O5 O2 39.0(10) . 4_645
O3 O5 O2 90.0(14) 2_655 4_645
O1 O5 O2 43.4(12) . 4_645
O3 O5 O2 91.9(12) 1_455 4_645
O1 O5 O2 84.2(13) 4_545 4_645
Ga3 O5 O2 111.9(18) . 4_545
Ga1 O5 O2 98.8(15) . 4_545
Ta O5 O2 98.8(15) . 4_545
La1 O5 O2 18.0(8) 2_556 4_545
O2 O5 O2 80.8(17) 1_545 4_545
O3 O5 O2 92.2(14) . 4_545
O3 O5 O2 92.0(13) 2_655 4_545
O1 O5 O2 33.2(11) . 4_545
O3 O5 O2 35.6(10) 1_455 4_545
O1 O5 O2 50.1(12) 4_545 4_545
O2 O5 O2 64.6(11) 4_645 4_545
Ga4 O6 Ta 113.9(16) 3_544 1_655
Ga4 O6 Ga1 113.9(16) 3_544 1_655
Ta O6 Ga1 0.0(5) 1_655 1_655
Ga4 O6 La1 138.4(15) 3_544 2_656
Ta O6 La1 107.3(13) 1_655 2_656
Ga1 O6 La1 107.3(13) 1_655 2_656
Ga4 O6 O3 113.7(17) 3_544 .
Ta O6 O3 87.9(12) 1_655 .
Ga1 O6 O3 87.9(12) 1_655 .
La1 O6 O3 61.7(10) 2_656 .
Ga4 O6 O2 38.3(15) 3_544 1_545
Ta O6 O2 149(2) 1_655 1_545
Ga1 O6 O2 149(2) 1_655 1_545
La1 O6 O2 100.4(15) 2_656 1_545
O3 O6 O2 94.3(18) . 1_545
Ga4 O6 O1 91.7(13) 3_544 4_645
Ta O6 O1 144.1(17) 1_655 4_645
Ga1 O6 O1 144.1(17) 1_655 4_645
La1 O6 O1 55.0(12) 2_656 4_645
O3 O6 O1 105.0(16) . 4_645
O2 O6 O1 64.2(15) 1_545 4_645
Ga4 O6 O2 131(2) 3_544 1_645
Ta O6 O2 87.2(17) 1_655 1_645
Ga1 O6 O2 87.2(17) 1_655 1_645
La1 O6 O2 54.8(15) 2_656 1_645
O3 O6 O2 111.0(19) . 1_645
O2 O6 O2 120(3) 1_545 1_645
O1 O6 O2 56.9(15) 4_645 1_645
Ga4 O6 O2 112.7(14) 3_544 4_645
Ta O6 O2 122.4(13) 1_655 4_645
Ga1 O6 O2 122.4(13) 1_655 4_645
La1 O6 O2 33.5(9) 2_656 4_645
O3 O6 O2 42.4(10) . 4_645
O2 O6 O2 76.1(13) 1_545 4_645
O1 O6 O2 62.5(16) 4_645 4_645
O2 O6 O2 87.2(15) 1_645 4_645
Ga4 O6 O1 148.6(14) 3_544 1_655
Ta O6 O1 87.3(11) 1_655 1_655
Ga1 O6 O1 87.3(11) 1_655 1_655
La1 O6 O1 27.1(10) 2_656 1_655
O3 O6 O1 40.9(11) . 1_655
O2 O6 O1 113.8(16) 1_545 1_655
O1 O6 O1 81.8(14) 4_645 1_655
O2 O6 O1 70.1(17) 1_645 1_655
O2 O6 O1 37.7(10) 4_645 1_655
Ga4 O6 O3 82.8(12) 3_544 2_655
Ta O6 O3 79.1(10) 1_655 2_655
Ga1 O6 O3 79.1(10) 1_655 2_655
La1 O6 O3 100.2(9) 2_656 2_655
O3 O6 O3 38.7(11) . 2_655
O2 O6 O3 83.7(17) 1_545 2_655
O1 O6 O3 131.0(12) 4_645 2_655
O2 O6 O3 146.4(17) 1_645 2_655
O2 O6 O3 74.9(10) 4_645 2_655
O1 O6 O3 78.7(9) 1_655 2_655
Ga4 O6 O2 82.7(12) 3_544 2_645
Ta O6 O2 37.4(10) 1_655 2_645
Ga1 O6 O2 37.4(10) 1_655 2_645
La1 O6 O2 132.1(12) 2_656 2_645
O3 O6 O2 81.8(14) . 2_645
O2 O6 O2 112.8(16) 1_545 2_645
O1 O6 O2 172.6(16) 4_645 2_645
O2 O6 O2 123.9(14) 1_645 2_645
O2 O6 O2 124.1(16) 4_645 2_645
O1 O6 O2 105.5(13) 1_655 2_645
O3 O6 O2 53.2(9) 2_655 2_645
Ga4 O7 Ta 107.0(19) 3_554 1_565
Ga4 O7 Ga1 107.0(19) 3_554 1_565
Ta O7 Ga1 0.0 1_565 1_565
Ga4 O7 La2 139(2) 3_554 .
Ta O7 La2 109.4(18) 1_565 .
Ga1 O7 La2 109.4(18) 1_565 .
Ga4 O7 O2 37.9(13) 3_554 .
Ta O7 O2 86(2) 1_565 .
Ga1 O7 O2 86(2) 1_565 .
La2 O7 O2 127(2) . .
Ga4 O7 O1 86.9(18) 3_554 .
Ta O7 O1 134.4(17) 1_565 .
Ga1 O7 O1 134.4(17) 1_565 .
La2 O7 O1 53.2(13) . .
O2 O7 O1 80(2) . .
Ga4 O7 O3 118.8(15) 3_554 2_655
Ta O7 O3 133.1(19) 1_565 2_655
Ga1 O7 O3 133.1(19) 1_565 2_655
La2 O7 O3 36.3(8) . 2_655
O2 O7 O3 137(2) . 2_655
O1 O7 O3 61.3(13) . 2_655
Ga4 O7 O1 159.6(17) 3_554 2
Ta O7 O1 92.5(16) 1_565 2
Ga1 O7 O1 92.5(16) 1_565 2
La2 O7 O1 30.9(10) . 2
O2 O7 O1 154(2) . 2
O1 O7 O1 84(2) . 2
O3 O7 O1 41.0(9) 2_655 2
Ga4 O7 O3 77.8(13) 3_554 .
Ta O7 O3 174.9(19) 1_565 .
Ga1 O7 O3 174.9(19) 1_565 .
La2 O7 O3 66.9(9) . .
O2 O7 O3 99.3(19) . .
O1 O7 O3 46.6(8) . .
O3 O7 O3 41.8(10) 2_655 .
O1 O7 O3 82.5(10) 2 .
Ga4 O7 O2 91.3(15) 3_554 2_655
Ta O7 O2 84.7(16) 1_565 2_655
Ga1 O7 O2 84.7(16) 1_565 2_655
La2 O7 O2 111.2(17) . 2_655
O2 O7 O2 121(2) . 2_655
O1 O7 O2 139.4(15) . 2_655
O3 O7 O2 84.8(13) 2_655 2_655
O1 O7 O2 84.4(14) 2 2_655
O3 O7 O2 93.4(10) . 2_655
Ga4 O7 O3 125.6(17) 3_554 1_455
Ta O7 O3 108.8(14) 1_565 1_455
Ga1 O7 O3 108.8(14) 1_565 1_455
La2 O7 O3 20.2(7) . 1_455
O2 O7 O3 106.9(18) . 1_455
O1 O7 O3 39.2(11) . 1_455
O3 O7 O3 51.4(9) 2_655 1_455
O1 O7 O3 49.5(9) 2 1_455
O3 O7 O3 69.0(7) . 1_455
O2 O7 O3 131.3(14) 2_655 1_455
Ga4 O7 O2 142.9(18) 3_554 2
Ta O7 O2 43.5(14) 1_565 2
Ga1 O7 O2 43.5(14) 1_565 2
La2 O7 O2 78.6(14) . 2
O2 O7 O2 129(2) . 2
O1 O7 O2 129.1(15) . 2
O3 O7 O2 90.6(14) 2_655 2
O1 O7 O2 52.4(13) 2 2
O3 O7 O2 131.4(14) . 2
O2 O7 O2 67.8(11) 2_655 2
O3 O7 O2 89.9(10) 1_455 2
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La1 O4 2.14(6) 3_545
La1 O5 2.49(4) 2_556
La1 O6 2.36(3) 2_656
La1 O1 2.46(6) 2_556
La1 O2 2.62(7) 3_545
La1 O1 2.48(6) 3_545
La1 O3 2.68(4) 2_656
La1 O2 2.47(7) 2_546
La1 Ga2 3.370(10) 3_445
La1 Ga2 3.377(9) 2_656
La1 Ta 3.470(6) 1_556
La1 Ga1 3.470(6) 1_556
La2 O7 2.28(4) .
La2 O7 2.28(4) 2
La2 O1 2.54(7) 2
La2 O1 2.54(7) .
La2 O3 2.48(3) 1_455
La2 O3 2.48(3) 2_655
La2 O4 3.37(6) 2
La2 O4 3.37(6) .
La2 Ga2 3.363(5) 1_455
La2 Ga2 3.363(5) 2_655
La2 Ta 3.466(10) 1_565
La2 Ga1 3.466(10) 1_565
Ga1 O6 1.94(3) 1_455
Ga1 O6 1.94(3) 2_655
Ga1 O7 1.96(4) 2_545
Ga1 O7 1.96(4) 1_545
Ga1 O5 1.97(4) .
Ga1 O5 1.97(4) 2
Ga1 O2 3.41(7) 2_545
Ga1 O2 3.41(7) 1_545
Ga1 La2 3.466(10) 1_545
Ga1 La1 3.470(6) 2_556
Ga1 La1 3.470(6) 1_554
Ga1 O3 3.36(3) 1_455
Ta O6 1.94(3) 1_455
Ta O6 1.94(3) 2_655
Ta O7 1.96(4) 2_545
Ta O7 1.96(4) 1_545
Ta O5 1.97(4) .
Ta O5 1.97(4) 2
Ta Ga3 3.095(9) .
Ta Ga3 3.095(9) 1_455
Ta Ga4 3.154(10) 3_444
Ta Ga4 3.154(10) 4_645
Ta Ga4 3.115(12) 4_545
Ta Ga4 3.115(12) 3_544
Ga2 O3 1.89(3) .
Ga2 O1 1.764(19) .
Ga2 O2 1.82(7) 4_645
Ga2 O4 1.89(5) 1_655
Ga2 O1 3.25(2) 1_655
Ga2 La1 3.370(10) 3_654
Ga2 La2 3.363(5) 1_655
Ga2 La1 3.377(9) 2_656
Ga2 La1 3.491(9) 2_556
Ga2 La1 3.515(8) 3_554
Ga2 O2 3.98(7) .
Ga3 O5 1.88(4) .
Ga3 O5 1.88(4) 2_655
Ga3 O3 1.80(3) .
Ga3 O3 1.80(3) 2_655
Ga3 Ta 3.095(9) 1_655
Ga3 O1 3.56(5) .
Ga3 O1 3.56(5) 2_655
Ga3 O2 3.83(7) 1_545
Ga3 O2 3.83(7) 2_645
Ga3 O3 4.25(3) 1_455
Ga3 O3 4.25(3) 2_755
Ga4 O2 1.85(6) 3_545
Ga4 O7 1.91(4) 3_545
Ga4 O4 1.84(5) 3_645
Ga4 O6 1.82(3) 3
Ga4 Ta 3.154(10) 3_655
Ga4 Ta 3.115(12) 3
Ga4 O1 3.48(6) 2_656
Ga4 O1 3.58(6) 3_545
Ga4 La1 3.616(12) 1_655
Ga4 O3 3.92(3) 3
Ga4 O3 4.28(3) 2_656
O1 La1 2.46(6) 2_556
O1 La1 2.48(6) 3_554
O1 O3 2.86(6) 1_455
O1 O4 3.13(6) .
O1 O2 2.77(7) 4_545
O1 O7 3.13(7) .
O1 O3 3.17(4) .
O1 O5 3.37(7) .
O1 O6 2.91(7) 4_655
O1 O2 3.08(8) 4_645
O1 Ga2 3.25(2) 1_455
O1 O4 3.01(7) 1_655
O1 O4 3.08(9) 4_545
O1 Ga4 3.48(6) 2_656
O1 Ga4 3.58(6) 3_554
O1 O2 3.88(9) .
O1 O3 3.65(7) 2_655
O1 O6 4.31(6) 1_455
O1 O5 4.16(6) 4
O1 O7 4.21(7) 2
O1 O3 4.54(7) 4_655
O1 Ga3 4.59(5) 1_455
O1 O2 4.30(10) 1_545
O1 Ga4 4.49(4) 2_556
O1 Ga4 4.63(5) 3_454
O1 O4 5.33(9) 2
O1 O5 4.50(7) 4_655
O1 O7 4.79(7) 4_545
O1 Ga1 4.62(6) 3
O1 Ta 4.62(6) 3
O1 Ga1 4.72(6) 1_565
O1 Ta 4.72(6) 1_565
O1 O6 4.56(6) 1_465
O1 La1 4.79(4) 2_656
O1 La2 4.82(3) 1_655
O1 O6 5.01(5) .
O1 La1 4.78(4) 3_654
O1 O1 4.95(13) 2
O1 Ga2 4.83(6) 4_645
O1 Ga2 4.87(6) 2_655
O1 Ga2 4.85(6) 4_655
O1 O1 4.84(6) 4_545
O1 O1 4.84(6) 4
O1 O5 5.15(7) 2
O1 O7 4.81(6) 2_655
O1 O1 5.01298(17) 1_455
O1 O1 5.0130(3) 1_655
O1 Ga4 5.16(6) 3_544
O1 Ga4 5.32(6) 4_655
O1 Ga3 5.19(6) 3
O1 O2 5.80(8) 1_455
O1 O1 5.74(10) 2_655
O1 O3 5.65(6) 2
O1 Ga2 5.71(5) 4_545
O1 O1 5.65(6) 4_645
O1 O1 5.65(6) 4_655
O1 Ga2 5.74(6) 2
O1 Ga2 5.73(5) 4
O1 La1 5.85(6) 1_554
O1 La2 5.75(7) 3_545
O1 La1 5.83(6) 2_566
O1 O3 6.18(7) 4_645
O1 O2 6.08(8) 1_445
O1 O3 6.26(5) 4
O1 O2 6.19(9) 3_544
O1 La1 6.28(3) 2_456
O1 La2 6.32(4) 1_455
O1 La1 6.30(3) 3_454
O1 O2 6.97(10) 2
O1 O2 6.84(7) 1_655
O1 O3 6.71(5) 2_755
O1 O2 7.10(9) 2_655
O1 O3 6.73(7) 3_455
O1 O3 6.87(7) 3
O1 O3 7.23(6) 4_755
O2 Ga4 1.85(6) 3_554
O2 Ga2 1.82(7) 4_655
O2 O5 2.21(8) 1_565
O2 La1 2.62(7) 3_554
O2 O7 2.94(8) .
O2 La1 2.47(7) 2_566
O2 O3 2.88(7) 4_655
O2 O4 2.32(7) 4
O2 O6 2.89(7) 1_565
O2 O1 2.77(7) 4
O2 O4 2.72(7) 1_655
O2 O6 2.90(8) 1_465
O2 O1 3.08(8) 4_655
O2 Ta 3.41(7) 1_565
O2 Ga1 3.41(7) 1_565
O2 O4 3.83(7) .
O2 Ga3 3.83(7) 1_565
O2 O6 4.24(8) 4_655
O2 La1 4.12(7) 3_654
O2 La1 4.05(6) 2_666
O2 O5 4.49(9) 4_655
O2 Ga4 4.31(6) 3_454
O2 O3 4.19(6) 1_565
O2 La2 4.17(6) 3
O2 Ga4 4.10(6) 2_666
O2 Ga3 4.39(8) 3
O2 O7 4.42(7) 2_655
O2 Ga2 4.37(6) 4
O2 O2 4.53(6) 4_645
O2 O2 4.53(6) 4_655
O2 O1 4.30(10) 1_565
O2 O7 4.56(8) 2
O2 O5 4.88(7) 4
O2 Ta 4.67(6) 1_665
O2 Ga1 4.67(6) 1_665
O2 O6 4.74(8) 2_665
O2 Ga2 4.41(7) 1_565
O2 Ga4 4.86(6) 4_655
O2 O3 4.71(7) 1_465
O2 O5 4.83(7) 2_665
O2 O2 5.0130(5) 1_455
O2 O2 5.0130(6) 1_655
O2 O7 4.94(7) 4_655
O2 Ga4 5.22(8) 2_656
O2 O2 5.02(7) 4_545
O2 O2 5.02(7) 4
O2 O3 5.63(7) .
O2 Ga2 5.47(6) 1_455
O2 La2 5.26(6) 3_655
O2 O3 5.16(8) 2_665
O2 La2 5.66(6) 1_655
O2 Ta 5.53(7) 3
O2 Ga1 5.53(7) 3
O2 Ga3 5.44(7) 1_465
O2 O3 5.39(8) 3
O2 O1 5.80(8) 1_655
O2 O3 5.78(8) 4_755
O2 O3 6.03(7) 1_455
O2 O3 5.79(7) 4
O2 La1 6.15(7) 2_556
O2 La2 5.83(8) 1_565
O2 O3 5.81(7) 3_455
O2 O3 6.39(7) 2_655
O2 O1 6.08(8) 1_665
O2 O2 6.44(13) 2_655
O2 O1 6.19(9) 3
O2 O2 6.80(14) 2
O2 O1 6.97(10) 2
O2 O1 6.84(7) 1_455
O2 O1 7.10(9) 2_655
O2 O1 7.21(10) 2_565
O2 O1 7.08(8) 1_465
O2 O3 7.19(7) 2_765
O2 O1 7.34(9) 2_665
O2 O3 7.20(8) 2_565
O2 O1 7.54(9) 3_655
O2 O1 7.49(6) 4_455
O3 La2 2.48(3) 1_655
O3 La1 2.68(4) 2_656
O3 O6 2.82(4) .
O3 O1 2.86(6) 1_655
O3 O2 2.88(7) 4_645
O3 O4 3.25(6) 1_655
O3 O5 2.93(4) .
O3 O5 2.98(5) 2_655
O3 O3 2.98(8) 2_655
O3 O5 3.49(5) 1_655
O3 Ta 3.36(3) 1_655
O3 Ga1 3.36(3) 1_655
O3 O1 3.65(7) 2_655
O3 Ga2 3.71(4) 2_655
O3 O3 3.67(6) 2_755
O3 Ga4 3.92(3) 3_544
O3 O7 3.91(5) 2_655
O3 La1 4.16(3) 2_556
O3 La1 4.26(3) 3_654
O3 Ga4 4.28(3) 2_656
O3 Ga4 4.37(3) 3_554
O3 O2 4.19(6) 1_545
O3 Ga3 4.25(3) 1_655
O3 O7 4.36(5) .
O3 O4 3.81(6) 4_545
O3 Ga2 4.40(4) 1_655
O3 O6 4.60(5) 2_655
O3 O1 4.54(7) 4_645
O3 O7 4.49(5) 1_655
O3 Ga2 4.66(3) 4_645
O3 O6 4.60(4) 2_755
O3 La1 4.49(3) 1_654
O3 O7 4.63(5) 2_645
O3 O4 5.01(7) 2
O3 O4 4.67(7) 4_645
O3 O2 4.71(7) 1_645
O3 Ga4 4.73(3) 4_645
O3 O6 5.01(4) 4_655
O3 O7 5.02(5) 1_545
O3 O5 5.06(5) 4_655
O3 O3 5.01300(13) 1_655
O3 O3 5.01300(10) 1_455
O3 O6 5.00(5) 4_755
O3 O7 5.38(6) 4_645
O3 Ga4 5.11(3) 4_655
O3 O7 5.13(5) 1_645
O3 O4 5.68(6) 2_655
O3 La1 5.34(3) 3_554
O3 Ga2 5.27(3) 2_755
O3 O2 5.16(8) 2_645
O3 Ta 5.45(3) 1_665
O3 Ga1 5.45(3) 1_665
O3 Ga4 5.48(3) 3_644
O3 O2 5.39(8) 3_544
O3 La1 5.53(4) 1_554
O3 O1 5.65(6) 2
O3 Ga4 5.78(4) 2_756
O3 O2 5.78(8) 4_745
O3 O2 6.03(7) 1_655
O3 O2 5.79(7) 4_545
O3 La1 5.97(3) 3_644
O3 O2 5.81(7) 3_644
O3 La1 5.91(3) 4_655
O3 O1 6.18(7) 4_655
O3 O2 6.39(7) 2_655
O3 O1 6.26(5) 4_545
O3 O3 6.49(5) 4_655
O3 O3 6.49(5) 4_645
O3 La2 6.41(4) 3_645
O3 O3 6.84(6) 4_755
O3 O3 6.84(6) 4_745
O3 O1 6.73(7) 3_644
O3 O1 6.87(7) 3_544
O4 Ga4 1.84(5) 3_454
O4 Ga2 1.89(5) 1_455
O4 La1 2.14(6) 3_554
O4 O3 3.25(6) 1_455
O4 O2 2.32(7) 4_545
O4 O2 2.72(7) 1_455
O4 O1 3.01(7) 1_455
O4 O1 3.08(9) 4
O4 O3 3.81(6) 4
O5 La1 2.49(4) 2_556
O5 O2 2.21(8) 1_545
O5 O3 2.98(5) 2_655
O5 O3 3.49(5) 1_455
O5 O1 4.16(6) 4_545
O5 O2 4.49(9) 4_645
O5 O2 4.88(7) 4_545
O6 Ga4 1.82(3) 3_544
O6 Ta 1.94(3) 1_655
O6 Ga1 1.94(3) 1_655
O6 La1 2.36(3) 2_656
O6 O2 2.89(7) 1_545
O6 O1 2.91(7) 4_645
O6 O2 2.90(8) 1_645
O6 O2 4.24(8) 4_645
O6 O1 4.31(6) 1_655
O6 O3 4.60(5) 2_655
O6 O2 4.74(8) 2_645
O7 Ga4 1.91(4) 3_554
O7 Ta 1.96(4) 1_565
O7 Ga1 1.96(4) 1_565
O7 O3 3.91(5) 2_655
O7 O1 4.21(7) 2
O7 O2 4.42(7) 2_655
O7 O3 4.49(5) 1_455
O7 O2 4.56(8) 2
loop_
_cod_related_suboptimal_struct
2103513
2103514
